# Electronic Supplementary Material (ESI) for Catalysis Science & Technology.
# This journal is © The Royal Society of Chemistry 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1871471'
_audit_update_record             
;
2018-10-04 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H81 As2 Co K5 Mo12 N6 O74'
_chemical_formula_weight         3409.68

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.6422(2)
_cell_length_b                   12.1336(2)
_cell_length_c                   17.7687(3)
_cell_angle_alpha                76.6610(10)
_cell_angle_beta                 89.6320(10)
_cell_angle_gamma                84.5510(10)
_cell_volume                     2430.98(7)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    17082
_cell_measurement_theta_min      1.757
_cell_measurement_theta_max      24.995

_exptl_crystal_description       block
_exptl_crystal_colour            red
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.329
_exptl_crystal_F_000             1658
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    2.664
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.519
_exptl_absorpt_correction_T_max  0.572
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'


_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean 0.01
_diffrn_reflns_number            17082
_diffrn_reflns_av_unetI/netI     0.0435
_diffrn_reflns_av_R_equivalents  0.0280
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         1.757
_diffrn_reflns_theta_max         24.995
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measured_fraction_theta_full 0.968
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_Laue_measured_fraction_full 0.968
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_point_group_measured_fraction_full 0.968
_reflns_number_total             8505
_reflns_number_gt                6870
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0443P)²+8.2491P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8505
_refine_ls_number_parameters     677
_refine_ls_number_restraints     18
_refine_ls_R_factor_all          0.0493
_refine_ls_R_factor_gt           0.0368
_refine_ls_wR_factor_ref         0.1008
_refine_ls_wR_factor_gt          0.0919
_refine_ls_goodness_of_fit_ref   1.045
_refine_ls_restrained_S_all      1.047
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
As1 As 0.67513(5) 1.26851(5) 0.72070(3) 0.01924(14) Uani 1 1 d . . . . .
Mo1 Mo 0.91742(4) 1.32788(4) 0.59805(3) 0.02329(13) Uani 1 1 d . . . . .
Mo2 Mo 0.69554(4) 1.23429(4) 0.52789(3) 0.02344(13) Uani 1 1 d . . . . .
Mo3 Mo 0.42002(4) 1.24577(4) 0.61756(3) 0.02191(13) Uani 1 1 d . . . . .
Mo4 Mo 0.38829(4) 1.35959(4) 0.76681(3) 0.02231(13) Uani 1 1 d . . . . .
Mo5 Mo 0.62928(5) 1.46575(4) 0.84532(3) 0.02319(13) Uani 1 1 d . . . . .
Mo6 Mo 0.88256(4) 1.43374(4) 0.76881(3) 0.02316(13) Uani 1 1 d . . . . .
Co1 Co 0.30829(14) 1.00173(13) 0.56778(9) 0.0244(4) Uani 0.5 1 d . . P . .
K2 K 0.19297(14) 1.49644(13) 0.59576(9) 0.0425(4) Uani 1 1 d . . . . .
K3 K 0.57928(18) 1.52742(14) 0.60276(10) 0.0554(5) Uani 1 1 d . . . . .
O1 O 0.7334(3) 1.3045(3) 0.6254(2) 0.0239(9) Uani 1 1 d . . . . .
O2 O 0.5287(3) 1.3158(3) 0.6916(2) 0.0220(9) Uani 1 1 d . . . . .
O3 O 0.7064(3) 1.3950(3) 0.7490(2) 0.0220(9) Uani 1 1 d . . . . .
O4 O 0.8537(4) 1.2711(4) 0.5149(2) 0.0285(10) Uani 1 1 d . . . . .
O5 O 0.5648(3) 1.1836(3) 0.5875(2) 0.0249(9) Uani 1 1 d . . . . .
O6 O 0.3157(3) 1.2932(3) 0.6915(2) 0.0251(9) Uani 1 1 d . . . . .
O7 O 0.5086(3) 1.3721(3) 0.8360(2) 0.0245(9) Uani 1 1 d . . . . .
O8 O 0.7883(4) 1.4880(3) 0.8467(2) 0.0291(10) Uani 1 1 d . . . . .
O9 O 0.9253(3) 1.3313(3) 0.7046(2) 0.0255(9) Uani 1 1 d . . . . .
O10 O 1.0618(4) 1.3038(4) 0.5797(3) 0.0363(11) Uani 1 1 d . . . . .
O11 O 0.8857(4) 1.4701(4) 0.5585(2) 0.0337(10) Uani 1 1 d . . . . .
O12 O 0.9345(4) 1.1372(3) 0.6571(3) 0.0302(10) Uani 1 1 d . . . . .
O13 O 0.7794(4) 1.0739(3) 0.6145(3) 0.0311(10) Uani 1 1 d . . . . .
O14 O 0.6988(4) 1.1448(4) 0.4647(3) 0.0377(11) Uani 1 1 d . . . . .
O15 O 0.6308(4) 1.3605(4) 0.4751(3) 0.0342(11) Uani 1 1 d . . . . .
O16 O 0.3320(4) 1.1587(4) 0.5857(3) 0.0310(10) Uani 1 1 d . . . . .
O17 O 0.4028(4) 1.3709(4) 0.5490(2) 0.0306(10) Uani 1 1 d . . . . .
O18 O 0.4574(4) 1.0894(3) 0.7212(2) 0.0333(10) Uani 1 1 d . . . . .
O19 O 0.4407(4) 1.1724(4) 0.8219(2) 0.0332(10) Uani 1 1 d . . . . .
O20 O 0.3714(4) 1.4974(3) 0.7137(3) 0.0331(10) Uani 1 1 d . . . . .
O21 O 0.2770(4) 1.3501(4) 0.8302(3) 0.0398(12) Uani 1 1 d . . . . .
O22 O 0.5937(4) 1.4912(4) 0.9345(3) 0.0364(11) Uani 1 1 d . . . . .
O23 O 0.5762(4) 1.5882(4) 0.7817(3) 0.0358(11) Uani 1 1 d . . . . .
O24 O 0.6999(4) 1.2895(4) 0.9138(2) 0.0318(10) Uani 1 1 d . . . . .
O25 O 0.8695(3) 1.2603(3) 0.8575(2) 0.0280(10) Uani 1 1 d . . . . .
O26 O 1.0123(4) 1.4312(4) 0.8144(3) 0.0366(11) Uani 1 1 d . . . . .
O27 O 0.8740(4) 1.5583(4) 0.7002(3) 0.0374(11) Uani 1 1 d . . . . .
N1 N 0.9466(6) 0.6470(5) 0.8883(4) 0.0513(17) Uani 1 1 d . . . . .
H1A H 1.0109 0.6320 0.9138 0.062 Uiso 1 1 calc R U . . .
H1B H 0.8950 0.5996 0.8974 0.062 Uiso 1 1 calc R U . . .
N2 N 0.5915(5) 0.6707(4) 1.0126(3) 0.0393(14) Uani 1 1 d . . . . .
H2A H 0.6240 0.6721 1.0557 0.047 Uiso 1 1 calc R U . . .
H2B H 0.5767 0.6069 1.0035 0.047 Uiso 1 1 calc R U . . .
N3 N 0.8934(5) 0.8025(5) 1.1192(4) 0.059(2) Uani 1 1 d . . . . .
H3B H 0.9329 0.7473 1.1052 0.070 Uiso 1 1 calc R U . . .
H3C H 0.8739 0.7955 1.1667 0.070 Uiso 1 1 calc R U . . .
C1 C 0.8655(5) 1.0627(5) 0.6597(4) 0.0279(14) Uani 1 1 d . . . . .
C2 C 0.8853(6) 0.9543(5) 0.7196(4) 0.0306(14) Uani 1 1 d . . . . .
C3 C 0.9879(6) 0.9279(6) 0.7617(4) 0.0438(18) Uani 1 1 d . . . . .
H3A H 1.0439 0.9790 0.7530 0.053 Uiso 1 1 calc R U . . .
C4 C 1.0081(7) 0.8267(6) 0.8165(5) 0.048(2) Uani 1 1 d . . . . .
H4A H 1.0781 0.8102 0.8436 0.058 Uiso 1 1 calc R U . . .
C5 C 0.9258(7) 0.7491(6) 0.8319(4) 0.0406(17) Uani 1 1 d . . . . .
C6 C 0.8217(8) 0.7764(7) 0.7908(5) 0.059(2) Uani 1 1 d . . . . .
H6A H 0.7646 0.7266 0.8006 0.070 Uiso 1 1 calc R U . . .
C7 C 0.8031(7) 0.8768(7) 0.7357(5) 0.052(2) Uani 1 1 d . . . . .
H7A H 0.7332 0.8933 0.7085 0.062 Uiso 1 1 calc R U . . .
C8 C 0.4638(5) 1.0883(5) 0.7919(4) 0.0283(14) Uani 1 1 d . . . . .
C9 C 0.5035(6) 0.9770(5) 0.8477(4) 0.0312(15) Uani 1 1 d . . . . .
C10 C 0.5553(7) 0.9780(6) 0.9159(5) 0.055(2) Uani 1 1 d . . . . .
H10A H 0.5706 1.0471 0.9260 0.066 Uiso 1 1 calc R U . . .
C11 C 0.5860(8) 0.8770(6) 0.9711(5) 0.060(2) Uani 1 1 d . . . . .
H11A H 0.6222 0.8781 1.0174 0.072 Uiso 1 1 calc R U . . .
C12 C 0.5616(6) 0.7766(6) 0.9551(4) 0.0363(16) Uani 1 1 d . . . . .
C13 C 0.5134(8) 0.7729(6) 0.8863(4) 0.057(2) Uani 1 1 d . . . . .
H13A H 0.4995 0.7036 0.8759 0.068 Uiso 1 1 calc R U . . .
C14 C 0.4851(8) 0.8743(6) 0.8315(5) 0.055(2) Uani 1 1 d . . . . .
H14A H 0.4538 0.8726 0.7838 0.066 Uiso 1 1 calc R U . . .
C15 C 0.7918(5) 1.2304(5) 0.9061(3) 0.0265(14) Uani 1 1 d . . . . .
C16 C 0.8116(5) 1.1150(5) 0.9590(4) 0.0285(14) Uani 1 1 d . . . . .
C17 C 0.8667(6) 1.0247(6) 0.9345(4) 0.0393(17) Uani 1 1 d . . . . .
H17A H 0.8881 1.0334 0.8831 0.047 Uiso 1 1 calc R U . . .
C18 C 0.8910(6) 0.9188(6) 0.9870(5) 0.0462(19) Uani 1 1 d . . . . .
H18A H 0.9278 0.8570 0.9708 0.055 Uiso 1 1 calc R U . . .
C19 C 0.8593(6) 0.9092(6) 1.0619(4) 0.0387(17) Uani 1 1 d . . . . .
C20 C 0.8011(6) 0.9974(6) 1.0872(4) 0.0426(18) Uani 1 1 d . . . . .
H20A H 0.7797 0.9879 1.1387 0.051 Uiso 1 1 calc R U . . .
C21 C 0.7750(6) 1.1005(6) 1.0352(4) 0.0400(17) Uani 1 1 d . . . . .
H21A H 0.7330 1.1601 1.0509 0.048 Uiso 1 1 calc R U . . .
O1W O 0.1293(9) 1.0399(10) 0.5684(6) 0.029(3) Uani 0.5 1 d . U P . .
O1WA O 0.1488(11) 1.0639(10) 0.5299(9) 0.053(4) Uani 0.5 1 d . U P . .
O2W O 0.3075(7) 1.0798(7) 0.4495(5) 0.031(2) Uani 0.5 1 d . U P . .
O3W O 0.2830(8) 0.9288(6) 0.6856(4) 0.028(2) Uani 0.5 1 d . . P . .
OW4 O 0.8467(5) 0.8543(5) 0.2636(3) 0.0699(19) Uani 1 1 d . . . . .
OW5 O 0.1080(6) 1.6365(7) 0.6918(5) 0.101(3) Uani 1 1 d . . . . .
OW6 O 0.0281(6) 0.8510(7) 0.5760(5) 0.101(3) Uani 1 1 d . . . . .
OW7 O 0.1995(6) 1.2888(5) 0.4362(3) 0.076(2) Uani 1 1 d . . . . .
OW8 O 0.1683(5) 1.3599(6) -0.0274(4) 0.0712(18) Uani 1 1 d . . . . .
OW9 O 0.7081(8) 0.3057(7) 0.2282(6) 0.117(3) Uani 1 1 d . . . . .
OW1 O 0.2215(9) 1.5995(8) -0.0671(6) 0.135(4) Uani 1 1 d . . . . .
OW2 O 0.5942(12) 1.7531(10) 0.6344(8) 0.067(4) Uani 0.5 1 d . . P . .
OW3 O 0.4983(17) 1.7329(11) 0.6499(8) 0.097(6) Uani 0.5 1 d . . P . .
K1 K 0.5262(3) 1.0390(3) 0.4052(2) 0.0500(9) Uani 0.5 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
As1 O2 1.786(4) . ?
As1 O3 1.790(4) . ?
As1 O1 1.794(4) . ?
As1 K3 3.4398(17) . ?
Mo1 O11 1.712(4) . ?
Mo1 O10 1.720(4) . ?
Mo1 O9 1.906(4) . ?
Mo1 O4 1.945(4) . ?
Mo1 O1 2.224(4) . ?
Mo1 O12 2.300(4) . ?
Mo1 Mo2 3.2813(7) . ?
Mo1 K2 3.7689(16) 2_686 ?
Mo1 K2 3.9602(17) 1_655 ?
Mo2 O15 1.709(4) . ?
Mo2 O14 1.731(4) . ?
Mo2 O5 1.917(4) . ?
Mo2 O4 1.936(4) . ?
Mo2 O1 2.164(4) . ?
Mo2 O13 2.321(4) . ?
Mo2 K2 3.8266(17) 2_686 ?
Mo2 K3 4.1831(19) . ?
Mo2 K1 4.193(3) . ?
Mo3 O17 1.710(4) . ?
Mo3 O16 1.725(4) . ?
Mo3 O5 1.905(4) . ?
Mo3 O6 1.931(4) . ?
Mo3 O2 2.190(4) . ?
Mo3 O18 2.328(4) . ?
Mo3 Mo4 3.2645(7) . ?
Mo3 K1 3.568(3) 2_676 ?
Mo3 K2 3.7855(17) . ?
Mo3 K3 3.9961(19) . ?
Mo3 K3 4.2346(17) 2_686 ?
Mo4 O21 1.707(4) . ?
Mo4 O20 1.714(4) . ?
Mo4 O7 1.909(4) . ?
Mo4 O6 1.948(4) . ?
Mo4 O2 2.208(4) . ?
Mo4 O19 2.282(4) . ?
Mo4 K2 3.7693(16) . ?
Mo4 K3 3.9529(19) . ?
Mo5 O23 1.710(4) . ?
Mo5 O22 1.723(4) . ?
Mo5 O8 1.897(4) . ?
Mo5 O7 1.920(4) . ?
Mo5 O3 2.232(4) . ?
Mo5 O24 2.282(4) . ?
Mo5 Mo6 3.2663(7) . ?
Mo5 K3 4.2350(18) . ?
Mo6 O27 1.704(4) . ?
Mo6 O26 1.712(4) . ?
Mo6 O9 1.903(4) . ?
Mo6 O8 1.953(4) . ?
Mo6 O3 2.195(4) . ?
Mo6 O25 2.337(4) . ?
Co1 O1WA 1.997(12) . ?
Co1 K1 1.977(4) 2_676 ?
Co1 O14 2.000(5) 2_676 ?
Co1 O16 2.046(4) . ?
Co1 O3W 2.107(8) . ?
Co1 O2W 2.097(9) . ?
Co1 O1W 2.092(11) . ?
Co1 K1 3.809(4) . ?
K2 OW5 2.788(7) . ?
K2 O11 2.823(5) 2_686 ?
K2 O15 2.906(5) 2_686 ?
K2 O6 2.906(4) . ?
K2 O20 2.963(5) . ?
K2 O17 2.972(5) . ?
K2 O10 2.978(5) 1_455 ?
K2 O4 3.046(4) 2_686 ?
K2 Mo1 3.7689(16) 2_686 ?
K2 Mo2 3.8267(17) 2_686 ?
K3 O17 2.710(4) 2_686 ?
K3 O2 2.799(4) . ?
K3 O15 2.879(5) 2_686 ?
K3 OW3 2.883(15) . ?
K3 OW2 2.940(13) . ?
K3 O3 3.033(4) . ?
K3 O1 3.047(4) . ?
K3 O20 3.106(5) . ?
K3 O17 3.216(5) . ?
K3 O15 3.389(5) . ?
K3 O23 3.425(5) . ?
O4 K2 3.046(4) 2_686 ?
O5 K1 2.969(5) 2_676 ?
O10 K2 2.978(5) 1_655 ?
O11 K2 2.823(5) 2_686 ?
O12 C1 1.258(7) . ?
O13 C1 1.266(7) . ?
O14 Co1 2.000(5) 2_676 ?
O14 K1 2.818(5) . ?
O15 K3 2.879(5) 2_686 ?
O15 K2 2.906(5) 2_686 ?
O16 K1 2.753(5) 2_676 ?
O17 K3 2.710(4) 2_686 ?
O18 C8 1.257(7) . ?
O18 K1 3.010(6) 2_676 ?
O19 C8 1.262(7) . ?
O24 C15 1.255(7) . ?
O25 C15 1.267(7) . ?
N1 C5 1.404(9) . ?
N1 H1A 0.8600 . ?
N1 H1B 0.8600 . ?
N2 C12 1.460(8) . ?
N2 H2A 0.8600 . ?
N2 H2B 0.8600 . ?
N3 C19 1.473(8) . ?
N3 H3B 0.8600 . ?
N3 H3C 0.8600 . ?
C1 C2 1.489(9) . ?
C2 C3 1.384(9) . ?
C2 C7 1.388(9) . ?
C3 C4 1.382(10) . ?
C3 H3A 0.9300 . ?
C4 C5 1.389(10) . ?
C4 H4A 0.9300 . ?
C5 C6 1.390(11) . ?
C6 C7 1.376(10) . ?
C6 H6A 0.9300 . ?
C7 H7A 0.9300 . ?
C8 C9 1.513(8) . ?
C9 C10 1.360(10) . ?
C9 C14 1.378(10) . ?
C10 C11 1.399(10) . ?
C10 H10A 0.9300 . ?
C11 C12 1.368(10) . ?
C11 H11A 0.9300 . ?
C12 C13 1.362(10) . ?
C13 C14 1.394(10) . ?
C13 H13A 0.9300 . ?
C14 H14A 0.9300 . ?
C15 C16 1.494(8) . ?
C16 C17 1.372(9) . ?
C16 C21 1.394(9) . ?
C17 C18 1.407(10) . ?
C17 H17A 0.9300 . ?
C18 C19 1.361(11) . ?
C18 H18A 0.9300 . ?
C19 C20 1.374(10) . ?
C20 C21 1.382(9) . ?
C20 H20A 0.9300 . ?
C21 H21A 0.9300 . ?
O1W O1WA 0.722(15) . ?
O2W K1 2.695(9) . ?
O2W K1 3.211(9) 2_676 ?
O3W K1 2.742(10) 2_676 ?
OW2 OW3 1.18(2) . ?
OW2 K1 2.710(13) 2_686 ?
OW3 K1 2.702(14) 2_686 ?
K1 Co1 1.977(4) 2_676 ?
K1 OW3 2.702(14) 2_686 ?
K1 OW2 2.710(13) 2_686 ?
K1 O3W 2.742(10) 2_676 ?
K1 O16 2.753(5) 2_676 ?
K1 O5 2.969(5) 2_676 ?
K1 O18 3.010(6) 2_676 ?
K1 O2W 3.212(9) 2_676 ?
K1 K1 3.351(8) 2_676 ?
K1 Mo3 3.568(3) 2_676 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 As1 O3 96.32(17) . . ?
O2 As1 O1 95.78(18) . . ?
O3 As1 O1 96.67(18) . . ?
O2 As1 K3 54.19(13) . . ?
O3 As1 K3 61.70(13) . . ?
O1 As1 K3 62.15(13) . . ?
O11 Mo1 O10 103.7(2) . . ?
O11 Mo1 O9 99.45(19) . . ?
O10 Mo1 O9 100.2(2) . . ?
O11 Mo1 O4 97.65(19) . . ?
O10 Mo1 O4 98.9(2) . . ?
O9 Mo1 O4 150.45(17) . . ?
O11 Mo1 O1 92.02(18) . . ?
O10 Mo1 O1 163.26(19) . . ?
O9 Mo1 O1 82.46(16) . . ?
O4 Mo1 O1 73.01(16) . . ?
O11 Mo1 O12 172.15(19) . . ?
O10 Mo1 O12 84.11(19) . . ?
O9 Mo1 O12 78.27(16) . . ?
O4 Mo1 O12 81.52(17) . . ?
O1 Mo1 O12 80.26(14) . . ?
O11 Mo1 Mo2 98.30(15) . . ?
O10 Mo1 Mo2 128.98(15) . . ?
O9 Mo1 Mo2 120.81(12) . . ?
O4 Mo1 Mo2 32.19(12) . . ?
O1 Mo1 Mo2 40.91(10) . . ?
O12 Mo1 Mo2 76.80(10) . . ?
O11 Mo1 K2 44.72(15) . 2_686 ?
O10 Mo1 K2 101.07(16) . 2_686 ?
O9 Mo1 K2 141.90(13) . 2_686 ?
O4 Mo1 K2 53.57(13) . 2_686 ?
O1 Mo1 K2 86.01(10) . 2_686 ?
O12 Mo1 K2 135.08(11) . 2_686 ?
Mo2 Mo1 K2 65.32(3) . 2_686 ?
O11 Mo1 K2 68.67(15) . 1_655 ?
O10 Mo1 K2 44.17(16) . 1_655 ?
O9 Mo1 K2 80.36(12) . 1_655 ?
O4 Mo1 K2 128.55(12) . 1_655 ?
O1 Mo1 K2 151.42(10) . 1_655 ?
O12 Mo1 K2 117.93(11) . 1_655 ?
Mo2 Mo1 K2 157.54(3) . 1_655 ?
K2 Mo1 K2 93.61(3) 2_686 1_655 ?
O15 Mo2 O14 103.9(2) . . ?
O15 Mo2 O5 97.97(19) . . ?
O14 Mo2 O5 99.0(2) . . ?
O15 Mo2 O4 97.6(2) . . ?
O14 Mo2 O4 97.2(2) . . ?
O5 Mo2 O4 154.08(17) . . ?
O15 Mo2 O1 93.64(18) . . ?
O14 Mo2 O1 161.57(19) . . ?
O5 Mo2 O1 83.90(16) . . ?
O4 Mo2 O1 74.58(16) . . ?
O15 Mo2 O13 172.00(19) . . ?
O14 Mo2 O13 83.90(19) . . ?
O5 Mo2 O13 78.80(16) . . ?
O4 Mo2 O13 82.93(17) . . ?
O1 Mo2 O13 78.79(15) . . ?
O15 Mo2 Mo1 99.36(15) . . ?
O14 Mo2 Mo1 127.05(16) . . ?
O5 Mo2 Mo1 124.01(12) . . ?
O4 Mo2 Mo1 32.37(12) . . ?
O1 Mo2 Mo1 42.30(11) . . ?
O13 Mo2 Mo1 76.84(10) . . ?
O15 Mo2 K2 45.79(15) . 2_686 ?
O14 Mo2 K2 102.73(16) . 2_686 ?
O5 Mo2 K2 141.26(12) . 2_686 ?
O4 Mo2 K2 52.05(13) . 2_686 ?
O1 Mo2 K2 85.35(11) . 2_686 ?
O13 Mo2 K2 134.87(11) . 2_686 ?
Mo1 Mo2 K2 63.50(3) . 2_686 ?
O15 Mo2 K3 51.31(15) . . ?
O14 Mo2 K3 153.86(16) . . ?
O5 Mo2 K3 79.19(12) . . ?
O4 Mo2 K3 94.80(13) . . ?
O1 Mo2 K3 44.57(11) . . ?
O13 Mo2 K3 120.70(11) . . ?
Mo1 Mo2 K3 71.70(3) . . ?
K2 Mo2 K3 67.25(4) 2_686 . ?
O15 Mo2 K1 93.57(16) . . ?
O14 Mo2 K1 29.52(16) . . ?
O5 Mo2 K1 73.04(13) . . ?
O4 Mo2 K1 126.33(13) . . ?
O1 Mo2 K1 156.57(12) . . ?
O13 Mo2 K1 92.47(11) . . ?
Mo1 Mo2 K1 156.32(5) . . ?
K2 Mo2 K1 115.26(6) 2_686 . ?
K3 Mo2 K1 131.12(5) . . ?
O17 Mo3 O16 104.4(2) . . ?
O17 Mo3 O5 99.96(19) . . ?
O16 Mo3 O5 98.72(18) . . ?
O17 Mo3 O6 96.33(18) . . ?
O16 Mo3 O6 97.60(19) . . ?
O5 Mo3 O6 153.25(17) . . ?
O17 Mo3 O2 92.87(18) . . ?
O16 Mo3 O2 162.05(18) . . ?
O5 Mo3 O2 82.95(15) . . ?
O6 Mo3 O2 75.14(15) . . ?
O17 Mo3 O18 171.88(18) . . ?
O16 Mo3 O18 83.64(18) . . ?
O5 Mo3 O18 79.88(17) . . ?
O6 Mo3 O18 81.03(16) . . ?
O2 Mo3 O18 79.04(15) . . ?
O17 Mo3 Mo4 96.15(14) . . ?
O16 Mo3 Mo4 128.70(15) . . ?
O5 Mo3 Mo4 123.52(12) . . ?
O6 Mo3 Mo4 32.84(11) . . ?
O2 Mo3 Mo4 42.30(10) . . ?
O18 Mo3 Mo4 77.44(11) . . ?
O17 Mo3 K1 129.75(16) . 2_676 ?
O16 Mo3 K1 48.69(15) . 2_676 ?
O5 Mo3 K1 56.30(13) . 2_676 ?
O6 Mo3 K1 124.89(14) . 2_676 ?
O2 Mo3 K1 122.24(11) . 2_676 ?
O18 Mo3 K1 56.83(13) . 2_676 ?
Mo4 Mo3 K1 134.10(7) . 2_676 ?
O17 Mo3 K2 49.40(15) . . ?
O16 Mo3 K2 95.34(14) . . ?
O5 Mo3 K2 148.84(12) . . ?
O6 Mo3 K2 48.89(12) . . ?
O2 Mo3 K2 92.05(10) . . ?
O18 Mo3 K2 129.47(12) . . ?
Mo4 Mo3 K2 64.14(3) . . ?
K1 Mo3 K2 144.03(6) 2_676 . ?
O17 Mo3 K3 51.25(15) . . ?
O16 Mo3 K3 155.41(15) . . ?
O5 Mo3 K3 84.60(12) . . ?
O6 Mo3 K3 89.30(12) . . ?
O2 Mo3 K3 42.37(10) . . ?
O18 Mo3 K3 120.83(11) . . ?
Mo4 Mo3 K3 65.06(3) . . ?
K1 Mo3 K3 140.89(7) 2_676 . ?
K2 Mo3 K3 71.57(4) . . ?
O17 Mo3 K3 21.06(14) . 2_686 ?
O16 Mo3 K3 92.75(15) . 2_686 ?
O5 Mo3 K3 84.55(12) . 2_686 ?
O6 Mo3 K3 115.68(12) . 2_686 ?
O2 Mo3 K3 105.20(11) . 2_686 ?
O18 Mo3 K3 163.27(12) . 2_686 ?
Mo4 Mo3 K3 116.80(3) . 2_686 ?
K1 Mo3 K3 108.97(7) 2_676 2_686 ?
K2 Mo3 K3 67.05(4) . 2_686 ?
K3 Mo3 K3 63.17(4) . 2_686 ?
O21 Mo4 O20 104.6(2) . . ?
O21 Mo4 O7 98.4(2) . . ?
O20 Mo4 O7 99.35(19) . . ?
O21 Mo4 O6 96.6(2) . . ?
O20 Mo4 O6 96.39(19) . . ?
O7 Mo4 O6 154.76(17) . . ?
O21 Mo4 O2 162.60(19) . . ?
O20 Mo4 O2 91.30(18) . . ?
O7 Mo4 O2 85.62(16) . . ?
O6 Mo4 O2 74.38(15) . . ?
O21 Mo4 O19 86.6(2) . . ?
O20 Mo4 O19 168.70(19) . . ?
O7 Mo4 O19 79.12(16) . . ?
O6 Mo4 O19 81.59(16) . . ?
O2 Mo4 O19 77.44(15) . . ?
O21 Mo4 Mo3 127.69(16) . . ?
O20 Mo4 Mo3 95.28(15) . . ?
O7 Mo4 Mo3 125.71(12) . . ?
O6 Mo4 Mo3 32.51(12) . . ?
O2 Mo4 Mo3 41.86(10) . . ?
O19 Mo4 Mo3 77.00(11) . . ?
O21 Mo4 K2 92.93(16) . . ?
O20 Mo4 K2 49.63(15) . . ?
O7 Mo4 K2 148.90(12) . . ?
O6 Mo4 K2 49.40(12) . . ?
O2 Mo4 K2 92.18(10) . . ?
O19 Mo4 K2 130.66(12) . . ?
Mo3 Mo4 K2 64.66(3) . . ?
O21 Mo4 K3 153.35(17) . . ?
O20 Mo4 K3 48.86(16) . . ?
O7 Mo4 K3 85.37(12) . . ?
O6 Mo4 K3 90.32(12) . . ?
O2 Mo4 K3 43.48(10) . . ?
O19 Mo4 K3 119.89(12) . . ?
Mo3 Mo4 K3 66.45(3) . . ?
K2 Mo4 K3 72.22(4) . . ?
O23 Mo5 O22 103.6(2) . . ?
O23 Mo5 O8 100.7(2) . . ?
O22 Mo5 O8 98.5(2) . . ?
O23 Mo5 O7 99.0(2) . . ?
O22 Mo5 O7 98.13(19) . . ?
O8 Mo5 O7 150.39(17) . . ?
O23 Mo5 O3 91.24(18) . . ?
O22 Mo5 O3 164.64(19) . . ?
O8 Mo5 O3 74.52(16) . . ?
O7 Mo5 O3 83.16(15) . . ?
O23 Mo5 O24 170.96(19) . . ?
O22 Mo5 O24 84.93(19) . . ?
O8 Mo5 O24 80.73(17) . . ?
O7 Mo5 O24 76.53(16) . . ?
O3 Mo5 O24 80.47(15) . . ?
O23 Mo5 Mo6 98.28(16) . . ?
O22 Mo5 Mo6 129.74(16) . . ?
O8 Mo5 Mo6 32.50(12) . . ?
O7 Mo5 Mo6 122.43(12) . . ?
O3 Mo5 Mo6 42.02(10) . . ?
O24 Mo5 Mo6 78.02(11) . . ?
O23 Mo5 K3 50.95(15) . . ?
O22 Mo5 K3 151.78(16) . . ?
O8 Mo5 K3 98.43(13) . . ?
O7 Mo5 K3 77.32(12) . . ?
O3 Mo5 K3 43.48(10) . . ?
O24 Mo5 K3 120.05(12) . . ?
Mo6 Mo5 K3 72.51(3) . . ?
O27 Mo6 O26 103.6(2) . . ?
O27 Mo6 O9 99.0(2) . . ?
O26 Mo6 O9 99.7(2) . . ?
O27 Mo6 O8 97.6(2) . . ?
O26 Mo6 O8 95.8(2) . . ?
O9 Mo6 O8 153.91(17) . . ?
O27 Mo6 O3 95.25(19) . . ?
O26 Mo6 O3 159.81(19) . . ?
O9 Mo6 O3 84.18(16) . . ?
O8 Mo6 O3 74.35(15) . . ?
O27 Mo6 O25 172.36(19) . . ?
O26 Mo6 O25 84.00(18) . . ?
O9 Mo6 O25 80.04(16) . . ?
O8 Mo6 O25 80.86(16) . . ?
O3 Mo6 O25 77.11(14) . . ?
O27 Mo6 Mo5 98.42(17) . . ?
O26 Mo6 Mo5 125.39(16) . . ?
O9 Mo6 Mo5 125.38(12) . . ?
O8 Mo6 Mo5 31.45(12) . . ?
O3 Mo6 Mo5 42.90(10) . . ?
O25 Mo6 Mo5 76.32(10) . . ?
O1WA Co1 K1 171.4(4) . 2_676 ?
O1WA Co1 O14 94.5(4) . 2_676 ?
K1 Co1 O14 90.23(17) 2_676 2_676 ?
O1WA Co1 O16 87.9(4) . . ?
K1 Co1 O16 86.34(16) 2_676 . ?
O14 Co1 O16 170.7(2) 2_676 . ?
O1WA Co1 O3W 102.6(5) . . ?
K1 Co1 O3W 84.3(3) 2_676 . ?
O14 Co1 O3W 94.0(3) 2_676 . ?
O16 Co1 O3W 94.2(2) . . ?
O1WA Co1 O2W 69.1(5) . . ?
K1 Co1 O2W 104.0(3) 2_676 . ?
O14 Co1 O2W 86.4(3) 2_676 . ?
O16 Co1 O2W 86.1(3) . . ?
O3W Co1 O2W 171.7(4) . . ?
O1WA Co1 O1W 20.2(4) . . ?
K1 Co1 O1W 166.0(3) 2_676 . ?
O14 Co1 O1W 95.0(4) 2_676 . ?
O16 Co1 O1W 90.3(4) . . ?
O3W Co1 O1W 82.4(4) . . ?
O2W Co1 O1W 89.3(4) . . ?
O1WA Co1 K1 112.2(5) . . ?
K1 Co1 K1 61.50(16) 2_676 . ?
O14 Co1 K1 79.89(15) 2_676 . ?
O16 Co1 K1 90.91(14) . . ?
O3W Co1 K1 145.0(3) . . ?
O2W Co1 K1 43.2(2) . . ?
O1W Co1 K1 132.2(3) . . ?
OW5 K2 O11 122.0(2) . 2_686 ?
OW5 K2 O15 95.94(17) . 2_686 ?
O11 K2 O15 83.28(13) 2_686 2_686 ?
OW5 K2 O6 108.3(2) . . ?
O11 K2 O6 127.75(13) 2_686 . ?
O15 K2 O6 106.00(13) 2_686 . ?
OW5 K2 O20 70.8(2) . . ?
O11 K2 O20 152.58(14) 2_686 . ?
O15 K2 O20 70.76(13) 2_686 . ?
O6 K2 O20 55.52(11) . . ?
OW5 K2 O17 144.88(19) . . ?
O11 K2 O17 86.62(13) 2_686 . ?
O15 K2 O17 65.36(13) 2_686 . ?
O6 K2 O17 55.03(11) . . ?
O20 K2 O17 74.84(13) . . ?
OW5 K2 O10 118.98(17) . 1_455 ?
O11 K2 O10 70.13(13) 2_686 1_455 ?
O15 K2 O10 143.61(14) 2_686 1_455 ?
O6 K2 O10 74.17(12) . 1_455 ?
O20 K2 O10 127.88(13) . 1_455 ?
O17 K2 O10 88.09(13) . 1_455 ?
OW5 K2 O4 76.6(2) . 2_686 ?
O11 K2 O4 55.88(12) 2_686 2_686 ?
O15 K2 O4 54.91(12) 2_686 2_686 ?
O6 K2 O4 160.91(13) . 2_686 ?
O20 K2 O4 111.70(12) . 2_686 ?
O17 K2 O4 110.24(12) . 2_686 ?
O10 K2 O4 120.41(13) 1_455 2_686 ?
OW5 K2 Mo1 100.4(2) . 2_686 ?
O11 K2 Mo1 25.25(9) 2_686 2_686 ?
O15 K2 Mo1 70.98(9) 2_686 2_686 ?
O6 K2 Mo1 151.35(10) . 2_686 ?
O20 K2 Mo1 139.44(10) . 2_686 ?
O17 K2 Mo1 100.76(9) . 2_686 ?
O10 K2 Mo1 91.56(10) 1_455 2_686 ?
O4 K2 Mo1 30.92(8) 2_686 2_686 ?
OW5 K2 Mo4 83.5(2) . . ?
O11 K2 Mo4 154.22(11) 2_686 . ?
O15 K2 Mo4 91.41(9) 2_686 . ?
O6 K2 Mo4 30.59(8) . . ?
O20 K2 Mo4 26.15(8) . . ?
O17 K2 Mo4 68.36(9) . . ?
O10 K2 Mo4 101.76(10) 1_455 . ?
O4 K2 Mo4 137.83(9) 2_686 . ?
Mo1 K2 Mo4 162.21(5) 2_686 . ?
OW5 K2 Mo3 134.7(2) . . ?
O11 K2 Mo3 103.21(10) 2_686 . ?
O15 K2 Mo3 87.29(10) 2_686 . ?
O6 K2 Mo3 30.03(8) . . ?
O20 K2 Mo3 67.78(9) . . ?
O17 K2 Mo3 25.90(8) . . ?
O10 K2 Mo3 75.63(9) 1_455 . ?
O4 K2 Mo3 136.13(9) 2_686 . ?
Mo1 K2 Mo3 122.96(5) 2_686 . ?
Mo4 K2 Mo3 51.20(2) . . ?
OW5 K2 Mo2 85.29(17) . 2_686 ?
O11 K2 Mo2 70.27(9) 2_686 2_686 ?
O15 K2 Mo2 24.93(9) 2_686 2_686 ?
O6 K2 Mo2 130.86(9) . 2_686 ?
O20 K2 Mo2 88.29(9) . 2_686 ?
O17 K2 Mo2 86.49(9) . 2_686 ?
O10 K2 Mo2 140.27(10) 1_455 2_686 ?
O4 K2 Mo2 30.07(8) 2_686 2_686 ?
Mo1 K2 Mo2 51.18(2) 2_686 2_686 ?
Mo4 K2 Mo2 112.52(4) . 2_686 ?
Mo3 K2 Mo2 110.67(4) . 2_686 ?
O17 K3 O2 137.65(14) 2_686 . ?
O17 K3 O15 63.84(13) 2_686 2_686 ?
O2 K3 O15 107.49(14) . 2_686 ?
O17 K3 OW3 95.4(3) 2_686 . ?
O2 K3 OW3 120.0(4) . . ?
O15 K3 OW3 66.6(3) 2_686 . ?
O17 K3 OW2 86.9(3) 2_686 . ?
O2 K3 OW2 134.6(3) . . ?
O15 K3 OW2 81.8(3) 2_686 . ?
OW3 K3 OW2 23.4(4) . . ?
O17 K3 O3 146.13(14) 2_686 . ?
O2 K3 O3 54.19(11) . . ?
O15 K3 O3 150.00(14) 2_686 . ?
OW3 K3 O3 100.2(3) . . ?
OW2 K3 O3 95.7(3) . . ?
O17 K3 O1 104.91(13) 2_686 . ?
O2 K3 O1 53.84(11) . . ?
O15 K3 O1 140.78(14) 2_686 . ?
OW3 K3 O1 151.4(3) . . ?
OW2 K3 O1 136.9(3) . . ?
O3 K3 O1 52.26(11) . . ?
O17 K3 O20 132.87(14) 2_686 . ?
O2 K3 O20 56.90(11) . . ?
O15 K3 O20 69.07(13) 2_686 . ?
OW3 K3 O20 66.8(4) . . ?
OW2 K3 O20 88.5(3) . . ?
O3 K3 O20 81.01(11) . . ?
O1 K3 O20 110.09(12) . . ?
O17 K3 O17 86.89(13) 2_686 . ?
O2 K3 O17 55.94(11) . . ?
O15 K3 O17 62.48(12) 2_686 . ?
OW3 K3 O17 121.4(4) . . ?
OW2 K3 O17 142.7(3) . . ?
O3 K3 O17 109.48(11) . . ?
O1 K3 O17 80.16(11) . . ?
O20 K3 O17 69.53(12) . . ?
O17 K3 O15 61.54(12) 2_686 . ?
O2 K3 O15 78.71(11) . . ?
O15 K3 O15 93.35(12) 2_686 . ?
OW3 K3 O15 155.2(3) . . ?
OW2 K3 O15 146.3(3) . . ?
O3 K3 O15 104.16(11) . . ?
O1 K3 O15 52.07(11) . . ?
O20 K3 O15 121.03(13) . . ?
O17 K3 O15 53.14(11) . . ?
O17 K3 O23 140.99(13) 2_686 . ?
O2 K3 O23 81.08(11) . . ?
O15 K3 O23 106.33(13) 2_686 . ?
OW3 K3 O23 49.5(3) . . ?
OW2 K3 O23 54.1(3) . . ?
O3 K3 O23 51.76(10) . . ?
O1 K3 O23 103.99(11) . . ?
O20 K3 O23 56.10(12) . . ?
O17 K3 O23 123.62(12) . . ?
O15 K3 O23 155.23(11) . . ?
O17 K3 As1 135.87(11) 2_686 . ?
O2 K3 As1 31.17(8) . . ?
O15 K3 As1 138.44(11) 2_686 . ?
OW3 K3 As1 127.2(3) . . ?
OW2 K3 As1 126.9(3) . . ?
O3 K3 As1 31.32(7) . . ?
O1 K3 As1 31.37(8) . . ?
O20 K3 As1 81.20(9) . . ?
O17 K3 As1 80.52(8) . . ?
O15 K3 As1 77.40(8) . . ?
O23 K3 As1 77.89(8) . . ?
As1 O1 Mo2 127.2(2) . . ?
As1 O1 Mo1 125.6(2) . . ?
Mo2 O1 Mo1 96.79(15) . . ?
As1 O1 K3 86.49(15) . . ?
Mo2 O1 K3 105.53(15) . . ?
Mo1 O1 K3 113.55(15) . . ?
As1 O2 Mo3 127.19(19) . . ?
As1 O2 Mo4 126.2(2) . . ?
Mo3 O2 Mo4 95.84(15) . . ?
As1 O2 K3 94.64(16) . . ?
Mo3 O2 K3 105.81(15) . . ?
Mo4 O2 K3 103.64(14) . . ?
As1 O3 Mo6 123.1(2) . . ?
As1 O3 Mo5 127.9(2) . . ?
Mo6 O3 Mo5 95.08(14) . . ?
As1 O3 K3 86.98(14) . . ?
Mo6 O3 K3 118.09(15) . . ?
Mo5 O3 K3 106.09(14) . . ?
Mo2 O4 Mo1 115.4(2) . . ?
Mo2 O4 K2 97.87(16) . 2_686 ?
Mo1 O4 K2 95.52(16) . 2_686 ?
Mo3 O5 Mo2 138.8(2) . . ?
Mo3 O5 K1 91.44(15) . 2_676 ?
Mo2 O5 K1 123.93(19) . 2_676 ?
Mo3 O6 Mo4 114.64(19) . . ?
Mo3 O6 K2 101.08(16) . . ?
Mo4 O6 K2 100.00(16) . . ?
Mo4 O7 Mo5 141.2(2) . . ?
Mo5 O8 Mo6 116.0(2) . . ?
Mo6 O9 Mo1 138.7(2) . . ?
Mo1 O10 K2 112.1(2) . 1_655 ?
Mo1 O11 K2 110.0(2) . 2_686 ?
C1 O12 Mo1 130.8(4) . . ?
C1 O13 Mo2 130.0(4) . . ?
Mo2 O14 Co1 156.8(3) . 2_676 ?
Mo2 O14 K1 132.9(2) . . ?
Co1 O14 K1 44.56(12) 2_676 . ?
Mo2 O15 K3 144.6(2) . 2_686 ?
Mo2 O15 K2 109.3(2) . 2_686 ?
K3 O15 K2 103.84(14) 2_686 2_686 ?
Mo2 O15 K3 105.51(18) . . ?
K3 O15 K3 86.65(12) 2_686 . ?
K2 O15 K3 89.52(12) 2_686 . ?
Mo3 O16 Co1 148.8(3) . . ?
Mo3 O16 K1 103.23(19) . 2_676 ?
Co1 O16 K1 45.78(12) . 2_676 ?
Mo3 O17 K3 145.8(2) . 2_686 ?
Mo3 O17 K2 104.70(18) . . ?
K3 O17 K2 102.88(14) 2_686 . ?
Mo3 O17 K3 104.25(18) . . ?
K3 O17 K3 93.11(13) 2_686 . ?
K2 O17 K3 94.69(12) . . ?
C8 O18 Mo3 128.1(4) . . ?
C8 O18 K1 149.1(4) . 2_676 ?
Mo3 O18 K1 82.82(14) . 2_676 ?
C8 O19 Mo4 131.0(4) . . ?
Mo4 O20 K2 104.22(19) . . ?
Mo4 O20 K3 106.58(19) . . ?
K2 O20 K3 97.21(13) . . ?
Mo5 O23 K3 106.25(18) . . ?
C15 O24 Mo5 130.1(4) . . ?
C15 O25 Mo6 129.6(4) . . ?
C5 N1 H1A 120.0 . . ?
C5 N1 H1B 120.0 . . ?
H1A N1 H1B 120.0 . . ?
C12 N2 H2A 120.0 . . ?
C12 N2 H2B 120.0 . . ?
H2A N2 H2B 120.0 . . ?
C19 N3 H3B 120.0 . . ?
C19 N3 H3C 120.0 . . ?
H3B N3 H3C 120.0 . . ?
O12 C1 O13 124.2(6) . . ?
O12 C1 C2 118.4(6) . . ?
O13 C1 C2 117.4(5) . . ?
C3 C2 C7 117.6(6) . . ?
C3 C2 C1 120.3(6) . . ?
C7 C2 C1 122.0(6) . . ?
C4 C3 C2 120.9(7) . . ?
C4 C3 H3A 119.6 . . ?
C2 C3 H3A 119.6 . . ?
C3 C4 C5 121.1(7) . . ?
C3 C4 H4A 119.4 . . ?
C5 C4 H4A 119.4 . . ?
C4 C5 C6 118.1(7) . . ?
C4 C5 N1 120.8(7) . . ?
C6 C5 N1 121.1(7) . . ?
C7 C6 C5 120.2(7) . . ?
C7 C6 H6A 119.9 . . ?
C5 C6 H6A 119.9 . . ?
C6 C7 C2 122.0(7) . . ?
C6 C7 H7A 119.0 . . ?
C2 C7 H7A 119.0 . . ?
O18 C8 O19 126.2(6) . . ?
O18 C8 C9 118.1(6) . . ?
O19 C8 C9 115.7(6) . . ?
C10 C9 C14 119.3(6) . . ?
C10 C9 C8 119.7(6) . . ?
C14 C9 C8 121.0(6) . . ?
C9 C10 C11 121.2(7) . . ?
C9 C10 H10A 119.4 . . ?
C11 C10 H10A 119.4 . . ?
C12 C11 C10 118.3(7) . . ?
C12 C11 H11A 120.9 . . ?
C10 C11 H11A 120.9 . . ?
C11 C12 C13 121.7(7) . . ?
C11 C12 N2 118.9(6) . . ?
C13 C12 N2 119.4(6) . . ?
C12 C13 C14 119.2(7) . . ?
C12 C13 H13A 120.4 . . ?
C14 C13 H13A 120.4 . . ?
C9 C14 C13 120.3(7) . . ?
C9 C14 H14A 119.9 . . ?
C13 C14 H14A 119.9 . . ?
O24 C15 O25 125.7(6) . . ?
O24 C15 C16 117.3(5) . . ?
O25 C15 C16 117.1(5) . . ?
C17 C16 C21 119.9(6) . . ?
C17 C16 C15 121.5(6) . . ?
C21 C16 C15 118.6(6) . . ?
C16 C17 C18 120.3(7) . . ?
C16 C17 H17A 119.9 . . ?
C18 C17 H17A 119.9 . . ?
C19 C18 C17 118.3(7) . . ?
C19 C18 H18A 120.8 . . ?
C17 C18 H18A 120.8 . . ?
C18 C19 C20 122.5(6) . . ?
C18 C19 N3 119.2(7) . . ?
C20 C19 N3 118.2(7) . . ?
C19 C20 C21 119.0(7) . . ?
C19 C20 H20A 120.5 . . ?
C21 C20 H20A 120.5 . . ?
C20 C21 C16 119.9(7) . . ?
C20 C21 H21A 120.1 . . ?
C16 C21 H21A 120.1 . . ?
O1WA O1W Co1 72.4(16) . . ?
O1W O1WA Co1 87.4(16) . . ?
Co1 O2W K1 104.6(3) . . ?
Co1 O2W K1 36.68(17) . 2_676 ?
K1 O2W K1 68.5(2) . 2_676 ?
Co1 O3W K1 45.84(19) . 2_676 ?
OW3 OW2 K1 77.0(10) . 2_686 ?
OW3 OW2 K3 75.6(10) . . ?
K1 OW2 K3 136.9(5) 2_686 . ?
OW2 OW3 K1 77.8(10) . 2_686 ?
OW2 OW3 K3 81.0(11) . . ?
K1 OW3 K3 140.5(7) 2_686 . ?
Co1 K1 OW3 105.9(4) 2_676 2_686 ?
Co1 K1 OW2 129.6(3) 2_676 2_686 ?
OW3 K1 OW2 25.2(4) 2_686 2_686 ?
Co1 K1 O2W 149.6(3) 2_676 . ?
OW3 K1 O2W 81.7(5) 2_686 . ?
OW2 K1 O2W 57.1(3) 2_686 . ?
Co1 K1 O3W 49.87(19) 2_676 2_676 ?
OW3 K1 O3W 78.6(5) 2_686 2_676 ?
OW2 K1 O3W 101.8(4) 2_686 2_676 ?
O2W K1 O3W 156.9(3) . 2_676 ?
Co1 K1 O16 47.87(12) 2_676 2_676 ?
OW3 K1 O16 145.6(5) 2_686 2_676 ?
OW2 K1 O16 167.7(4) 2_686 2_676 ?
O2W K1 O16 132.5(2) . 2_676 ?
O3W K1 O16 67.2(2) 2_676 2_676 ?
Co1 K1 O14 45.21(12) 2_676 . ?
OW3 K1 O14 68.4(4) 2_686 . ?
OW2 K1 O14 87.2(3) 2_686 . ?
O2W K1 O14 117.6(2) . . ?
O3W K1 O14 65.4(2) 2_676 . ?
O16 K1 O14 92.74(16) 2_676 . ?
Co1 K1 O5 103.83(15) 2_676 2_676 ?
OW3 K1 O5 148.0(4) 2_686 2_676 ?
OW2 K1 O5 126.6(3) 2_686 2_676 ?
O2W K1 O5 78.6(2) . 2_676 ?
O3W K1 O5 113.1(2) 2_676 2_676 ?
O16 K1 O5 57.45(13) 2_676 2_676 ?
O14 K1 O5 143.52(18) . 2_676 ?
Co1 K1 O18 91.69(15) 2_676 2_676 ?
OW3 K1 O18 112.8(4) 2_686 2_676 ?
OW2 K1 O18 114.6(3) 2_686 2_676 ?
O2W K1 O18 112.8(2) . 2_676 ?
O3W K1 O18 65.2(2) 2_676 2_676 ?
O16 K1 O18 56.56(13) 2_676 2_676 ?
O14 K1 O18 128.95(18) . 2_676 ?
O5 K1 O18 54.48(12) 2_676 2_676 ?
Co1 K1 O2W 39.31(17) 2_676 2_676 ?
OW3 K1 O2W 121.7(3) 2_686 2_676 ?
OW2 K1 O2W 131.8(3) 2_686 2_676 ?
O2W K1 O2W 111.5(2) . 2_676 ?
O3W K1 O2W 89.2(2) 2_676 2_676 ?
O16 K1 O2W 55.95(18) 2_676 2_676 ?
O14 K1 O2W 55.00(18) . 2_676 ?
O5 K1 O2W 89.07(19) 2_676 2_676 ?
O18 K1 O2W 112.51(19) 2_676 2_676 ?
Co1 K1 K1 87.27(16) 2_676 2_676 ?
OW3 K1 K1 112.9(4) 2_686 2_676 ?
OW2 K1 K1 101.7(3) 2_686 2_676 ?
O2W K1 K1 63.1(2) . 2_676 ?
O3W K1 K1 136.6(2) 2_676 2_676 ?
O16 K1 K1 90.41(16) 2_676 2_676 ?
O14 K1 K1 79.82(15) . 2_676 ?
O5 K1 K1 79.92(15) 2_676 2_676 ?
O18 K1 K1 132.70(17) 2_676 2_676 ?
O2W K1 K1 48.44(18) 2_676 2_676 ?
Co1 K1 Mo3 75.88(10) 2_676 2_676 ?
OW3 K1 Mo3 152.7(4) 2_686 2_676 ?
OW2 K1 Mo3 150.0(3) 2_686 2_676 ?
O2W K1 Mo3 110.8(2) . 2_676 ?
O3W K1 Mo3 82.78(17) 2_676 2_676 ?
O16 K1 Mo3 28.08(9) 2_676 2_676 ?
O14 K1 Mo3 120.80(14) . 2_676 ?
O5 K1 Mo3 32.26(8) 2_676 2_676 ?
O18 K1 Mo3 40.35(9) 2_676 2_676 ?
O2W K1 Mo3 77.35(16) 2_676 2_676 ?
K1 K1 Mo3 94.36(12) 2_676 2_676 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 As1 O1 Mo2 -62.8(3) . . . . ?
O3 As1 O1 Mo2 -159.9(2) . . . . ?
K3 As1 O1 Mo2 -106.9(3) . . . . ?
O2 As1 O1 Mo1 160.7(2) . . . . ?
O3 As1 O1 Mo1 63.6(3) . . . . ?
K3 As1 O1 Mo1 116.6(3) . . . . ?
O2 As1 O1 K3 44.06(15) . . . . ?
O3 As1 O1 K3 -53.02(15) . . . . ?
O3 As1 O2 Mo3 162.0(2) . . . . ?
O1 As1 O2 Mo3 64.6(3) . . . . ?
K3 As1 O2 Mo3 113.9(3) . . . . ?
O3 As1 O2 Mo4 -62.5(3) . . . . ?
O1 As1 O2 Mo4 -159.9(2) . . . . ?
K3 As1 O2 Mo4 -110.6(3) . . . . ?
O3 As1 O2 K3 48.09(16) . . . . ?
O1 As1 O2 K3 -49.31(16) . . . . ?
O2 As1 O3 Mo6 -165.2(2) . . . . ?
O1 As1 O3 Mo6 -68.6(2) . . . . ?
K3 As1 O3 Mo6 -121.9(2) . . . . ?
O2 As1 O3 Mo5 64.8(3) . . . . ?
O1 As1 O3 Mo5 161.4(2) . . . . ?
K3 As1 O3 Mo5 108.1(3) . . . . ?
O2 As1 O3 K3 -43.27(15) . . . . ?
O1 As1 O3 K3 53.33(16) . . . . ?
O23 Mo5 O8 Mo6 -88.7(3) . . . . ?
O22 Mo5 O8 Mo6 165.6(2) . . . . ?
O7 Mo5 O8 Mo6 42.1(5) . . . . ?
O3 Mo5 O8 Mo6 -0.38(19) . . . . ?
O24 Mo5 O8 Mo6 82.2(2) . . . . ?
K3 Mo5 O8 Mo6 -37.0(2) . . . . ?
O11 Mo1 O10 K2 37.9(2) . . . 1_655 ?
O9 Mo1 O10 K2 -64.5(2) . . . 1_655 ?
O4 Mo1 O10 K2 138.13(19) . . . 1_655 ?
O1 Mo1 O10 K2 -162.4(5) . . . 1_655 ?
O12 Mo1 O10 K2 -141.4(2) . . . 1_655 ?
Mo2 Mo1 O10 K2 150.83(9) . . . 1_655 ?
K2 Mo1 O10 K2 83.72(17) 2_686 . . 1_655 ?
O10 Mo1 O11 K2 92.0(2) . . . 2_686 ?
O9 Mo1 O11 K2 -164.96(18) . . . 2_686 ?
O4 Mo1 O11 K2 -9.1(2) . . . 2_686 ?
O1 Mo1 O11 K2 -82.27(19) . . . 2_686 ?
Mo2 Mo1 O11 K2 -41.66(17) . . . 2_686 ?
K2 Mo1 O11 K2 119.36(19) 1_655 . . 2_686 ?
O15 Mo2 O14 Co1 -144.5(7) . . . 2_676 ?
O5 Mo2 O14 Co1 -43.9(7) . . . 2_676 ?
O4 Mo2 O14 Co1 115.7(7) . . . 2_676 ?
O1 Mo2 O14 Co1 53.8(11) . . . 2_676 ?
O13 Mo2 O14 Co1 33.7(7) . . . 2_676 ?
Mo1 Mo2 O14 Co1 102.1(7) . . . 2_676 ?
K2 Mo2 O14 Co1 168.4(7) 2_686 . . 2_676 ?
K3 Mo2 O14 Co1 -127.7(6) . . . 2_676 ?
K1 Mo2 O14 Co1 -72.4(7) . . . 2_676 ?
O15 Mo2 O14 K1 -72.1(3) . . . . ?
O5 Mo2 O14 K1 28.5(3) . . . . ?
O4 Mo2 O14 K1 -171.9(3) . . . . ?
O1 Mo2 O14 K1 126.2(5) . . . . ?
O13 Mo2 O14 K1 106.1(3) . . . . ?
Mo1 Mo2 O14 K1 174.48(19) . . . . ?
K2 Mo2 O14 K1 -119.3(3) 2_686 . . . ?
K3 Mo2 O14 K1 -55.3(6) . . . . ?
O14 Mo2 O15 K3 64.0(4) . . . 2_686 ?
O5 Mo2 O15 K3 -37.4(4) . . . 2_686 ?
O4 Mo2 O15 K3 163.4(4) . . . 2_686 ?
O1 Mo2 O15 K3 -121.7(4) . . . 2_686 ?
Mo1 Mo2 O15 K3 -163.9(4) . . . 2_686 ?
K2 Mo2 O15 K3 158.4(5) 2_686 . . 2_686 ?
K3 Mo2 O15 K3 -106.6(4) . . . 2_686 ?
K1 Mo2 O15 K3 36.0(4) . . . 2_686 ?
O14 Mo2 O15 K2 -94.4(2) . . . 2_686 ?
O5 Mo2 O15 K2 164.25(18) . . . 2_686 ?
O4 Mo2 O15 K2 5.0(2) . . . 2_686 ?
O1 Mo2 O15 K2 79.92(18) . . . 2_686 ?
Mo1 Mo2 O15 K2 37.70(17) . . . 2_686 ?
K3 Mo2 O15 K2 95.0(2) . . . 2_686 ?
K1 Mo2 O15 K2 -122.39(16) . . . 2_686 ?
O14 Mo2 O15 K3 170.60(18) . . . . ?
O5 Mo2 O15 K3 69.21(18) . . . . ?
O4 Mo2 O15 K3 -90.03(17) . . . . ?
O1 Mo2 O15 K3 -15.12(17) . . . . ?
Mo1 Mo2 O15 K3 -57.34(14) . . . . ?
K2 Mo2 O15 K3 -95.0(2) 2_686 . . . ?
K1 Mo2 O15 K3 142.57(13) . . . . ?
O17 Mo3 O16 Co1 137.0(5) . . . . ?
O5 Mo3 O16 Co1 34.3(5) . . . . ?
O6 Mo3 O16 Co1 -124.4(5) . . . . ?
O2 Mo3 O16 Co1 -59.7(9) . . . . ?
O18 Mo3 O16 Co1 -44.4(5) . . . . ?
Mo4 Mo3 O16 Co1 -112.7(5) . . . . ?
K1 Mo3 O16 Co1 6.2(4) 2_676 . . . ?
K2 Mo3 O16 Co1 -173.6(5) . . . . ?
K3 Mo3 O16 Co1 130.4(4) . . . . ?
K3 Mo3 O16 Co1 119.2(5) 2_686 . . . ?
O17 Mo3 O16 K1 130.8(2) . . . 2_676 ?
O5 Mo3 O16 K1 28.1(2) . . . 2_676 ?
O6 Mo3 O16 K1 -130.60(19) . . . 2_676 ?
O2 Mo3 O16 K1 -65.9(6) . . . 2_676 ?
O18 Mo3 O16 K1 -50.58(19) . . . 2_676 ?
Mo4 Mo3 O16 K1 -118.88(15) . . . 2_676 ?
K2 Mo3 O16 K1 -179.78(15) . . . 2_676 ?
K3 Mo3 O16 K1 124.2(3) . . . 2_676 ?
K3 Mo3 O16 K1 113.03(16) 2_686 . . 2_676 ?
O16 Mo3 O17 K3 -58.2(4) . . . 2_686 ?
O5 Mo3 O17 K3 43.6(4) . . . 2_686 ?
O6 Mo3 O17 K3 -157.7(4) . . . 2_686 ?
O2 Mo3 O17 K3 126.9(4) . . . 2_686 ?
Mo4 Mo3 O17 K3 169.2(4) . . . 2_686 ?
K1 Mo3 O17 K3 -10.5(5) 2_676 . . 2_686 ?
K2 Mo3 O17 K3 -142.8(5) . . . 2_686 ?
K3 Mo3 O17 K3 118.3(5) . . . 2_686 ?
O16 Mo3 O17 K2 84.7(2) . . . . ?
O5 Mo3 O17 K2 -173.58(16) . . . . ?
O6 Mo3 O17 K2 -14.88(18) . . . . ?
O2 Mo3 O17 K2 -90.24(16) . . . . ?
Mo4 Mo3 O17 K2 -47.93(14) . . . . ?
K1 Mo3 O17 K2 132.34(12) 2_676 . . . ?
K3 Mo3 O17 K2 -98.86(18) . . . . ?
K3 Mo3 O17 K2 142.8(5) 2_686 . . . ?
O16 Mo3 O17 K3 -176.48(17) . . . . ?
O5 Mo3 O17 K3 -74.72(17) . . . . ?
O6 Mo3 O17 K3 83.98(17) . . . . ?
O2 Mo3 O17 K3 8.62(16) . . . . ?
Mo4 Mo3 O17 K3 50.93(13) . . . . ?
K1 Mo3 O17 K3 -128.80(13) 2_676 . . . ?
K2 Mo3 O17 K3 98.86(18) . . . . ?
K3 Mo3 O17 K3 -118.3(5) 2_686 . . . ?
O21 Mo4 O20 K2 -81.2(2) . . . . ?
O7 Mo4 O20 K2 177.53(16) . . . . ?
O6 Mo4 O20 K2 17.33(19) . . . . ?
O2 Mo4 O20 K2 91.76(17) . . . . ?
O19 Mo4 O20 K2 96.3(9) . . . . ?
Mo3 Mo4 O20 K2 50.00(14) . . . . ?
K3 Mo4 O20 K2 102.2(2) . . . . ?
O21 Mo4 O20 K3 176.64(19) . . . . ?
O7 Mo4 O20 K3 75.38(18) . . . . ?
O6 Mo4 O20 K3 -84.82(18) . . . . ?
O2 Mo4 O20 K3 -10.40(17) . . . . ?
O19 Mo4 O20 K3 -5.9(10) . . . . ?
Mo3 Mo4 O20 K3 -52.15(14) . . . . ?
K2 Mo4 O20 K3 -102.2(2) . . . . ?
O22 Mo5 O23 K3 -166.19(18) . . . . ?
O8 Mo5 O23 K3 92.26(18) . . . . ?
O7 Mo5 O23 K3 -65.49(19) . . . . ?
O3 Mo5 O23 K3 17.78(17) . . . . ?
Mo6 Mo5 O23 K3 59.39(15) . . . . ?
Mo1 O12 C1 O13 16.5(9) . . . . ?
Mo1 O12 C1 C2 -163.2(4) . . . . ?
Mo2 O13 C1 O12 -11.5(9) . . . . ?
Mo2 O13 C1 C2 168.3(4) . . . . ?
O12 C1 C2 C3 -11.6(9) . . . . ?
O13 C1 C2 C3 168.6(6) . . . . ?
O12 C1 C2 C7 168.1(7) . . . . ?
O13 C1 C2 C7 -11.7(10) . . . . ?
C7 C2 C3 C4 1.5(11) . . . . ?
C1 C2 C3 C4 -178.8(7) . . . . ?
C2 C3 C4 C5 -1.0(12) . . . . ?
C3 C4 C5 C6 -0.3(12) . . . . ?
C3 C4 C5 N1 -179.2(7) . . . . ?
C4 C5 C6 C7 1.1(13) . . . . ?
N1 C5 C6 C7 180.0(8) . . . . ?
C5 C6 C7 C2 -0.6(14) . . . . ?
C3 C2 C7 C6 -0.7(12) . . . . ?
C1 C2 C7 C6 179.6(8) . . . . ?
Mo3 O18 C8 O19 6.9(9) . . . . ?
K1 O18 C8 O19 -175.0(5) 2_676 . . . ?
Mo3 O18 C8 C9 -172.7(4) . . . . ?
K1 O18 C8 C9 5.4(11) 2_676 . . . ?
Mo4 O19 C8 O18 -3.7(10) . . . . ?
Mo4 O19 C8 C9 176.0(4) . . . . ?
O18 C8 C9 C10 153.7(7) . . . . ?
O19 C8 C9 C10 -26.0(10) . . . . ?
O18 C8 C9 C14 -28.1(10) . . . . ?
O19 C8 C9 C14 152.2(7) . . . . ?
C14 C9 C10 C11 -2.6(13) . . . . ?
C8 C9 C10 C11 175.6(8) . . . . ?
C9 C10 C11 C12 -0.6(14) . . . . ?
C10 C11 C12 C13 3.0(14) . . . . ?
C10 C11 C12 N2 -179.1(8) . . . . ?
C11 C12 C13 C14 -1.9(14) . . . . ?
N2 C12 C13 C14 -179.9(7) . . . . ?
C10 C9 C14 C13 3.7(13) . . . . ?
C8 C9 C14 C13 -174.6(8) . . . . ?
C12 C13 C14 C9 -1.4(14) . . . . ?
Mo5 O24 C15 O25 2.5(9) . . . . ?
Mo5 O24 C15 C16 -177.8(4) . . . . ?
Mo6 O25 C15 O24 3.6(9) . . . . ?
Mo6 O25 C15 C16 -176.1(4) . . . . ?
O24 C15 C16 C17 144.8(6) . . . . ?
O25 C15 C16 C17 -35.4(9) . . . . ?
O24 C15 C16 C21 -36.4(9) . . . . ?
O25 C15 C16 C21 143.3(6) . . . . ?
C21 C16 C17 C18 -2.9(10) . . . . ?
C15 C16 C17 C18 175.8(6) . . . . ?
C16 C17 C18 C19 -0.5(11) . . . . ?
C17 C18 C19 C20 2.4(11) . . . . ?
C17 C18 C19 N3 -174.3(6) . . . . ?
C18 C19 C20 C21 -0.9(11) . . . . ?
N3 C19 C20 C21 175.9(6) . . . . ?
C19 C20 C21 C16 -2.5(11) . . . . ?
C17 C16 C21 C20 4.4(10) . . . . ?
C15 C16 C21 C20 -174.3(6) . . . . ?
K3 OW2 OW3 K1 -146.5(4) . . . 2_686 ?
K1 OW2 OW3 K3 146.5(4) 2_686 . . . ?

_refine_diff_density_max         2.174
_refine_diff_density_min         -0.813
_refine_diff_density_rms         0.139

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2
_database_code_depnum_ccdc_archive 'CCDC 1871472'
_audit_update_record             
;
2018-10-04 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H83 As2 K5 Mo12 N6 Ni O75'
_chemical_formula_weight         3427.45

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.6585(5)
_cell_length_b                   12.1103(5)
_cell_length_c                   17.7420(7)
_cell_angle_alpha                76.859(2)
_cell_angle_beta                 89.702(3)
_cell_angle_gamma                84.663(3)
_cell_volume                     2428.46(17)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    28043
_cell_measurement_theta_min      1.734
_cell_measurement_theta_max      27.510

_exptl_crystal_description       block
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.344
_exptl_crystal_F_000             1669
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.19
_exptl_absorpt_coefficient_mu    2.691
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.515
_exptl_absorpt_correction_T_max  0.600
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean 0.01
_diffrn_reflns_number            28043
_diffrn_reflns_av_unetI/netI     0.0549
_diffrn_reflns_av_R_equivalents  0.0387
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         1.734
_diffrn_reflns_theta_max         27.510
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             11141
_reflns_number_gt                8566
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0603P)²+1.4463P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         11141
_refine_ls_number_parameters     685
_refine_ls_number_restraints     30
_refine_ls_R_factor_all          0.0584
_refine_ls_R_factor_gt           0.0414
_refine_ls_wR_factor_ref         0.1152
_refine_ls_wR_factor_gt          0.1065
_refine_ls_goodness_of_fit_ref   1.028
_refine_ls_restrained_S_all      1.033
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.11804(4) 0.06660(4) 0.23092(3) 0.02131(11) Uani 1 1 d . . . . .
Mo2 Mo 0.37076(4) 0.03495(4) 0.15430(3) 0.02097(11) Uani 1 1 d . . . . .
Mo3 Mo 0.61174(4) 0.14085(4) 0.23362(3) 0.01997(11) Uani 1 1 d . . . . .
Mo4 Mo 0.30460(4) 0.26744(4) 0.47222(3) 0.02136(11) Uani 1 1 d . . . . .
Mo5 Mo 0.08307(4) 0.17246(4) 0.40208(3) 0.02140(11) Uani 1 1 d . . . . .
Mo6 Mo 0.58014(4) 0.25500(3) 0.38312(3) 0.01982(11) Uani 1 1 d . . . . .
As1 As 0.32542(4) 0.23227(4) 0.27954(3) 0.01744(12) Uani 1 1 d . . . . .
Ni1 Ni 0.69228(12) 0.49650(11) 0.43452(8) 0.0223(3) Uani 0.5 1 d . . P . .
K1 K 0.80612(13) 0.00336(12) 0.40450(8) 0.0411(3) Uani 1 1 d . . . . .
K2 K 0.57881(16) 0.02772(12) 0.60334(9) 0.0554(4) Uani 1 1 d . . . . .
K3 K 0.4723(4) 0.4576(3) 0.6016(2) 0.0429(9) Uani 0.5 1 d . . P . .
O1 O 0.5443(3) 0.4117(3) 0.2797(2) 0.0301(9) Uani 1 1 d . . . . .
O2 O 0.1312(3) 0.2408(3) 0.1429(2) 0.0265(8) Uani 1 1 d . . . . .
O3 O 0.4063(3) 0.0096(3) 0.0651(2) 0.0326(9) Uani 1 1 d . . . . .
O4 O 0.2943(3) 0.1051(3) 0.2511(2) 0.0215(8) Uani 1 1 d . . . . .
O5 O 0.3689(3) 0.1419(3) 0.5261(2) 0.0331(9) Uani 1 1 d . . . . .
O6 O 0.3003(3) 0.3578(4) 0.5345(2) 0.0363(10) Uani 1 1 d . . . . .
O7 O -0.0611(3) 0.1956(3) 0.4205(2) 0.0339(9) Uani 1 1 d . . . . .
O8 O -0.0113(3) 0.0683(3) 0.1854(2) 0.0348(10) Uani 1 1 d . . . . .
O9 O 0.7231(3) 0.1501(4) 0.1705(2) 0.0359(10) Uani 1 1 d . . . . .
O10 O 0.1149(4) 0.0302(3) 0.4418(2) 0.0336(9) Uani 1 1 d . . . . .
O11 O 0.6844(3) 0.2069(3) 0.3095(2) 0.0244(8) Uani 1 1 d . . . . .
O12 O 0.4920(3) 0.1288(3) 0.1641(2) 0.0227(8) Uani 1 1 d . . . . .
O13 O 0.5969(3) 0.1303(3) 0.4519(2) 0.0293(9) Uani 1 1 d . . . . .
O14 O 0.4721(3) 0.1847(3) 0.3090(2) 0.0200(7) Uani 1 1 d . . . . .
O15 O 0.4350(3) 0.3174(3) 0.4128(2) 0.0234(8) Uani 1 1 d . . . . .
O16 O 0.2120(3) 0.0130(3) 0.1533(2) 0.0272(8) Uani 1 1 d . . . . .
O17 O 0.6683(3) 0.3428(3) 0.4156(2) 0.0293(9) Uani 1 1 d . . . . .
O18 O 0.0660(3) 0.3633(3) 0.3429(2) 0.0286(9) Uani 1 1 d . . . . .
O19 O 0.1262(4) -0.0583(3) 0.2997(2) 0.0346(10) Uani 1 1 d . . . . .
O20 O 0.5601(3) 0.3280(3) 0.1791(2) 0.0294(9) Uani 1 1 d . . . . .
O21 O 0.2213(3) 0.4262(3) 0.3854(2) 0.0290(9) Uani 1 1 d . . . . .
O22 O 0.0751(3) 0.1691(3) 0.2955(2) 0.0248(8) Uani 1 1 d . . . . .
O23 O 0.3004(3) 0.2115(3) 0.0860(2) 0.0297(9) Uani 1 1 d . . . . .
O24 O 0.1468(3) 0.2297(3) 0.4857(2) 0.0267(8) Uani 1 1 d . . . . .
O25 O 0.4241(4) -0.0877(3) 0.2176(2) 0.0337(9) Uani 1 1 d . . . . .
O26 O 0.2667(3) 0.1968(3) 0.3749(2) 0.0207(7) Uani 1 1 d . . . . .
O27 O 0.6271(3) 0.0025(3) 0.2866(2) 0.0313(9) Uani 1 1 d . . . . .
C1 C 0.5176(6) 0.6274(5) 0.1685(4) 0.0412(16) Uani 1 1 d . . . . .
H1A H 0.5508 0.6300 0.2155 0.049 Uiso 1 1 calc R U . . .
C2 C 0.1144(5) 0.5458(4) 0.2798(3) 0.0263(12) Uani 1 1 d . . . . .
C3 C 0.4877(6) 0.7277(5) 0.1133(4) 0.0449(17) Uani 1 1 d . . . . .
H3A H 0.5014 0.7975 0.1233 0.054 Uiso 1 1 calc R U . . .
C4 C 0.1790(6) 0.7234(5) 0.2079(4) 0.0484(18) Uani 1 1 d . . . . .
H4A H 0.2364 0.7729 0.1971 0.058 Uiso 1 1 calc R U . . .
C5 C 0.1986(6) 0.6223(5) 0.2634(4) 0.0440(17) Uani 1 1 d . . . . .
H5A H 0.2688 0.6052 0.2900 0.053 Uiso 1 1 calc R U . . .
C6 C -0.0086(6) 0.6740(5) 0.1841(4) 0.0428(16) Uani 1 1 d . . . . .
H6A H -0.0788 0.6906 0.1573 0.051 Uiso 1 1 calc R U . . .
C7 C 0.4139(6) 0.6235(5) 0.0302(4) 0.0481(18) Uani 1 1 d . . . . .
H7A H 0.3767 0.6225 -0.0159 0.058 Uiso 1 1 calc R U . . .
C8 C 0.4445(6) 0.5212(5) 0.0844(4) 0.0455(17) Uani 1 1 d . . . . .
H8A H 0.4289 0.4521 0.0741 0.055 Uiso 1 1 calc R U . . .
C9 C 0.0743(6) 0.7510(5) 0.1683(4) 0.0377(15) Uani 1 1 d . . . . .
C10 C 0.0117(5) 0.5732(5) 0.2388(4) 0.0396(16) Uani 1 1 d . . . . .
H10A H -0.0450 0.5228 0.2483 0.048 Uiso 1 1 calc R U . . .
C11 C 0.1980(5) 0.5035(5) -0.0878(4) 0.0368(15) Uani 1 1 d . . . . .
H11A H 0.2202 0.5127 -0.1391 0.044 Uiso 1 1 calc R U . . .
C12 C 0.2251(5) 0.4001(5) -0.0347(3) 0.0361(15) Uani 1 1 d . . . . .
H12A H 0.2677 0.3406 -0.0503 0.043 Uiso 1 1 calc R U . . .
C13 C 0.4386(5) 0.7238(4) 0.0450(3) 0.0292(13) Uani 1 1 d . . . . .
C14 C 0.1380(5) 0.5913(5) -0.0630(4) 0.0364(15) Uani 1 1 d . . . . .
C15 C 0.2092(4) 0.2708(4) 0.0943(3) 0.0232(11) Uani 1 1 d . . . . .
C16 C 0.1071(5) 0.5805(5) 0.0135(4) 0.0393(16) Uani 1 1 d . . . . .
H16A H 0.0697 0.6417 0.0302 0.047 Uiso 1 1 calc R U . . .
C17 C 0.1332(5) 0.4768(5) 0.0646(3) 0.0332(13) Uani 1 1 d . . . . .
H17A H 0.1126 0.4684 0.1162 0.040 Uiso 1 1 calc R U . . .
C18 C 0.1889(4) 0.3860(4) 0.0410(3) 0.0261(12) Uani 1 1 d . . . . .
C19 C 0.4976(5) 0.5236(4) 0.1530(3) 0.0282(12) Uani 1 1 d . . . . .
C20 C 0.5373(4) 0.4126(4) 0.2083(3) 0.0249(12) Uani 1 1 d . . . . .
C21 C 0.1350(5) 0.4380(4) 0.3404(3) 0.0255(12) Uani 1 1 d . . . . .
N1 N 0.1057(4) 0.6979(4) -0.1195(4) 0.0501(17) Uani 1 1 d . . . . .
H1B H 0.1244 0.7046 -0.1672 0.060 Uiso 1 1 calc R U . . .
H1C H 0.0681 0.7539 -0.1051 0.060 Uiso 1 1 calc R U . . .
N2 N 0.0545(5) 0.8530(4) 0.1118(3) 0.0464(14) Uani 1 1 d . . . . .
H2A H 0.1076 0.8987 0.1015 0.056 Uiso 1 1 calc R U . . .
H2B H -0.0106 0.8696 0.0875 0.056 Uiso 1 1 calc R U . . .
N3 N 0.4087(4) 0.8291(4) -0.0133(3) 0.0365(12) Uani 1 1 d . . . . .
H3B H 0.3759 0.8268 -0.0561 0.044 Uiso 1 1 calc R U . . .
H3C H 0.4238 0.8934 -0.0047 0.044 Uiso 1 1 calc R U . . .
O1W O 0.8680(5) 0.4566(6) 0.4339(4) 0.0153(15) Uani 0.5 1 d . U P . .
O1WA O 0.8494(7) 0.4326(7) 0.4731(6) 0.035(2) Uani 0.5 1 d . U P . .
O2W O 0.7154(7) 0.5697(5) 0.3163(4) 0.0247(16) Uani 0.5 1 d . U P . .
O3W O 0.6924(7) 0.4193(6) 0.5507(4) 0.0288(17) Uani 0.5 1 d . . P . .
O4W O 0.5106(10) 0.5276(10) 0.4367(7) 0.038(3) Uani 0.5 1 d . . P . .
OW1 O 0.5039(14) 0.7681(9) 0.3487(7) 0.086(4) Uani 0.5 1 d . . P . .
OW2 O 0.4098(10) 0.7451(9) 0.3671(7) 0.062(3) Uani 0.5 1 d . . P . .
OW3 O 0.7091(7) 0.8061(6) 0.2284(5) 0.110(3) Uani 1 1 d . U . . .
OW4 O 0.7791(7) 0.9002(6) 0.0677(5) 0.121(3) Uani 1 1 d . U . . .
OW5 O 0.9730(5) -0.3553(6) 0.4254(4) 0.089(2) Uani 1 1 d . . . . .
OW6 O 0.7991(5) 0.2120(4) 0.5649(3) 0.0745(18) Uani 1 1 d . . . . .
OW7 O 0.8320(4) 0.1397(5) 0.0290(3) 0.0624(15) Uani 1 1 d . . . . .
OW8 O 0.8481(4) 0.3533(5) 0.2643(3) 0.0690(18) Uani 1 1 d . . . . .
OW9 O 0.8944(6) -0.1363(6) 0.3085(4) 0.094(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O19 1.709(4) . ?
Mo1 O8 1.710(4) . ?
Mo1 O22 1.905(4) . ?
Mo1 O16 1.942(4) . ?
Mo1 O4 2.197(3) . ?
Mo1 O2 2.339(3) . ?
Mo1 Mo2 3.2651(6) . ?
Mo2 O25 1.712(4) . ?
Mo2 O3 1.721(4) . ?
Mo2 O16 1.895(4) . ?
Mo2 O12 1.926(3) . ?
Mo2 O4 2.230(3) . ?
Mo2 O23 2.284(3) . ?
Mo3 O9 1.705(4) . ?
Mo3 O27 1.718(4) . ?
Mo3 O12 1.905(4) . ?
Mo3 O11 1.949(4) . ?
Mo3 O14 2.205(3) . ?
Mo3 O20 2.279(4) . ?
Mo3 Mo6 3.2626(7) . ?
Mo4 O5 1.710(4) . ?
Mo4 O6 1.721(4) . ?
Mo4 O15 1.912(3) . ?
Mo4 O24 1.938(4) . ?
Mo4 O26 2.159(4) . ?
Mo4 O21 2.310(4) . ?
Mo4 Mo5 3.2832(6) . ?
Mo5 O10 1.713(4) . ?
Mo5 O7 1.720(4) . ?
Mo5 O22 1.903(4) . ?
Mo5 O24 1.952(4) . ?
Mo5 O26 2.224(3) . ?
Mo5 O18 2.301(3) . ?
Mo6 O13 1.709(4) . ?
Mo6 O17 1.733(4) . ?
Mo6 O15 1.909(3) . ?
Mo6 O11 1.928(4) . ?
Mo6 O14 2.184(3) . ?
Mo6 O1 2.329(4) . ?
As1 O14 1.794(3) . ?
As1 O4 1.794(3) . ?
As1 O26 1.796(3) . ?
Ni1 O6 1.973(4) 2_666 ?
Ni1 O1WA 1.982(9) . ?
Ni1 O17 2.010(4) . ?
Ni1 K3 2.013(5) 2_666 ?
Ni1 O3W 2.061(7) . ?
Ni1 O1W 2.061(7) . ?
Ni1 O2W 2.110(7) . ?
Ni1 O4W 2.118(11) . ?
K3 O4W 0.696(9) 2_666 ?
K3 Ni1 2.013(5) 2_666 ?
O1 C20 1.268(7) . ?
O2 C15 1.271(6) . ?
O6 Ni1 1.973(4) 2_666 ?
O18 C21 1.259(6) . ?
O20 C20 1.256(6) . ?
O21 C21 1.265(6) . ?
O23 C15 1.254(6) . ?
C1 C19 1.386(8) . ?
C1 C3 1.394(8) . ?
C1 H1A 0.9300 . ?
C2 C10 1.377(8) . ?
C2 C5 1.397(8) . ?
C2 C21 1.490(7) . ?
C3 C13 1.354(9) . ?
C3 H3A 0.9300 . ?
C4 C5 1.387(8) . ?
C4 C9 1.385(9) . ?
C4 H4A 0.9300 . ?
C5 H5A 0.9300 . ?
C6 C10 1.378(8) . ?
C6 C9 1.389(8) . ?
C6 H6A 0.9300 . ?
C7 C13 1.356(8) . ?
C7 C8 1.402(8) . ?
C7 H7A 0.9300 . ?
C8 C19 1.375(9) . ?
C8 H8A 0.9300 . ?
C9 N2 1.403(7) . ?
C10 H10A 0.9300 . ?
C11 C14 1.373(9) . ?
C11 C12 1.395(8) . ?
C11 H11A 0.9300 . ?
C12 C18 1.383(8) . ?
C12 H12A 0.9300 . ?
C13 N3 1.463(7) . ?
C14 C16 1.383(9) . ?
C14 N1 1.463(7) . ?
C15 C18 1.496(7) . ?
C16 C17 1.380(8) . ?
C16 H16A 0.9300 . ?
C17 C18 1.372(8) . ?
C17 H17A 0.9300 . ?
C19 C20 1.507(7) . ?
N1 H1B 0.8600 . ?
N1 H1C 0.8600 . ?
N2 H2A 0.8600 . ?
N2 H2B 0.8600 . ?
N3 H3B 0.8600 . ?
N3 H3C 0.8600 . ?
O1W O1WA 0.730(9) . ?
O4W K3 0.696(9) 2_666 ?
OW1 OW2 1.183(16) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O19 Mo1 O8 103.32(19) . . ?
O19 Mo1 O22 98.82(18) . . ?
O8 Mo1 O22 99.70(18) . . ?
O19 Mo1 O16 97.85(17) . . ?
O8 Mo1 O16 95.90(18) . . ?
O22 Mo1 O16 153.84(14) . . ?
O19 Mo1 O4 95.19(17) . . ?
O8 Mo1 O4 160.11(16) . . ?
O22 Mo1 O4 84.38(14) . . ?
O16 Mo1 O4 74.14(14) . . ?
O19 Mo1 O2 172.34(17) . . ?
O8 Mo1 O2 84.34(16) . . ?
O22 Mo1 O2 79.82(14) . . ?
O16 Mo1 O2 80.97(14) . . ?
O4 Mo1 O2 77.19(13) . . ?
O19 Mo1 Mo2 98.63(14) . . ?
O8 Mo1 Mo2 125.36(14) . . ?
O22 Mo1 Mo2 125.50(10) . . ?
O16 Mo1 Mo2 31.27(11) . . ?
O4 Mo1 Mo2 42.87(9) . . ?
O2 Mo1 Mo2 76.40(9) . . ?
O25 Mo2 O3 103.45(19) . . ?
O25 Mo2 O16 100.82(17) . . ?
O3 Mo2 O16 98.90(18) . . ?
O25 Mo2 O12 98.73(17) . . ?
O3 Mo2 O12 98.11(17) . . ?
O16 Mo2 O12 150.24(15) . . ?
O25 Mo2 O4 91.17(16) . . ?
O3 Mo2 O4 164.90(16) . . ?
O16 Mo2 O4 74.23(14) . . ?
O12 Mo2 O4 83.18(13) . . ?
O25 Mo2 O23 171.03(17) . . ?
O3 Mo2 O23 84.95(17) . . ?
O16 Mo2 O23 80.70(14) . . ?
O12 Mo2 O23 76.68(14) . . ?
O4 Mo2 O23 80.70(13) . . ?
O25 Mo2 Mo1 98.43(14) . . ?
O3 Mo2 Mo1 129.82(14) . . ?
O16 Mo2 Mo1 32.14(11) . . ?
O12 Mo2 Mo1 122.51(10) . . ?
O4 Mo2 Mo1 42.09(9) . . ?
O23 Mo2 Mo1 78.08(9) . . ?
O9 Mo3 O27 104.88(19) . . ?
O9 Mo3 O12 98.39(18) . . ?
O27 Mo3 O12 99.12(17) . . ?
O9 Mo3 O11 96.55(18) . . ?
O27 Mo3 O11 96.47(17) . . ?
O12 Mo3 O11 154.81(15) . . ?
O9 Mo3 O14 162.62(16) . . ?
O27 Mo3 O14 90.98(16) . . ?
O12 Mo3 O14 85.81(14) . . ?
O11 Mo3 O14 74.23(13) . . ?
O9 Mo3 O20 86.77(17) . . ?
O27 Mo3 O20 168.35(16) . . ?
O12 Mo3 O20 79.07(14) . . ?
O11 Mo3 O20 81.66(14) . . ?
O14 Mo3 O20 77.43(13) . . ?
O9 Mo3 Mo6 127.62(14) . . ?
O27 Mo3 Mo6 95.35(14) . . ?
O12 Mo3 Mo6 125.70(10) . . ?
O11 Mo3 Mo6 32.51(10) . . ?
O14 Mo3 Mo6 41.72(9) . . ?
O20 Mo3 Mo6 76.86(10) . . ?
O5 Mo4 O6 103.8(2) . . ?
O5 Mo4 O15 98.13(17) . . ?
O6 Mo4 O15 99.28(17) . . ?
O5 Mo4 O24 97.24(17) . . ?
O6 Mo4 O24 96.78(17) . . ?
O15 Mo4 O24 154.40(16) . . ?
O5 Mo4 O26 94.32(17) . . ?
O6 Mo4 O26 160.93(17) . . ?
O15 Mo4 O26 83.83(14) . . ?
O24 Mo4 O26 74.70(14) . . ?
O5 Mo4 O21 172.36(17) . . ?
O6 Mo4 O21 83.70(17) . . ?
O15 Mo4 O21 78.92(14) . . ?
O24 Mo4 O21 83.20(15) . . ?
O26 Mo4 O21 78.41(13) . . ?
O5 Mo4 Mo5 99.54(14) . . ?
O6 Mo4 Mo5 126.67(14) . . ?
O15 Mo4 Mo5 124.00(11) . . ?
O24 Mo4 Mo5 32.55(11) . . ?
O26 Mo4 Mo5 42.26(9) . . ?
O21 Mo4 Mo5 76.71(9) . . ?
O10 Mo5 O7 103.46(19) . . ?
O10 Mo5 O22 99.77(17) . . ?
O7 Mo5 O22 100.14(18) . . ?
O10 Mo5 O24 97.43(18) . . ?
O7 Mo5 O24 98.98(18) . . ?
O22 Mo5 O24 150.45(14) . . ?
O10 Mo5 O26 92.17(16) . . ?
O7 Mo5 O26 163.34(16) . . ?
O22 Mo5 O26 82.55(14) . . ?
O24 Mo5 O26 72.93(13) . . ?
O10 Mo5 O18 172.13(16) . . ?
O7 Mo5 O18 84.38(16) . . ?
O22 Mo5 O18 78.02(15) . . ?
O24 Mo5 O18 81.67(15) . . ?
O26 Mo5 O18 80.09(12) . . ?
O10 Mo5 Mo4 98.31(14) . . ?
O7 Mo5 Mo4 129.16(14) . . ?
O22 Mo5 Mo4 120.71(10) . . ?
O24 Mo5 Mo4 32.29(10) . . ?
O26 Mo5 Mo4 40.74(9) . . ?
O18 Mo5 Mo4 76.73(9) . . ?
O13 Mo6 O17 104.12(18) . . ?
O13 Mo6 O15 99.89(17) . . ?
O17 Mo6 O15 98.77(16) . . ?
O13 Mo6 O11 96.36(16) . . ?
O17 Mo6 O11 97.77(16) . . ?
O15 Mo6 O11 153.19(16) . . ?
O13 Mo6 O14 93.05(16) . . ?
O17 Mo6 O14 162.15(15) . . ?
O15 Mo6 O14 82.81(14) . . ?
O11 Mo6 O14 75.13(14) . . ?
O13 Mo6 O1 172.39(16) . . ?
O17 Mo6 O1 83.38(16) . . ?
O15 Mo6 O1 79.97(14) . . ?
O11 Mo6 O1 81.14(15) . . ?
O14 Mo6 O1 79.37(13) . . ?
O13 Mo6 Mo3 96.47(13) . . ?
O17 Mo6 Mo3 128.85(13) . . ?
O15 Mo6 Mo3 123.27(11) . . ?
O11 Mo6 Mo3 32.90(11) . . ?
O14 Mo6 Mo3 42.22(9) . . ?
O1 Mo6 Mo3 77.51(10) . . ?
O14 As1 O4 96.16(16) . . ?
O14 As1 O26 95.87(16) . . ?
O4 As1 O26 96.69(15) . . ?
O6 Ni1 O1WA 95.2(3) 2_666 . ?
O6 Ni1 O17 171.65(18) 2_666 . ?
O1WA Ni1 O17 87.6(3) . . ?
O6 Ni1 K3 90.62(17) 2_666 2_666 ?
O1WA Ni1 K3 173.3(3) . 2_666 ?
O17 Ni1 K3 86.19(16) . 2_666 ?
O6 Ni1 O3W 87.4(2) 2_666 . ?
O1WA Ni1 O3W 68.6(4) . . ?
O17 Ni1 O3W 86.3(2) . . ?
K3 Ni1 O3W 108.3(3) 2_666 . ?
O6 Ni1 O1W 95.7(2) 2_666 . ?
O1WA Ni1 O1W 20.7(3) . . ?
O17 Ni1 O1W 89.7(2) . . ?
K3 Ni1 O1W 161.6(2) 2_666 . ?
O3W Ni1 O1W 89.3(3) . . ?
O6 Ni1 O2W 93.4(2) 2_666 . ?
O1WA Ni1 O2W 103.9(4) . . ?
O17 Ni1 O2W 93.6(2) . . ?
K3 Ni1 O2W 79.1(2) 2_666 . ?
O3W Ni1 O2W 172.6(3) . . ?
O1W Ni1 O2W 83.3(3) . . ?
O6 Ni1 O4W 87.1(3) 2_666 . ?
O1WA Ni1 O4W 157.6(4) . . ?
O17 Ni1 O4W 87.4(3) . . ?
K3 Ni1 O4W 19.2(3) 2_666 . ?
O3W Ni1 O4W 89.3(4) . . ?
O1W Ni1 O4W 176.8(4) . . ?
O2W Ni1 O4W 98.2(4) . . ?
O4W K3 Ni1 89.0(13) 2_666 2_666 ?
C20 O1 Mo6 128.0(3) . . ?
C15 O2 Mo1 129.4(3) . . ?
As1 O4 Mo1 122.88(17) . . ?
As1 O4 Mo2 127.81(17) . . ?
Mo1 O4 Mo2 95.04(14) . . ?
Mo4 O6 Ni1 156.6(3) . 2_666 ?
Mo6 O11 Mo3 114.59(17) . . ?
Mo3 O12 Mo2 141.11(18) . . ?
As1 O14 Mo6 127.11(17) . . ?
As1 O14 Mo3 125.99(18) . . ?
Mo6 O14 Mo3 96.05(13) . . ?
Mo6 O15 Mo4 139.00(19) . . ?
Mo2 O16 Mo1 116.59(18) . . ?
Mo6 O17 Ni1 149.2(2) . . ?
C21 O18 Mo5 130.7(3) . . ?
C20 O20 Mo3 131.8(3) . . ?
C21 O21 Mo4 130.7(3) . . ?
Mo5 O22 Mo1 138.6(2) . . ?
C15 O23 Mo2 130.0(3) . . ?
Mo4 O24 Mo5 115.16(17) . . ?
As1 O26 Mo4 127.09(17) . . ?
As1 O26 Mo5 125.71(18) . . ?
Mo4 O26 Mo5 97.00(13) . . ?
C19 C1 C3 119.7(6) . . ?
C19 C1 H1A 120.1 . . ?
C3 C1 H1A 120.1 . . ?
C10 C2 C5 118.1(5) . . ?
C10 C2 C21 121.1(5) . . ?
C5 C2 C21 120.8(5) . . ?
C13 C3 C1 120.0(6) . . ?
C13 C3 H3A 120.0 . . ?
C1 C3 H3A 120.0 . . ?
C5 C4 C9 120.3(6) . . ?
C5 C4 H4A 119.8 . . ?
C9 C4 H4A 119.8 . . ?
C4 C5 C2 120.9(6) . . ?
C4 C5 H5A 119.5 . . ?
C2 C5 H5A 119.5 . . ?
C10 C6 C9 120.8(6) . . ?
C10 C6 H6A 119.6 . . ?
C9 C6 H6A 119.6 . . ?
C13 C7 C8 119.9(6) . . ?
C13 C7 H7A 120.1 . . ?
C8 C7 H7A 120.1 . . ?
C19 C8 C7 119.6(6) . . ?
C19 C8 H8A 120.2 . . ?
C7 C8 H8A 120.2 . . ?
C4 C9 C6 118.5(6) . . ?
C4 C9 N2 120.4(6) . . ?
C6 C9 N2 121.0(6) . . ?
C2 C10 C6 121.3(5) . . ?
C2 C10 H10A 119.4 . . ?
C6 C10 H10A 119.4 . . ?
C14 C11 C12 118.9(6) . . ?
C14 C11 H11A 120.5 . . ?
C12 C11 H11A 120.5 . . ?
C18 C12 C11 120.2(6) . . ?
C18 C12 H12A 119.9 . . ?
C11 C12 H12A 119.9 . . ?
C7 C13 C3 121.1(5) . . ?
C7 C13 N3 118.9(6) . . ?
C3 C13 N3 120.0(5) . . ?
C11 C14 C16 121.5(5) . . ?
C11 C14 N1 118.7(6) . . ?
C16 C14 N1 119.8(6) . . ?
O23 C15 O2 125.8(5) . . ?
O23 C15 C18 117.2(4) . . ?
O2 C15 C18 117.0(5) . . ?
C17 C16 C14 118.4(6) . . ?
C17 C16 H16A 120.8 . . ?
C14 C16 H16A 120.8 . . ?
C18 C17 C16 121.4(6) . . ?
C18 C17 H17A 119.3 . . ?
C16 C17 H17A 119.3 . . ?
C17 C18 C12 119.4(5) . . ?
C17 C18 C15 121.8(5) . . ?
C12 C18 C15 118.8(5) . . ?
C8 C19 C1 119.5(5) . . ?
C8 C19 C20 119.0(5) . . ?
C1 C19 C20 121.4(5) . . ?
O20 C20 O1 125.5(5) . . ?
O20 C20 C19 116.5(5) . . ?
O1 C20 C19 118.0(5) . . ?
O18 C21 O21 123.8(5) . . ?
O18 C21 C2 117.8(5) . . ?
O21 C21 C2 118.4(5) . . ?
C14 N1 H1B 120.0 . . ?
C14 N1 H1C 120.0 . . ?
H1B N1 H1C 120.0 . . ?
C9 N2 H2A 120.0 . . ?
C9 N2 H2B 120.0 . . ?
H2A N2 H2B 120.0 . . ?
C13 N3 H3B 120.0 . . ?
C13 N3 H3C 120.0 . . ?
H3B N3 H3C 120.0 . . ?
O1WA O1W Ni1 73.6(9) . . ?
O1W O1WA Ni1 85.8(10) . . ?
K3 O4W Ni1 71.8(11) 2_666 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O14 As1 O4 Mo1 165.27(19) . . . . ?
O26 As1 O4 Mo1 68.6(2) . . . . ?
O14 As1 O4 Mo2 -65.4(2) . . . . ?
O26 As1 O4 Mo2 -162.1(2) . . . . ?
O5 Mo4 O6 Ni1 143.5(6) . . . 2_666 ?
O15 Mo4 O6 Ni1 42.7(6) . . . 2_666 ?
O24 Mo4 O6 Ni1 -117.3(6) . . . 2_666 ?
O26 Mo4 O6 Ni1 -55.3(9) . . . 2_666 ?
O21 Mo4 O6 Ni1 -35.0(6) . . . 2_666 ?
Mo5 Mo4 O6 Ni1 -103.2(6) . . . 2_666 ?
O4 As1 O14 Mo6 -161.9(2) . . . . ?
O26 As1 O14 Mo6 -64.5(2) . . . . ?
O4 As1 O14 Mo3 62.6(2) . . . . ?
O26 As1 O14 Mo3 160.0(2) . . . . ?
O25 Mo2 O16 Mo1 88.7(2) . . . . ?
O3 Mo2 O16 Mo1 -165.7(2) . . . . ?
O12 Mo2 O16 Mo1 -41.6(4) . . . . ?
O4 Mo2 O16 Mo1 0.51(17) . . . . ?
O23 Mo2 O16 Mo1 -82.4(2) . . . . ?
O13 Mo6 O17 Ni1 -136.1(4) . . . . ?
O15 Mo6 O17 Ni1 -33.6(5) . . . . ?
O11 Mo6 O17 Ni1 125.3(4) . . . . ?
O14 Mo6 O17 Ni1 60.2(8) . . . . ?
O1 Mo6 O17 Ni1 45.2(4) . . . . ?
Mo3 Mo6 O17 Ni1 113.3(4) . . . . ?
O14 As1 O26 Mo4 62.7(2) . . . . ?
O4 As1 O26 Mo4 159.7(2) . . . . ?
O14 As1 O26 Mo5 -160.2(2) . . . . ?
O4 As1 O26 Mo5 -63.3(2) . . . . ?
C19 C1 C3 C13 0.4(11) . . . . ?
C9 C4 C5 C2 0.9(11) . . . . ?
C10 C2 C5 C4 0.5(10) . . . . ?
C21 C2 C5 C4 -179.0(6) . . . . ?
C13 C7 C8 C19 1.2(11) . . . . ?
C5 C4 C9 C6 -1.8(11) . . . . ?
C5 C4 C9 N2 -179.6(7) . . . . ?
C10 C6 C9 C4 1.3(10) . . . . ?
C10 C6 C9 N2 179.1(6) . . . . ?
C5 C2 C10 C6 -1.0(10) . . . . ?
C21 C2 C10 C6 178.5(6) . . . . ?
C9 C6 C10 C2 0.2(11) . . . . ?
C14 C11 C12 C18 1.9(9) . . . . ?
C8 C7 C13 C3 -3.2(11) . . . . ?
C8 C7 C13 N3 178.4(6) . . . . ?
C1 C3 C13 C7 2.4(11) . . . . ?
C1 C3 C13 N3 -179.2(6) . . . . ?
C12 C11 C14 C16 2.0(9) . . . . ?
C12 C11 C14 N1 -177.6(5) . . . . ?
Mo2 O23 C15 O2 -3.3(9) . . . . ?
Mo2 O23 C15 C18 178.2(4) . . . . ?
Mo1 O2 C15 O23 -3.2(8) . . . . ?
Mo1 O2 C15 C18 175.2(3) . . . . ?
C11 C14 C16 C17 -3.1(9) . . . . ?
N1 C14 C16 C17 176.5(5) . . . . ?
C14 C16 C17 C18 0.3(9) . . . . ?
C16 C17 C18 C12 3.4(9) . . . . ?
C16 C17 C18 C15 -175.0(5) . . . . ?
C11 C12 C18 C17 -4.5(9) . . . . ?
C11 C12 C18 C15 173.9(5) . . . . ?
O23 C15 C18 C17 -146.0(6) . . . . ?
O2 C15 C18 C17 35.4(8) . . . . ?
O23 C15 C18 C12 35.6(8) . . . . ?
O2 C15 C18 C12 -143.0(6) . . . . ?
C7 C8 C19 C1 1.6(10) . . . . ?
C7 C8 C19 C20 -175.8(6) . . . . ?
C3 C1 C19 C8 -2.4(10) . . . . ?
C3 C1 C19 C20 175.0(6) . . . . ?
Mo3 O20 C20 O1 3.9(8) . . . . ?
Mo3 O20 C20 C19 -175.7(3) . . . . ?
Mo6 O1 C20 O20 -7.6(8) . . . . ?
Mo6 O1 C20 C19 172.0(3) . . . . ?
C8 C19 C20 O20 26.1(8) . . . . ?
C1 C19 C20 O20 -151.3(6) . . . . ?
C8 C19 C20 O1 -153.5(6) . . . . ?
C1 C19 C20 O1 29.1(8) . . . . ?
Mo5 O18 C21 O21 -15.9(8) . . . . ?
Mo5 O18 C21 C2 163.0(4) . . . . ?
Mo4 O21 C21 O18 10.5(8) . . . . ?
Mo4 O21 C21 C2 -168.4(3) . . . . ?
C10 C2 C21 O18 13.3(8) . . . . ?
C5 C2 C21 O18 -167.2(6) . . . . ?
C10 C2 C21 O21 -167.7(6) . . . . ?
C5 C2 C21 O21 11.8(8) . . . . ?

_refine_diff_density_max         2.057
_refine_diff_density_min         -1.027
_refine_diff_density_rms         0.157

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_5
_database_code_depnum_ccdc_archive 'CCDC 1871475'
_audit_update_record             
;
2018-10-08 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H86 Co Cs4 Mo12 N6 Na2 O78 Te2'
_chemical_formula_weight         3966.20

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.7267(12)
_cell_length_b                   12.4654(13)
_cell_length_c                   18.6945(19)
_cell_angle_alpha                74.384(4)
_cell_angle_beta                 85.990(4)
_cell_angle_gamma                84.238(4)
_cell_volume                     2615.9(5)
_cell_formula_units_Z            1
_cell_measurement_temperature    220(2)
_cell_measurement_reflns_used    24024
_cell_measurement_theta_min      1.702
_cell_measurement_theta_max      25.00

_exptl_crystal_description       block
_exptl_crystal_colour            red
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.518
_exptl_crystal_F_000             1880
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    3.581
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.425
_exptl_absorpt_correction_T_max  0.471
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            24024
_diffrn_reflns_av_unetI/netI     0.0395
_diffrn_reflns_av_R_equivalents  0.0325
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         1.702
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.969
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.969
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.969
_reflns_number_total             9176
_reflns_number_gt                8301
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0430P)²+21.9842P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         9176
_refine_ls_number_parameters     704
_refine_ls_number_restraints     96
_refine_ls_R_factor_all          0.0418
_refine_ls_R_factor_gt           0.0375
_refine_ls_wR_factor_ref         0.0982
_refine_ls_wR_factor_gt          0.0956
_refine_ls_goodness_of_fit_ref   1.021
_refine_ls_restrained_S_all      1.036
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.36062(5) 0.06121(5) 0.15805(3) 0.01833(13) Uani 1 1 d . . . . .
Mo2 Mo 0.30987(4) 0.27611(5) 0.47020(3) 0.01523(13) Uani 1 1 d . . . . .
Mo3 Mo 0.58829(4) 0.26628(5) 0.36730(3) 0.01715(13) Uani 1 1 d . . . . .
Mo4 Mo 0.07866(4) 0.19348(5) 0.41091(3) 0.01551(13) Uani 1 1 d . . . . .
Mo5 Mo 0.10411(4) 0.08958(5) 0.24555(3) 0.01412(12) Uani 1 1 d . . . . .
Mo6 Mo 0.61075(4) 0.16200(5) 0.22035(3) 0.01523(13) Uani 1 1 d . . . . .
Te1 Te 0.32392(3) 0.24929(3) 0.28034(2) 0.01390(10) Uani 1 1 d . . . . .
Co1 Co 0.31107(14) 0.50348(15) 0.56954(9) 0.0160(4) Uani 0.5 1 d . . P . .
Cs1 Cs 0.83141(3) 0.00204(4) 0.38458(2) 0.02613(12) Uani 1 1 d . . . . .
Cs2 Cs 0.58540(4) 0.04477(5) 0.59796(3) 0.03812(14) Uani 1 1 d . . . . .
O1 O 0.1039(4) 0.0529(4) 0.4495(2) 0.0248(11) Uani 1 1 d . . . . .
O2 O 0.2663(3) 0.2068(4) 0.3785(2) 0.0156(9) Uani 1 1 d . . . . .
O3 O 0.3648(4) 0.1471(4) 0.5194(3) 0.0250(11) Uani 1 1 d . . . . .
O4 O 0.6322(4) 0.0262(4) 0.2719(3) 0.0249(10) Uani 1 1 d . . . . .
O5 O 0.4072(4) -0.0638(4) 0.2170(3) 0.0272(11) Uani 1 1 d . . . . .
O6 O 0.4832(4) 0.1466(4) 0.1667(2) 0.0198(10) Uani 1 1 d . . . . .
O7 O 0.2870(3) 0.1197(4) 0.2585(2) 0.0160(9) Uani 1 1 d . . . . .
O8 O 0.6068(4) 0.1395(4) 0.4311(3) 0.0258(11) Uani 1 1 d . . . . .
O9 O 0.7170(4) 0.1728(4) 0.1512(3) 0.0262(11) Uani 1 1 d . . . . .
O10 O 0.4414(3) 0.3186(4) 0.4056(2) 0.0178(9) Uani 1 1 d . . . . .
O11 O 0.1132(4) -0.0339(4) 0.3138(3) 0.0258(11) Uani 1 1 d . . . . .
O12 O -0.0297(4) 0.0941(4) 0.2122(3) 0.0224(10) Uani 1 1 d . . . . .
O13 O 0.3117(4) 0.3601(4) 0.5300(3) 0.0254(11) Uani 1 1 d . . . . .
O14 O 0.4743(3) 0.1917(4) 0.3050(2) 0.0172(9) Uani 1 1 d . . . . .
O15 O 0.6846(3) 0.2276(4) 0.2882(2) 0.0195(10) Uani 1 1 d . . . . .
O16 O 0.1482(4) 0.2459(4) 0.4853(2) 0.0205(10) Uani 1 1 d . . . . .
O17 O 0.0732(3) 0.1886(4) 0.3090(2) 0.0159(9) Uani 1 1 d . . . . .
O18 O 0.1961(4) 0.0426(4) 0.1667(2) 0.0207(10) Uani 1 1 d . . . . .
O19 O -0.0646(4) 0.2212(5) 0.4326(3) 0.0287(12) Uani 1 1 d . . . . .
O20 O 0.5354(4) 0.4179(4) 0.2723(3) 0.0246(11) Uani 1 1 d . . . . .
O21 O 0.1242(4) 0.2609(4) 0.1645(2) 0.0215(10) Uani 1 1 d . . . . .
O22 O 0.3897(4) 0.0399(5) 0.0715(3) 0.0338(13) Uani 1 1 d . . . . .
O23 O 0.6758(4) 0.3494(5) 0.3950(3) 0.0329(13) Uani 1 1 d . . . . .
O24 O 0.5492(4) 0.3425(4) 0.1749(3) 0.0258(11) Uani 1 1 d . . . . .
O25 O 0.2919(4) 0.2394(4) 0.1023(3) 0.0256(11) Uani 1 1 d . . . . .
O26 O 0.0788(4) 0.3765(4) 0.3494(3) 0.0263(11) Uani 1 1 d . . . . .
O27 O 0.2367(4) 0.4326(4) 0.3860(3) 0.0251(11) Uani 1 1 d . . . . .
C1 C 0.4609(10) 0.7363(7) 0.1235(4) 0.054(3) Uani 1 1 d . . . . .
H1A H 0.4604 0.8016 0.1386 0.065 Uiso 1 1 calc R U . . .
C2 C 0.2351(7) 0.4407(8) -0.0055(5) 0.050(3) Uani 1 1 d . . . . .
H2A H 0.2925 0.3922 -0.0194 0.060 Uiso 1 1 calc R U . . .
C3 C 0.4915(9) 0.6341(7) 0.1724(4) 0.048(2) Uani 1 1 d . . . . .
H3A H 0.5113 0.6320 0.2201 0.058 Uiso 1 1 calc R U . . .
C4 C 0.2077(7) 0.5450(9) -0.0534(5) 0.054(3) Uani 1 1 d . . . . .
H4A H 0.2454 0.5661 -0.0999 0.065 Uiso 1 1 calc R U . . .
C5 C 0.1873(7) 0.7434(7) 0.2278(5) 0.044(2) Uani 1 1 d . . . . .
H5A H 0.2410 0.7960 0.2192 0.053 Uiso 1 1 calc R U . . .
C6 C 0.4310(8) 0.7415(6) 0.0524(4) 0.0360(19) Uani 1 1 d . . . . .
C7 C 0.0869(7) 0.7682(6) 0.1900(4) 0.0301(16) Uani 1 1 d . . . . .
C8 C 0.0723(7) 0.5902(7) 0.0365(4) 0.0336(18) Uani 1 1 d . . . . .
H8A H 0.0194 0.6422 0.0508 0.040 Uiso 1 1 calc R U . . .
C9 C 0.0079(6) 0.6875(6) 0.2024(4) 0.0294(17) Uani 1 1 d . . . . .
H9A H -0.0598 0.7039 0.1771 0.035 Uiso 1 1 calc R U . . .
C10 C 0.2082(7) 0.6414(7) 0.2782(5) 0.039(2) Uani 1 1 d . . . . .
H10A H 0.2757 0.6259 0.3037 0.047 Uiso 1 1 calc R U . . .
C11 C 0.4283(7) 0.6423(7) 0.0322(4) 0.0367(19) Uani 1 1 d . . . . .
H11A H 0.4053 0.6440 -0.0147 0.044 Uiso 1 1 calc R U . . .
C12 C 0.4596(7) 0.5416(7) 0.0818(4) 0.0333(18) Uani 1 1 d . . . . .
H12A H 0.4580 0.4760 0.0674 0.040 Uiso 1 1 calc R U . . .
C13 C 0.5293(6) 0.4247(6) 0.2033(4) 0.0247(15) Uani 1 1 d . . . . .
C14 C 0.1261(6) 0.6155(7) -0.0321(4) 0.036(2) Uani 1 1 d . . . . .
C15 C 0.4935(6) 0.5351(6) 0.1523(4) 0.0257(15) Uani 1 1 d . . . . .
C16 C 0.0287(6) 0.5850(6) 0.2513(4) 0.0274(16) Uani 1 1 d . . . . .
H16A H -0.0236 0.5314 0.2579 0.033 Uiso 1 1 calc R U . . .
C17 C 0.0974(6) 0.4858(6) 0.0848(4) 0.0300(17) Uani 1 1 d . . . . .
H17A H 0.0612 0.4669 0.1319 0.036 Uiso 1 1 calc R U . . .
C18 C 0.1289(6) 0.5605(6) 0.2915(4) 0.0239(15) Uani 1 1 d . . . . .
C19 C 0.1997(5) 0.2940(6) 0.1132(4) 0.0207(14) Uani 1 1 d . . . . .
C20 C 0.1493(5) 0.4495(6) 0.3460(4) 0.0210(14) Uani 1 1 d . . . . .
C21 C 0.1775(5) 0.4092(6) 0.0624(4) 0.0243(16) Uani 1 1 d . . . . .
N1 N 0.0927(6) 0.7239(6) -0.0852(4) 0.051(2) Uani 1 1 d . . . . .
H1B H 0.1253 0.7411 -0.1290 0.061 Uiso 1 1 calc R U . . .
H1C H 0.0407 0.7697 -0.0723 0.061 Uiso 1 1 calc R U . . .
N2 N 0.0642(6) 0.8740(5) 0.1386(4) 0.0400(17) Uani 1 1 d . . . . .
H2B H 0.1132 0.9233 0.1308 0.048 Uiso 1 1 calc R U . . .
H2C H 0.0015 0.8888 0.1152 0.048 Uiso 1 1 calc R U . . .
N3 N 0.3966(8) 0.8442(6) 0.0028(4) 0.052(2) Uani 1 1 d . . . . .
H3B H 0.3939 0.9050 0.0166 0.062 Uiso 1 1 calc R U . . .
H3C H 0.3783 0.8464 -0.0413 0.062 Uiso 1 1 calc R U . . .
O1W O 0.4794(11) 0.4499(10) 0.6135(8) 0.049(3) Uani 0.5 1 d . U P . .
O1WA O 0.4940(15) 0.4878(16) 0.5512(11) 0.086(5) Uani 0.5 1 d . U P . .
O2W O 0.3077(16) 0.4026(16) 0.6765(10) 0.089(5) Uani 0.5 1 d . U P . .
O3W O 0.2916(12) 0.5974(11) 0.4601(7) 0.055(3) Uani 0.5 1 d . U P . .
Na1 Na 0.1450(5) 0.5493(5) 0.5404(3) 0.0243(14) Uani 0.6 1 d . U P . .
Na1A Na 0.1416(6) 0.5280(7) 0.5810(6) 0.0273(19) Uani 0.4 1 d . . P . .
OW1 O 0.4361(14) 0.2140(13) 0.6869(9) 0.051(4) Uani 0.5 1 d . U P . .
OW2 O 0.492(2) 0.240(2) 0.6708(14) 0.112(8) Uani 0.5 1 d . U P . .
OW3 O 0.8017(7) 0.1998(7) 0.5662(4) 0.076(2) Uani 1 1 d . U . . .
OW4 O 0.8055(12) -0.1936(10) 0.3086(6) 0.136(5) Uani 1 1 d . U . . .
OW5 O 0.7359(11) 0.7864(13) 0.0808(8) 0.154(5) Uani 1 1 d . U . . .
OW6 O 0.7661(11) 0.5623(12) 0.1990(8) 0.148(5) Uani 1 1 d . U . . .
OW7 O 0.9785(8) 0.6487(8) 0.4232(5) 0.093(3) Uani 1 1 d . U . . .
OW8 O 0.8385(9) 0.1146(8) 0.0061(5) 0.090(3) Uani 1 1 d . U . . .
OW9 O 0.0915(8) 0.1495(7) 0.0267(5) 0.088(3) Uani 1 1 d . U . . .
OW10 O 0.8112(8) 0.9309(7) 0.1550(5) 0.084(3) Uani 1 1 d . U . . .
OW11 O 0.8792(5) 0.3465(5) 0.2313(4) 0.0451(15) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O5 1.712(5) . ?
Mo1 O22 1.715(5) . ?
Mo1 O6 1.912(4) . ?
Mo1 O18 1.957(4) . ?
Mo1 O25 2.276(5) . ?
Mo1 O7 2.277(4) . ?
Mo1 Mo5 3.3554(8) . ?
Mo1 Cs2 4.4658(9) 2_656 ?
Mo2 O3 1.710(5) . ?
Mo2 O13 1.727(4) . ?
Mo2 O10 1.918(4) . ?
Mo2 O16 1.956(4) . ?
Mo2 O2 2.226(4) . ?
Mo2 O27 2.284(5) . ?
Mo2 Mo4 3.3520(8) . ?
Mo2 Cs1 4.1944(8) 2_656 ?
Mo2 Cs2 4.4677(8) . ?
Mo2 Cs2 4.5463(9) 2_656 ?
Mo3 O8 1.709(5) . ?
Mo3 O23 1.724(5) . ?
Mo3 O15 1.933(4) . ?
Mo3 O10 1.939(4) . ?
Mo3 O14 2.250(4) . ?
Mo3 O20 2.286(5) . ?
Mo3 Mo6 3.3254(8) . ?
Mo3 Cs1 4.0930(8) . ?
Mo3 Cs2 4.4327(9) 2_656 ?
Mo3 Cs2 4.4506(8) . ?
Mo4 O1 1.710(5) . ?
Mo4 O19 1.723(4) . ?
Mo4 O17 1.929(4) . ?
Mo4 O16 1.945(4) . ?
Mo4 O2 2.252(4) . ?
Mo4 O26 2.262(5) . ?
Mo4 Cs1 4.0700(7) 1_455 ?
Mo4 Cs1 4.0865(8) 2_656 ?
Mo5 O11 1.714(5) . ?
Mo5 O12 1.719(4) . ?
Mo5 O17 1.922(4) . ?
Mo5 O18 1.948(4) . ?
Mo5 O7 2.255(4) . ?
Mo5 O21 2.285(4) . ?
Mo5 Cs1 4.0229(7) 1_455 ?
Mo6 O4 1.711(5) . ?
Mo6 O9 1.719(4) . ?
Mo6 O6 1.911(4) . ?
Mo6 O15 1.970(4) . ?
Mo6 O24 2.244(5) . ?
Mo6 O14 2.246(4) . ?
Mo6 Cs1 4.1081(8) . ?
Mo6 Cs2 4.3423(8) 2_656 ?
Te1 O2 1.865(4) . ?
Te1 O7 1.867(4) . ?
Te1 O14 1.876(4) . ?
Te1 Cs2 3.8482(7) 2_656 ?
Co1 Na1A 1.986(7) . ?
Co1 Na1 2.043(6) . ?
Co1 O2W 2.056(18) . ?
Co1 O3W 2.080(13) . ?
Co1 O13 2.110(5) . ?
Co1 O23 2.133(5) 2_666 ?
Co1 O1WA 2.146(18) . ?
Co1 O1W 2.165(14) . ?
Cs1 O1 3.121(5) 2_656 ?
Cs1 OW4 3.183(12) . ?
Cs1 O4 3.192(5) . ?
Cs1 O8 3.194(5) . ?
Cs1 O3 3.234(5) 2_656 ?
Cs1 O15 3.294(5) . ?
Cs1 O16 3.378(5) 2_656 ?
Cs1 O19 3.450(5) 1_655 ?
Cs1 O12 3.465(4) 1_655 ?
Cs1 O11 3.504(5) 1_655 ?
Cs1 O1 3.668(5) 1_655 ?
Cs1 O17 3.800(4) 1_655 ?
Cs2 O8 3.026(5) . ?
Cs2 O3 3.056(5) . ?
Cs2 O14 3.134(5) 2_656 ?
Cs2 OW2 3.16(3) . ?
Cs2 O7 3.260(4) 2_656 ?
Cs2 OW3 3.267(9) . ?
Cs2 OW1 3.320(16) . ?
Cs2 O2 3.365(4) 2_656 ?
Cs2 O4 3.411(5) 2_656 ?
Cs2 O5 3.538(5) 2_656 ?
Cs2 O8 3.540(5) 2_656 ?
Cs2 O3 3.639(5) 2_656 ?
O1 Cs1 3.121(5) 2_656 ?
O1 Cs1 3.668(5) 1_455 ?
O2 Cs2 3.365(4) 2_656 ?
O3 Cs1 3.234(5) 2_656 ?
O3 Cs2 3.639(5) 2_656 ?
O4 Cs2 3.411(5) 2_656 ?
O5 Cs2 3.538(5) 2_656 ?
O7 Cs2 3.260(4) 2_656 ?
O8 Cs2 3.540(5) 2_656 ?
O11 Cs1 3.504(5) 1_455 ?
O12 Cs1 3.465(4) 1_455 ?
O13 Na1 2.949(7) . ?
O14 Cs2 3.134(5) 2_656 ?
O16 Cs1 3.378(5) 2_656 ?
O17 Cs1 3.800(4) 1_455 ?
O19 Cs1 3.450(5) 1_455 ?
O20 C13 1.276(8) . ?
O21 C19 1.271(8) . ?
O23 Co1 2.133(5) 2_666 ?
O23 Na1A 2.877(9) 2_666 ?
O23 Na1 3.030(7) 2_666 ?
O24 C13 1.270(8) . ?
O25 C19 1.252(8) . ?
O26 C20 1.275(8) . ?
O27 C20 1.277(8) . ?
C1 C6 1.381(11) . ?
C1 C3 1.383(12) . ?
C1 H1A 0.9300 . ?
C2 C21 1.374(10) . ?
C2 C4 1.388(12) . ?
C2 H2A 0.9300 . ?
C3 C15 1.380(10) . ?
C3 H3A 0.9300 . ?
C4 C14 1.346(13) . ?
C4 H4A 0.9300 . ?
C5 C10 1.375(12) . ?
C5 C7 1.380(11) . ?
C5 H5A 0.9300 . ?
C6 C11 1.390(11) . ?
C6 N3 1.404(10) . ?
C7 C9 1.398(10) . ?
C7 N2 1.421(10) . ?
C8 C14 1.361(11) . ?
C8 C17 1.387(11) . ?
C8 H8A 0.9300 . ?
C9 C16 1.367(11) . ?
C9 H9A 0.9300 . ?
C10 C18 1.401(10) . ?
C10 H10A 0.9300 . ?
C11 C12 1.378(11) . ?
C11 H11A 0.9300 . ?
C12 C15 1.382(10) . ?
C12 H12A 0.9300 . ?
C13 C15 1.487(10) . ?
C14 N1 1.481(10) . ?
C16 C18 1.402(10) . ?
C16 H16A 0.9300 . ?
C17 C21 1.397(11) . ?
C17 H17A 0.9300 . ?
C18 C20 1.490(10) . ?
C19 C21 1.503(9) . ?
N1 H1B 0.8600 . ?
N1 H1C 0.8600 . ?
N2 H2B 0.8600 . ?
N2 H2C 0.8600 . ?
N3 H3B 0.8600 . ?
N3 H3C 0.8600 . ?
O1W O1WA 1.14(2) . ?
O2W Na1A 2.79(2) . ?
O3W Na1 2.221(15) . ?
O3W Na1A 2.765(16) . ?
Na1 Na1A 0.733(9) . ?
Na1 OW7 2.885(11) 2_666 ?
Na1 OW7 2.967(12) 1_455 ?
Na1 O23 3.030(7) 2_666 ?
Na1A OW7 2.752(12) 2_666 ?
Na1A O23 2.877(9) 2_666 ?
OW1 OW2 0.77(3) . ?
OW7 Na1A 2.752(12) 2_666 ?
OW7 Na1 2.885(11) 2_666 ?
OW7 Na1 2.967(12) 1_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Mo1 O22 103.5(3) . . ?
O5 Mo1 O6 98.8(2) . . ?
O22 Mo1 O6 102.2(2) . . ?
O5 Mo1 O18 98.6(2) . . ?
O22 Mo1 O18 98.6(2) . . ?
O6 Mo1 O18 148.85(19) . . ?
O5 Mo1 O25 167.8(2) . . ?
O22 Mo1 O25 88.6(2) . . ?
O6 Mo1 O25 77.32(18) . . ?
O18 Mo1 O25 80.27(18) . . ?
O5 Mo1 O7 89.0(2) . . ?
O22 Mo1 O7 165.9(2) . . ?
O6 Mo1 O7 82.05(16) . . ?
O18 Mo1 O7 72.62(16) . . ?
O25 Mo1 O7 79.07(16) . . ?
O5 Mo1 Mo5 96.50(16) . . ?
O22 Mo1 Mo5 128.28(17) . . ?
O6 Mo1 Mo5 121.33(13) . . ?
O18 Mo1 Mo5 30.67(13) . . ?
O25 Mo1 Mo5 76.27(11) . . ?
O7 Mo1 Mo5 41.97(10) . . ?
O5 Mo1 Cs2 47.37(16) . 2_656 ?
O22 Mo1 Cs2 149.38(19) . 2_656 ?
O6 Mo1 Cs2 77.59(13) . 2_656 ?
O18 Mo1 Cs2 95.80(13) . 2_656 ?
O25 Mo1 Cs2 120.48(12) . 2_656 ?
O7 Mo1 Cs2 44.53(11) . 2_656 ?
Mo5 Mo1 Cs2 72.615(16) . 2_656 ?
O3 Mo2 O13 104.7(2) . . ?
O3 Mo2 O10 98.5(2) . . ?
O13 Mo2 O10 101.5(2) . . ?
O3 Mo2 O16 96.8(2) . . ?
O13 Mo2 O16 98.5(2) . . ?
O10 Mo2 O16 150.70(18) . . ?
O3 Mo2 O2 91.1(2) . . ?
O13 Mo2 O2 162.8(2) . . ?
O10 Mo2 O2 82.51(16) . . ?
O16 Mo2 O2 72.38(16) . . ?
O3 Mo2 O27 168.9(2) . . ?
O13 Mo2 O27 86.3(2) . . ?
O10 Mo2 O27 78.01(18) . . ?
O16 Mo2 O27 82.17(18) . . ?
O2 Mo2 O27 78.07(17) . . ?
O3 Mo2 Mo4 97.40(16) . . ?
O13 Mo2 Mo4 127.18(15) . . ?
O10 Mo2 Mo4 122.03(13) . . ?
O16 Mo2 Mo4 30.66(12) . . ?
O2 Mo2 Mo4 41.82(10) . . ?
O27 Mo2 Mo4 76.10(11) . . ?
O3 Mo2 Cs1 45.47(15) . 2_656 ?
O13 Mo2 Cs1 99.65(16) . 2_656 ?
O10 Mo2 Cs1 142.13(14) . 2_656 ?
O16 Mo2 Cs1 52.42(14) . 2_656 ?
O2 Mo2 Cs1 86.45(11) . 2_656 ?
O27 Mo2 Cs1 134.58(11) . 2_656 ?
Mo4 Mo2 Cs1 64.447(15) . 2_656 ?
O3 Mo2 Cs2 27.56(15) . . ?
O13 Mo2 Cs2 89.13(17) . . ?
O10 Mo2 Cs2 79.50(13) . . ?
O16 Mo2 Cs2 122.16(14) . . ?
O2 Mo2 Cs2 108.07(11) . . ?
O27 Mo2 Cs2 155.67(11) . . ?
Mo4 Mo2 Cs2 124.54(2) . . ?
Cs1 Mo2 Cs2 69.756(14) 2_656 . ?
O3 Mo2 Cs2 48.27(16) . 2_656 ?
O13 Mo2 Cs2 151.98(17) . 2_656 ?
O10 Mo2 Cs2 79.20(13) . 2_656 ?
O16 Mo2 Cs2 92.90(14) . 2_656 ?
O2 Mo2 Cs2 45.04(11) . 2_656 ?
O27 Mo2 Cs2 120.68(12) . 2_656 ?
Mo4 Mo2 Cs2 71.415(16) . 2_656 ?
Cs1 Mo2 Cs2 67.626(14) 2_656 2_656 ?
Cs2 Mo2 Cs2 63.254(15) . 2_656 ?
O8 Mo3 O23 104.4(3) . . ?
O8 Mo3 O15 97.0(2) . . ?
O23 Mo3 O15 100.1(2) . . ?
O8 Mo3 O10 98.5(2) . . ?
O23 Mo3 O10 99.5(2) . . ?
O15 Mo3 O10 151.08(18) . . ?
O8 Mo3 O14 89.3(2) . . ?
O23 Mo3 O14 165.9(2) . . ?
O15 Mo3 O14 74.14(16) . . ?
O10 Mo3 O14 81.79(16) . . ?
O8 Mo3 O20 167.8(2) . . ?
O23 Mo3 O20 87.8(2) . . ?
O15 Mo3 O20 81.37(18) . . ?
O10 Mo3 O20 78.33(18) . . ?
O14 Mo3 O20 78.62(17) . . ?
O8 Mo3 Mo6 95.08(16) . . ?
O23 Mo3 Mo6 130.74(17) . . ?
O15 Mo3 Mo6 31.90(12) . . ?
O10 Mo3 Mo6 122.02(13) . . ?
O14 Mo3 Mo6 42.24(10) . . ?
O20 Mo3 Mo6 77.06(12) . . ?
O8 Mo3 Cs1 47.39(15) . . ?
O23 Mo3 Cs1 94.92(18) . . ?
O15 Mo3 Cs1 52.49(14) . . ?
O10 Mo3 Cs1 145.59(14) . . ?
O14 Mo3 Cs1 91.61(11) . . ?
O20 Mo3 Cs1 133.59(12) . . ?
Mo6 Mo3 Cs1 66.317(16) . . ?
O8 Mo3 Cs2 48.52(16) . 2_656 ?
O23 Mo3 Cs2 152.3(2) . 2_656 ?
O15 Mo3 Cs2 90.08(13) . 2_656 ?
O10 Mo3 Cs2 82.21(13) . 2_656 ?
O14 Mo3 Cs2 41.73(11) . 2_656 ?
O20 Mo3 Cs2 119.27(12) . 2_656 ?
Mo6 Mo3 Cs2 66.295(15) . 2_656 ?
Cs1 Mo3 Cs2 70.995(15) . 2_656 ?
O8 Mo3 Cs2 26.84(15) . . ?
O23 Mo3 Cs2 88.68(19) . . ?
O15 Mo3 Cs2 121.65(14) . . ?
O10 Mo3 Cs2 79.82(13) . . ?
O14 Mo3 Cs2 105.35(11) . . ?
O20 Mo3 Cs2 156.97(12) . . ?
Mo6 Mo3 Cs2 121.42(2) . . ?
Cs1 Mo3 Cs2 69.405(14) . . ?
Cs2 Mo3 Cs2 64.303(15) 2_656 . ?
O1 Mo4 O19 103.9(2) . . ?
O1 Mo4 O17 97.5(2) . . ?
O19 Mo4 O17 101.1(2) . . ?
O1 Mo4 O16 98.3(2) . . ?
O19 Mo4 O16 100.3(2) . . ?
O17 Mo4 O16 149.30(18) . . ?
O1 Mo4 O2 90.63(19) . . ?
O19 Mo4 O2 164.6(2) . . ?
O17 Mo4 O2 81.75(16) . . ?
O16 Mo4 O2 71.99(16) . . ?
O1 Mo4 O26 169.1(2) . . ?
O19 Mo4 O26 86.9(2) . . ?
O17 Mo4 O26 78.24(18) . . ?
O16 Mo4 O26 81.27(19) . . ?
O2 Mo4 O26 78.87(16) . . ?
O1 Mo4 Mo2 98.13(16) . . ?
O19 Mo4 Mo2 129.39(17) . . ?
O17 Mo4 Mo2 120.54(12) . . ?
O16 Mo4 Mo2 30.86(12) . . ?
O2 Mo4 Mo2 41.23(10) . . ?
O26 Mo4 Mo2 75.91(12) . . ?
O1 Mo4 Cs1 64.30(16) . 1_455 ?
O19 Mo4 Cs1 57.04(17) . 1_455 ?
O17 Mo4 Cs1 68.13(12) . 1_455 ?
O16 Mo4 Cs1 142.56(13) . 1_455 ?
O2 Mo4 Cs1 136.44(11) . 1_455 ?
O26 Mo4 Cs1 122.01(12) . 1_455 ?
Mo2 Mo4 Cs1 162.07(2) . 1_455 ?
O1 Mo4 Cs1 45.01(16) . 2_656 ?
O19 Mo4 Cs1 97.72(17) . 2_656 ?
O17 Mo4 Cs1 141.46(13) . 2_656 ?
O16 Mo4 Cs1 55.20(14) . 2_656 ?
O2 Mo4 Cs1 88.82(11) . 2_656 ?
O26 Mo4 Cs1 136.41(12) . 2_656 ?
Mo2 Mo4 Cs1 67.819(16) . 2_656 ?
Cs1 Mo4 Cs1 95.557(15) 1_455 2_656 ?
O11 Mo5 O12 103.2(2) . . ?
O11 Mo5 O17 97.8(2) . . ?
O12 Mo5 O17 100.5(2) . . ?
O11 Mo5 O18 99.3(2) . . ?
O12 Mo5 O18 98.9(2) . . ?
O17 Mo5 O18 150.38(18) . . ?
O11 Mo5 O7 92.2(2) . . ?
O12 Mo5 O7 163.80(19) . . ?
O17 Mo5 O7 82.10(16) . . ?
O18 Mo5 O7 73.29(16) . . ?
O11 Mo5 O21 168.5(2) . . ?
O12 Mo5 O21 88.03(19) . . ?
O17 Mo5 O21 77.63(17) . . ?
O18 Mo5 O21 80.87(18) . . ?
O7 Mo5 O21 76.83(16) . . ?
O11 Mo5 Mo1 98.79(17) . . ?
O12 Mo5 Mo1 128.19(15) . . ?
O17 Mo5 Mo1 122.28(12) . . ?
O18 Mo5 Mo1 30.84(12) . . ?
O7 Mo5 Mo1 42.48(10) . . ?
O21 Mo5 Mo1 75.44(11) . . ?
O11 Mo5 Cs1 60.25(16) . 1_455 ?
O12 Mo5 Cs1 58.94(15) . 1_455 ?
O17 Mo5 Cs1 69.40(12) . 1_455 ?
O18 Mo5 Cs1 140.20(13) . 1_455 ?
O7 Mo5 Cs1 135.51(11) . 1_455 ?
O21 Mo5 Cs1 126.08(11) . 1_455 ?
Mo1 Mo5 Cs1 158.45(2) . 1_455 ?
O4 Mo6 O9 103.5(2) . . ?
O4 Mo6 O6 98.5(2) . . ?
O9 Mo6 O6 99.8(2) . . ?
O4 Mo6 O15 96.0(2) . . ?
O9 Mo6 O15 99.19(19) . . ?
O6 Mo6 O15 152.62(18) . . ?
O4 Mo6 O24 165.8(2) . . ?
O9 Mo6 O24 90.7(2) . . ?
O6 Mo6 O24 79.90(19) . . ?
O15 Mo6 O24 80.35(18) . . ?
O4 Mo6 O14 88.9(2) . . ?
O9 Mo6 O14 166.4(2) . . ?
O6 Mo6 O14 83.59(17) . . ?
O15 Mo6 O14 73.57(16) . . ?
O24 Mo6 O14 76.87(17) . . ?
O4 Mo6 Mo3 94.26(16) . . ?
O9 Mo6 Mo3 129.45(16) . . ?
O6 Mo6 Mo3 124.08(13) . . ?
O15 Mo6 Mo3 31.23(12) . . ?
O24 Mo6 Mo3 75.46(12) . . ?
O14 Mo6 Mo3 42.34(11) . . ?
O4 Mo6 Cs1 46.84(15) . . ?
O9 Mo6 Cs1 93.15(17) . . ?
O6 Mo6 Cs1 145.13(14) . . ?
O15 Mo6 Cs1 52.27(14) . . ?
O24 Mo6 Cs1 132.47(12) . . ?
O14 Mo6 Cs1 91.28(11) . . ?
Mo3 Mo6 Cs1 65.840(16) . . ?
O4 Mo6 Cs2 46.93(16) . 2_656 ?
O9 Mo6 Cs2 149.52(18) . 2_656 ?
O6 Mo6 Cs2 81.07(13) . 2_656 ?
O15 Mo6 Cs2 92.26(13) . 2_656 ?
O24 Mo6 Cs2 119.13(12) . 2_656 ?
O14 Mo6 Cs2 43.81(12) . 2_656 ?
Mo3 Mo6 Cs2 69.181(17) . 2_656 ?
Cs1 Mo6 Cs2 71.794(14) . 2_656 ?
O2 Te1 O7 94.07(18) . . ?
O2 Te1 O14 93.71(18) . . ?
O7 Te1 O14 93.78(19) . . ?
O2 Te1 Cs2 60.97(14) . 2_656 ?
O7 Te1 Cs2 57.76(13) . 2_656 ?
O14 Te1 Cs2 53.92(14) . 2_656 ?
Na1A Co1 Na1 20.9(3) . . ?
Na1A Co1 O2W 87.4(6) . . ?
Na1 Co1 O2W 107.5(6) . . ?
Na1A Co1 O3W 85.7(5) . . ?
Na1 Co1 O3W 65.2(4) . . ?
O2W Co1 O3W 171.7(7) . . ?
Na1A Co1 O13 95.8(3) . . ?
Na1 Co1 O13 90.5(2) . . ?
O2W Co1 O13 89.1(5) . . ?
O3W Co1 O13 87.1(4) . . ?
Na1A Co1 O23 88.5(3) . 2_666 ?
Na1 Co1 O23 93.0(2) . 2_666 ?
O2W Co1 O23 93.0(6) . 2_666 ?
O3W Co1 O23 91.3(4) . 2_666 ?
O13 Co1 O23 175.2(2) . 2_666 ?
Na1A Co1 O1WA 176.0(6) . . ?
Na1 Co1 O1WA 155.8(6) . . ?
O2W Co1 O1WA 96.3(8) . . ?
O3W Co1 O1WA 90.8(7) . . ?
O13 Co1 O1WA 85.9(5) . . ?
O23 Co1 O1WA 89.6(5) 2_666 . ?
Na1A Co1 O1W 152.5(5) . . ?
Na1 Co1 O1W 173.4(4) . . ?
O2W Co1 O1W 66.2(6) . . ?
O3W Co1 O1W 121.2(5) . . ?
O13 Co1 O1W 91.5(3) . . ?
O23 Co1 O1W 85.5(3) 2_666 . ?
O1WA Co1 O1W 30.7(5) . . ?
O1 Cs1 OW4 120.5(2) 2_656 . ?
O1 Cs1 O4 146.45(12) 2_656 . ?
OW4 Cs1 O4 60.1(3) . . ?
O1 Cs1 O8 86.64(12) 2_656 . ?
OW4 Cs1 O8 119.5(3) . . ?
O4 Cs1 O8 68.71(12) . . ?
O1 Cs1 O3 73.75(12) 2_656 2_656 ?
OW4 Cs1 O3 72.9(2) . 2_656 ?
O4 Cs1 O3 75.14(12) . 2_656 ?
O8 Cs1 O3 64.46(13) . 2_656 ?
O1 Cs1 O15 127.62(12) 2_656 . ?
OW4 Cs1 O15 107.3(3) . . ?
O4 Cs1 O15 49.98(11) . . ?
O8 Cs1 O15 49.75(11) . . ?
O3 Cs1 O15 103.55(11) 2_656 . ?
O1 Cs1 O16 50.26(11) 2_656 2_656 ?
OW4 Cs1 O16 70.7(2) . 2_656 ?
O4 Cs1 O16 113.87(11) . 2_656 ?
O8 Cs1 O16 106.06(11) . 2_656 ?
O3 Cs1 O16 49.05(11) 2_656 2_656 ?
O15 Cs1 O16 152.45(10) . 2_656 ?
O1 Cs1 O19 65.94(12) 2_656 1_655 ?
OW4 Cs1 O19 162.4(2) . 1_655 ?
O4 Cs1 O19 125.04(12) . 1_655 ?
O8 Cs1 O19 75.82(12) . 1_655 ?
O3 Cs1 O19 124.10(11) 2_656 1_655 ?
O15 Cs1 O19 75.06(11) . 1_655 ?
O16 Cs1 O19 115.51(11) 2_656 1_655 ?
O1 Cs1 O12 136.42(11) 2_656 1_655 ?
OW4 Cs1 O12 77.3(2) . 1_655 ?
O4 Cs1 O12 77.04(11) . 1_655 ?
O8 Cs1 O12 120.84(12) . 1_655 ?
O3 Cs1 O12 146.52(11) 2_656 1_655 ?
O15 Cs1 O12 71.19(11) . 1_655 ?
O16 Cs1 O12 131.92(11) 2_656 1_655 ?
O19 Cs1 O12 87.34(11) 1_655 1_655 ?
O1 Cs1 O11 95.43(12) 2_656 1_655 ?
OW4 Cs1 O11 80.1(2) . 1_655 ?
O4 Cs1 O11 116.49(12) . 1_655 ?
O8 Cs1 O11 155.73(12) . 1_655 ?
O3 Cs1 O11 139.25(12) 2_656 1_655 ?
O15 Cs1 O11 113.46(10) . 1_655 ?
O16 Cs1 O11 93.55(11) 2_656 1_655 ?
O19 Cs1 O11 82.95(11) 1_655 1_655 ?
O12 Cs1 O11 45.42(11) 1_655 1_655 ?
O1 Cs1 O1 54.52(13) 2_656 1_655 ?
OW4 Cs1 O1 123.4(3) . 1_655 ?
O4 Cs1 O1 157.46(11) . 1_655 ?
O8 Cs1 O1 116.42(12) . 1_655 ?
O3 Cs1 O1 127.32(11) 2_656 1_655 ?
O15 Cs1 O1 114.72(11) . 1_655 ?
O16 Cs1 O1 86.53(10) 2_656 1_655 ?
O19 Cs1 O1 44.50(11) 1_655 1_655 ?
O12 Cs1 O1 82.14(10) 1_655 1_655 ?
O11 Cs1 O1 49.49(11) 1_655 1_655 ?
O1 Cs1 O17 95.34(10) 2_656 1_655 ?
OW4 Cs1 O17 117.1(2) . 1_655 ?
O4 Cs1 O17 114.48(11) . 1_655 ?
O8 Cs1 O17 111.84(11) . 1_655 ?
O3 Cs1 O17 168.40(10) 2_656 1_655 ?
O15 Cs1 O17 79.80(10) . 1_655 ?
O16 Cs1 O17 126.38(10) 2_656 1_655 ?
O19 Cs1 O17 45.52(10) 1_655 1_655 ?
O12 Cs1 O17 45.07(9) 1_655 1_655 ?
O11 Cs1 O17 43.89(10) 1_655 1_655 ?
O1 Cs1 O17 43.02(9) 1_655 1_655 ?
O8 Cs2 O3 63.24(12) . . ?
O8 Cs2 O14 131.12(12) . 2_656 ?
O3 Cs2 O14 104.55(12) . 2_656 ?
O8 Cs2 OW2 108.7(5) . . ?
O3 Cs2 OW2 74.9(5) . . ?
O14 Cs2 OW2 113.0(5) 2_656 . ?
O8 Cs2 O7 144.15(11) . 2_656 ?
O3 Cs2 O7 149.80(11) . 2_656 ?
O14 Cs2 O7 50.54(10) 2_656 2_656 ?
OW2 Cs2 O7 98.0(5) . 2_656 ?
O8 Cs2 OW3 73.86(16) . . ?
O3 Cs2 OW3 116.93(15) . . ?
O14 Cs2 OW3 138.48(14) 2_656 . ?
OW2 Cs2 OW3 78.1(5) . . ?
O7 Cs2 OW3 89.23(14) 2_656 . ?
O8 Cs2 OW1 114.2(3) . . ?
O3 Cs2 OW1 69.1(3) . . ?
O14 Cs2 OW1 102.2(3) 2_656 . ?
OW2 Cs2 OW1 13.4(5) . . ?
O7 Cs2 OW1 97.2(3) 2_656 . ?
OW3 Cs2 OW1 91.4(3) . . ?
O8 Cs2 O2 101.95(11) . 2_656 ?
O3 Cs2 O2 132.72(12) . 2_656 ?
O14 Cs2 O2 49.51(10) 2_656 2_656 ?
OW2 Cs2 O2 146.6(5) . 2_656 ?
O7 Cs2 O2 48.65(10) 2_656 2_656 ?
OW3 Cs2 O2 98.56(14) . 2_656 ?
OW1 Cs2 O2 143.8(3) . 2_656 ?
O8 Cs2 O4 136.47(12) . 2_656 ?
O3 Cs2 O4 74.36(12) . 2_656 ?
O14 Cs2 O4 50.37(11) 2_656 2_656 ?
OW2 Cs2 O4 66.8(5) . 2_656 ?
O7 Cs2 O4 75.88(10) 2_656 2_656 ?
OW3 Cs2 O4 138.94(15) . 2_656 ?
OW1 Cs2 O4 54.0(3) . 2_656 ?
O2 Cs2 O4 99.44(11) 2_656 2_656 ?
O8 Cs2 O5 152.90(13) . 2_656 ?
O3 Cs2 O5 115.14(12) . 2_656 ?
O14 Cs2 O5 75.98(11) 2_656 2_656 ?
OW2 Cs2 O5 49.4(5) . 2_656 ?
O7 Cs2 O5 48.87(11) 2_656 2_656 ?
OW3 Cs2 O5 84.68(15) . 2_656 ?
OW1 Cs2 O5 48.8(3) . 2_656 ?
O2 Cs2 O5 97.37(10) 2_656 2_656 ?
O4 Cs2 O5 56.62(11) 2_656 2_656 ?
O8 Cs2 O8 88.23(13) . 2_656 ?
O3 Cs2 O8 62.12(12) . 2_656 ?
O14 Cs2 O8 49.29(11) 2_656 2_656 ?
OW2 Cs2 O8 119.6(5) . 2_656 ?
O7 Cs2 O8 99.19(11) 2_656 2_656 ?
OW3 Cs2 O8 158.63(15) . 2_656 ?
OW1 Cs2 O8 106.9(3) . 2_656 ?
O2 Cs2 O8 73.40(10) 2_656 2_656 ?
O4 Cs2 O8 62.42(11) 2_656 2_656 ?
O5 Cs2 O8 115.63(11) 2_656 2_656 ?
O8 Cs2 O3 61.09(12) . 2_656 ?
O3 Cs2 O3 90.60(12) . 2_656 ?
O14 Cs2 O3 72.62(11) 2_656 2_656 ?
OW2 Cs2 O3 165.2(5) . 2_656 ?
O7 Cs2 O3 95.94(11) 2_656 2_656 ?
OW3 Cs2 O3 107.13(15) . 2_656 ?
OW1 Cs2 O3 157.4(3) . 2_656 ?
O2 Cs2 O3 47.51(10) 2_656 2_656 ?
O4 Cs2 O3 112.26(11) 2_656 2_656 ?
O5 Cs2 O3 143.53(11) 2_656 2_656 ?
O8 Cs2 O3 52.71(10) 2_656 2_656 ?
Mo4 O1 Cs1 112.2(2) . 2_656 ?
Mo4 O1 Cs1 90.86(18) . 1_455 ?
Cs1 O1 Cs1 125.48(13) 2_656 1_455 ?
Te1 O2 Mo2 125.7(2) . . ?
Te1 O2 Mo4 123.8(2) . . ?
Mo2 O2 Mo4 96.95(15) . . ?
Te1 O2 Cs2 90.03(15) . 2_656 ?
Mo2 O2 Cs2 107.06(15) . 2_656 ?
Mo4 O2 Cs2 112.50(15) . 2_656 ?
Mo2 O3 Cs2 137.4(2) . . ?
Mo2 O3 Cs1 112.4(2) . 2_656 ?
Cs2 O3 Cs1 104.04(14) . 2_656 ?
Mo2 O3 Cs2 111.2(2) . 2_656 ?
Cs2 O3 Cs2 89.41(12) . 2_656 ?
Cs1 O3 Cs2 90.11(11) 2_656 2_656 ?
Mo6 O4 Cs1 110.1(2) . . ?
Mo6 O4 Cs2 111.6(2) . 2_656 ?
Cs1 O4 Cs2 97.28(12) . 2_656 ?
Mo1 O5 Cs2 111.8(2) . 2_656 ?
Mo6 O6 Mo1 148.6(3) . . ?
Te1 O7 Mo5 121.7(2) . . ?
Te1 O7 Mo1 124.3(2) . . ?
Mo5 O7 Mo1 95.55(15) . . ?
Te1 O7 Cs2 93.27(15) . 2_656 ?
Mo5 O7 Cs2 116.39(16) . 2_656 ?
Mo1 O7 Cs2 106.15(15) . 2_656 ?
Mo3 O8 Cs2 138.4(2) . . ?
Mo3 O8 Cs1 109.4(2) . . ?
Cs2 O8 Cs1 103.12(14) . . ?
Mo3 O8 Cs2 110.3(2) . 2_656 ?
Cs2 O8 Cs2 91.77(13) . 2_656 ?
Cs1 O8 Cs2 94.69(12) . 2_656 ?
Mo2 O10 Mo3 145.2(3) . . ?
Mo5 O11 Cs1 94.62(19) . 1_455 ?
Mo5 O12 Cs1 95.91(18) . 1_455 ?
Mo2 O13 Co1 161.1(3) . . ?
Mo2 O13 Na1 126.9(3) . . ?
Co1 O13 Na1 43.86(15) . . ?
Te1 O14 Mo6 123.0(2) . . ?
Te1 O14 Mo3 124.2(2) . . ?
Mo6 O14 Mo3 95.41(15) . . ?
Te1 O14 Cs2 97.16(16) . 2_656 ?
Mo6 O14 Cs2 106.45(16) . 2_656 ?
Mo3 O14 Cs2 109.73(15) . 2_656 ?
Mo3 O15 Mo6 116.9(2) . . ?
Mo3 O15 Cs1 99.78(17) . . ?
Mo6 O15 Cs1 99.50(17) . . ?
Mo4 O16 Mo2 118.5(2) . . ?
Mo4 O16 Cs1 96.59(17) . 2_656 ?
Mo2 O16 Cs1 100.27(17) . 2_656 ?
Mo5 O17 Mo4 142.1(2) . . ?
Mo5 O17 Cs1 82.33(13) . 1_455 ?
Mo4 O17 Cs1 83.76(13) . 1_455 ?
Mo5 O18 Mo1 118.5(2) . . ?
Mo4 O19 Cs1 98.2(2) . 1_455 ?
C13 O20 Mo3 129.3(4) . . ?
C19 O21 Mo5 131.2(4) . . ?
Mo3 O23 Co1 147.5(3) . 2_666 ?
Mo3 O23 Na1A 167.4(3) . 2_666 ?
Co1 O23 Na1A 43.62(18) 2_666 2_666 ?
Mo3 O23 Na1 168.4(3) . 2_666 ?
Co1 O23 Na1 42.34(14) 2_666 2_666 ?
Na1A O23 Na1 13.96(18) 2_666 2_666 ?
C13 O24 Mo6 133.8(5) . . ?
C19 O25 Mo1 131.1(4) . . ?
C20 O26 Mo4 132.6(4) . . ?
C20 O27 Mo2 131.2(4) . . ?
C6 C1 C3 120.2(8) . . ?
C6 C1 H1A 119.9 . . ?
C3 C1 H1A 119.9 . . ?
C21 C2 C4 120.0(8) . . ?
C21 C2 H2A 120.0 . . ?
C4 C2 H2A 120.0 . . ?
C15 C3 C1 121.8(8) . . ?
C15 C3 H3A 119.1 . . ?
C1 C3 H3A 119.1 . . ?
C14 C4 C2 119.4(7) . . ?
C14 C4 H4A 120.3 . . ?
C2 C4 H4A 120.3 . . ?
C10 C5 C7 120.3(7) . . ?
C10 C5 H5A 119.8 . . ?
C7 C5 H5A 119.8 . . ?
C1 C6 C11 118.7(7) . . ?
C1 C6 N3 120.9(7) . . ?
C11 C6 N3 120.3(7) . . ?
C5 C7 C9 119.3(7) . . ?
C5 C7 N2 120.6(7) . . ?
C9 C7 N2 120.1(7) . . ?
C14 C8 C17 119.1(8) . . ?
C14 C8 H8A 120.5 . . ?
C17 C8 H8A 120.5 . . ?
C16 C9 C7 120.9(7) . . ?
C16 C9 H9A 119.5 . . ?
C7 C9 H9A 119.5 . . ?
C5 C10 C18 120.8(7) . . ?
C5 C10 H10A 119.6 . . ?
C18 C10 H10A 119.6 . . ?
C12 C11 C6 120.0(7) . . ?
C12 C11 H11A 120.0 . . ?
C6 C11 H11A 120.0 . . ?
C11 C12 C15 122.0(7) . . ?
C11 C12 H12A 119.0 . . ?
C15 C12 H12A 119.0 . . ?
O24 C13 O20 124.3(7) . . ?
O24 C13 C15 117.1(6) . . ?
O20 C13 C15 118.5(6) . . ?
C4 C14 C8 122.3(7) . . ?
C4 C14 N1 119.0(7) . . ?
C8 C14 N1 118.7(8) . . ?
C3 C15 C12 117.2(7) . . ?
C3 C15 C13 122.6(7) . . ?
C12 C15 C13 120.2(6) . . ?
C9 C16 C18 120.0(7) . . ?
C9 C16 H16A 120.0 . . ?
C18 C16 H16A 120.0 . . ?
C8 C17 C21 119.5(7) . . ?
C8 C17 H17A 120.3 . . ?
C21 C17 H17A 120.3 . . ?
C10 C18 C16 118.6(7) . . ?
C10 C18 C20 121.8(6) . . ?
C16 C18 C20 119.6(6) . . ?
O25 C19 O21 125.5(6) . . ?
O25 C19 C21 117.3(6) . . ?
O21 C19 C21 117.2(6) . . ?
O26 C20 O27 124.0(6) . . ?
O26 C20 C18 117.8(6) . . ?
O27 C20 C18 118.2(6) . . ?
C2 C21 C17 119.4(7) . . ?
C2 C21 C19 121.2(7) . . ?
C17 C21 C19 119.4(6) . . ?
C14 N1 H1B 120.0 . . ?
C14 N1 H1C 120.0 . . ?
H1B N1 H1C 120.0 . . ?
C7 N2 H2B 120.0 . . ?
C7 N2 H2C 120.0 . . ?
H2B N2 H2C 120.0 . . ?
C6 N3 H3B 120.0 . . ?
C6 N3 H3C 120.0 . . ?
H3B N3 H3C 120.0 . . ?
O1WA O1W Co1 73.8(12) . . ?
O1W O1WA Co1 75.6(12) . . ?
Co1 O2W Na1A 45.3(4) . . ?
Co1 O3W Na1 56.6(4) . . ?
Co1 O3W Na1A 45.7(3) . . ?
Na1 O3W Na1A 11.4(2) . . ?
Na1A Na1 Co1 75.1(8) . . ?
Na1A Na1 O3W 132.0(10) . . ?
Co1 Na1 O3W 58.2(4) . . ?
Na1A Na1 OW7 72.3(9) . 2_666 ?
Co1 Na1 OW7 108.5(3) . 2_666 ?
O3W Na1 OW7 130.5(4) . 2_666 ?
Na1A Na1 O13 90.2(9) . . ?
Co1 Na1 O13 45.68(15) . . ?
O3W Na1 O13 66.2(4) . . ?
OW7 Na1 O13 72.7(2) 2_666 . ?
Na1A Na1 OW7 135.7(9) . 1_455 ?
Co1 Na1 OW7 149.1(3) . 1_455 ?
O3W Na1 OW7 91.2(4) . 1_455 ?
OW7 Na1 OW7 87.4(3) 2_666 1_455 ?
O13 Na1 OW7 121.4(3) . 1_455 ?
Na1A Na1 O23 71.1(9) . 2_666 ?
Co1 Na1 O23 44.68(16) . 2_666 ?
O3W Na1 O23 68.0(4) . 2_666 ?
OW7 Na1 O23 139.4(3) 2_666 2_666 ?
O13 Na1 O23 90.3(2) . 2_666 ?
OW7 Na1 O23 131.9(3) 1_455 2_666 ?
Na1 Na1A Co1 84.0(9) . . ?
Na1 Na1A OW7 93.0(10) . 2_666 ?
Co1 Na1A OW7 115.6(4) . 2_666 ?
Na1 Na1A O3W 36.7(8) . . ?
Co1 Na1A O3W 48.6(4) . . ?
OW7 Na1A O3W 114.7(4) 2_666 . ?
Na1 Na1A O2W 129.4(10) . . ?
Co1 Na1A O2W 47.3(4) . . ?
OW7 Na1A O2W 96.4(5) 2_666 . ?
O3W Na1A O2W 95.8(5) . . ?
Na1 Na1A O23 94.9(9) . 2_666 ?
Co1 Na1A O23 47.84(19) . 2_666 ?
OW7 Na1A O23 160.4(4) 2_666 2_666 ?
O3W Na1A O23 64.5(3) . 2_666 ?
O2W Na1A O23 64.8(5) . 2_666 ?
OW2 OW1 Cs2 72(3) . . ?
OW1 OW2 Cs2 95(3) . . ?
Na1A OW7 Na1 14.71(19) 2_666 2_666 ?
Na1A OW7 Na1 103.8(4) 2_666 1_655 ?
Na1 OW7 Na1 92.6(3) 2_666 1_655 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O19 Mo4 O1 Cs1 -87.1(2) . . . 2_656 ?
O17 Mo4 O1 Cs1 169.46(18) . . . 2_656 ?
O16 Mo4 O1 Cs1 15.8(2) . . . 2_656 ?
O2 Mo4 O1 Cs1 87.70(19) . . . 2_656 ?
O26 Mo4 O1 Cs1 103.0(10) . . . 2_656 ?
Mo2 Mo4 O1 Cs1 47.00(17) . . . 2_656 ?
Cs1 Mo4 O1 Cs1 -129.3(2) 1_455 . . 2_656 ?
O19 Mo4 O1 Cs1 42.2(2) . . . 1_455 ?
O17 Mo4 O1 Cs1 -61.27(15) . . . 1_455 ?
O16 Mo4 O1 Cs1 145.09(13) . . . 1_455 ?
O2 Mo4 O1 Cs1 -143.03(13) . . . 1_455 ?
O26 Mo4 O1 Cs1 -127.7(10) . . . 1_455 ?
Mo2 Mo4 O1 Cs1 176.28(5) . . . 1_455 ?
Cs1 Mo4 O1 Cs1 129.3(2) 2_656 . . 1_455 ?
O7 Te1 O2 Mo2 160.6(3) . . . . ?
O14 Te1 O2 Mo2 66.5(3) . . . . ?
Cs2 Te1 O2 Mo2 111.2(3) 2_656 . . . ?
O7 Te1 O2 Mo4 -68.1(3) . . . . ?
O14 Te1 O2 Mo4 -162.1(3) . . . . ?
Cs2 Te1 O2 Mo4 -117.4(3) 2_656 . . . ?
O7 Te1 O2 Cs2 49.38(15) . . . 2_656 ?
O14 Te1 O2 Cs2 -44.69(16) . . . 2_656 ?
O13 Mo2 O3 Cs2 -57.6(4) . . . . ?
O10 Mo2 O3 Cs2 46.7(3) . . . . ?
O16 Mo2 O3 Cs2 -158.3(3) . . . . ?
O2 Mo2 O3 Cs2 129.3(3) . . . . ?
O27 Mo2 O3 Cs2 117.6(9) . . . . ?
Mo4 Mo2 O3 Cs2 170.8(3) . . . . ?
Cs1 Mo2 O3 Cs2 -146.7(4) 2_656 . . . ?
Cs2 Mo2 O3 Cs2 113.9(4) 2_656 . . . ?
O13 Mo2 O3 Cs1 89.2(2) . . . 2_656 ?
O10 Mo2 O3 Cs1 -166.52(18) . . . 2_656 ?
O16 Mo2 O3 Cs1 -11.5(2) . . . 2_656 ?
O2 Mo2 O3 Cs1 -83.93(19) . . . 2_656 ?
O27 Mo2 O3 Cs1 -95.7(10) . . . 2_656 ?
Mo4 Mo2 O3 Cs1 -42.45(17) . . . 2_656 ?
Cs2 Mo2 O3 Cs1 146.7(4) . . . 2_656 ?
Cs2 Mo2 O3 Cs1 -99.3(2) 2_656 . . 2_656 ?
O13 Mo2 O3 Cs2 -171.52(18) . . . 2_656 ?
O10 Mo2 O3 Cs2 -67.20(19) . . . 2_656 ?
O16 Mo2 O3 Cs2 87.78(18) . . . 2_656 ?
O2 Mo2 O3 Cs2 15.39(17) . . . 2_656 ?
O27 Mo2 O3 Cs2 3.6(11) . . . 2_656 ?
Mo4 Mo2 O3 Cs2 56.88(15) . . . 2_656 ?
Cs1 Mo2 O3 Cs2 99.3(2) 2_656 . . 2_656 ?
Cs2 Mo2 O3 Cs2 -113.9(4) . . . 2_656 ?
O9 Mo6 O4 Cs1 81.5(2) . . . . ?
O6 Mo6 O4 Cs1 -176.16(18) . . . . ?
O15 Mo6 O4 Cs1 -19.4(2) . . . . ?
O24 Mo6 O4 Cs1 -93.9(8) . . . . ?
O14 Mo6 O4 Cs1 -92.80(18) . . . . ?
Mo3 Mo6 O4 Cs1 -50.76(16) . . . . ?
Cs2 Mo6 O4 Cs1 -106.9(2) 2_656 . . . ?
O9 Mo6 O4 Cs2 -171.59(19) . . . 2_656 ?
O6 Mo6 O4 Cs2 -69.3(2) . . . 2_656 ?
O15 Mo6 O4 Cs2 87.43(19) . . . 2_656 ?
O24 Mo6 O4 Cs2 13.0(9) . . . 2_656 ?
O14 Mo6 O4 Cs2 14.08(17) . . . 2_656 ?
Mo3 Mo6 O4 Cs2 56.11(15) . . . 2_656 ?
Cs1 Mo6 O4 Cs2 106.9(2) . . . 2_656 ?
O22 Mo1 O5 Cs2 168.9(2) . . . 2_656 ?
O6 Mo1 O5 Cs2 64.1(2) . . . 2_656 ?
O18 Mo1 O5 Cs2 -90.0(2) . . . 2_656 ?
O25 Mo1 O5 Cs2 -6.2(10) . . . 2_656 ?
O7 Mo1 O5 Cs2 -17.72(17) . . . 2_656 ?
Mo5 Mo1 O5 Cs2 -59.09(16) . . . 2_656 ?
O2 Te1 O7 Mo5 72.3(2) . . . . ?
O14 Te1 O7 Mo5 166.3(2) . . . . ?
Cs2 Te1 O7 Mo5 124.0(3) 2_656 . . . ?
O2 Te1 O7 Mo1 -163.8(2) . . . . ?
O14 Te1 O7 Mo1 -69.8(3) . . . . ?
Cs2 Te1 O7 Mo1 -112.1(3) 2_656 . . . ?
O2 Te1 O7 Cs2 -51.69(15) . . . 2_656 ?
O14 Te1 O7 Cs2 42.31(15) . . . 2_656 ?
O23 Mo3 O8 Cs2 56.0(4) . . . . ?
O15 Mo3 O8 Cs2 158.4(3) . . . . ?
O10 Mo3 O8 Cs2 -46.1(4) . . . . ?
O14 Mo3 O8 Cs2 -127.7(3) . . . . ?
O20 Mo3 O8 Cs2 -120.3(8) . . . . ?
Mo6 Mo3 O8 Cs2 -169.6(3) . . . . ?
Cs1 Mo3 O8 Cs2 139.4(4) . . . . ?
Cs2 Mo3 O8 Cs2 -117.7(4) 2_656 . . . ?
O23 Mo3 O8 Cs1 -83.4(2) . . . . ?
O15 Mo3 O8 Cs1 19.0(2) . . . . ?
O10 Mo3 O8 Cs1 174.45(18) . . . . ?
O14 Mo3 O8 Cs1 92.87(18) . . . . ?
O20 Mo3 O8 Cs1 100.3(9) . . . . ?
Mo6 Mo3 O8 Cs1 50.98(16) . . . . ?
Cs2 Mo3 O8 Cs1 102.9(2) 2_656 . . . ?
Cs2 Mo3 O8 Cs1 -139.4(4) . . . . ?
O23 Mo3 O8 Cs2 173.76(19) . . . 2_656 ?
O15 Mo3 O8 Cs2 -83.91(19) . . . 2_656 ?
O10 Mo3 O8 Cs2 71.59(19) . . . 2_656 ?
O14 Mo3 O8 Cs2 -9.99(17) . . . 2_656 ?
O20 Mo3 O8 Cs2 -2.6(10) . . . 2_656 ?
Mo6 Mo3 O8 Cs2 -51.88(14) . . . 2_656 ?
Cs1 Mo3 O8 Cs2 -102.9(2) . . . 2_656 ?
Cs2 Mo3 O8 Cs2 117.7(4) . . . 2_656 ?
O12 Mo5 O11 Cs1 -41.9(2) . . . 1_455 ?
O17 Mo5 O11 Cs1 60.85(16) . . . 1_455 ?
O18 Mo5 O11 Cs1 -143.40(14) . . . 1_455 ?
O7 Mo5 O11 Cs1 143.18(14) . . . 1_455 ?
O21 Mo5 O11 Cs1 126.5(10) . . . 1_455 ?
Mo1 Mo5 O11 Cs1 -174.63(7) . . . 1_455 ?
O11 Mo5 O12 Cs1 42.6(2) . . . 1_455 ?
O17 Mo5 O12 Cs1 -58.09(17) . . . 1_455 ?
O18 Mo5 O12 Cs1 144.43(16) . . . 1_455 ?
O7 Mo5 O12 Cs1 -155.8(6) . . . 1_455 ?
O21 Mo5 O12 Cs1 -135.12(16) . . . 1_455 ?
Mo1 Mo5 O12 Cs1 155.19(6) . . . 1_455 ?
O3 Mo2 O13 Co1 159.8(8) . . . . ?
O10 Mo2 O13 Co1 57.7(9) . . . . ?
O16 Mo2 O13 Co1 -100.8(8) . . . . ?
O2 Mo2 O13 Co1 -44.2(13) . . . . ?
O27 Mo2 O13 Co1 -19.3(8) . . . . ?
Mo4 Mo2 O13 Co1 -88.8(8) . . . . ?
Cs1 Mo2 O13 Co1 -153.9(8) 2_656 . . . ?
Cs2 Mo2 O13 Co1 136.8(8) . . . . ?
Cs2 Mo2 O13 Co1 146.2(6) 2_656 . . . ?
O3 Mo2 O13 Na1 -146.5(3) . . . . ?
O10 Mo2 O13 Na1 111.4(3) . . . . ?
O16 Mo2 O13 Na1 -47.1(3) . . . . ?
O2 Mo2 O13 Na1 9.5(8) . . . . ?
O27 Mo2 O13 Na1 34.4(3) . . . . ?
Mo4 Mo2 O13 Na1 -35.0(4) . . . . ?
Cs1 Mo2 O13 Na1 -100.2(3) 2_656 . . . ?
Cs2 Mo2 O13 Na1 -169.5(3) . . . . ?
Cs2 Mo2 O13 Na1 -160.06(19) 2_656 . . . ?
O2 Te1 O14 Mo6 164.5(3) . . . . ?
O7 Te1 O14 Mo6 70.2(3) . . . . ?
Cs2 Te1 O14 Mo6 115.0(3) 2_656 . . . ?
O2 Te1 O14 Mo3 -70.2(3) . . . . ?
O7 Te1 O14 Mo3 -164.6(2) . . . . ?
Cs2 Te1 O14 Mo3 -119.8(3) 2_656 . . . ?
O2 Te1 O14 Cs2 49.54(16) . . . 2_656 ?
O7 Te1 O14 Cs2 -44.79(16) . . . 2_656 ?
O1 Mo4 O19 Cs1 -46.2(2) . . . 1_455 ?
O17 Mo4 O19 Cs1 54.57(19) . . . 1_455 ?
O16 Mo4 O19 Cs1 -147.53(17) . . . 1_455 ?
O2 Mo4 O19 Cs1 153.9(6) . . . 1_455 ?
O26 Mo4 O19 Cs1 131.93(17) . . . 1_455 ?
Mo2 Mo4 O19 Cs1 -159.20(6) . . . 1_455 ?
Cs1 Mo4 O19 Cs1 -91.64(11) 2_656 . . 1_455 ?
O8 Mo3 O23 Co1 -120.6(6) . . . 2_666 ?
O15 Mo3 O23 Co1 139.5(6) . . . 2_666 ?
O10 Mo3 O23 Co1 -19.2(6) . . . 2_666 ?
O14 Mo3 O23 Co1 74.9(10) . . . 2_666 ?
O20 Mo3 O23 Co1 58.6(6) . . . 2_666 ?
Mo6 Mo3 O23 Co1 129.4(5) . . . 2_666 ?
Cs1 Mo3 O23 Co1 -167.8(6) . . . 2_666 ?
Cs2 Mo3 O23 Co1 -110.5(6) 2_656 . . 2_666 ?
Cs2 Mo3 O23 Co1 -98.6(6) . . . 2_666 ?
O8 Mo3 O23 Na1A 92.5(17) . . . 2_666 ?
O15 Mo3 O23 Na1A -7.4(18) . . . 2_666 ?
O10 Mo3 O23 Na1A -166.0(17) . . . 2_666 ?
O14 Mo3 O23 Na1A -72(2) . . . 2_666 ?
O20 Mo3 O23 Na1A -88.2(17) . . . 2_666 ?
Mo6 Mo3 O23 Na1A -17.4(19) . . . 2_666 ?
Cs1 Mo3 O23 Na1A 45.3(17) . . . 2_666 ?
Cs2 Mo3 O23 Na1A 102.6(17) 2_656 . . 2_666 ?
Cs2 Mo3 O23 Na1A 114.5(17) . . . 2_666 ?
O8 Mo3 O23 Na1 22.1(14) . . . 2_666 ?
O15 Mo3 O23 Na1 -77.8(14) . . . 2_666 ?
O10 Mo3 O23 Na1 123.5(14) . . . 2_666 ?
O14 Mo3 O23 Na1 -142.4(12) . . . 2_666 ?
O20 Mo3 O23 Na1 -158.7(14) . . . 2_666 ?
Mo6 Mo3 O23 Na1 -87.9(14) . . . 2_666 ?
Cs1 Mo3 O23 Na1 -25.1(14) . . . 2_666 ?
Cs2 Mo3 O23 Na1 32.2(16) 2_656 . . 2_666 ?
Cs2 Mo3 O23 Na1 44.1(14) . . . 2_666 ?
C6 C1 C3 C15 0.0(17) . . . . ?
C21 C2 C4 C14 1.4(15) . . . . ?
C3 C1 C6 C11 2.4(15) . . . . ?
C3 C1 C6 N3 178.2(10) . . . . ?
C10 C5 C7 C9 -1.3(13) . . . . ?
C10 C5 C7 N2 179.2(8) . . . . ?
C5 C7 C9 C16 0.0(12) . . . . ?
N2 C7 C9 C16 179.5(7) . . . . ?
C7 C5 C10 C18 0.7(14) . . . . ?
C1 C6 C11 C12 -2.7(13) . . . . ?
N3 C6 C11 C12 -178.5(8) . . . . ?
C6 C11 C12 C15 0.6(12) . . . . ?
Mo6 O24 C13 O20 -4.5(10) . . . . ?
Mo6 O24 C13 C15 177.2(4) . . . . ?
Mo3 O20 C13 O24 2.6(10) . . . . ?
Mo3 O20 C13 C15 -179.2(4) . . . . ?
C2 C4 C14 C8 2.9(14) . . . . ?
C2 C4 C14 N1 -176.5(8) . . . . ?
C17 C8 C14 C4 -3.7(12) . . . . ?
C17 C8 C14 N1 175.7(7) . . . . ?
C1 C3 C15 C12 -2.2(14) . . . . ?
C1 C3 C15 C13 178.2(9) . . . . ?
C11 C12 C15 C3 1.9(12) . . . . ?
C11 C12 C15 C13 -178.5(7) . . . . ?
O24 C13 C15 C3 -166.7(8) . . . . ?
O20 C13 C15 C3 14.9(11) . . . . ?
O24 C13 C15 C12 13.7(10) . . . . ?
O20 C13 C15 C12 -164.7(7) . . . . ?
C7 C9 C16 C18 1.9(11) . . . . ?
C14 C8 C17 C21 0.3(11) . . . . ?
C5 C10 C18 C16 1.2(12) . . . . ?
C5 C10 C18 C20 -179.7(8) . . . . ?
C9 C16 C18 C10 -2.4(11) . . . . ?
C9 C16 C18 C20 178.4(7) . . . . ?
Mo1 O25 C19 O21 5.2(10) . . . . ?
Mo1 O25 C19 C21 -176.0(4) . . . . ?
Mo5 O21 C19 O25 -10.2(10) . . . . ?
Mo5 O21 C19 C21 171.1(4) . . . . ?
Mo4 O26 C20 O27 -7.0(10) . . . . ?
Mo4 O26 C20 C18 172.3(4) . . . . ?
Mo2 O27 C20 O26 3.9(10) . . . . ?
Mo2 O27 C20 C18 -175.4(4) . . . . ?
C10 C18 C20 O26 -173.0(7) . . . . ?
C16 C18 C20 O26 6.1(10) . . . . ?
C10 C18 C20 O27 6.3(10) . . . . ?
C16 C18 C20 O27 -174.6(6) . . . . ?
C4 C2 C21 C17 -4.6(13) . . . . ?
C4 C2 C21 C19 175.8(8) . . . . ?
C8 C17 C21 C2 3.8(11) . . . . ?
C8 C17 C21 C19 -176.6(6) . . . . ?
O25 C19 C21 C2 19.5(10) . . . . ?
O21 C19 C21 C2 -161.7(7) . . . . ?
O25 C19 C21 C17 -160.1(6) . . . . ?
O21 C19 C21 C17 18.7(9) . . . . ?
O3W Na1 Na1A Co1 -13.7(12) . . . . ?
OW7 Na1 Na1A Co1 115.4(4) 2_666 . . . ?
O13 Na1 Na1A Co1 43.6(2) . . . . ?
OW7 Na1 Na1A Co1 -177.9(10) 1_455 . . . ?
O23 Na1 Na1A Co1 -46.6(2) 2_666 . . . ?
Co1 Na1 Na1A OW7 -115.4(4) . . . 2_666 ?
O3W Na1 Na1A OW7 -129.1(10) . . . 2_666 ?
O13 Na1 Na1A OW7 -71.8(3) . . . 2_666 ?
OW7 Na1 Na1A OW7 66.7(12) 1_455 . . 2_666 ?
O23 Na1 Na1A OW7 -162.1(5) 2_666 . . 2_666 ?
Co1 Na1 Na1A O3W 13.7(12) . . . . ?
OW7 Na1 Na1A O3W 129.1(10) 2_666 . . . ?
O13 Na1 Na1A O3W 57.3(10) . . . . ?
OW7 Na1 Na1A O3W -164(2) 1_455 . . . ?
O23 Na1 Na1A O3W -33.0(13) 2_666 . . . ?
Co1 Na1 Na1A O2W -14.6(10) . . . . ?
O3W Na1 Na1A O2W -28(2) . . . . ?
OW7 Na1 Na1A O2W 100.8(11) 2_666 . . . ?
O13 Na1 Na1A O2W 29.0(11) . . . . ?
OW7 Na1 Na1A O2W 167.5(6) 1_455 . . . ?
O23 Na1 Na1A O2W -61.2(10) 2_666 . . . ?
Co1 Na1 Na1A O23 46.6(2) . . . 2_666 ?
O3W Na1 Na1A O23 33.0(13) . . . 2_666 ?
OW7 Na1 Na1A O23 162.1(5) 2_666 . . 2_666 ?
O13 Na1 Na1A O23 90.3(3) . . . 2_666 ?
OW7 Na1 Na1A O23 -131.2(10) 1_455 . . 2_666 ?

_refine_diff_density_max         1.863
_refine_diff_density_min         -1.712
_refine_diff_density_rms         0.169

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_7
_database_code_depnum_ccdc_archive 'CCDC 1871477'
_audit_update_record             
;
2018-10-08 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H75 Cs4 K Mo12 N6 O72 Te2 Zn'
_chemical_formula_weight         3858.69

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.6855(4)
_cell_length_b                   12.3860(6)
_cell_length_c                   18.6191(8)
_cell_angle_alpha                74.699(3)
_cell_angle_beta                 85.651(3)
_cell_angle_gamma                83.954(3)
_cell_volume                     2581.64(19)
_cell_formula_units_Z            1
_cell_measurement_temperature    220(2)
_cell_measurement_reflns_used    20806
_cell_measurement_theta_min      1.755
_cell_measurement_theta_max      25.00

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.482
_exptl_crystal_F_000             1821
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.22
_exptl_absorpt_coefficient_mu    3.724
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.410
_exptl_absorpt_correction_T_max  0.441
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            20806
_diffrn_reflns_av_unetI/netI     0.0650
_diffrn_reflns_av_R_equivalents  0.0476
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         1.755
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.956
_diffrn_measured_fraction_theta_full 0.930
_diffrn_reflns_Laue_measured_fraction_max 0.956
_diffrn_reflns_Laue_measured_fraction_full 0.930
_diffrn_reflns_point_group_measured_fraction_max 0.956
_diffrn_reflns_point_group_measured_fraction_full 0.930
_reflns_number_total             8686
_reflns_number_gt                7206
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0638P)²+26.7537P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8686
_refine_ls_number_parameters     675
_refine_ls_number_restraints     444
_refine_ls_R_factor_all          0.0619
_refine_ls_R_factor_gt           0.0508
_refine_ls_wR_factor_ref         0.1420
_refine_ls_wR_factor_gt          0.1340
_refine_ls_goodness_of_fit_ref   1.053
_refine_ls_restrained_S_all      1.046
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.11252(6) -0.34066(7) 0.22072(4) 0.01855(19) Uani 1 1 d . U . . .
Mo2 Mo -0.19293(7) -0.22348(7) 0.46915(4) 0.01853(19) Uani 1 1 d . U . . .
Mo3 Mo -0.42239(6) -0.30719(7) 0.40975(4) 0.01845(19) Uani 1 1 d . U . . .
Mo4 Mo -0.39370(6) -0.41314(6) 0.24422(4) 0.01652(19) Uani 1 1 d . U . . .
Mo5 Mo -0.13592(7) -0.44318(7) 0.15754(4) 0.0198(2) Uani 1 1 d . U . . .
Mo6 Mo 0.08700(7) -0.23412(7) 0.36748(5) 0.0219(2) Uani 1 1 d . U . . .
Te1 Te -0.17538(5) -0.25371(5) 0.28002(3) 0.01607(15) Uani 1 1 d . U . . .
Zn1 Zn 0.1876(2) -0.0045(2) 0.43218(16) 0.0391(6) Uani 0.5 1 d . U P . .
Cs1 Cs 0.33263(5) -0.49914(6) 0.38532(4) 0.02995(18) Uani 1 1 d . U . . .
Cs2 Cs -0.08250(7) -0.54846(7) 0.40160(4) 0.0447(2) Uani 1 1 d . U . . .
K1 K 0.3567(9) -0.0264(10) 0.4122(8) 0.023(2) Uani 0.2 1 d . U P . .
K1A K 0.3582(7) -0.0459(7) 0.4533(6) 0.0313(19) Uani 0.3 1 d . U P . .
O1 O -0.5267(5) -0.4073(6) 0.2101(4) 0.0263(15) Uani 1 1 d . U . . .
O2 O -0.1378(6) -0.3526(6) 0.5194(4) 0.0275(15) Uani 1 1 d . U . . .
O3 O -0.3853(6) -0.5375(6) 0.3115(4) 0.0277(16) Uani 1 1 d . U . . .
O4 O 0.0468(6) -0.1605(5) 0.1753(4) 0.0279(16) Uani 1 1 d . U . . .
O5 O -0.0127(5) -0.3578(5) 0.1666(4) 0.0228(14) Uani 1 1 d . U . . .
O6 O -0.0606(5) -0.1815(5) 0.4045(4) 0.0216(14) Uani 1 1 d . U . . .
O7 O -0.3002(5) -0.4608(5) 0.1656(3) 0.0219(14) Uani 1 1 d . U . . .
O8 O -0.2346(5) -0.2950(5) 0.3777(3) 0.0171(13) Uani 1 1 d . U . . .
O9 O -0.0907(6) -0.5682(5) 0.2166(4) 0.0261(15) Uani 1 1 d . U . . .
O10 O -0.2109(5) -0.3841(5) 0.2573(3) 0.0177(13) Uani 1 1 d . U . . .
O11 O 0.2189(5) -0.3276(6) 0.1514(4) 0.0299(16) Uani 1 1 d . U . . .
O12 O -0.3721(5) -0.2412(5) 0.1638(4) 0.0230(15) Uani 1 1 d . U . . .
O13 O 0.1847(5) -0.2732(6) 0.2879(4) 0.0225(14) Uani 1 1 d . U . . .
O14 O 0.1357(5) -0.4768(5) 0.2719(4) 0.0257(15) Uani 1 1 d . U . . .
O15 O -0.2038(5) -0.2652(6) 0.1014(4) 0.0269(15) Uani 1 1 d . U . . .
O16 O -0.2648(6) -0.0673(6) 0.3839(4) 0.0295(16) Uani 1 1 d . U . . .
O17 O -0.1047(6) -0.4649(7) 0.0702(4) 0.0363(18) Uani 1 1 d . U . . .
O18 O -0.4265(5) -0.3133(5) 0.3080(3) 0.0192(13) Uani 1 1 d . U . . .
O19 O 0.1729(6) -0.1495(7) 0.3952(5) 0.0392(19) Uani 1 1 d . U . . .
O20 O -0.4207(6) -0.1249(5) 0.3464(4) 0.0278(16) Uani 1 1 d . U . . .
O21 O -0.1928(6) -0.1374(6) 0.5284(4) 0.0307(16) Uani 1 1 d . U . . .
O22 O 0.0349(6) -0.0818(6) 0.2713(4) 0.0299(16) Uani 1 1 d . U . . .
O23 O -0.0251(5) -0.3110(5) 0.3052(3) 0.0182(13) Uani 1 1 d . U . . .
O24 O -0.3537(5) -0.2525(6) 0.4838(3) 0.0230(14) Uani 1 1 d . U . . .
O25 O -0.3975(6) -0.4483(6) 0.4491(4) 0.0256(15) Uani 1 1 d . U . . .
O26 O -0.5661(6) -0.2783(6) 0.4299(4) 0.0335(17) Uani 1 1 d . U . . .
O27 O 0.1055(6) -0.3609(6) 0.4318(4) 0.0298(16) Uani 1 1 d . U . . .
C1 C -0.0351(12) 0.2363(11) 0.1192(7) 0.051(3) Uani 1 1 d . U . . .
H1A H -0.0309 0.3035 0.1319 0.061 Uiso 1 1 calc R U . . .
C2 C -0.2929(9) 0.0368(10) -0.0570(7) 0.045(3) Uani 1 1 d . U . . .
H2A H -0.2581 0.0548 -0.1047 0.054 Uiso 1 1 calc R U . . .
C3 C -0.0712(11) 0.2376(9) 0.0515(6) 0.039(3) Uani 1 1 d . U . . .
C4 C -0.4095(9) 0.2662(9) 0.1864(6) 0.030(2) Uani 1 1 d . U . . .
C5 C -0.2648(10) -0.0644(11) -0.0088(7) 0.048(3) Uani 1 1 d . U . . .
H5A H -0.2076 -0.1140 -0.0229 0.057 Uiso 1 1 calc R U . . .
C6 C -0.3118(9) 0.2419(10) 0.2241(7) 0.039(3) Uani 1 1 d . U . . .
H6A H -0.2580 0.2946 0.2161 0.047 Uiso 1 1 calc R U . . .
C7 C -0.0042(12) 0.1345(10) 0.1697(7) 0.046(3) Uani 1 1 d . U . . .
H7A H 0.0186 0.1340 0.2166 0.055 Uiso 1 1 calc R U . . .
C8 C -0.0455(10) 0.0391(10) 0.0819(6) 0.036(3) Uani 1 1 d . U . . .
H8A H -0.0507 -0.0273 0.0684 0.043 Uiso 1 1 calc R U . . .
C9 C -0.3735(9) 0.1127(10) -0.0346(6) 0.036(3) Uani 1 1 d . U . . .
C10 C -0.3514(8) -0.0519(8) 0.3435(6) 0.025(2) Uani 1 1 d . U . . .
C11 C -0.4888(9) 0.1872(9) 0.1978(6) 0.032(2) Uani 1 1 d . U . . .
H11A H -0.5553 0.2036 0.1711 0.039 Uiso 1 1 calc R U . . .
C12 C -0.0072(9) 0.0335(8) 0.1509(6) 0.029(2) Uani 1 1 d . U . . .
C13 C -0.4700(9) 0.0853(9) 0.2480(6) 0.033(2) Uani 1 1 d . U . . .
H13A H -0.5244 0.0332 0.2552 0.040 Uiso 1 1 calc R U . . .
C14 C -0.4244(10) 0.0882(9) 0.0346(6) 0.035(3) Uani 1 1 d . U . . .
H14A H -0.4768 0.1407 0.0498 0.041 Uiso 1 1 calc R U . . .
C15 C -0.0766(10) 0.1403(10) 0.0317(6) 0.039(3) Uani 1 1 d . U . . .
H15A H -0.1009 0.1418 -0.0150 0.047 Uiso 1 1 calc R U . . .
C16 C 0.0290(8) -0.0780(8) 0.2033(6) 0.026(2) Uani 1 1 d . U . . .
C17 C -0.2920(9) 0.1388(9) 0.2743(6) 0.037(3) Uani 1 1 d . U . . .
H17A H -0.2239 0.1230 0.2993 0.044 Uiso 1 1 calc R U . . .
C18 C -0.3700(8) 0.0576(8) 0.2888(5) 0.023(2) Uani 1 1 d . U . . .
C19 C -0.3978(9) -0.0162(8) 0.0827(6) 0.027(2) Uani 1 1 d . U . . .
H19A H -0.4325 -0.0337 0.1305 0.032 Uiso 1 1 calc R U . . .
C20 C -0.2959(8) -0.2085(8) 0.1120(5) 0.023(2) Uani 1 1 d . U . . .
C21 C -0.3204(8) -0.0941(8) 0.0605(5) 0.024(2) Uani 1 1 d . U . . .
N1 N -0.4066(8) 0.2195(8) -0.0871(6) 0.046(3) Uani 1 1 d . U . . .
H1B H -0.4582 0.2663 -0.0740 0.055 Uiso 1 1 calc R U . . .
H1C H -0.3745 0.2357 -0.1313 0.055 Uiso 1 1 calc R U . . .
N2 N -0.1030(10) 0.3420(8) 0.0001(6) 0.054(3) Uani 1 1 d . U . . .
H2B H -0.0992 0.4039 0.0120 0.065 Uiso 1 1 calc R U . . .
H2C H -0.1259 0.3430 -0.0429 0.065 Uiso 1 1 calc R U . . .
N3 N -0.4324(9) 0.3729(8) 0.1340(5) 0.041(2) Uani 1 1 d . U . . .
H3A H -0.3835 0.4225 0.1262 0.050 Uiso 1 1 calc R U . . .
H3B H -0.4950 0.3872 0.1105 0.050 Uiso 1 1 calc R U . . .
O2W O 0.229(2) -0.0985(17) 0.5387(12) 0.075(6) Uani 0.5 1 d . U P . .
OW1 O 0.3066(18) -0.7002(18) 0.3084(12) 0.070(6) Uiso 0.5 1 d . . P . .
OW2 O 0.3142(11) 0.4317(10) 0.1523(8) 0.094(4) Uani 1 1 d . U . . .
OW3 O -0.2961(10) -0.6968(10) 0.4341(6) 0.087(4) Uani 1 1 d . U . . .
OW4 O -0.3793(6) 0.1554(7) 0.7666(5) 0.046(2) Uani 1 1 d . U . . .
OW5 O 0.2363(18) 0.285(2) 0.0843(13) 0.084(7) Uani 0.5 1 d . U P . .
OW6 O 0.0393(16) -0.7320(13) 0.3227(9) 0.051(5) Uani 0.5 1 d . U P . .
OW7 O 0.4856(13) 0.1378(14) 0.4285(9) 0.044(4) Uani 0.5 1 d . U P . .
OW8 O 0.5913(11) 0.6504(10) 0.0260(7) 0.092(4) Uani 1 1 d . U . . .
OW9 O 0.3315(11) 0.6205(10) 0.0073(6) 0.088(4) Uani 1 1 d . U . . .
O1WA O -0.0431(15) 0.0535(15) 0.4419(10) 0.050(4) Uiso 0.5 1 d . . P . .
OW10 O -0.7380(19) 0.0642(19) 0.2073(15) 0.084(7) Uani 0.5 1 d . U P . .
O1W O 0.013(2) 0.0462(18) 0.3923(14) 0.082(6) Uani 0.5 1 d . U P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O14 1.708(7) . ?
Mo1 O11 1.711(7) . ?
Mo1 O5 1.899(6) . ?
Mo1 O13 1.958(6) . ?
Mo1 O23 2.234(6) . ?
Mo1 O4 2.242(7) . ?
Mo1 Mo6 3.3158(11) . ?
Mo2 O2 1.712(7) . ?
Mo2 O21 1.725(7) . ?
Mo2 O6 1.914(6) . ?
Mo2 O24 1.935(6) . ?
Mo2 O8 2.222(6) . ?
Mo2 O16 2.282(7) . ?
Mo2 Mo3 3.3360(11) . ?
Mo2 K1A 4.208(7) 2_556 ?
Mo3 O25 1.711(7) . ?
Mo3 O26 1.714(6) . ?
Mo3 O18 1.920(6) . ?
Mo3 O24 1.944(6) . ?
Mo3 O8 2.240(6) . ?
Mo3 O20 2.257(7) . ?
Mo3 K1 4.115(11) 1_455 ?
Mo3 K1A 4.127(7) 1_455 ?
Mo4 O3 1.709(7) . ?
Mo4 O1 1.710(6) . ?
Mo4 O18 1.921(6) . ?
Mo4 O7 1.939(6) . ?
Mo4 O10 2.245(6) . ?
Mo4 O12 2.283(6) . ?
Mo4 Mo5 3.3407(11) . ?
Mo5 O9 1.704(7) . ?
Mo5 O17 1.723(7) . ?
Mo5 O5 1.916(6) . ?
Mo5 O7 1.946(6) . ?
Mo5 O10 2.256(6) . ?
Mo5 O15 2.264(6) . ?
Mo6 O27 1.709(7) . ?
Mo6 O19 1.721(7) . ?
Mo6 O6 1.923(6) . ?
Mo6 O13 1.934(6) . ?
Mo6 O23 2.246(6) . ?
Mo6 O22 2.297(7) . ?
Te1 O8 1.855(6) . ?
Te1 O10 1.867(6) . ?
Te1 O23 1.869(6) . ?
Zn1 K1 1.986(11) . ?
Zn1 K1A 2.048(9) . ?
Zn1 O2W 2.08(2) . ?
Zn1 O21 2.083(7) 2_556 ?
Zn1 O19 2.112(8) . ?
Zn1 O1W 2.19(3) . ?
K1 K1A 0.741(12) . ?
K1 O2W 2.68(3) . ?
K1 OW7 2.746(18) . ?
K1 O19 2.842(14) . ?
K1 O21 3.009(13) 2_556 ?
K1 O20 3.065(13) 1_655 ?
K1 O26 3.093(14) 1_655 ?
K1 Mo3 4.115(11) 1_655 ?
K1 K1A 4.610(15) 2_656 ?
K1A O2W 2.13(3) . ?
K1A OW7 2.767(17) . ?
K1A OW7 2.88(2) 2_656 ?
K1A O21 2.896(10) 2_556 ?
K1A O19 3.030(11) . ?
K1A O26 3.055(10) 1_655 ?
K1A O20 3.363(11) 1_655 ?
K1A OW3 3.437(15) 2_546 ?
K1A Mo3 4.127(7) 1_655 ?
K1A Mo2 4.208(7) 2_556 ?
O4 C16 1.257(12) . ?
O12 C20 1.276(11) . ?
O15 C20 1.254(11) . ?
O16 C10 1.274(12) . ?
O20 C10 1.264(12) . ?
O20 K1 3.065(13) 1_455 ?
O20 K1A 3.363(11) 1_455 ?
O21 Zn1 2.083(7) 2_556 ?
O21 K1A 2.896(10) 2_556 ?
O21 K1 3.008(13) 2_556 ?
O22 C16 1.261(12) . ?
O26 K1A 3.055(10) 1_455 ?
O26 K1 3.093(14) 1_455 ?
C1 C3 1.355(17) . ?
C1 C7 1.391(17) . ?
C1 H1A 0.9300 . ?
C2 C5 1.360(16) . ?
C2 C9 1.381(17) . ?
C2 H2A 0.9300 . ?
C3 C15 1.358(16) . ?
C3 N2 1.423(14) . ?
C4 C6 1.350(15) . ?
C4 C11 1.383(15) . ?
C4 N3 1.432(13) . ?
C5 C21 1.377(15) . ?
C5 H5A 0.9300 . ?
C6 C17 1.378(15) . ?
C6 H6A 0.9300 . ?
C7 C12 1.390(15) . ?
C7 H7A 0.9300 . ?
C8 C12 1.374(15) . ?
C8 C15 1.383(16) . ?
C8 H8A 0.9300 . ?
C9 C14 1.349(16) . ?
C9 N1 1.457(13) . ?
C10 C18 1.472(14) . ?
C11 C13 1.366(15) . ?
C11 H11A 0.9300 . ?
C12 C16 1.506(14) . ?
C13 C18 1.405(14) . ?
C13 H13A 0.9300 . ?
C14 C19 1.384(14) . ?
C14 H14A 0.9300 . ?
C15 H15A 0.9300 . ?
C17 C18 1.388(14) . ?
C17 H17A 0.9300 . ?
C19 C21 1.375(14) . ?
C19 H19A 0.9300 . ?
C20 C21 1.499(13) . ?
N1 H1B 0.8600 . ?
N1 H1C 0.8600 . ?
N2 H2B 0.8600 . ?
N2 H2C 0.8600 . ?
N3 H3A 0.8600 . ?
N3 H3B 0.8600 . ?
OW3 K1A 3.437(15) 2_546 ?
OW7 K1A 2.88(2) 2_656 ?
O1WA O1W 1.11(2) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O14 Mo1 O11 103.9(3) . . ?
O14 Mo1 O5 98.4(3) . . ?
O11 Mo1 O5 99.3(3) . . ?
O14 Mo1 O13 96.4(3) . . ?
O11 Mo1 O13 98.6(3) . . ?
O5 Mo1 O13 153.1(3) . . ?
O14 Mo1 O23 89.3(3) . . ?
O11 Mo1 O23 165.6(3) . . ?
O5 Mo1 O23 84.2(2) . . ?
O13 Mo1 O23 73.7(2) . . ?
O14 Mo1 O4 165.7(3) . . ?
O11 Mo1 O4 90.3(3) . . ?
O5 Mo1 O4 79.4(3) . . ?
O13 Mo1 O4 80.7(3) . . ?
O23 Mo1 O4 76.5(2) . . ?
O14 Mo1 Mo6 94.7(2) . . ?
O11 Mo1 Mo6 128.9(2) . . ?
O5 Mo1 Mo6 124.67(19) . . ?
O13 Mo1 Mo6 31.36(17) . . ?
O23 Mo1 Mo6 42.39(15) . . ?
O4 Mo1 Mo6 75.52(17) . . ?
O2 Mo2 O21 104.7(3) . . ?
O2 Mo2 O6 98.8(3) . . ?
O21 Mo2 O6 101.5(3) . . ?
O2 Mo2 O24 97.1(3) . . ?
O21 Mo2 O24 98.3(3) . . ?
O6 Mo2 O24 150.6(3) . . ?
O2 Mo2 O8 91.3(3) . . ?
O21 Mo2 O8 162.6(3) . . ?
O6 Mo2 O8 82.5(2) . . ?
O24 Mo2 O8 72.5(2) . . ?
O2 Mo2 O16 169.1(3) . . ?
O21 Mo2 O16 86.2(3) . . ?
O6 Mo2 O16 77.5(3) . . ?
O24 Mo2 O16 82.2(3) . . ?
O8 Mo2 O16 78.1(2) . . ?
O2 Mo2 Mo3 97.6(2) . . ?
O21 Mo2 Mo3 127.1(2) . . ?
O6 Mo2 Mo3 121.93(19) . . ?
O24 Mo2 Mo3 30.78(18) . . ?
O8 Mo2 Mo3 41.82(15) . . ?
O16 Mo2 Mo3 76.23(17) . . ?
O2 Mo2 K1A 128.9(3) . 2_556 ?
O21 Mo2 K1A 32.1(3) . 2_556 ?
O6 Mo2 K1A 112.4(2) . 2_556 ?
O24 Mo2 K1A 75.1(2) . 2_556 ?
O8 Mo2 K1A 130.8(2) . 2_556 ?
O16 Mo2 K1A 61.6(2) . 2_556 ?
Mo3 Mo2 K1A 98.64(13) . 2_556 ?
O25 Mo3 O26 104.0(3) . . ?
O25 Mo3 O18 97.8(3) . . ?
O26 Mo3 O18 100.3(3) . . ?
O25 Mo3 O24 98.6(3) . . ?
O26 Mo3 O24 101.0(3) . . ?
O18 Mo3 O24 149.0(3) . . ?
O25 Mo3 O8 90.7(3) . . ?
O26 Mo3 O8 164.7(3) . . ?
O18 Mo3 O8 81.7(2) . . ?
O24 Mo3 O8 71.9(2) . . ?
O25 Mo3 O20 168.7(3) . . ?
O26 Mo3 O20 87.1(3) . . ?
O18 Mo3 O20 77.4(3) . . ?
O24 Mo3 O20 81.5(3) . . ?
O8 Mo3 O20 78.5(2) . . ?
O25 Mo3 Mo2 98.2(2) . . ?
O26 Mo3 Mo2 129.8(2) . . ?
O18 Mo3 Mo2 120.59(19) . . ?
O24 Mo3 Mo2 30.62(18) . . ?
O8 Mo3 Mo2 41.41(15) . . ?
O20 Mo3 Mo2 75.95(17) . . ?
O25 Mo3 K1 144.2(3) . 1_455 ?
O26 Mo3 K1 43.1(3) . 1_455 ?
O18 Mo3 K1 101.6(3) . 1_455 ?
O24 Mo3 K1 79.5(3) . 1_455 ?
O8 Mo3 K1 121.6(2) . 1_455 ?
O20 Mo3 K1 47.1(2) . 1_455 ?
Mo2 Mo3 K1 97.31(16) . 1_455 ?
O25 Mo3 K1A 136.4(3) . 1_455 ?
O26 Mo3 K1A 41.3(3) . 1_455 ?
O18 Mo3 K1A 111.7(2) . 1_455 ?
O24 Mo3 K1A 72.2(2) . 1_455 ?
O8 Mo3 K1A 123.8(2) . 1_455 ?
O20 Mo3 K1A 54.5(2) . 1_455 ?
Mo2 Mo3 K1A 93.62(13) . 1_455 ?
K1 Mo3 K1A 10.31(16) 1_455 1_455 ?
O3 Mo4 O1 103.4(3) . . ?
O3 Mo4 O18 98.5(3) . . ?
O1 Mo4 O18 100.2(3) . . ?
O3 Mo4 O7 98.8(3) . . ?
O1 Mo4 O7 98.9(3) . . ?
O18 Mo4 O7 150.5(3) . . ?
O3 Mo4 O10 92.4(3) . . ?
O1 Mo4 O10 163.3(3) . . ?
O18 Mo4 O10 82.6(2) . . ?
O7 Mo4 O10 72.9(2) . . ?
O3 Mo4 O12 168.6(3) . . ?
O1 Mo4 O12 87.8(3) . . ?
O18 Mo4 O12 77.5(2) . . ?
O7 Mo4 O12 81.0(2) . . ?
O10 Mo4 O12 76.6(2) . . ?
O3 Mo4 Mo5 98.4(2) . . ?
O1 Mo4 Mo5 128.0(2) . . ?
O18 Mo4 Mo5 122.51(18) . . ?
O7 Mo4 Mo5 30.74(18) . . ?
O10 Mo4 Mo5 42.21(15) . . ?
O12 Mo4 Mo5 75.45(15) . . ?
O9 Mo5 O17 103.8(3) . . ?
O9 Mo5 O5 98.9(3) . . ?
O17 Mo5 O5 101.7(3) . . ?
O9 Mo5 O7 98.5(3) . . ?
O17 Mo5 O7 98.9(3) . . ?
O5 Mo5 O7 149.0(3) . . ?
O9 Mo5 O10 88.8(3) . . ?
O17 Mo5 O10 165.9(3) . . ?
O5 Mo5 O10 82.3(2) . . ?
O7 Mo5 O10 72.6(2) . . ?
O9 Mo5 O15 168.0(3) . . ?
O17 Mo5 O15 88.2(3) . . ?
O5 Mo5 O15 77.5(3) . . ?
O7 Mo5 O15 80.2(3) . . ?
O10 Mo5 O15 79.4(2) . . ?
O9 Mo5 Mo4 96.3(2) . . ?
O17 Mo5 Mo4 128.5(2) . . ?
O5 Mo5 Mo4 121.54(19) . . ?
O7 Mo5 Mo4 30.63(18) . . ?
O10 Mo5 Mo4 41.95(15) . . ?
O15 Mo5 Mo4 76.47(17) . . ?
O27 Mo6 O19 104.5(4) . . ?
O27 Mo6 O6 98.7(3) . . ?
O19 Mo6 O6 99.6(3) . . ?
O27 Mo6 O13 97.4(3) . . ?
O19 Mo6 O13 100.3(3) . . ?
O6 Mo6 O13 150.3(3) . . ?
O27 Mo6 O23 89.1(3) . . ?
O19 Mo6 O23 165.9(3) . . ?
O6 Mo6 O23 81.6(2) . . ?
O13 Mo6 O23 73.9(2) . . ?
O27 Mo6 O22 168.0(3) . . ?
O19 Mo6 O22 87.5(3) . . ?
O6 Mo6 O22 78.3(3) . . ?
O13 Mo6 O22 80.8(3) . . ?
O23 Mo6 O22 79.0(2) . . ?
O27 Mo6 Mo1 95.2(2) . . ?
O19 Mo6 Mo1 130.9(3) . . ?
O6 Mo6 Mo1 121.56(18) . . ?
O13 Mo6 Mo1 31.79(17) . . ?
O23 Mo6 Mo1 42.13(15) . . ?
O22 Mo6 Mo1 76.98(17) . . ?
O8 Te1 O10 94.4(3) . . ?
O8 Te1 O23 93.8(3) . . ?
O10 Te1 O23 94.0(3) . . ?
K1 Zn1 K1A 21.1(3) . . ?
K1 Zn1 O2W 82.5(8) . . ?
K1A Zn1 O2W 61.9(7) . . ?
K1 Zn1 O21 95.3(4) . 2_556 ?
K1A Zn1 O21 89.0(3) . 2_556 ?
O2W Zn1 O21 86.6(6) . 2_556 ?
K1 Zn1 O19 87.7(4) . . ?
K1A Zn1 O19 93.5(3) . . ?
O2W Zn1 O19 92.7(6) . . ?
O21 Zn1 O19 176.8(3) 2_556 . ?
K1 Zn1 O1W 150.6(8) . . ?
K1A Zn1 O1W 171.6(7) . . ?
O2W Zn1 O1W 126.1(10) . . ?
O21 Zn1 O1W 93.5(5) 2_556 . ?
O19 Zn1 O1W 84.3(5) . . ?
K1A K1 Zn1 84.1(13) . . ?
K1A K1 O2W 35.7(12) . . ?
Zn1 K1 O2W 50.3(6) . . ?
K1A K1 OW7 83.9(13) . . ?
Zn1 K1 OW7 117.0(6) . . ?
O2W K1 OW7 108.8(7) . . ?
K1A K1 O19 97.5(14) . . ?
Zn1 K1 O19 48.0(3) . . ?
O2W K1 O19 66.6(6) . . ?
OW7 K1 O19 164.2(6) . . ?
K1A K1 O21 74.2(11) . 2_556 ?
Zn1 K1 O21 43.6(3) . 2_556 ?
O2W K1 O21 60.0(5) . 2_556 ?
OW7 K1 O21 73.6(4) . 2_556 ?
O19 K1 O21 91.5(4) . 2_556 ?
K1A K1 O20 107.5(13) . 1_655 ?
Zn1 K1 O20 155.7(6) . 1_655 ?
O2W K1 O20 132.8(7) . 1_655 ?
OW7 K1 O20 85.9(4) . 1_655 ?
O19 K1 O20 108.4(4) . 1_655 ?
O21 K1 O20 159.3(5) 2_556 1_655 ?
K1A K1 O26 80.1(12) . 1_655 ?
Zn1 K1 O26 110.4(5) . 1_655 ?
O2W K1 O26 85.0(6) . 1_655 ?
OW7 K1 O26 127.8(5) . 1_655 ?
O19 K1 O26 67.8(3) . 1_655 ?
O21 K1 O26 144.5(5) 2_556 1_655 ?
O20 K1 O26 53.3(3) 1_655 1_655 ?
K1A K1 Mo3 85.7(12) . 1_655 ?
Zn1 K1 Mo3 132.6(5) . 1_655 ?
O2W K1 Mo3 101.6(6) . 1_655 ?
OW7 K1 Mo3 107.7(4) . 1_655 ?
O19 K1 Mo3 88.1(3) . 1_655 ?
O21 K1 Mo3 159.7(5) 2_556 1_655 ?
O20 K1 Mo3 32.66(17) 1_655 1_655 ?
O26 K1 Mo3 22.24(15) 1_655 1_655 ?
K1A K1 K1A 56.2(13) . 2_656 ?
Zn1 K1 K1A 127.0(5) . 2_656 ?
O2W K1 K1A 90.1(6) . 2_656 ?
OW7 K1 K1A 36.0(4) . 2_656 ?
O19 K1 K1A 152.4(5) . 2_656 ?
O21 K1 K1A 88.9(3) 2_556 2_656 ?
O20 K1 K1A 76.0(3) 1_655 2_656 ?
O26 K1 K1A 96.9(3) 1_655 2_656 ?
Mo3 K1 K1A 82.2(2) 1_655 2_656 ?
K1 K1A Zn1 74.8(12) . . ?
K1 K1A O2W 132.6(15) . . ?
Zn1 K1A O2W 59.9(7) . . ?
K1 K1A OW7 80.7(13) . . ?
Zn1 K1A OW7 113.9(5) . . ?
O2W K1A OW7 128.4(7) . . ?
K1 K1A OW7 142.0(13) . 2_656 ?
Zn1 K1A OW7 143.1(5) . 2_656 ?
O2W K1A OW7 83.8(8) . 2_656 ?
OW7 K1A OW7 82.7(6) . 2_656 ?
K1 K1A O21 91.5(12) . 2_556 ?
Zn1 K1A O21 46.0(2) . 2_556 ?
O2W K1A O21 67.4(6) . 2_556 ?
OW7 K1A O21 75.1(4) . 2_556 ?
OW7 K1A O21 116.7(4) 2_656 2_556 ?
K1 K1A O19 68.4(12) . . ?
Zn1 K1A O19 44.1(2) . . ?
O2W K1A O19 69.7(6) . . ?
OW7 K1A O19 145.4(6) . . ?
OW7 K1A O19 131.5(5) 2_656 . ?
O21 K1A O19 90.1(3) 2_556 . ?
K1 K1A O26 86.1(12) . 1_655 ?
Zn1 K1A O26 110.0(4) . 1_655 ?
O2W K1A O26 96.4(6) . 1_655 ?
OW7 K1A O26 128.5(4) . 1_655 ?
OW7 K1A O26 78.1(4) 2_656 1_655 ?
O21 K1A O26 155.2(4) 2_556 1_655 ?
O19 K1A O26 66.0(3) . 1_655 ?
K1 K1A O20 60.3(11) . 1_655 ?
Zn1 K1A O20 130.5(4) . 1_655 ?
O2W K1A O20 146.6(6) . 1_655 ?
OW7 K1A O20 80.0(4) . 1_655 ?
OW7 K1A O20 83.3(3) 2_656 1_655 ?
O21 K1A O20 145.2(4) 2_556 1_655 ?
O19 K1A O20 97.0(3) . 1_655 ?
O26 K1A O20 50.7(2) 1_655 1_655 ?
K1 K1A OW3 127.7(13) . 2_546 ?
Zn1 K1A OW3 90.5(4) . 2_546 ?
O2W K1A OW3 46.4(6) . 2_546 ?
OW7 K1A OW3 148.0(6) . 2_546 ?
OW7 K1A OW3 65.7(4) 2_656 2_546 ?
O21 K1A OW3 113.7(4) 2_556 2_546 ?
O19 K1A OW3 66.6(3) . 2_546 ?
O26 K1A OW3 51.9(3) 1_655 2_546 ?
O20 K1A OW3 100.3(3) 1_655 2_546 ?
K1 K1A Mo3 84.0(12) . 1_655 ?
Zn1 K1A Mo3 129.4(3) . 1_655 ?
O2W K1A Mo3 113.7(6) . 1_655 ?
OW7 K1A Mo3 107.0(4) . 1_655 ?
OW7 K1A Mo3 68.7(3) 2_656 1_655 ?
O21 K1A Mo3 174.6(4) 2_556 1_655 ?
O19 K1A Mo3 85.4(2) . 1_655 ?
O26 K1A Mo3 21.72(14) 1_655 1_655 ?
O20 K1A Mo3 33.12(13) 1_655 1_655 ?
OW3 K1A Mo3 67.2(2) 2_546 1_655 ?
K1 K1A Mo2 104.8(12) . 2_556 ?
Zn1 K1A Mo2 63.3(2) . 2_556 ?
O2W K1A Mo2 67.7(5) . 2_556 ?
OW7 K1A Mo2 65.7(3) . 2_556 ?
OW7 K1A Mo2 99.0(3) 2_656 2_556 ?
O21 K1A Mo2 18.47(15) 2_556 2_556 ?
O19 K1A Mo2 106.8(3) . 2_556 ?
O26 K1A Mo2 164.2(3) 1_655 2_556 ?
O20 K1A Mo2 144.9(3) 1_655 2_556 ?
OW3 K1A Mo2 112.6(3) 2_546 2_556 ?
Mo3 K1A Mo2 166.9(3) 1_655 2_556 ?
C16 O4 Mo1 133.2(7) . . ?
Mo1 O5 Mo5 148.9(4) . . ?
Mo2 O6 Mo6 145.2(4) . . ?
Mo4 O7 Mo5 118.6(3) . . ?
Te1 O8 Mo2 125.4(3) . . ?
Te1 O8 Mo3 124.0(3) . . ?
Mo2 O8 Mo3 96.8(2) . . ?
Te1 O10 Mo4 121.2(3) . . ?
Te1 O10 Mo5 124.6(3) . . ?
Mo4 O10 Mo5 95.8(2) . . ?
C20 O12 Mo4 131.2(6) . . ?
Mo6 O13 Mo1 116.8(3) . . ?
C20 O15 Mo5 131.5(6) . . ?
C10 O16 Mo2 130.7(6) . . ?
Mo3 O18 Mo4 142.3(3) . . ?
Mo6 O19 Zn1 148.9(4) . . ?
Mo6 O19 K1 164.7(5) . . ?
Zn1 O19 K1 44.3(3) . . ?
Mo6 O19 K1A 167.8(4) . . ?
Zn1 O19 K1A 42.4(2) . . ?
K1 O19 K1A 14.0(3) . . ?
C10 O20 Mo3 132.5(6) . . ?
C10 O20 K1 102.7(6) . 1_455 ?
Mo3 O20 K1 100.2(3) . 1_455 ?
C10 O20 K1A 101.9(6) . 1_455 ?
Mo3 O20 K1A 92.4(3) . 1_455 ?
K1 O20 K1A 12.1(2) 1_455 1_455 ?
Mo2 O21 Zn1 161.8(4) . 2_556 ?
Mo2 O21 K1A 129.4(4) . 2_556 ?
Zn1 O21 K1A 45.0(2) 2_556 2_556 ?
Mo2 O21 K1 138.9(4) . 2_556 ?
Zn1 O21 K1 41.1(3) 2_556 2_556 ?
K1A O21 K1 14.2(2) 2_556 2_556 ?
C16 O22 Mo6 128.3(6) . . ?
Te1 O23 Mo1 122.7(3) . . ?
Te1 O23 Mo6 124.0(3) . . ?
Mo1 O23 Mo6 95.5(2) . . ?
Mo2 O24 Mo3 118.6(3) . . ?
Mo3 O26 K1A 117.0(4) . 1_455 ?
Mo3 O26 K1 114.7(4) . 1_455 ?
K1A O26 K1 13.8(2) 1_455 1_455 ?
C3 C1 C7 120.0(11) . . ?
C3 C1 H1A 120.0 . . ?
C7 C1 H1A 120.0 . . ?
C5 C2 C9 119.5(11) . . ?
C5 C2 H2A 120.2 . . ?
C9 C2 H2A 120.2 . . ?
C1 C3 C15 120.8(11) . . ?
C1 C3 N2 119.8(11) . . ?
C15 C3 N2 119.4(11) . . ?
C6 C4 C11 119.9(10) . . ?
C6 C4 N3 121.0(10) . . ?
C11 C4 N3 119.1(9) . . ?
C2 C5 C21 120.6(11) . . ?
C2 C5 H5A 119.7 . . ?
C21 C5 H5A 119.7 . . ?
C4 C6 C17 119.9(10) . . ?
C4 C6 H6A 120.1 . . ?
C17 C6 H6A 120.1 . . ?
C12 C7 C1 120.7(11) . . ?
C12 C7 H7A 119.7 . . ?
C1 C7 H7A 119.7 . . ?
C12 C8 C15 122.2(10) . . ?
C12 C8 H8A 118.9 . . ?
C15 C8 H8A 118.9 . . ?
C14 C9 C2 121.0(10) . . ?
C14 C9 N1 119.5(11) . . ?
C2 C9 N1 119.5(10) . . ?
O20 C10 O16 124.4(9) . . ?
O20 C10 C18 118.1(9) . . ?
O16 C10 C18 117.5(9) . . ?
C13 C11 C4 120.5(10) . . ?
C13 C11 H11A 119.8 . . ?
C4 C11 H11A 119.8 . . ?
C8 C12 C7 117.1(10) . . ?
C8 C12 C16 120.8(9) . . ?
C7 C12 C16 122.1(10) . . ?
C11 C13 C18 121.2(10) . . ?
C11 C13 H13A 119.4 . . ?
C18 C13 H13A 119.4 . . ?
C9 C14 C19 119.2(11) . . ?
C9 C14 H14A 120.4 . . ?
C19 C14 H14A 120.4 . . ?
C3 C15 C8 119.2(11) . . ?
C3 C15 H15A 120.4 . . ?
C8 C15 H15A 120.4 . . ?
O4 C16 O22 125.7(9) . . ?
O4 C16 C12 116.3(9) . . ?
O22 C16 C12 117.9(9) . . ?
C6 C17 C18 122.4(10) . . ?
C6 C17 H17A 118.8 . . ?
C18 C17 H17A 118.8 . . ?
C17 C18 C13 116.2(10) . . ?
C17 C18 C10 123.1(9) . . ?
C13 C18 C10 120.7(9) . . ?
C21 C19 C14 120.6(10) . . ?
C21 C19 H19A 119.7 . . ?
C14 C19 H19A 119.7 . . ?
O15 C20 O12 124.7(8) . . ?
O15 C20 C21 118.7(8) . . ?
O12 C20 C21 116.6(8) . . ?
C19 C21 C5 118.9(10) . . ?
C19 C21 C20 120.1(9) . . ?
C5 C21 C20 121.0(10) . . ?
C9 N1 H1B 120.0 . . ?
C9 N1 H1C 120.0 . . ?
H1B N1 H1C 120.0 . . ?
C3 N2 H2B 120.0 . . ?
C3 N2 H2C 120.0 . . ?
H2B N2 H2C 120.0 . . ?
C4 N3 H3A 120.0 . . ?
C4 N3 H3B 120.0 . . ?
H3A N3 H3B 120.0 . . ?
Zn1 O2W K1A 58.2(7) . . ?
Zn1 O2W K1 47.2(5) . . ?
K1A O2W K1 11.7(4) . . ?
K1 OW7 K1A 15.4(3) . . ?
K1 OW7 K1A 109.9(7) . 2_656 ?
K1A OW7 K1A 97.3(6) . 2_656 ?
O1WA O1W Zn1 106.1(19) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2W K1 K1A Zn1 -16.8(16) . . . . ?
OW7 K1 K1A Zn1 118.0(4) . . . . ?
O19 K1 K1A Zn1 -46.2(3) . . . . ?
O21 K1 K1A Zn1 43.3(4) 2_556 . . . ?
O20 K1 K1A Zn1 -158.2(8) 1_655 . . . ?
O26 K1 K1A Zn1 -111.9(3) 1_655 . . . ?
Mo3 K1 K1A Zn1 -133.6(3) 1_655 . . . ?
K1A K1 K1A Zn1 142.9(7) 2_656 . . . ?
Zn1 K1 K1A O2W 16.8(16) . . . . ?
OW7 K1 K1A O2W 134.8(15) . . . . ?
O19 K1 K1A O2W -29.4(18) . . . . ?
O21 K1 K1A O2W 60.1(14) 2_556 . . . ?
O20 K1 K1A O2W -141.4(12) 1_655 . . . ?
O26 K1 K1A O2W -95.1(15) 1_655 . . . ?
Mo3 K1 K1A O2W -116.8(15) 1_655 . . . ?
K1A K1 K1A O2W 160(2) 2_656 . . . ?
Zn1 K1 K1A OW7 -118.0(4) . . . . ?
O2W K1 K1A OW7 -134.8(15) . . . . ?
O19 K1 K1A OW7 -164.1(6) . . . . ?
O21 K1 K1A OW7 -74.7(4) 2_556 . . . ?
O20 K1 K1A OW7 83.8(7) 1_655 . . . ?
O26 K1 K1A OW7 130.1(4) 1_655 . . . ?
Mo3 K1 K1A OW7 108.4(4) 1_655 . . . ?
K1A K1 K1A OW7 24.9(8) 2_656 . . . ?
Zn1 K1 K1A OW7 176.8(17) . . . 2_656 ?
O2W K1 K1A OW7 160(3) . . . 2_656 ?
OW7 K1 K1A OW7 -65.2(19) . . . 2_656 ?
O19 K1 K1A OW7 130.6(17) . . . 2_656 ?
O21 K1 K1A OW7 -140(2) 2_556 . . 2_656 ?
O20 K1 K1A OW7 19(2) 1_655 . . 2_656 ?
O26 K1 K1A OW7 64.9(18) 1_655 . . 2_656 ?
Mo3 K1 K1A OW7 43.2(19) 1_655 . . 2_656 ?
K1A K1 K1A OW7 -40.3(14) 2_656 . . 2_656 ?
Zn1 K1 K1A O21 -43.3(4) . . . 2_556 ?
O2W K1 K1A O21 -60.1(14) . . . 2_556 ?
OW7 K1 K1A O21 74.7(4) . . . 2_556 ?
O19 K1 K1A O21 -89.5(5) . . . 2_556 ?
O20 K1 K1A O21 158.4(5) 1_655 . . 2_556 ?
O26 K1 K1A O21 -155.2(3) 1_655 . . 2_556 ?
Mo3 K1 K1A O21 -176.9(3) 1_655 . . 2_556 ?
K1A K1 K1A O21 99.5(8) 2_656 . . 2_556 ?
Zn1 K1 K1A O19 46.2(3) . . . . ?
O2W K1 K1A O19 29.4(18) . . . . ?
OW7 K1 K1A O19 164.1(6) . . . . ?
O21 K1 K1A O19 89.5(5) 2_556 . . . ?
O20 K1 K1A O19 -112.1(8) 1_655 . . . ?
O26 K1 K1A O19 -65.8(4) 1_655 . . . ?
Mo3 K1 K1A O19 -87.5(4) 1_655 . . . ?
K1A K1 K1A O19 -171.0(5) 2_656 . . . ?
Zn1 K1 K1A O26 111.9(3) . . . 1_655 ?
O2W K1 K1A O26 95.1(15) . . . 1_655 ?
OW7 K1 K1A O26 -130.1(4) . . . 1_655 ?
O19 K1 K1A O26 65.8(4) . . . 1_655 ?
O21 K1 K1A O26 155.2(3) 2_556 . . 1_655 ?
O20 K1 K1A O26 -46.3(7) 1_655 . . 1_655 ?
Mo3 K1 K1A O26 -21.70(15) 1_655 . . 1_655 ?
K1A K1 K1A O26 -105.2(8) 2_656 . . 1_655 ?
Zn1 K1 K1A O20 158.2(8) . . . 1_655 ?
O2W K1 K1A O20 141.4(12) . . . 1_655 ?
OW7 K1 K1A O20 -83.8(7) . . . 1_655 ?
O19 K1 K1A O20 112.1(8) . . . 1_655 ?
O21 K1 K1A O20 -158.4(5) 2_556 . . 1_655 ?
O26 K1 K1A O20 46.3(7) 1_655 . . 1_655 ?
Mo3 K1 K1A O20 24.6(6) 1_655 . . 1_655 ?
K1A K1 K1A O20 -58.9(12) 2_656 . . 1_655 ?
Zn1 K1 K1A OW3 78.6(11) . . . 2_546 ?
O2W K1 K1A OW3 61.8(15) . . . 2_546 ?
OW7 K1 K1A OW3 -163.5(11) . . . 2_546 ?
O19 K1 K1A OW3 32.4(14) . . . 2_546 ?
O21 K1 K1A OW3 121.9(12) 2_556 . . 2_546 ?
O20 K1 K1A OW3 -79.7(14) 1_655 . . 2_546 ?
O26 K1 K1A OW3 -33.4(11) 1_655 . . 2_546 ?
Mo3 K1 K1A OW3 -55.1(11) 1_655 . . 2_546 ?
K1A K1 K1A OW3 -138.6(17) 2_656 . . 2_546 ?
Zn1 K1 K1A Mo3 133.6(3) . . . 1_655 ?
O2W K1 K1A Mo3 116.8(15) . . . 1_655 ?
OW7 K1 K1A Mo3 -108.4(4) . . . 1_655 ?
O19 K1 K1A Mo3 87.5(4) . . . 1_655 ?
O21 K1 K1A Mo3 176.9(3) 2_556 . . 1_655 ?
O20 K1 K1A Mo3 -24.6(6) 1_655 . . 1_655 ?
O26 K1 K1A Mo3 21.70(15) 1_655 . . 1_655 ?
K1A K1 K1A Mo3 -83.5(7) 2_656 . . 1_655 ?
Zn1 K1 K1A Mo2 -56.4(6) . . . 2_556 ?
O2W K1 K1A Mo2 -73.1(14) . . . 2_556 ?
OW7 K1 K1A Mo2 61.6(6) . . . 2_556 ?
O19 K1 K1A Mo2 -102.5(5) . . . 2_556 ?
O21 K1 K1A Mo2 -13.0(3) 2_556 . . 2_556 ?
O20 K1 K1A Mo2 145.4(4) 1_655 . . 2_556 ?
O26 K1 K1A Mo2 -168.3(5) 1_655 . . 2_556 ?
Mo3 K1 K1A Mo2 170.0(4) 1_655 . . 2_556 ?
K1A K1 K1A Mo2 86.5(8) 2_656 . . 2_556 ?
O14 Mo1 O5 Mo5 20.0(7) . . . . ?
O11 Mo1 O5 Mo5 125.7(7) . . . . ?
O13 Mo1 O5 Mo5 -102.9(8) . . . . ?
O23 Mo1 O5 Mo5 -68.4(7) . . . . ?
O4 Mo1 O5 Mo5 -145.7(7) . . . . ?
Mo6 Mo1 O5 Mo5 -81.7(7) . . . . ?
O10 Te1 O8 Mo2 160.8(3) . . . . ?
O23 Te1 O8 Mo2 66.5(4) . . . . ?
O10 Te1 O8 Mo3 -68.3(4) . . . . ?
O23 Te1 O8 Mo3 -162.6(3) . . . . ?
O8 Te1 O10 Mo4 71.9(4) . . . . ?
O23 Te1 O10 Mo4 166.0(3) . . . . ?
O8 Te1 O10 Mo5 -164.0(3) . . . . ?
O23 Te1 O10 Mo5 -69.9(4) . . . . ?
O27 Mo6 O19 Zn1 -118.6(9) . . . . ?
O6 Mo6 O19 Zn1 -17.0(10) . . . . ?
O13 Mo6 O19 Zn1 140.9(9) . . . . ?
O23 Mo6 O19 Zn1 76.5(16) . . . . ?
O22 Mo6 O19 Zn1 60.7(9) . . . . ?
Mo1 Mo6 O19 Zn1 131.0(8) . . . . ?
O27 Mo6 O19 K1 97(2) . . . . ?
O6 Mo6 O19 K1 -161.6(19) . . . . ?
O13 Mo6 O19 K1 -4(2) . . . . ?
O23 Mo6 O19 K1 -68(3) . . . . ?
O22 Mo6 O19 K1 -84(2) . . . . ?
Mo1 Mo6 O19 K1 -14(2) . . . . ?
O27 Mo6 O19 K1A 36(2) . . . . ?
O6 Mo6 O19 K1A 138(2) . . . . ?
O13 Mo6 O19 K1A -64(2) . . . . ?
O23 Mo6 O19 K1A -128.7(19) . . . . ?
O22 Mo6 O19 K1A -145(2) . . . . ?
Mo1 Mo6 O19 K1A -74(2) . . . . ?
O2 Mo2 O21 Zn1 152.0(13) . . . 2_556 ?
O6 Mo2 O21 Zn1 49.7(13) . . . 2_556 ?
O24 Mo2 O21 Zn1 -108.3(13) . . . 2_556 ?
O8 Mo2 O21 Zn1 -51.8(19) . . . 2_556 ?
O16 Mo2 O21 Zn1 -26.7(13) . . . 2_556 ?
Mo3 Mo2 O21 Zn1 -96.3(13) . . . 2_556 ?
K1A Mo2 O21 Zn1 -64.4(12) 2_556 . . 2_556 ?
O2 Mo2 O21 K1A -143.6(5) . . . 2_556 ?
O6 Mo2 O21 K1A 114.1(5) . . . 2_556 ?
O24 Mo2 O21 K1A -43.9(5) . . . 2_556 ?
O8 Mo2 O21 K1A 12.5(13) . . . 2_556 ?
O16 Mo2 O21 K1A 37.6(5) . . . 2_556 ?
Mo3 Mo2 O21 K1A -31.9(6) . . . 2_556 ?
O2 Mo2 O21 K1 -128.6(6) . . . 2_556 ?
O6 Mo2 O21 K1 129.0(6) . . . 2_556 ?
O24 Mo2 O21 K1 -29.0(7) . . . 2_556 ?
O8 Mo2 O21 K1 27.5(14) . . . 2_556 ?
O16 Mo2 O21 K1 52.6(7) . . . 2_556 ?
Mo3 Mo2 O21 K1 -17.0(8) . . . 2_556 ?
K1A Mo2 O21 K1 14.9(4) 2_556 . . 2_556 ?
O8 Te1 O23 Mo1 164.7(4) . . . . ?
O10 Te1 O23 Mo1 70.0(4) . . . . ?
O8 Te1 O23 Mo6 -70.5(4) . . . . ?
O10 Te1 O23 Mo6 -165.3(4) . . . . ?
O25 Mo3 O26 K1A 148.0(4) . . . 1_455 ?
O18 Mo3 O26 K1A -111.1(4) . . . 1_455 ?
O24 Mo3 O26 K1A 46.2(4) . . . 1_455 ?
O8 Mo3 O26 K1A -14.8(13) . . . 1_455 ?
O20 Mo3 O26 K1A -34.6(4) . . . 1_455 ?
Mo2 Mo3 O26 K1A 34.4(5) . . . 1_455 ?
K1 Mo3 O26 K1A -15.1(3) 1_455 . . 1_455 ?
O25 Mo3 O26 K1 163.1(4) . . . 1_455 ?
O18 Mo3 O26 K1 -96.0(4) . . . 1_455 ?
O24 Mo3 O26 K1 61.3(4) . . . 1_455 ?
O8 Mo3 O26 K1 0.4(13) . . . 1_455 ?
O20 Mo3 O26 K1 -19.4(4) . . . 1_455 ?
Mo2 Mo3 O26 K1 49.6(5) . . . 1_455 ?
K1A Mo3 O26 K1 15.1(3) 1_455 . . 1_455 ?
C7 C1 C3 C15 -1(2) . . . . ?
C7 C1 C3 N2 179.8(12) . . . . ?
C9 C2 C5 C21 4(2) . . . . ?
C11 C4 C6 C17 -0.7(18) . . . . ?
N3 C4 C6 C17 179.9(10) . . . . ?
C3 C1 C7 C12 2(2) . . . . ?
C5 C2 C9 C14 0.3(18) . . . . ?
C5 C2 C9 N1 -177.8(11) . . . . ?
Mo3 O20 C10 O16 -5.4(15) . . . . ?
K1 O20 C10 O16 111.5(9) 1_455 . . . ?
K1A O20 C10 O16 99.2(9) 1_455 . . . ?
Mo3 O20 C10 C18 173.0(6) . . . . ?
K1 O20 C10 C18 -70.0(9) 1_455 . . . ?
K1A O20 C10 C18 -82.4(9) 1_455 . . . ?
Mo2 O16 C10 O20 3.4(15) . . . . ?
Mo2 O16 C10 C18 -175.1(6) . . . . ?
C6 C4 C11 C13 1.2(17) . . . . ?
N3 C4 C11 C13 -179.3(10) . . . . ?
C15 C8 C12 C7 2.0(17) . . . . ?
C15 C8 C12 C16 -178.3(10) . . . . ?
C1 C7 C12 C8 -2.3(18) . . . . ?
C1 C7 C12 C16 178.1(11) . . . . ?
C4 C11 C13 C18 -0.4(16) . . . . ?
C2 C9 C14 C19 -2.1(16) . . . . ?
N1 C9 C14 C19 176.0(10) . . . . ?
C1 C3 C15 C8 0.5(19) . . . . ?
N2 C3 C15 C8 180.0(11) . . . . ?
C12 C8 C15 C3 -1.2(18) . . . . ?
Mo1 O4 C16 O22 -7.6(16) . . . . ?
Mo1 O4 C16 C12 175.0(6) . . . . ?
Mo6 O22 C16 O4 3.0(15) . . . . ?
Mo6 O22 C16 C12 -179.7(6) . . . . ?
C8 C12 C16 O4 15.4(14) . . . . ?
C7 C12 C16 O4 -165.0(10) . . . . ?
C8 C12 C16 O22 -162.2(10) . . . . ?
C7 C12 C16 O22 17.4(15) . . . . ?
C4 C6 C17 C18 -0.7(18) . . . . ?
C6 C17 C18 C13 1.5(16) . . . . ?
C6 C17 C18 C10 -178.5(10) . . . . ?
C11 C13 C18 C17 -0.9(15) . . . . ?
C11 C13 C18 C10 179.1(9) . . . . ?
O20 C10 C18 C17 -171.8(9) . . . . ?
O16 C10 C18 C17 6.8(14) . . . . ?
O20 C10 C18 C13 8.2(14) . . . . ?
O16 C10 C18 C13 -173.2(9) . . . . ?
C9 C14 C19 C21 0.0(15) . . . . ?
Mo5 O15 C20 O12 4.8(15) . . . . ?
Mo5 O15 C20 C21 -174.9(6) . . . . ?
Mo4 O12 C20 O15 -10.8(15) . . . . ?
Mo4 O12 C20 C21 168.9(6) . . . . ?
C14 C19 C21 C5 3.7(15) . . . . ?
C14 C19 C21 C20 -177.5(9) . . . . ?
C2 C5 C21 C19 -5.5(18) . . . . ?
C2 C5 C21 C20 175.8(11) . . . . ?
O15 C20 C21 C19 -158.9(9) . . . . ?
O12 C20 C21 C19 21.4(14) . . . . ?
O15 C20 C21 C5 19.9(15) . . . . ?
O12 C20 C21 C5 -159.8(10) . . . . ?

_refine_diff_density_max         2.386
_refine_diff_density_min         -2.163
_refine_diff_density_rms         0.231

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_9
_database_code_depnum_ccdc_archive 'CCDC 1871479'
_audit_update_record             
;
2018-10-04 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C16 H78 As2 Co2 Mo12 N4 O75 Rb2'
_chemical_formula_weight         3116.74

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.8787(3)
_cell_length_b                   23.7424(5)
_cell_length_c                   15.8044(3)
_cell_angle_alpha                90
_cell_angle_beta                 120.0320(10)
_cell_angle_gamma                90
_cell_volume                     4508.60(17)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    47460
_cell_measurement_theta_min      1.715
_cell_measurement_theta_max      25.00

_exptl_crystal_description       block
_exptl_crystal_colour            red
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.296
_exptl_crystal_F_000             2999
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    3.877
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.395
_exptl_absorpt_correction_T_max  0.443
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            47460
_diffrn_reflns_av_unetI/netI     0.0326
_diffrn_reflns_av_R_equivalents  0.0439
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_theta_min         1.715
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measured_fraction_theta_full 0.976
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_Laue_measured_fraction_full 0.976
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_point_group_measured_fraction_full 0.976
_reflns_number_total             7949
_reflns_number_gt                6957
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0571P)²+83.0492P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         7949
_refine_ls_number_parameters     577
_refine_ls_number_restraints     85
_refine_ls_R_factor_all          0.0644
_refine_ls_R_factor_gt           0.0556
_refine_ls_wR_factor_ref         0.1528
_refine_ls_wR_factor_gt          0.1483
_refine_ls_goodness_of_fit_ref   1.137
_refine_ls_restrained_S_all      1.142
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.36813(7) 0.11990(3) 0.54939(6) 0.0193(2) Uani 1 1 d . . . . .
Mo2 Mo 0.56193(7) 0.20936(3) 0.57936(6) 0.0208(2) Uani 1 1 d . . . . .
Mo3 Mo 0.90622(7) 0.07818(3) 0.91212(6) 0.0217(2) Uani 1 1 d . . . . .
Mo4 Mo 0.69614(7) -0.02110(3) 0.87844(6) 0.0221(2) Uani 1 1 d . . . . .
Mo5 Mo 0.43862(7) -0.00164(3) 0.70327(6) 0.0203(2) Uani 1 1 d . . . . .
Mo6 Mo 0.84070(8) 0.18879(4) 0.77052(7) 0.0293(2) Uani 1 1 d . . . . .
As1 As 0.62048(8) 0.11710(4) 0.77869(7) 0.0173(2) Uani 1 1 d . . . . .
Co1 Co 0.90671(19) -0.06208(9) 0.82337(17) 0.0153(5) Uani 0.5 1 d . . P . .
Co2 Co 0.1295(2) 0.40534(13) 0.2195(2) 0.0343(7) Uani 0.5 1 d . . P . .
Rb1 Rb 0.66238(11) 0.03953(5) 0.60788(9) 0.0411(3) Uani 1 1 d . . . . .
O1 O 0.8191(7) 0.2188(3) 0.8967(5) 0.0381(19) Uani 1 1 d . . . . .
O2 O 0.3645(6) 0.1846(3) 0.6582(5) 0.0282(16) Uani 1 1 d . . . . .
O3 O 0.8616(6) 0.1436(3) 0.9922(5) 0.0299(16) Uani 1 1 d . . . . .
O4 O 0.5431(7) 0.2759(3) 0.5307(5) 0.0346(18) Uani 1 1 d . . . . .
O5 O 0.7419(7) -0.0663(3) 0.9746(6) 0.042(2) Uani 1 1 d . . . . .
O6 O 0.3216(6) -0.0335(3) 0.6920(6) 0.0372(18) Uani 1 1 d . . . . .
O7 O 0.9201(8) 0.2487(4) 0.7928(7) 0.056(3) Uani 1 1 d . . . . .
O8 O 0.3786(6) 0.0701(3) 0.6481(5) 0.0234(14) Uani 1 1 d . . . . .
O9 O 0.5454(5) 0.1333(3) 0.6512(5) 0.0206(14) Uani 1 1 d . . . . .
O10 O 0.9182(7) 0.0303(4) 0.8360(6) 0.041(2) Uani 1 1 d . . . . .
O11 O 0.4062(6) 0.1865(3) 0.5011(5) 0.0238(15) Uani 1 1 d . . . . .
O12 O 0.5454(6) -0.0504(3) 0.8069(5) 0.0239(15) Uani 1 1 d . . . . .
O13 O 0.7549(5) 0.1157(3) 0.7908(4) 0.0204(14) Uani 1 1 d . . . . .
O14 O 0.5973(5) 0.0429(2) 0.7648(4) 0.0188(13) Uani 1 1 d . . . . .
O15 O 0.9573(6) 0.1437(3) 0.8754(5) 0.0301(16) Uani 1 1 d . . . . .
O16 O 0.4908(6) 0.2480(3) 0.6722(5) 0.0305(17) Uani 1 1 d . . . . .
O17 O 0.6223(6) 0.0302(3) 0.9543(5) 0.0290(16) Uani 1 1 d . . . . .
O18 O 1.0224(6) 0.0676(3) 1.0241(5) 0.0315(17) Uani 1 1 d . . . . .
O19 O 0.2259(6) 0.1289(3) 0.4841(6) 0.0376(18) Uani 1 1 d . . . . .
O20 O 0.7443(6) -0.0496(3) 0.8052(5) 0.0303(16) Uani 1 1 d . . . . .
O21 O 0.3934(6) 0.0728(3) 0.4818(5) 0.0298(16) Uani 1 1 d . . . . .
O22 O 0.8463(7) 0.1568(4) 0.6764(6) 0.047(2) Uani 1 1 d . . . . .
O23 O 0.4525(6) -0.0307(3) 0.6105(5) 0.0334(17) Uani 1 1 d . . . . .
O24 O 0.6950(6) 0.2194(3) 0.7001(5) 0.0285(16) Uani 1 1 d . . . . .
O25 O 0.8007(6) 0.0384(3) 0.9336(5) 0.0231(14) Uani 1 1 d . . . . .
O26 O 0.6092(6) 0.1709(3) 0.5161(5) 0.0316(17) Uani 1 1 d . . . . .
O27 O 0.4461(6) 0.0431(3) 0.8357(5) 0.0331(17) Uani 1 1 d . . . . .
C1 C 0.8070(15) 0.2263(6) 1.0407(10) 0.061(4) Uani 1 1 d . . . . .
H1A H 0.8194 0.2024 1.0943 0.091 Uiso 1 1 calc R U . . .
H1B H 0.8552 0.2584 1.0652 0.091 Uiso 1 1 calc R U . . .
H1C H 0.7309 0.2386 1.0069 0.091 Uiso 1 1 calc R U . . .
C2 C 0.6044(12) 0.0967(5) 1.0860(9) 0.048(3) Uani 1 1 d . . . . .
H2A H 0.6580 0.1183 1.0772 0.057 Uiso 1 1 calc R U . . .
H2B H 0.6388 0.0612 1.1165 0.057 Uiso 1 1 calc R U . . .
C3 C 0.5047(11) 0.0858(5) 0.9898(9) 0.037(3) Uani 1 1 d . . . . .
H3A H 0.4737 0.1217 0.9584 0.045 Uiso 1 1 calc R U . . .
H3B H 0.4492 0.0671 1.0000 0.045 Uiso 1 1 calc R U . . .
C4 C 0.3961(11) 0.2635(5) 0.7595(9) 0.039(3) Uani 1 1 d . . . . .
H4A H 0.4342 0.2461 0.8237 0.046 Uiso 1 1 calc R U . . .
H4B H 0.3170 0.2626 0.7366 0.046 Uiso 1 1 calc R U . . .
C5 C 0.4331(10) 0.3242(4) 0.7688(9) 0.034(3) Uani 1 1 d . . . . .
H5A H 0.5136 0.3254 0.8001 0.040 Uiso 1 1 calc R U . . .
H5B H 0.4028 0.3403 0.7040 0.040 Uiso 1 1 calc R U . . .
C6 C 0.5268(9) 0.0501(4) 0.9215(8) 0.027(2) Uani 1 1 d . . . . .
C7 C 0.8313(9) 0.1937(4) 0.9706(8) 0.032(2) Uani 1 1 d . . . . .
C8 C 0.4185(9) 0.2290(4) 0.6907(7) 0.024(2) Uani 1 1 d . . . . .
N1 N 0.5739(11) 0.1282(4) 1.1507(8) 0.051(3) Uani 1 1 d . . . . .
H1D H 0.6348 0.1344 1.2082 0.076 Uiso 1 1 calc R U . . .
H1E H 0.5433 0.1610 1.1231 0.076 Uiso 1 1 calc R U . . .
H1F H 0.5255 0.1081 1.1595 0.076 Uiso 1 1 calc R U . . .
N2 N 0.3974(8) 0.3586(4) 0.8259(6) 0.033(2) Uani 1 1 d . . . . .
H2C H 0.4209 0.3938 0.8294 0.050 Uiso 1 1 calc R U . . .
H2D H 0.3235 0.3583 0.7969 0.050 Uiso 1 1 calc R U . . .
H2E H 0.4262 0.3445 0.8859 0.050 Uiso 1 1 calc R U . . .
O1W O 1.0830(15) -0.0657(7) 0.8483(10) 0.047(4) Uani 0.5 1 d . U P . .
O2W O 0.8515(9) -0.1501(5) 0.7965(9) 0.014(2) Uani 0.5 1 d . U P . .
O3W O 0.8552(10) -0.0470(5) 0.6691(9) 0.022(3) Uani 0.5 1 d . U P . .
O4W O 0.0562(16) 0.3303(7) 0.1489(14) 0.054(5) Uani 0.5 1 d . U P . .
O5W O 0.1296(15) 0.4359(8) 0.0920(14) 0.053(5) Uani 0.5 1 d . U P . .
O6W O 0.2070(16) 0.4783(8) 0.2928(16) 0.063(5) Uani 0.5 1 d . U P . .
O7W O 0.1282(12) 0.3842(7) 0.3413(11) 0.035(4) Uani 0.5 1 d . U P . .
O8W O 0.2830(11) 0.3725(5) 0.2672(10) 0.023(3) Uani 0.5 1 d . U P . .
O9W O -0.0333(16) 0.4464(9) 0.1621(15) 0.063(5) Uani 0.5 1 d . U P . .
OW1 O 0.298(5) 0.298(3) 0.473(5) 0.21(3) Uani 0.5 1 d . U P . .
OW2 O 0.262(2) 0.2780(12) 0.4359(19) 0.099(10) Uani 0.5 1 d D U P . .
OW3 O 0.103(3) 0.6293(14) 0.213(3) 0.135(12) Uani 0.5 1 d . U P . .
OW4 O 0.067(2) 0.1993(12) 0.4911(16) 0.091(9) Uani 0.5 1 d . . P . .
OW5 O 0.1008(16) 0.2381(9) 0.2739(15) 0.168(8) Uani 1 1 d D U . . .
OW6 O 0.2550(16) 0.6676(6) 0.1674(14) 0.146(7) Uani 1 1 d . . . . .
OW7 O 0.1448(14) 0.1940(7) 0.0417(11) 0.122(5) Uani 1 1 d . U . . .
OW8 O 0.7746(15) 0.0983(9) 0.4950(13) 0.151(8) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O21 1.700(7) . ?
Mo1 O19 1.723(8) . ?
Mo1 O8 1.905(7) . ?
Mo1 O11 1.940(7) . ?
Mo1 O9 2.186(7) . ?
Mo1 O2 2.325(7) . ?
Mo1 Mo2 3.2704(12) . ?
Mo2 O26 1.709(7) . ?
Mo2 O4 1.718(7) . ?
Mo2 O24 1.893(7) . ?
Mo2 O11 1.955(7) . ?
Mo2 O9 2.206(6) . ?
Mo2 O16 2.328(7) . ?
Mo3 O18 1.715(7) . ?
Mo3 O10 1.723(7) . ?
Mo3 O25 1.909(7) . ?
Mo3 O15 1.917(7) . ?
Mo3 O13 2.202(6) . ?
Mo3 O3 2.277(7) . ?
Mo3 Mo6 3.2703(12) . ?
Mo4 O5 1.703(8) . ?
Mo4 O20 1.738(7) . ?
Mo4 O25 1.897(7) . ?
Mo4 O12 1.942(7) . ?
Mo4 O14 2.225(6) . ?
Mo4 O17 2.280(7) . ?
Mo4 Mo5 3.2784(12) . ?
Mo5 O23 1.716(7) . ?
Mo5 O6 1.719(7) . ?
Mo5 O8 1.904(6) . ?
Mo5 O12 1.947(6) . ?
Mo5 O14 2.184(6) . ?
Mo5 O27 2.303(7) . ?
Mo6 O22 1.706(8) . ?
Mo6 O7 1.725(8) . ?
Mo6 O24 1.898(7) . ?
Mo6 O15 1.956(7) . ?
Mo6 O13 2.217(6) . ?
Mo6 O1 2.275(8) . ?
As1 O13 1.778(6) . ?
As1 O14 1.785(6) . ?
As1 O9 1.786(6) . ?
Co1 O18 2.103(8) 3_757 ?
Co1 O20 2.145(8) . ?
Co1 O2W 2.193(12) . ?
Co1 O10 2.201(9) . ?
Co1 O3W 2.200(13) . ?
Co1 O1W 2.277(18) . ?
Co2 O7W 1.998(15) . ?
Co2 O8W 2.025(14) . ?
Co2 O6W 2.062(18) . ?
Co2 O4W 2.077(17) . ?
Co2 O5W 2.141(19) . ?
Co2 O9W 2.20(2) . ?
O1 C7 1.246(13) . ?
O2 C8 1.247(12) . ?
O3 C7 1.250(13) . ?
O16 C8 1.261(12) . ?
O17 C6 1.250(13) . ?
O18 Co1 2.103(8) 3_757 ?
O27 C6 1.266(13) . ?
C1 C7 1.521(15) . ?
C1 H1A 0.9600 . ?
C1 H1B 0.9600 . ?
C1 H1C 0.9600 . ?
C2 C3 1.479(18) . ?
C2 N1 1.489(15) . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
C3 C6 1.520(14) . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
C4 C8 1.512(14) . ?
C4 C5 1.512(15) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 N2 1.475(13) . ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
N1 H1D 0.8900 . ?
N1 H1E 0.8900 . ?
N1 H1F 0.8900 . ?
N2 H2C 0.8900 . ?
N2 H2D 0.8900 . ?
N2 H2E 0.8900 . ?
OW1 OW2 0.72(7) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O21 Mo1 O19 103.9(4) . . ?
O21 Mo1 O8 98.7(3) . . ?
O19 Mo1 O8 99.4(3) . . ?
O21 Mo1 O11 96.1(3) . . ?
O19 Mo1 O11 96.8(3) . . ?
O8 Mo1 O11 154.7(3) . . ?
O21 Mo1 O9 92.8(3) . . ?
O19 Mo1 O9 162.3(3) . . ?
O8 Mo1 O9 83.7(3) . . ?
O11 Mo1 O9 75.1(3) . . ?
O21 Mo1 O2 170.8(3) . . ?
O19 Mo1 O2 85.3(3) . . ?
O8 Mo1 O2 79.9(3) . . ?
O11 Mo1 O2 82.2(3) . . ?
O9 Mo1 O2 78.0(2) . . ?
O21 Mo1 Mo2 96.0(2) . . ?
O19 Mo1 Mo2 128.2(3) . . ?
O8 Mo1 Mo2 124.4(2) . . ?
O11 Mo1 Mo2 33.04(19) . . ?
O9 Mo1 Mo2 42.11(16) . . ?
O2 Mo1 Mo2 77.57(17) . . ?
O26 Mo2 O4 104.3(4) . . ?
O26 Mo2 O24 101.0(3) . . ?
O4 Mo2 O24 100.9(3) . . ?
O26 Mo2 O11 96.2(3) . . ?
O4 Mo2 O11 95.8(3) . . ?
O24 Mo2 O11 152.3(3) . . ?
O26 Mo2 O9 91.9(3) . . ?
O4 Mo2 O9 162.0(3) . . ?
O24 Mo2 O9 83.3(3) . . ?
O11 Mo2 O9 74.4(3) . . ?
O26 Mo2 O16 170.9(3) . . ?
O4 Mo2 O16 84.4(3) . . ?
O24 Mo2 O16 79.8(3) . . ?
O11 Mo2 O16 79.9(3) . . ?
O9 Mo2 O16 79.2(2) . . ?
O26 Mo2 Mo1 95.5(2) . . ?
O4 Mo2 Mo1 127.0(3) . . ?
O24 Mo2 Mo1 123.0(2) . . ?
O11 Mo2 Mo1 32.75(19) . . ?
O9 Mo2 Mo1 41.64(17) . . ?
O16 Mo2 Mo1 76.71(17) . . ?
O18 Mo3 O10 104.7(4) . . ?
O18 Mo3 O25 98.8(3) . . ?
O10 Mo3 O25 98.5(4) . . ?
O18 Mo3 O15 97.6(3) . . ?
O10 Mo3 O15 98.3(4) . . ?
O25 Mo3 O15 152.6(3) . . ?
O18 Mo3 O13 162.3(3) . . ?
O10 Mo3 O13 92.4(3) . . ?
O25 Mo3 O13 82.7(3) . . ?
O15 Mo3 O13 75.2(3) . . ?
O18 Mo3 O3 84.5(3) . . ?
O10 Mo3 O3 170.6(3) . . ?
O25 Mo3 O3 78.0(3) . . ?
O15 Mo3 O3 81.9(3) . . ?
O13 Mo3 O3 78.6(2) . . ?
O18 Mo3 Mo6 128.3(3) . . ?
O10 Mo3 Mo6 98.2(3) . . ?
O25 Mo3 Mo6 122.91(19) . . ?
O15 Mo3 Mo6 32.8(2) . . ?
O13 Mo3 Mo6 42.44(16) . . ?
O3 Mo3 Mo6 76.86(18) . . ?
O5 Mo4 O20 104.7(4) . . ?
O5 Mo4 O25 101.6(3) . . ?
O20 Mo4 O25 97.8(3) . . ?
O5 Mo4 O12 96.1(3) . . ?
O20 Mo4 O12 97.7(3) . . ?
O25 Mo4 O12 152.7(3) . . ?
O5 Mo4 O14 162.7(3) . . ?
O20 Mo4 O14 90.9(3) . . ?
O25 Mo4 O14 83.3(3) . . ?
O12 Mo4 O14 74.1(2) . . ?
O5 Mo4 O17 86.1(4) . . ?
O20 Mo4 O17 169.2(3) . . ?
O25 Mo4 O17 78.6(3) . . ?
O12 Mo4 O17 82.0(3) . . ?
O14 Mo4 O17 78.6(2) . . ?
O5 Mo4 Mo5 127.2(3) . . ?
O20 Mo4 Mo5 96.5(2) . . ?
O25 Mo4 Mo5 122.91(19) . . ?
O12 Mo4 Mo5 32.57(18) . . ?
O14 Mo4 Mo5 41.49(16) . . ?
O17 Mo4 Mo5 77.39(19) . . ?
O23 Mo5 O6 103.8(4) . . ?
O23 Mo5 O8 100.3(3) . . ?
O6 Mo5 O8 99.9(3) . . ?
O23 Mo5 O12 96.6(3) . . ?
O6 Mo5 O12 96.2(3) . . ?
O8 Mo5 O12 153.0(3) . . ?
O23 Mo5 O14 93.2(3) . . ?
O6 Mo5 O14 161.7(3) . . ?
O8 Mo5 O14 83.3(3) . . ?
O12 Mo5 O14 74.9(2) . . ?
O23 Mo5 O27 171.4(3) . . ?
O6 Mo5 O27 84.7(3) . . ?
O8 Mo5 O27 79.3(3) . . ?
O12 Mo5 O27 80.9(3) . . ?
O14 Mo5 O27 78.2(3) . . ?
O23 Mo5 Mo4 97.1(3) . . ?
O6 Mo5 Mo4 126.9(3) . . ?
O8 Mo5 Mo4 123.7(2) . . ?
O12 Mo5 Mo4 32.48(19) . . ?
O14 Mo5 Mo4 42.44(16) . . ?
O27 Mo5 Mo4 76.32(19) . . ?
O22 Mo6 O7 104.0(5) . . ?
O22 Mo6 O24 99.2(4) . . ?
O7 Mo6 O24 100.8(4) . . ?
O22 Mo6 O15 96.6(4) . . ?
O7 Mo6 O15 96.1(4) . . ?
O24 Mo6 O15 153.3(3) . . ?
O22 Mo6 O13 92.2(4) . . ?
O7 Mo6 O13 162.0(4) . . ?
O24 Mo6 O13 83.8(3) . . ?
O15 Mo6 O13 74.1(3) . . ?
O22 Mo6 O1 170.9(4) . . ?
O7 Mo6 O1 85.1(4) . . ?
O24 Mo6 O1 79.9(3) . . ?
O15 Mo6 O1 81.1(3) . . ?
O13 Mo6 O1 78.6(3) . . ?
O22 Mo6 Mo3 96.9(3) . . ?
O7 Mo6 Mo3 126.3(3) . . ?
O24 Mo6 Mo3 123.9(2) . . ?
O15 Mo6 Mo3 32.0(2) . . ?
O13 Mo6 Mo3 42.08(16) . . ?
O1 Mo6 Mo3 76.41(19) . . ?
O13 As1 O14 96.3(3) . . ?
O13 As1 O9 96.6(3) . . ?
O14 As1 O9 96.1(3) . . ?
O18 Co1 O20 91.1(3) 3_757 . ?
O18 Co1 O2W 94.6(4) 3_757 . ?
O20 Co1 O2W 82.1(4) . . ?
O18 Co1 O10 89.3(3) 3_757 . ?
O20 Co1 O10 84.2(3) . . ?
O2W Co1 O10 165.8(4) . . ?
O18 Co1 O3W 170.6(4) 3_757 . ?
O20 Co1 O3W 95.3(4) . . ?
O2W Co1 O3W 93.0(4) . . ?
O10 Co1 O3W 84.6(4) . . ?
O18 Co1 O1W 87.4(4) 3_757 . ?
O20 Co1 O1W 173.9(5) . . ?
O2W Co1 O1W 103.8(5) . . ?
O10 Co1 O1W 89.9(5) . . ?
O3W Co1 O1W 85.6(5) . . ?
O7W Co2 O8W 93.5(6) . . ?
O7W Co2 O6W 85.6(8) . . ?
O8W Co2 O6W 87.6(7) . . ?
O7W Co2 O4W 93.7(7) . . ?
O8W Co2 O4W 90.7(7) . . ?
O6W Co2 O4W 178.1(9) . . ?
O7W Co2 O5W 174.7(7) . . ?
O8W Co2 O5W 89.1(6) . . ?
O6W Co2 O5W 90.0(8) . . ?
O4W Co2 O5W 90.9(8) . . ?
O7W Co2 O9W 90.3(7) . . ?
O8W Co2 O9W 175.3(7) . . ?
O6W Co2 O9W 89.9(8) . . ?
O4W Co2 O9W 91.9(8) . . ?
O5W Co2 O9W 86.9(7) . . ?
C7 O1 Mo6 131.0(7) . . ?
C8 O2 Mo1 129.2(6) . . ?
C7 O3 Mo3 130.2(7) . . ?
Mo5 O8 Mo1 140.1(4) . . ?
As1 O9 Mo1 127.3(3) . . ?
As1 O9 Mo2 127.2(3) . . ?
Mo1 O9 Mo2 96.2(2) . . ?
Mo3 O10 Co1 133.8(5) . . ?
Mo1 O11 Mo2 114.2(3) . . ?
Mo4 O12 Mo5 114.9(3) . . ?
As1 O13 Mo3 126.4(3) . . ?
As1 O13 Mo6 125.4(3) . . ?
Mo3 O13 Mo6 95.5(2) . . ?
As1 O14 Mo5 127.8(3) . . ?
As1 O14 Mo4 125.1(3) . . ?
Mo5 O14 Mo4 96.1(2) . . ?
Mo3 O15 Mo6 115.2(3) . . ?
C8 O16 Mo2 130.0(6) . . ?
C6 O17 Mo4 130.3(7) . . ?
Mo3 O18 Co1 148.3(4) . 3_757 ?
Mo4 O20 Co1 133.9(4) . . ?
Mo2 O24 Mo6 139.4(4) . . ?
Mo4 O25 Mo3 139.9(4) . . ?
C6 O27 Mo5 130.4(7) . . ?
C7 C1 H1A 109.5 . . ?
C7 C1 H1B 109.5 . . ?
H1A C1 H1B 109.5 . . ?
C7 C1 H1C 109.5 . . ?
H1A C1 H1C 109.5 . . ?
H1B C1 H1C 109.5 . . ?
C3 C2 N1 110.6(12) . . ?
C3 C2 H2A 109.5 . . ?
N1 C2 H2A 109.5 . . ?
C3 C2 H2B 109.5 . . ?
N1 C2 H2B 109.5 . . ?
H2A C2 H2B 108.1 . . ?
C2 C3 C6 114.2(10) . . ?
C2 C3 H3A 108.7 . . ?
C6 C3 H3A 108.7 . . ?
C2 C3 H3B 108.7 . . ?
C6 C3 H3B 108.7 . . ?
H3A C3 H3B 107.6 . . ?
C8 C4 C5 113.8(9) . . ?
C8 C4 H4A 108.8 . . ?
C5 C4 H4A 108.8 . . ?
C8 C4 H4B 108.8 . . ?
C5 C4 H4B 108.8 . . ?
H4A C4 H4B 107.7 . . ?
N2 C5 C4 112.8(9) . . ?
N2 C5 H5A 109.0 . . ?
C4 C5 H5A 109.0 . . ?
N2 C5 H5B 109.0 . . ?
C4 C5 H5B 109.0 . . ?
H5A C5 H5B 107.8 . . ?
O17 C6 O27 125.5(9) . . ?
O17 C6 C3 117.8(10) . . ?
O27 C6 C3 116.7(10) . . ?
O1 C7 O3 125.5(10) . . ?
O1 C7 C1 117.6(10) . . ?
O3 C7 C1 116.9(10) . . ?
O2 C8 O16 126.3(9) . . ?
O2 C8 C4 117.2(9) . . ?
O16 C8 C4 116.6(9) . . ?
C2 N1 H1D 109.5 . . ?
C2 N1 H1E 109.5 . . ?
H1D N1 H1E 109.5 . . ?
C2 N1 H1F 109.5 . . ?
H1D N1 H1F 109.5 . . ?
H1E N1 H1F 109.5 . . ?
C5 N2 H2C 109.5 . . ?
C5 N2 H2D 109.5 . . ?
H2C N2 H2D 109.5 . . ?
C5 N2 H2E 109.5 . . ?
H2C N2 H2E 109.5 . . ?
H2D N2 H2E 109.5 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O13 As1 O9 Mo1 159.5(4) . . . . ?
O14 As1 O9 Mo1 62.5(4) . . . . ?
O13 As1 O9 Mo2 -61.9(4) . . . . ?
O14 As1 O9 Mo2 -159.0(4) . . . . ?
O18 Mo3 O10 Co1 69.8(6) . . . . ?
O25 Mo3 O10 Co1 -31.7(6) . . . . ?
O15 Mo3 O10 Co1 170.0(5) . . . . ?
O13 Mo3 O10 Co1 -114.7(6) . . . . ?
Mo6 Mo3 O10 Co1 -156.9(5) . . . . ?
O14 As1 O13 Mo3 -66.3(4) . . . . ?
O9 As1 O13 Mo3 -163.2(4) . . . . ?
O14 As1 O13 Mo6 161.7(4) . . . . ?
O9 As1 O13 Mo6 64.8(4) . . . . ?
O13 As1 O14 Mo5 -160.7(4) . . . . ?
O9 As1 O14 Mo5 -63.4(4) . . . . ?
O13 As1 O14 Mo4 64.3(4) . . . . ?
O9 As1 O14 Mo4 161.6(4) . . . . ?
O10 Mo3 O18 Co1 -140.2(8) . . . 3_757 ?
O25 Mo3 O18 Co1 -38.9(8) . . . 3_757 ?
O15 Mo3 O18 Co1 119.1(8) . . . 3_757 ?
O13 Mo3 O18 Co1 54.7(15) . . . 3_757 ?
O3 Mo3 O18 Co1 38.1(8) . . . 3_757 ?
Mo6 Mo3 O18 Co1 106.5(8) . . . 3_757 ?
O5 Mo4 O20 Co1 -66.4(6) . . . . ?
O25 Mo4 O20 Co1 37.8(6) . . . . ?
O12 Mo4 O20 Co1 -164.8(5) . . . . ?
O14 Mo4 O20 Co1 121.2(5) . . . . ?
O17 Mo4 O20 Co1 107.6(16) . . . . ?
Mo5 Mo4 O20 Co1 162.4(5) . . . . ?
O26 Mo2 O24 Mo6 -16.1(6) . . . . ?
O4 Mo2 O24 Mo6 -123.1(6) . . . . ?
O11 Mo2 O24 Mo6 111.1(7) . . . . ?
O9 Mo2 O24 Mo6 74.6(6) . . . . ?
O16 Mo2 O24 Mo6 154.7(6) . . . . ?
Mo1 Mo2 O24 Mo6 88.0(6) . . . . ?
O22 Mo6 O24 Mo2 18.8(7) . . . . ?
O7 Mo6 O24 Mo2 125.1(6) . . . . ?
O15 Mo6 O24 Mo2 -106.7(8) . . . . ?
O13 Mo6 O24 Mo2 -72.5(6) . . . . ?
O1 Mo6 O24 Mo2 -152.0(6) . . . . ?
Mo3 Mo6 O24 Mo2 -86.0(6) . . . . ?
O5 Mo4 O25 Mo3 122.6(6) . . . . ?
O20 Mo4 O25 Mo3 15.8(6) . . . . ?
O12 Mo4 O25 Mo3 -108.1(7) . . . . ?
O14 Mo4 O25 Mo3 -74.2(5) . . . . ?
O17 Mo4 O25 Mo3 -153.9(6) . . . . ?
Mo5 Mo4 O25 Mo3 -87.2(6) . . . . ?
N1 C2 C3 C6 -175.8(9) . . . . ?
C8 C4 C5 N2 172.5(10) . . . . ?
Mo4 O17 C6 O27 3.5(15) . . . . ?
Mo4 O17 C6 C3 -176.4(7) . . . . ?
Mo5 O27 C6 O17 -4.3(15) . . . . ?
Mo5 O27 C6 C3 175.6(7) . . . . ?
C2 C3 C6 O17 5.1(14) . . . . ?
C2 C3 C6 O27 -174.8(9) . . . . ?
Mo6 O1 C7 O3 1.1(18) . . . . ?
Mo6 O1 C7 C1 -178.5(9) . . . . ?
Mo3 O3 C7 O1 0.0(17) . . . . ?
Mo3 O3 C7 C1 179.7(9) . . . . ?
Mo1 O2 C8 O16 -1.9(15) . . . . ?
Mo1 O2 C8 C4 178.6(7) . . . . ?
Mo2 O16 C8 O2 -3.3(16) . . . . ?
Mo2 O16 C8 C4 176.2(7) . . . . ?
C5 C4 C8 O2 -160.6(10) . . . . ?
C5 C4 C8 O16 19.9(15) . . . . ?

_refine_diff_density_max         2.004
_refine_diff_density_min         -1.199
_refine_diff_density_rms         0.209

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_11
_database_code_depnum_ccdc_archive 'CCDC 1871481'
_audit_update_record             
;
2018-10-04 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C16 H82 As2 Mo12 N4 O77 Rb2 Zn2'
_chemical_formula_weight         3165.70

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.8717(9)
_cell_length_b                   23.7484(13)
_cell_length_c                   15.8204(9)
_cell_angle_alpha                90
_cell_angle_beta                 119.884(4)
_cell_angle_gamma                90
_cell_volume                     4518.8(5)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    18929
_cell_measurement_theta_min      1.819
_cell_measurement_theta_max      24.998

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.327
_exptl_crystal_F_000             3051
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    4.035
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.379
_exptl_absorpt_correction_T_max  0.429
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            18929
_diffrn_reflns_av_unetI/netI     0.0436
_diffrn_reflns_av_R_equivalents  0.0312
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_theta_min         1.817
_diffrn_reflns_theta_max         24.998
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 0.973
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 0.973
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 0.973
_reflns_number_total             7942
_reflns_number_gt                6801
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0299P)²+173.2499P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         7942
_refine_ls_number_parameters     568
_refine_ls_number_restraints     42
_refine_ls_R_factor_all          0.0871
_refine_ls_R_factor_gt           0.0753
_refine_ls_wR_factor_ref         0.1779
_refine_ls_wR_factor_gt          0.1729
_refine_ls_goodness_of_fit_ref   1.189
_refine_ls_restrained_S_all      1.191
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.63198(9) 0.11984(4) 0.95036(8) 0.0200(3) Uani 1 1 d . . . . .
Mo2 Mo 0.43820(10) 0.20924(5) 0.92062(8) 0.0219(3) Uani 1 1 d . . . . .
Mo3 Mo 0.30496(10) -0.02136(5) 0.62239(9) 0.0235(3) Uani 1 1 d . . . . .
Mo4 Mo 0.56202(10) -0.00177(5) 0.79699(9) 0.0213(3) Uani 1 1 d . . . . .
Mo5 Mo 0.09501(10) 0.07779(5) 0.58871(8) 0.0236(3) Uani 1 1 d . . . . .
Mo6 Mo 0.15997(11) 0.18834(6) 0.73019(9) 0.0320(3) Uani 1 1 d . . . . .
As1 As 0.38040(11) 0.11688(5) 0.72166(9) 0.0179(3) Uani 1 1 d . . . . .
Zn1 Zn 0.0915(3) -0.06357(12) 0.6772(2) 0.0237(7) Uani 0.5 1 d . . P . .
Zn2 Zn 0.8693(3) 0.09503(15) 0.7798(3) 0.0337(8) Uani 0.5 1 d . . P . .
Rb1 Rb 0.33715(15) 0.03922(7) 0.89171(12) 0.0420(4) Uani 1 1 d . . . . .
O1 O 0.6779(9) -0.0334(4) 0.8076(9) 0.041(3) Uani 1 1 d . . . . .
O2 O 0.5553(9) 0.0432(4) 0.6646(8) 0.035(2) Uani 1 1 d . . . . .
O3 O 0.6351(8) 0.1846(4) 0.8407(7) 0.029(2) Uani 1 1 d . . . . .
O4 O 0.2573(8) -0.0498(4) 0.6957(7) 0.031(2) Uani 1 1 d . . . . .
O5 O -0.0209(8) 0.0672(4) 0.4779(8) 0.035(2) Uani 1 1 d . . . . .
O6 O 0.1393(8) 0.1436(4) 0.5078(7) 0.029(2) Uani 1 1 d . . . . .
O7 O 0.4562(9) 0.2755(4) 0.9682(7) 0.035(2) Uani 1 1 d . . . . .
O8 O 0.1808(10) 0.2188(4) 0.6034(7) 0.041(3) Uani 1 1 d . . . . .
O9 O 0.0822(9) 0.0300(5) 0.6650(8) 0.045(3) Uani 1 1 d . . . . .
O10 O 0.0806(10) 0.2476(6) 0.7094(9) 0.064(4) Uani 1 1 d . . . . .
O11 O 0.6210(8) 0.0699(4) 0.8516(7) 0.026(2) Uani 1 1 d . . . . .
O12 O 0.5930(8) 0.1863(4) 0.9982(6) 0.024(2) Uani 1 1 d . . . . .
O13 O 0.2463(7) 0.1153(4) 0.7099(6) 0.0216(19) Uani 1 1 d . . . . .
O14 O 0.4544(7) 0.1333(4) 0.8489(6) 0.023(2) Uani 1 1 d . . . . .
O15 O 0.4037(7) 0.0424(3) 0.7357(6) 0.0202(19) Uani 1 1 d . . . . .
O16 O 0.5094(9) 0.2477(4) 0.8277(7) 0.031(2) Uani 1 1 d . . . . .
O17 O 0.4553(7) -0.0502(4) 0.6937(7) 0.023(2) Uani 1 1 d . . . . .
O18 O 0.3792(8) 0.0301(4) 0.5469(7) 0.029(2) Uani 1 1 d . . . . .
O19 O 0.6069(8) 0.0731(4) 1.0186(7) 0.030(2) Uani 1 1 d . . . . .
O20 O 0.1548(10) 0.1557(6) 0.8242(8) 0.052(3) Uani 1 1 d . . . . .
O21 O 0.3060(9) 0.2191(4) 0.8001(7) 0.030(2) Uani 1 1 d . . . . .
O22 O 0.1999(7) 0.0379(4) 0.5670(6) 0.024(2) Uani 1 1 d . . . . .
O23 O 0.0439(8) 0.1434(4) 0.6254(7) 0.032(2) Uani 1 1 d . . . . .
O24 O 0.3906(8) 0.1709(4) 0.9843(7) 0.031(2) Uani 1 1 d . . . . .
O25 O 0.7734(8) 0.1295(4) 1.0154(8) 0.037(3) Uani 1 1 d . . . . .
O26 O 0.2590(10) -0.0664(4) 0.5258(8) 0.044(3) Uani 1 1 d . . . . .
O27 O 0.5487(9) -0.0303(4) 0.8905(7) 0.034(2) Uani 1 1 d . . . . .
C1 C 0.193(2) 0.2268(8) 0.4590(15) 0.064(6) Uani 1 1 d . . . . .
H1A H 0.2152 0.2643 0.4834 0.097 Uiso 1 1 calc R U . . .
H1B H 0.2513 0.2087 0.4533 0.097 Uiso 1 1 calc R U . . .
H1C H 0.1268 0.2282 0.3962 0.097 Uiso 1 1 calc R U . . .
C2 C 0.3973(19) 0.0970(7) 0.4155(14) 0.056(5) Uani 1 1 d . . . . .
H2A H 0.3631 0.0614 0.3853 0.067 Uiso 1 1 calc R U . . .
H2B H 0.3437 0.1185 0.4245 0.067 Uiso 1 1 calc R U . . .
C3 C 0.4965(16) 0.0861(6) 0.5114(12) 0.041(4) Uani 1 1 d . . . . .
H3A H 0.5271 0.1219 0.5432 0.050 Uiso 1 1 calc R U . . .
H3B H 0.5523 0.0675 0.5014 0.050 Uiso 1 1 calc R U . . .
C4 C 0.5673(15) 0.3241(6) 0.7320(12) 0.036(4) Uani 1 1 d . . . . .
H4A H 0.4869 0.3253 0.7013 0.043 Uiso 1 1 calc R U . . .
H4B H 0.5979 0.3403 0.7966 0.043 Uiso 1 1 calc R U . . .
C5 C 0.6046(14) 0.2630(6) 0.7414(11) 0.038(4) Uani 1 1 d . . . . .
H5A H 0.5672 0.2455 0.6775 0.045 Uiso 1 1 calc R U . . .
H5B H 0.6839 0.2620 0.7650 0.045 Uiso 1 1 calc R U . . .
C6 C 0.4734(14) 0.0499(6) 0.5790(12) 0.033(4) Uani 1 1 d . . . . .
C7 C 0.1692(13) 0.1932(7) 0.5298(11) 0.036(4) Uani 1 1 d . . . . .
C8 C 0.5807(12) 0.2296(5) 0.8094(10) 0.022(3) Uani 1 1 d . . . . .
N1 N 0.4257(15) 0.1282(6) 0.3506(11) 0.057(5) Uani 1 1 d . . . . .
H1D H 0.3643 0.1340 0.2935 0.085 Uiso 1 1 calc R U . . .
H1E H 0.4559 0.1611 0.3776 0.085 Uiso 1 1 calc R U . . .
H1F H 0.4739 0.1082 0.3412 0.085 Uiso 1 1 calc R U . . .
N2 N 0.6023(11) 0.3587(5) 0.6742(9) 0.034(3) Uani 1 1 d . . . . .
H2C H 0.5786 0.3939 0.6707 0.051 Uiso 1 1 calc R U . . .
H2D H 0.6762 0.3584 0.7026 0.051 Uiso 1 1 calc R U . . .
H2E H 0.5733 0.3445 0.6143 0.051 Uiso 1 1 calc R U . . .
O1W O -0.0911(17) -0.0662(9) 0.6501(13) 0.107(6) Uani 1 1 d . U . . .
O2W O 0.1508(11) -0.1519(6) 0.7042(11) 0.064(4) Uani 1 1 d . U . . .
O3W O 0.1425(14) -0.0461(7) 0.8343(12) 0.087(5) Uani 1 1 d . U . . .
O4W O 0.939(2) 0.1708(9) 0.8483(18) 0.051(6) Uani 0.5 1 d . . P . .
O5W O 0.8722(19) 0.0645(11) 0.9088(19) 0.054(7) Uani 0.5 1 d . . P . .
O6W O 1.031(2) 0.0559(13) 0.8356(19) 0.063(8) Uani 0.5 1 d . . P . .
O7W O 0.795(2) 0.0202(10) 0.708(2) 0.069(9) Uani 0.5 1 d . . P . .
O8W O 0.8698(15) 0.1170(9) 0.6552(13) 0.030(4) Uani 0.5 1 d . U P . .
O9W O 0.7146(16) 0.1281(7) 0.7319(15) 0.025(4) Uani 0.5 1 d . . P . .
OW1 O 0.100(5) 0.1276(18) 0.207(4) 0.16(2) Uani 0.5 1 d . . P . .
OW2 O 0.269(2) 0.7819(13) 0.447(2) 0.079(9) Uani 0.5 1 d . U P . .
OW3 O 0.064(3) 0.6984(15) 0.490(2) 0.089(10) Uani 0.5 1 d . U P . .
OW4 O 0.258(2) 0.1691(8) 0.173(2) 0.164(11) Uani 1 1 d . . . . .
OW5 O 0.103(2) 0.7385(11) 0.276(2) 0.167(11) Uani 1 1 d . . . . .
OW6 O 0.223(2) 0.0998(13) 0.0036(19) 0.170(12) Uani 1 1 d . . . . .
OW7 O 0.1421(18) 0.6944(9) 0.0400(15) 0.121(7) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O19 1.701(9) . ?
Mo1 O25 1.717(10) . ?
Mo1 O11 1.906(9) . ?
Mo1 O12 1.940(9) . ?
Mo1 O14 2.192(9) . ?
Mo1 O3 2.335(9) . ?
Mo1 Mo2 3.2702(16) . ?
Mo1 Rb1 4.180(2) . ?
Mo1 Rb1 4.4305(18) 3_657 ?
Mo2 O24 1.715(10) . ?
Mo2 O7 1.709(9) . ?
Mo2 O21 1.889(10) . ?
Mo2 O12 1.946(9) . ?
Mo2 O14 2.201(8) . ?
Mo2 O16 2.327(10) . ?
Mo2 Rb1 4.2234(19) . ?
Mo3 O26 1.708(10) . ?
Mo3 O4 1.733(10) . ?
Mo3 O22 1.898(9) . ?
Mo3 O17 1.935(9) . ?
Mo3 O15 2.221(8) . ?
Mo3 O18 2.281(10) . ?
Mo3 Mo4 3.2783(17) . ?
Mo3 Rb1 4.304(2) . ?
Mo4 O1 1.705(10) . ?
Mo4 O27 1.719(10) . ?
Mo4 O11 1.900(9) . ?
Mo4 O17 1.943(9) . ?
Mo4 O15 2.177(9) . ?
Mo4 O2 2.311(10) . ?
Mo4 Rb1 4.193(2) . ?
Mo5 O5 1.707(10) . ?
Mo5 O9 1.729(10) . ?
Mo5 O22 1.905(9) . ?
Mo5 O23 1.917(10) . ?
Mo5 O13 2.206(9) . ?
Mo5 O6 2.290(9) . ?
Mo5 Mo6 3.2718(18) . ?
Mo5 Rb1 4.365(2) . ?
Mo6 O20 1.710(12) . ?
Mo6 O10 1.715(11) . ?
Mo6 O21 1.905(11) . ?
Mo6 O23 1.955(10) . ?
Mo6 O13 2.220(9) . ?
Mo6 O8 2.282(11) . ?
Mo6 Rb1 4.342(2) . ?
As1 O13 1.775(9) . ?
As1 O14 1.788(9) . ?
As1 O15 1.792(8) . ?
As1 Rb1 3.551(2) . ?
Zn1 O5 2.143(11) 3_556 ?
Zn1 O4 2.192(10) . ?
Zn1 O2W 2.216(14) . ?
Zn1 O9 2.230(12) . ?
Zn1 O3W 2.258(18) . ?
Zn1 O1W 2.35(2) . ?
Zn1 Rb1 4.191(3) . ?
Zn2 O8W 2.042(19) . ?
Zn2 O9W 2.043(19) . ?
Zn2 O4W 2.07(2) . ?
Zn2 O7W 2.08(2) . ?
Zn2 O5W 2.15(3) . ?
Zn2 O6W 2.17(3) . ?
Rb1 O19 2.939(9) 3_657 ?
Rb1 O27 2.998(10) 3_657 ?
Rb1 O14 3.033(9) . ?
Rb1 O15 3.037(9) . ?
Rb1 O13 3.084(8) . ?
Rb1 O3W 3.127(17) . ?
Rb1 OW6 3.24(3) 1_556 ?
Rb1 O19 3.346(11) . ?
Rb1 O24 3.376(10) . ?
Rb1 O27 3.375(11) . ?
Rb1 O4 3.449(10) . ?
Rb1 O20 3.536(14) . ?
O2 C6 1.272(19) . ?
O3 C8 1.258(15) . ?
O5 Zn1 2.143(11) 3_556 ?
O6 C7 1.240(18) . ?
O8 C7 1.250(19) . ?
O16 C8 1.239(16) . ?
O18 C6 1.235(18) . ?
O19 Rb1 2.939(9) 3_657 ?
O27 Rb1 2.998(10) 3_657 ?
C1 C7 1.54(2) . ?
C1 H1A 0.9600 . ?
C1 H1B 0.9600 . ?
C1 H1C 0.9600 . ?
C2 N1 1.47(2) . ?
C2 C3 1.48(3) . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
C3 C6 1.525(19) . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
C4 N2 1.479(18) . ?
C4 C5 1.52(2) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 C8 1.501(19) . ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
N1 H1D 0.8900 . ?
N1 H1E 0.8900 . ?
N1 H1F 0.8900 . ?
N2 H2C 0.8900 . ?
N2 H2D 0.8900 . ?
N2 H2E 0.8900 . ?
OW6 Rb1 3.24(3) 1_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O19 Mo1 O25 103.9(5) . . ?
O19 Mo1 O11 99.0(4) . . ?
O25 Mo1 O11 100.1(5) . . ?
O19 Mo1 O12 95.6(4) . . ?
O25 Mo1 O12 96.6(4) . . ?
O11 Mo1 O12 154.4(4) . . ?
O19 Mo1 O14 92.9(4) . . ?
O25 Mo1 O14 161.9(4) . . ?
O11 Mo1 O14 83.6(4) . . ?
O12 Mo1 O14 74.7(3) . . ?
O19 Mo1 O3 170.7(4) . . ?
O25 Mo1 O3 85.3(4) . . ?
O11 Mo1 O3 79.9(4) . . ?
O12 Mo1 O3 82.3(4) . . ?
O14 Mo1 O3 77.9(3) . . ?
O19 Mo1 Mo2 95.8(3) . . ?
O25 Mo1 Mo2 127.7(3) . . ?
O11 Mo1 Mo2 124.2(3) . . ?
O12 Mo1 Mo2 32.8(3) . . ?
O14 Mo1 Mo2 42.0(2) . . ?
O3 Mo1 Mo2 77.5(2) . . ?
O19 Mo1 Rb1 49.9(3) . . ?
O25 Mo1 Rb1 153.3(4) . . ?
O11 Mo1 Rb1 82.1(3) . . ?
O12 Mo1 Rb1 91.5(3) . . ?
O14 Mo1 Rb1 44.5(2) . . ?
O3 Mo1 Rb1 121.0(2) . . ?
Mo2 Mo1 Rb1 67.80(4) . . ?
O19 Mo1 Rb1 22.9(3) . 3_657 ?
O25 Mo1 Rb1 90.9(4) . 3_657 ?
O11 Mo1 Rb1 83.0(3) . 3_657 ?
O12 Mo1 Rb1 116.2(3) . 3_657 ?
O14 Mo1 Rb1 107.2(2) . 3_657 ?
O3 Mo1 Rb1 161.5(2) . 3_657 ?
Mo2 Mo1 Rb1 118.44(4) . 3_657 ?
Rb1 Mo1 Rb1 62.85(4) . 3_657 ?
O24 Mo2 O7 104.1(5) . . ?
O24 Mo2 O21 101.2(5) . . ?
O7 Mo2 O21 100.7(5) . . ?
O24 Mo2 O12 96.2(4) . . ?
O7 Mo2 O12 96.1(5) . . ?
O21 Mo2 O12 151.9(4) . . ?
O24 Mo2 O14 92.1(4) . . ?
O7 Mo2 O14 162.2(4) . . ?
O21 Mo2 O14 83.0(4) . . ?
O12 Mo2 O14 74.4(3) . . ?
O24 Mo2 O16 171.1(4) . . ?
O7 Mo2 O16 84.4(4) . . ?
O21 Mo2 O16 79.5(4) . . ?
O12 Mo2 O16 80.0(4) . . ?
O14 Mo2 O16 79.1(3) . . ?
O24 Mo2 Mo1 95.8(3) . . ?
O7 Mo2 Mo1 127.3(4) . . ?
O21 Mo2 Mo1 122.7(3) . . ?
O12 Mo2 Mo1 32.6(3) . . ?
O14 Mo2 Mo1 41.8(2) . . ?
O16 Mo2 Mo1 76.6(2) . . ?
O24 Mo2 Rb1 49.6(3) . . ?
O7 Mo2 Rb1 153.7(4) . . ?
O21 Mo2 Rb1 84.6(3) . . ?
O12 Mo2 Rb1 90.2(3) . . ?
O14 Mo2 Rb1 43.5(2) . . ?
O16 Mo2 Rb1 122.0(2) . . ?
Mo1 Mo2 Rb1 66.40(4) . . ?
O26 Mo3 O4 104.9(5) . . ?
O26 Mo3 O22 101.1(5) . . ?
O4 Mo3 O22 97.9(4) . . ?
O26 Mo3 O17 96.5(5) . . ?
O4 Mo3 O17 97.6(4) . . ?
O22 Mo3 O17 152.6(4) . . ?
O26 Mo3 O15 162.6(5) . . ?
O4 Mo3 O15 90.8(4) . . ?
O22 Mo3 O15 83.7(3) . . ?
O17 Mo3 O15 73.6(3) . . ?
O26 Mo3 O18 86.0(5) . . ?
O4 Mo3 O18 169.0(4) . . ?
O22 Mo3 O18 78.7(4) . . ?
O17 Mo3 O18 81.8(4) . . ?
O15 Mo3 O18 78.5(3) . . ?
O26 Mo3 Mo4 127.4(4) . . ?
O4 Mo3 Mo4 96.3(3) . . ?
O22 Mo3 Mo4 123.1(3) . . ?
O17 Mo3 Mo4 32.4(3) . . ?
O15 Mo3 Mo4 41.3(2) . . ?
O18 Mo3 Mo4 77.3(3) . . ?
O26 Mo3 Rb1 154.7(4) . . ?
O4 Mo3 Rb1 49.8(3) . . ?
O22 Mo3 Rb1 83.5(3) . . ?
O17 Mo3 Rb1 89.5(3) . . ?
O15 Mo3 Rb1 41.9(2) . . ?
O18 Mo3 Rb1 119.2(2) . . ?
Mo4 Mo3 Rb1 65.52(4) . . ?
O1 Mo4 O27 104.0(5) . . ?
O1 Mo4 O11 100.3(5) . . ?
O27 Mo4 O11 99.7(4) . . ?
O1 Mo4 O17 96.2(4) . . ?
O27 Mo4 O17 97.3(4) . . ?
O11 Mo4 O17 152.6(4) . . ?
O1 Mo4 O15 161.5(5) . . ?
O27 Mo4 O15 93.2(4) . . ?
O11 Mo4 O15 83.2(3) . . ?
O17 Mo4 O15 74.5(3) . . ?
O1 Mo4 O2 84.4(5) . . ?
O27 Mo4 O2 171.5(4) . . ?
O11 Mo4 O2 79.2(4) . . ?
O17 Mo4 O2 80.8(4) . . ?
O15 Mo4 O2 78.3(4) . . ?
O1 Mo4 Mo3 126.6(4) . . ?
O27 Mo4 Mo3 97.5(3) . . ?
O11 Mo4 Mo3 123.5(3) . . ?
O17 Mo4 Mo3 32.2(3) . . ?
O15 Mo4 Mo3 42.3(2) . . ?
O2 Mo4 Mo3 76.5(3) . . ?
O1 Mo4 Rb1 154.1(4) . . ?
O27 Mo4 Rb1 50.6(3) . . ?
O11 Mo4 Rb1 81.8(3) . . ?
O17 Mo4 Rb1 92.7(3) . . ?
O15 Mo4 Rb1 44.2(2) . . ?
O2 Mo4 Rb1 121.0(3) . . ?
Mo3 Mo4 Rb1 69.11(4) . . ?
O5 Mo5 O9 104.4(5) . . ?
O5 Mo5 O22 98.9(5) . . ?
O9 Mo5 O22 98.8(5) . . ?
O5 Mo5 O23 97.4(5) . . ?
O9 Mo5 O23 98.0(5) . . ?
O22 Mo5 O23 152.8(4) . . ?
O5 Mo5 O13 162.5(4) . . ?
O9 Mo5 O13 92.4(4) . . ?
O22 Mo5 O13 82.9(4) . . ?
O23 Mo5 O13 75.2(4) . . ?
O5 Mo5 O6 84.5(4) . . ?
O9 Mo5 O6 171.0(4) . . ?
O22 Mo5 O6 78.3(4) . . ?
O23 Mo5 O6 81.8(4) . . ?
O13 Mo5 O6 78.9(3) . . ?
O5 Mo5 Mo6 128.2(4) . . ?
O9 Mo5 Mo6 97.9(4) . . ?
O22 Mo5 Mo6 123.2(3) . . ?
O23 Mo5 Mo6 32.7(3) . . ?
O13 Mo5 Mo6 42.5(2) . . ?
O6 Mo5 Mo6 77.0(2) . . ?
O5 Mo5 Rb1 155.9(3) . . ?
O9 Mo5 Rb1 52.1(4) . . ?
O22 Mo5 Rb1 81.6(3) . . ?
O23 Mo5 Rb1 92.1(3) . . ?
O13 Mo5 Rb1 41.5(2) . . ?
O6 Mo5 Rb1 118.9(2) . . ?
Mo6 Mo5 Rb1 67.55(4) . . ?
O20 Mo6 O10 103.7(7) . . ?
O20 Mo6 O21 99.3(5) . . ?
O10 Mo6 O21 101.1(6) . . ?
O20 Mo6 O23 96.7(5) . . ?
O10 Mo6 O23 96.1(5) . . ?
O21 Mo6 O23 152.9(4) . . ?
O20 Mo6 O13 91.8(5) . . ?
O10 Mo6 O13 162.7(5) . . ?
O21 Mo6 O13 83.6(4) . . ?
O23 Mo6 O13 74.1(4) . . ?
O20 Mo6 O8 170.6(5) . . ?
O10 Mo6 O8 85.5(6) . . ?
O21 Mo6 O8 79.9(4) . . ?
O23 Mo6 O8 80.7(4) . . ?
O13 Mo6 O8 78.9(3) . . ?
O20 Mo6 Mo5 96.6(4) . . ?
O10 Mo6 Mo5 126.5(4) . . ?
O21 Mo6 Mo5 123.8(3) . . ?
O23 Mo6 Mo5 32.0(3) . . ?
O13 Mo6 Mo5 42.2(2) . . ?
O8 Mo6 Mo5 76.4(3) . . ?
O20 Mo6 Rb1 51.3(4) . . ?
O10 Mo6 Rb1 154.6(5) . . ?
O21 Mo6 Rb1 81.1(3) . . ?
O23 Mo6 Rb1 92.2(3) . . ?
O13 Mo6 Rb1 42.2(2) . . ?
O8 Mo6 Rb1 119.5(3) . . ?
Mo5 Mo6 Rb1 68.31(4) . . ?
O13 As1 O14 96.1(4) . . ?
O13 As1 O15 96.1(4) . . ?
O14 As1 O15 96.3(4) . . ?
O13 As1 Rb1 60.3(3) . . ?
O14 As1 Rb1 58.6(3) . . ?
O15 As1 Rb1 58.8(3) . . ?
O5 Zn1 O4 90.6(4) 3_556 . ?
O5 Zn1 O2W 95.5(5) 3_556 . ?
O4 Zn1 O2W 81.5(4) . . ?
O5 Zn1 O9 88.2(4) 3_556 . ?
O4 Zn1 O9 82.8(4) . . ?
O2W Zn1 O9 163.9(5) . . ?
O5 Zn1 O3W 169.0(5) 3_556 . ?
O4 Zn1 O3W 95.4(5) . . ?
O2W Zn1 O3W 94.5(6) . . ?
O9 Zn1 O3W 83.4(5) . . ?
O5 Zn1 O1W 87.4(5) 3_556 . ?
O4 Zn1 O1W 172.6(6) . . ?
O2W Zn1 O1W 105.8(6) . . ?
O9 Zn1 O1W 90.0(6) . . ?
O3W Zn1 O1W 85.6(6) . . ?
O5 Zn1 Rb1 132.4(3) 3_556 . ?
O4 Zn1 Rb1 55.2(3) . . ?
O2W Zn1 Rb1 108.8(4) . . ?
O9 Zn1 Rb1 58.5(3) . . ?
O3W Zn1 Rb1 47.1(4) . . ?
O1W Zn1 Rb1 122.0(5) . . ?
O8W Zn2 O9W 93.0(8) . . ?
O8W Zn2 O4W 93.4(9) . . ?
O9W Zn2 O4W 89.3(9) . . ?
O8W Zn2 O7W 86.2(11) . . ?
O9W Zn2 O7W 89.0(9) . . ?
O4W Zn2 O7W 178.3(11) . . ?
O8W Zn2 O5W 174.9(9) . . ?
O9W Zn2 O5W 90.1(8) . . ?
O4W Zn2 O5W 90.7(10) . . ?
O7W Zn2 O5W 89.8(12) . . ?
O8W Zn2 O6W 90.1(9) . . ?
O9W Zn2 O6W 176.3(9) . . ?
O4W Zn2 O6W 92.5(11) . . ?
O7W Zn2 O6W 89.2(11) . . ?
O5W Zn2 O6W 86.7(9) . . ?
O19 Rb1 O27 61.3(3) 3_657 3_657 ?
O19 Rb1 O14 137.3(3) 3_657 . ?
O27 Rb1 O14 105.9(3) 3_657 . ?
O19 Rb1 O15 107.5(2) 3_657 . ?
O27 Rb1 O15 137.3(3) 3_657 . ?
O14 Rb1 O15 52.1(2) . . ?
O19 Rb1 O13 150.3(3) 3_657 . ?
O27 Rb1 O13 148.2(3) 3_657 . ?
O14 Rb1 O13 51.4(2) . . ?
O15 Rb1 O13 51.4(2) . . ?
O19 Rb1 O3W 62.2(4) 3_657 . ?
O27 Rb1 O3W 100.0(4) 3_657 . ?
O14 Rb1 O3W 153.4(4) . . ?
O15 Rb1 O3W 110.4(4) . . ?
O13 Rb1 O3W 102.5(4) . . ?
O19 Rb1 OW6 102.9(5) 3_657 1_556 ?
O27 Rb1 OW6 61.6(5) 3_657 1_556 ?
O14 Rb1 OW6 104.9(6) . 1_556 ?
O15 Rb1 OW6 149.6(5) . 1_556 ?
O13 Rb1 OW6 99.6(4) . 1_556 ?
O3W Rb1 OW6 82.0(7) . 1_556 ?
O19 Rb1 O19 88.9(3) 3_657 . ?
O27 Rb1 O19 62.3(3) 3_657 . ?
O14 Rb1 O19 52.6(2) . . ?
O15 Rb1 O19 77.3(2) . . ?
O13 Rb1 O19 103.5(2) . . ?
O3W Rb1 O19 151.1(3) . . ?
OW6 Rb1 O19 105.6(6) 1_556 . ?
O19 Rb1 O24 133.1(3) 3_657 . ?
O27 Rb1 O24 72.0(3) 3_657 . ?
O14 Rb1 O24 52.3(2) . . ?
O15 Rb1 O24 103.9(2) . . ?
O13 Rb1 O24 76.2(2) . . ?
O3W Rb1 O24 134.2(4) . . ?
OW6 Rb1 O24 54.0(6) 1_556 . ?
O19 Rb1 O24 65.1(2) . . ?
O19 Rb1 O27 62.5(2) 3_657 . ?
O27 Rb1 O27 90.5(3) 3_657 . ?
O14 Rb1 O27 78.1(2) . . ?
O15 Rb1 O27 52.4(2) . . ?
O13 Rb1 O27 103.5(2) . . ?
O3W Rb1 O27 108.0(4) . . ?
OW6 Rb1 O27 151.9(5) 1_556 . ?
O19 Rb1 O27 53.5(2) . . ?
O24 Rb1 O27 116.9(2) . . ?
O19 Rb1 O4 76.5(2) 3_657 . ?
O27 Rb1 O4 137.7(3) 3_657 . ?
O14 Rb1 O4 102.6(2) . . ?
O15 Rb1 O4 51.4(2) . . ?
O13 Rb1 O4 73.8(2) . . ?
O3W Rb1 O4 59.8(4) . . ?
OW6 Rb1 O4 137.6(6) 1_556 . ?
O19 Rb1 O4 116.7(2) . . ?
O24 Rb1 O4 149.4(2) . . ?
O27 Rb1 O4 65.5(2) . . ?
O19 Rb1 O20 146.4(3) 3_657 . ?
O27 Rb1 O20 106.9(3) 3_657 . ?
O14 Rb1 O20 74.8(3) . . ?
O15 Rb1 O20 101.3(2) . . ?
O13 Rb1 O20 50.3(2) . . ?
O3W Rb1 O20 92.0(4) . . ?
OW6 Rb1 O20 49.2(4) 1_556 . ?
O19 Rb1 O20 114.3(3) . . ?
O24 Rb1 O20 51.3(3) . . ?
O27 Rb1 O20 150.9(3) . . ?
O4 Rb1 O20 110.3(2) . . ?
C6 O2 Mo4 129.4(9) . . ?
C8 O3 Mo1 128.5(9) . . ?
Mo3 O4 Zn1 133.9(5) . . ?
Mo3 O4 Rb1 107.7(4) . . ?
Zn1 O4 Rb1 93.3(3) . . ?
Mo5 O5 Zn1 147.3(6) . 3_556 ?
C7 O6 Mo5 129.6(10) . . ?
C7 O8 Mo6 130.6(10) . . ?
Mo5 O9 Zn1 133.8(7) . . ?
Mo5 O9 Rb1 105.4(4) . . ?
Zn1 O9 Rb1 89.3(3) . . ?
Mo4 O11 Mo1 140.4(5) . . ?
Mo1 O12 Mo2 114.6(4) . . ?
As1 O13 Mo5 126.4(5) . . ?
As1 O13 Mo6 125.5(5) . . ?
Mo5 O13 Mo6 95.3(3) . . ?
As1 O13 Rb1 89.7(3) . . ?
Mo5 O13 Rb1 110.1(3) . . ?
Mo6 O13 Rb1 108.8(3) . . ?
As1 O14 Mo1 126.7(5) . . ?
As1 O14 Mo2 127.6(5) . . ?
Mo1 O14 Mo2 96.2(3) . . ?
As1 O14 Rb1 91.1(3) . . ?
Mo1 O14 Rb1 105.1(3) . . ?
Mo2 O14 Rb1 106.5(3) . . ?
As1 O15 Mo4 127.6(4) . . ?
As1 O15 Mo3 124.9(4) . . ?
Mo4 O15 Mo3 96.4(3) . . ?
As1 O15 Rb1 90.9(3) . . ?
Mo4 O15 Rb1 105.9(3) . . ?
Mo3 O15 Rb1 108.9(3) . . ?
C8 O16 Mo2 130.6(8) . . ?
Mo3 O17 Mo4 115.4(4) . . ?
C6 O18 Mo3 130.5(10) . . ?
Mo1 O19 Rb1 144.1(5) . 3_657 ?
Mo1 O19 Rb1 107.3(4) . . ?
Rb1 O19 Rb1 91.1(3) 3_657 . ?
Mo6 O20 Rb1 106.5(5) . . ?
Mo2 O21 Mo6 139.0(5) . . ?
Mo3 O22 Mo5 139.9(5) . . ?
Mo5 O23 Mo6 115.4(5) . . ?
Mo2 O24 Rb1 107.6(4) . . ?
Mo4 O27 Rb1 142.7(5) . 3_657 ?
Mo4 O27 Rb1 106.2(4) . . ?
Rb1 O27 Rb1 89.5(3) 3_657 . ?
C7 C1 H1A 109.5 . . ?
C7 C1 H1B 109.5 . . ?
H1A C1 H1B 109.5 . . ?
C7 C1 H1C 109.5 . . ?
H1A C1 H1C 109.5 . . ?
H1B C1 H1C 109.5 . . ?
N1 C2 C3 111.8(17) . . ?
N1 C2 H2A 109.3 . . ?
C3 C2 H2A 109.3 . . ?
N1 C2 H2B 109.3 . . ?
C3 C2 H2B 109.3 . . ?
H2A C2 H2B 107.9 . . ?
C2 C3 C6 114.0(15) . . ?
C2 C3 H3A 108.8 . . ?
C6 C3 H3A 108.8 . . ?
C2 C3 H3B 108.8 . . ?
C6 C3 H3B 108.8 . . ?
H3A C3 H3B 107.7 . . ?
N2 C4 C5 112.9(13) . . ?
N2 C4 H4A 109.0 . . ?
C5 C4 H4A 109.0 . . ?
N2 C4 H4B 109.0 . . ?
C5 C4 H4B 109.0 . . ?
H4A C4 H4B 107.8 . . ?
C8 C5 C4 112.9(12) . . ?
C8 C5 H5A 109.0 . . ?
C4 C5 H5A 109.0 . . ?
C8 C5 H5B 109.0 . . ?
C4 C5 H5B 109.0 . . ?
H5A C5 H5B 107.8 . . ?
O18 C6 O2 126.2(13) . . ?
O18 C6 C3 118.4(15) . . ?
O2 C6 C3 115.4(14) . . ?
O6 C7 O8 126.4(14) . . ?
O6 C7 C1 116.8(15) . . ?
O8 C7 C1 116.8(15) . . ?
O16 C8 O3 126.5(12) . . ?
O16 C8 C5 118.1(11) . . ?
O3 C8 C5 115.3(12) . . ?
C2 N1 H1D 109.5 . . ?
C2 N1 H1E 109.5 . . ?
H1D N1 H1E 109.5 . . ?
C2 N1 H1F 109.5 . . ?
H1D N1 H1F 109.5 . . ?
H1E N1 H1F 109.5 . . ?
C4 N2 H2C 109.5 . . ?
C4 N2 H2D 109.5 . . ?
H2C N2 H2D 109.5 . . ?
C4 N2 H2E 109.5 . . ?
H2C N2 H2E 109.5 . . ?
H2D N2 H2E 109.5 . . ?
Zn1 O3W Rb1 101.0(6) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O26 Mo3 O4 Zn1 -65.4(8) . . . . ?
O22 Mo3 O4 Zn1 38.4(8) . . . . ?
O17 Mo3 O4 Zn1 -164.2(7) . . . . ?
O15 Mo3 O4 Zn1 122.2(7) . . . . ?
O18 Mo3 O4 Zn1 110(2) . . . . ?
Mo4 Mo3 O4 Zn1 163.2(6) . . . . ?
Rb1 Mo3 O4 Zn1 112.9(8) . . . . ?
O26 Mo3 O4 Rb1 -178.3(4) . . . . ?
O22 Mo3 O4 Rb1 -74.5(4) . . . . ?
O17 Mo3 O4 Rb1 82.9(4) . . . . ?
O15 Mo3 O4 Rb1 9.3(3) . . . . ?
O18 Mo3 O4 Rb1 -3(2) . . . . ?
Mo4 Mo3 O4 Rb1 50.3(3) . . . . ?
O9 Mo5 O5 Zn1 -142.6(11) . . . 3_556 ?
O22 Mo5 O5 Zn1 -41.0(11) . . . 3_556 ?
O23 Mo5 O5 Zn1 117.1(11) . . . 3_556 ?
O13 Mo5 O5 Zn1 54(2) . . . 3_556 ?
O6 Mo5 O5 Zn1 36.1(11) . . . 3_556 ?
Mo6 Mo5 O5 Zn1 104.9(11) . . . 3_556 ?
Rb1 Mo5 O5 Zn1 -130.5(8) . . . 3_556 ?
O5 Mo5 O9 Zn1 69.4(9) . . . . ?
O22 Mo5 O9 Zn1 -32.3(8) . . . . ?
O23 Mo5 O9 Zn1 169.2(8) . . . . ?
O13 Mo5 O9 Zn1 -115.4(8) . . . . ?
Mo6 Mo5 O9 Zn1 -157.8(7) . . . . ?
Rb1 Mo5 O9 Zn1 -104.4(9) . . . . ?
O5 Mo5 O9 Rb1 173.8(4) . . . . ?
O22 Mo5 O9 Rb1 72.1(4) . . . . ?
O23 Mo5 O9 Rb1 -86.4(4) . . . . ?
O13 Mo5 O9 Rb1 -11.0(4) . . . . ?
Mo6 Mo5 O9 Rb1 -53.4(4) . . . . ?
O1 Mo4 O11 Mo1 -126.0(8) . . . . ?
O27 Mo4 O11 Mo1 -19.7(9) . . . . ?
O17 Mo4 O11 Mo1 107.9(10) . . . . ?
O15 Mo4 O11 Mo1 72.4(8) . . . . ?
O2 Mo4 O11 Mo1 151.8(8) . . . . ?
Mo3 Mo4 O11 Mo1 86.1(8) . . . . ?
Rb1 Mo4 O11 Mo1 27.8(7) . . . . ?
O14 As1 O13 Mo5 -163.5(5) . . . . ?
O15 As1 O13 Mo5 -66.5(6) . . . . ?
Rb1 As1 O13 Mo5 -115.1(6) . . . . ?
O14 As1 O13 Mo6 64.7(6) . . . . ?
O15 As1 O13 Mo6 161.7(5) . . . . ?
Rb1 As1 O13 Mo6 113.1(6) . . . . ?
O14 As1 O13 Rb1 -48.4(3) . . . . ?
O15 As1 O13 Rb1 48.6(3) . . . . ?
O13 As1 O14 Mo1 159.4(6) . . . . ?
O15 As1 O14 Mo1 62.5(6) . . . . ?
Rb1 As1 O14 Mo1 109.9(6) . . . . ?
O13 As1 O14 Mo2 -62.4(6) . . . . ?
O15 As1 O14 Mo2 -159.3(6) . . . . ?
Rb1 As1 O14 Mo2 -112.0(6) . . . . ?
O13 As1 O14 Rb1 49.5(3) . . . . ?
O15 As1 O14 Rb1 -47.3(3) . . . . ?
O13 As1 O15 Mo4 -160.5(6) . . . . ?
O14 As1 O15 Mo4 -63.7(6) . . . . ?
Rb1 As1 O15 Mo4 -110.9(6) . . . . ?
O13 As1 O15 Mo3 64.4(6) . . . . ?
O14 As1 O15 Mo3 161.2(5) . . . . ?
Rb1 As1 O15 Mo3 114.0(6) . . . . ?
O13 As1 O15 Rb1 -49.6(3) . . . . ?
O14 As1 O15 Rb1 47.3(4) . . . . ?
O25 Mo1 O19 Rb1 -56.9(9) . . . 3_657 ?
O11 Mo1 O19 Rb1 46.0(9) . . . 3_657 ?
O12 Mo1 O19 Rb1 -155.1(8) . . . 3_657 ?
O14 Mo1 O19 Rb1 130.0(8) . . . 3_657 ?
Mo2 Mo1 O19 Rb1 172.0(8) . . . 3_657 ?
Rb1 Mo1 O19 Rb1 117.6(10) . . . 3_657 ?
O25 Mo1 O19 Rb1 -174.5(4) . . . . ?
O11 Mo1 O19 Rb1 -71.6(4) . . . . ?
O12 Mo1 O19 Rb1 87.3(4) . . . . ?
O14 Mo1 O19 Rb1 12.3(4) . . . . ?
Mo2 Mo1 O19 Rb1 54.3(3) . . . . ?
Rb1 Mo1 O19 Rb1 -117.6(10) 3_657 . . . ?
O10 Mo6 O20 Rb1 -174.5(5) . . . . ?
O21 Mo6 O20 Rb1 -70.5(5) . . . . ?
O23 Mo6 O20 Rb1 87.5(4) . . . . ?
O13 Mo6 O20 Rb1 13.3(4) . . . . ?
Mo5 Mo6 O20 Rb1 55.3(4) . . . . ?
O24 Mo2 O21 Mo6 -15.8(9) . . . . ?
O7 Mo2 O21 Mo6 -122.7(8) . . . . ?
O12 Mo2 O21 Mo6 111.4(10) . . . . ?
O14 Mo2 O21 Mo6 74.9(8) . . . . ?
O16 Mo2 O21 Mo6 155.1(8) . . . . ?
Mo1 Mo2 O21 Mo6 88.6(8) . . . . ?
Rb1 Mo2 O21 Mo6 31.2(7) . . . . ?
O26 Mo3 O22 Mo5 123.3(8) . . . . ?
O4 Mo3 O22 Mo5 16.3(8) . . . . ?
O17 Mo3 O22 Mo5 -107.5(10) . . . . ?
O15 Mo3 O22 Mo5 -73.6(7) . . . . ?
O18 Mo3 O22 Mo5 -153.1(8) . . . . ?
Mo4 Mo3 O22 Mo5 -86.5(8) . . . . ?
Rb1 Mo3 O22 Mo5 -31.5(7) . . . . ?
O7 Mo2 O24 Rb1 177.1(4) . . . . ?
O21 Mo2 O24 Rb1 72.9(4) . . . . ?
O12 Mo2 O24 Rb1 -84.9(4) . . . . ?
O14 Mo2 O24 Rb1 -10.4(4) . . . . ?
Mo1 Mo2 O24 Rb1 -52.1(3) . . . . ?
O1 Mo4 O27 Rb1 62.8(9) . . . 3_657 ?
O11 Mo4 O27 Rb1 -40.5(9) . . . 3_657 ?
O17 Mo4 O27 Rb1 161.1(8) . . . 3_657 ?
O15 Mo4 O27 Rb1 -124.1(8) . . . 3_657 ?
Mo3 Mo4 O27 Rb1 -166.4(7) . . . 3_657 ?
Rb1 Mo4 O27 Rb1 -111.4(9) . . . 3_657 ?
O1 Mo4 O27 Rb1 174.2(4) . . . . ?
O11 Mo4 O27 Rb1 70.9(4) . . . . ?
O17 Mo4 O27 Rb1 -87.5(4) . . . . ?
O15 Mo4 O27 Rb1 -12.7(4) . . . . ?
Mo3 Mo4 O27 Rb1 -55.0(3) . . . . ?
N1 C2 C3 C6 -175.5(13) . . . . ?
N2 C4 C5 C8 173.4(13) . . . . ?
Mo3 O18 C6 O2 4(2) . . . . ?
Mo3 O18 C6 C3 -176.1(9) . . . . ?
Mo4 O2 C6 O18 -5(2) . . . . ?
Mo4 O2 C6 C3 175.2(9) . . . . ?
C2 C3 C6 O18 5(2) . . . . ?
C2 C3 C6 O2 -175.1(13) . . . . ?
Mo5 O6 C7 O8 -1(2) . . . . ?
Mo5 O6 C7 C1 -179.9(12) . . . . ?
Mo6 O8 C7 O6 2(2) . . . . ?
Mo6 O8 C7 C1 -178.6(12) . . . . ?
Mo2 O16 C8 O3 -2(2) . . . . ?
Mo2 O16 C8 C5 176.5(10) . . . . ?
Mo1 O3 C8 O16 -3(2) . . . . ?
Mo1 O3 C8 C5 178.1(9) . . . . ?
C4 C5 C8 O16 20(2) . . . . ?
C4 C5 C8 O3 -161.4(13) . . . . ?

_refine_diff_density_max         1.697
_refine_diff_density_min         -1.462
_refine_diff_density_rms         0.230

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_8
_database_code_depnum_ccdc_archive 'CCDC 1871478'
_audit_update_record             
;
2018-10-08 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H83 Cs4 K Mn Mo12 N6 O76 Te2'
_chemical_formula_weight         3920.30

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.651(3)
_cell_length_b                   12.303(4)
_cell_length_c                   18.630(5)
_cell_angle_alpha                74.094(12)
_cell_angle_beta                 85.386(13)
_cell_angle_gamma                84.132(12)
_cell_volume                     2551.0(13)
_cell_formula_units_Z            1
_cell_measurement_temperature    220(2)
_cell_measurement_reflns_used    18646
_cell_measurement_theta_min      1.760
_cell_measurement_theta_max      25.00

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.552
_exptl_crystal_F_000             1857
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    3.663
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.416
_exptl_absorpt_correction_T_max  0.463
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            18646
_diffrn_reflns_av_unetI/netI     0.0686
_diffrn_reflns_av_R_equivalents  0.0556
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         1.760
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.916
_diffrn_measured_fraction_theta_full 0.890
_diffrn_reflns_Laue_measured_fraction_max 0.916
_diffrn_reflns_Laue_measured_fraction_full 0.890
_diffrn_reflns_point_group_measured_fraction_max 0.916
_diffrn_reflns_point_group_measured_fraction_full 0.890
_reflns_number_total             8217
_reflns_number_gt                7259
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0736P)²+23.6575P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8217
_refine_ls_number_parameters     703
_refine_ls_number_restraints     114
_refine_ls_R_factor_all          0.0556
_refine_ls_R_factor_gt           0.0504
_refine_ls_wR_factor_ref         0.1452
_refine_ls_wR_factor_gt          0.1403
_refine_ls_goodness_of_fit_ref   1.048
_refine_ls_restrained_S_all      1.059
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo -0.08863(6) 1.23563(7) 0.13534(4) 0.0176(2) Uani 1 1 d . . . . .
Mo2 Mo 0.19048(6) 1.22690(6) 0.03230(4) 0.01419(19) Uani 1 1 d . . . . .
Mo3 Mo 0.13741(6) 1.44317(7) 0.34279(4) 0.01517(19) Uani 1 1 d . . . . .
Mo4 Mo -0.11288(6) 1.34256(6) 0.28078(4) 0.01395(19) Uani 1 1 d . . . . .
Mo5 Mo 0.39469(6) 1.41430(6) 0.25503(4) 0.01196(18) Uani 1 1 d . . . . .
Mo6 Mo 0.42126(6) 1.31070(6) 0.08961(4) 0.01309(18) Uani 1 1 d . . . . .
Cs1 Cs 0.08429(6) 1.55188(6) 0.09762(4) 0.0387(2) Uani 1 1 d . . . . .
Cs2 Cs -0.33186(4) 1.49970(5) 0.11523(3) 0.02040(16) Uani 1 1 d . . . . .
Te1 Te 0.17412(4) 1.25575(5) 0.22074(3) 0.01162(15) Uani 1 1 d . . . . .
Mn1 Mn 0.1878(2) 1.0005(2) -0.07212(15) 0.0171(6) Uani 0.5 1 d . . P . .
O1 O -0.1762(6) 1.1501(7) 0.1105(4) 0.0367(19) Uani 1 1 d . . . . .
O2 O 0.2638(5) 1.0702(5) 0.1169(4) 0.0240(15) Uani 1 1 d . . . . .
O3 O 0.3522(5) 1.2570(5) 0.0165(3) 0.0178(13) Uani 1 1 d . . . . .
O4 O -0.0352(6) 1.0855(5) 0.2303(4) 0.0252(15) Uani 1 1 d . . . . .
O5 O 0.4204(5) 1.1269(5) 0.1524(4) 0.0227(15) Uani 1 1 d . . . . .
O6 O 0.1067(5) 1.4622(6) 0.4303(4) 0.0282(16) Uani 1 1 d . . . . .
O7 O 0.3025(5) 1.4597(5) 0.3343(3) 0.0152(13) Uani 1 1 d . . . . .
O8 O 0.0246(5) 1.3134(5) 0.1961(3) 0.0135(12) Uani 1 1 d . . . . .
O9 O 0.2047(5) 1.2639(5) 0.3979(3) 0.0190(14) Uani 1 1 d . . . . .
O10 O -0.1086(6) 1.3620(6) 0.0702(4) 0.0253(15) Uani 1 1 d . . . . .
O11 O 0.5276(5) 1.4082(5) 0.2884(3) 0.0194(14) Uani 1 1 d . . . . .
O12 O -0.0491(6) 1.1613(5) 0.3269(4) 0.0247(15) Uani 1 1 d . . . . .
O13 O 0.1883(6) 1.1417(6) -0.0264(4) 0.0255(15) Uani 1 1 d . . . . .
O14 O 0.5644(5) 1.2827(6) 0.0671(4) 0.0232(15) Uani 1 1 d . . . . .
O15 O 0.2326(5) 1.2981(5) 0.1229(3) 0.0148(13) Uani 1 1 d . . . . .
O16 O -0.2189(5) 1.3299(6) 0.3506(4) 0.0253(15) Uani 1 1 d . . . . .
O17 O 0.3731(5) 1.2415(5) 0.3347(3) 0.0165(13) Uani 1 1 d . . . . .
O18 O -0.1851(5) 1.2758(5) 0.2143(3) 0.0191(14) Uani 1 1 d . . . . .
O19 O 0.4270(5) 1.3153(5) 0.1911(3) 0.0123(12) Uani 1 1 d . . . . .
O20 O 0.0140(5) 1.3583(5) 0.3346(3) 0.0159(13) Uani 1 1 d . . . . .
O21 O 0.2115(5) 1.3853(5) 0.2424(3) 0.0142(12) Uani 1 1 d . . . . .
O22 O 0.3852(5) 1.5405(5) 0.1874(3) 0.0220(14) Uani 1 1 d . . . . .
O23 O 0.1359(5) 1.3572(5) -0.0176(3) 0.0210(14) Uani 1 1 d . . . . .
O24 O 0.0919(5) 1.5704(5) 0.2837(4) 0.0238(15) Uani 1 1 d . . . . .
O25 O 0.0587(5) 1.1850(5) 0.0969(3) 0.0175(13) Uani 1 1 d . . . . .
O26 O -0.1365(6) 1.4805(5) 0.2295(4) 0.0228(14) Uani 1 1 d . . . . .
O27 O 0.3963(5) 1.4523(5) 0.0502(3) 0.0185(13) Uani 1 1 d . . . . .
C1 C 0.2933(9) 0.9573(12) 0.5553(7) 0.053(4) Uani 1 1 d . . . . .
H1A H 0.2559 0.9368 0.6025 0.064 Uiso 1 1 calc R U . . .
C2 C 0.0702(11) 0.7595(8) 0.4494(6) 0.036(3) Uani 1 1 d . . . . .
C3 C 0.2648(9) 1.0620(11) 0.5066(6) 0.044(3) Uani 1 1 d . . . . .
H3A H 0.2073 1.1113 0.5209 0.053 Uiso 1 1 calc R U . . .
C4 C 0.0021(12) 0.8669(9) 0.3307(6) 0.043(3) Uani 1 1 d . . . . .
H4A H -0.0228 0.8687 0.2842 0.051 Uiso 1 1 calc R U . . .
C5 C 0.3112(9) 0.7581(9) 0.2754(7) 0.036(3) Uani 1 1 d . . . . .
H5A H 0.2570 0.7047 0.2844 0.043 Uiso 1 1 calc R U . . .
C6 C 0.0349(13) 0.7636(9) 0.3802(6) 0.047(3) Uani 1 1 d . . . . .
H6A H 0.0331 0.6968 0.3663 0.056 Uiso 1 1 calc R U . . .
C7 C 0.4107(9) 0.7339(8) 0.3130(5) 0.025(2) Uani 1 1 d . . . . .
C8 C 0.3755(8) 0.8852(9) 0.5341(6) 0.033(3) Uani 1 1 d . U . . .
C9 C 0.4906(9) 0.8151(8) 0.3010(5) 0.027(2) Uani 1 1 d . . . . .
H9A H 0.5582 0.7991 0.3267 0.033 Uiso 1 1 calc R U . . .
C10 C 0.2912(9) 0.8615(9) 0.2243(6) 0.033(3) Uani 1 1 d . . . . .
H10A H 0.2244 0.8772 0.1978 0.040 Uiso 1 1 calc R U . . .
C11 C 0.0453(9) 0.9613(8) 0.4193(6) 0.027(2) Uani 1 1 d . . . . .
H11A H 0.0505 1.0281 0.4327 0.032 Uiso 1 1 calc R U . . .
C12 C 0.3500(7) 1.0532(8) 0.1566(5) 0.022(2) Uani 1 1 d . . . . .
C13 C 0.0768(10) 0.8598(9) 0.4687(6) 0.033(2) Uani 1 1 d . . . . .
H13A H 0.1026 0.8580 0.5150 0.039 Uiso 1 1 calc R U . . .
C14 C 0.0059(9) 0.9675(8) 0.3503(5) 0.025(2) Uani 1 1 d . . . . .
C15 C 0.4272(9) 0.9115(8) 0.4646(6) 0.027(2) Uani 1 1 d . . . . .
H15A H 0.4807 0.8592 0.4498 0.032 Uiso 1 1 calc R U . . .
C16 C -0.0288(8) 1.0780(8) 0.2992(5) 0.024(2) Uani 1 1 d . . . . .
C17 C 0.4682(8) 0.9187(8) 0.2510(5) 0.022(2) Uani 1 1 d . . . . .
H17A H 0.5205 0.9736 0.2436 0.026 Uiso 1 1 calc R U . . .
C18 C 0.3704(7) 0.9424(7) 0.2118(5) 0.0182(19) Uani 1 1 d . . . . .
C19 C 0.4007(8) 1.0152(8) 0.4161(5) 0.022(2) Uani 1 1 d . . . . .
H19A H 0.4366 1.0335 0.3684 0.027 Uiso 1 1 calc R U . . .
C20 C 0.2969(7) 1.2090(8) 0.3862(5) 0.018(2) Uani 1 1 d . . . . .
C21 C 0.3203(7) 1.0934(8) 0.4378(5) 0.022(2) Uani 1 1 d . . . . .
N1 N 0.4094(7) 0.7771(8) 0.5864(5) 0.041(2) Uani 1 1 d . U . . .
H1B H 0.4618 0.7310 0.5730 0.049 Uiso 1 1 calc R U . . .
H1C H 0.3772 0.7594 0.6308 0.049 Uiso 1 1 calc R U . . .
N2 N 0.1045(10) 0.6560(8) 0.4993(5) 0.047(3) Uani 1 1 d . . . . .
H2A H 0.1037 0.5938 0.4868 0.056 Uiso 1 1 calc R U . . .
H2B H 0.1265 0.6544 0.5426 0.056 Uiso 1 1 calc R U . . .
N3 N 0.4331(8) 0.6272(7) 0.3655(5) 0.035(2) Uani 1 1 d . . . . .
H3B H 0.3839 0.5770 0.3739 0.043 Uiso 1 1 calc R U . . .
H3C H 0.4959 0.6127 0.3889 0.043 Uiso 1 1 calc R U . . .
K1 K 0.3557(12) 0.9514(11) -0.0489(9) 0.039(3) Uani 0.25 1 d . U P . .
K1A K 0.3609(13) 0.9730(14) -0.0860(9) 0.043(4) Uani 0.25 1 d . U P . .
O1W O 0.247(3) 0.896(3) 0.0471(17) 0.117(10) Uani 0.5 1 d . U P . .
O1WA O 0.160(2) 0.894(2) 0.0372(14) 0.089(7) Uani 0.5 1 d . U P . .
O2W O 0.2023(16) 1.1261(16) -0.1784(10) 0.057(5) Uani 0.5 1 d . U P . .
O3W O 0.0086(14) 1.0497(13) -0.1131(10) 0.045(4) Uani 0.5 1 d . U P . .
OW1 O -0.0323(16) 1.7327(15) 0.1794(9) 0.137(6) Uani 1 1 d . U . . .
OW2 O -0.3107(19) 1.6975(16) 0.1896(11) 0.059(5) Uani 0.5 1 d . U P . .
OW2A O -0.402(3) 1.705(3) 0.172(2) 0.140(12) Uani 0.5 1 d . U P . .
OW4 O -0.2365(14) 0.7251(16) 0.4137(11) 0.054(5) Uani 0.5 1 d . U P . .
OW5 O 0.2617(13) 1.0612(13) -0.2995(9) 0.042(4) Uani 0.5 1 d . U P . .
OW6 O 0.4837(10) 1.1456(10) -0.0718(7) 0.087(3) Uani 1 1 d . U . . .
OW7 O -0.3103(10) 1.5722(9) 0.3456(7) 0.082(3) Uani 1 1 d . U . . .
OW8 O 0.3356(10) 0.6143(9) 0.5085(6) 0.075(3) Uani 1 1 d . U . . .
OW9 O 0.5933(10) 0.6514(8) 0.5278(6) 0.075(3) Uani 1 1 d . U . . .
OW10 O -0.3814(6) 1.1563(6) 0.2688(4) 0.0384(19) Uani 1 1 d . U . . .
OW11 O 0.3009(9) 1.7007(10) 0.0660(5) 0.077(3) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O10 1.697(7) . ?
Mo1 O1 1.710(6) . ?
Mo1 O25 1.918(6) . ?
Mo1 O18 1.921(6) . ?
Mo1 O8 2.243(5) . ?
Mo1 O4 2.254(7) . ?
Mo1 Cs2 4.0431(14) . ?
Mo1 Cs1 4.4098(16) 2_585 ?
Mo1 Cs1 4.4237(15) . ?
Mo2 O23 1.706(6) . ?
Mo2 O13 1.713(6) . ?
Mo2 O25 1.895(6) . ?
Mo2 O3 1.942(6) . ?
Mo2 O15 2.211(5) . ?
Mo2 O2 2.268(7) . ?
Mo2 Cs2 4.1133(13) 2_585 ?
Mo2 Cs1 4.4009(14) 2_585 ?
Mo3 O24 1.709(6) . ?
Mo3 O6 1.714(7) . ?
Mo3 O20 1.900(6) . ?
Mo3 O7 1.944(6) . ?
Mo3 O9 2.251(6) . ?
Mo3 O21 2.258(6) . ?
Mo3 Cs1 4.4690(16) . ?
Mo4 O16 1.706(6) . ?
Mo4 O26 1.711(6) . ?
Mo4 O20 1.906(6) . ?
Mo4 O18 1.945(6) . ?
Mo4 O8 2.229(6) . ?
Mo4 O12 2.231(6) . ?
Mo4 Cs2 4.0924(13) . ?
Mo4 Cs1 4.3227(14) . ?
Mo5 O11 1.702(6) . ?
Mo5 O22 1.710(6) . ?
Mo5 O19 1.916(6) . ?
Mo5 O7 1.928(6) . ?
Mo5 O21 2.241(5) . ?
Mo5 O17 2.260(6) . ?
Mo5 Cs2 3.9859(13) 1_655 ?
Mo6 O27 1.700(6) . ?
Mo6 O14 1.711(6) . ?
Mo6 O19 1.914(6) . ?
Mo6 O3 1.927(6) . ?
Mo6 O15 2.244(6) . ?
Mo6 O5 2.244(6) . ?
Mo6 Cs2 4.0131(12) 1_655 ?
Mo6 Cs2 4.0439(14) 2_585 ?
Mo6 K1A 4.113(16) 2_675 ?
Mo6 K1 4.128(13) 2_675 ?
Cs1 O10 3.014(7) 2_585 ?
Cs1 O23 3.028(6) 2_585 ?
Cs1 O8 3.118(6) . ?
Cs1 OW1 3.167(16) . ?
Cs1 OW11 3.191(13) . ?
Cs1 O21 3.266(6) . ?
Cs1 O15 3.344(6) . ?
Cs1 O26 3.418(7) . ?
Cs1 O24 3.545(7) . ?
Cs1 O10 3.561(7) . ?
Cs1 O23 3.609(7) . ?
Cs1 Te1 3.8284(13) . ?
Cs2 OW2A 3.02(3) . ?
Cs2 O27 3.113(6) 2_585 ?
Cs2 O10 3.141(7) . ?
Cs2 OW2 3.151(18) . ?
Cs2 O23 3.165(6) 2_585 ?
Cs2 O26 3.187(6) . ?
Cs2 O18 3.268(6) . ?
Cs2 O3 3.311(6) 2_585 ?
Cs2 O14 3.397(6) 1_455 ?
Cs2 O11 3.449(6) 1_455 ?
Cs2 O22 3.499(6) 1_455 ?
Cs2 O27 3.636(6) 1_455 ?
Te1 O15 1.847(6) . ?
Te1 O21 1.848(5) . ?
Te1 O8 1.856(5) . ?
Mn1 K1A 2.018(15) . ?
Mn1 K1 2.033(14) . ?
Mn1 O1WA 2.12(2) . ?
Mn1 O13 2.134(7) . ?
Mn1 O2W 2.158(17) . ?
Mn1 O1 2.181(7) 2_575 ?
Mn1 O3W 2.248(17) . ?
Mn1 O1W 2.36(3) . ?
O1 Mn1 2.181(7) 2_575 ?
O1 K1A 2.888(17) 2_575 ?
O1 K1 2.994(15) 2_575 ?
O2 C12 1.262(11) . ?
O3 Cs2 3.311(6) 2_585 ?
O4 C16 1.270(11) . ?
O5 C12 1.266(11) . ?
O5 K1A 3.036(16) 2_675 ?
O5 K1 3.339(16) 2_675 ?
O9 C20 1.247(11) . ?
O10 Cs1 3.014(7) 2_585 ?
O11 Cs2 3.450(6) 1_655 ?
O12 C16 1.261(12) . ?
O13 K1 2.988(15) . ?
O13 K1A 3.103(16) . ?
O14 K1 3.036(14) 2_675 ?
O14 K1A 3.109(17) 2_675 ?
O14 Cs2 3.397(6) 1_655 ?
O17 C20 1.262(10) . ?
O19 Cs2 3.735(5) 1_655 ?
O22 Cs2 3.499(6) 1_655 ?
O23 Cs1 3.028(6) 2_585 ?
O23 Cs2 3.165(6) 2_585 ?
O27 Cs2 3.113(6) 2_585 ?
O27 Cs2 3.636(6) 1_655 ?
C1 C8 1.349(17) . ?
C1 C3 1.383(16) . ?
C2 C6 1.372(16) . ?
C2 C13 1.387(14) . ?
C2 N2 1.397(14) . ?
C3 C21 1.362(14) . ?
C4 C14 1.388(14) . ?
C4 C6 1.388(16) . ?
C5 C7 1.367(14) . ?
C5 C10 1.375(15) . ?
C7 C9 1.397(14) . ?
C7 N3 1.419(12) . ?
C8 C15 1.353(15) . ?
C8 N1 1.456(13) . ?
C9 C17 1.372(13) . ?
C10 C18 1.387(13) . ?
C11 C13 1.369(14) . ?
C11 C14 1.380(14) . ?
C12 C18 1.475(13) . ?
C12 K1A 3.532(17) 2_675 ?
C14 C16 1.469(14) . ?
C15 C19 1.368(13) . ?
C17 C18 1.366(12) . ?
C17 K1A 3.536(18) 2_675 ?
C19 C21 1.390(14) . ?
C20 C21 1.495(13) . ?
K1 K1A 0.670(16) . ?
K1 O1W 2.10(4) . ?
K1 O1WA 2.71(3) . ?
K1 OW6 2.860(18) . ?
K1 OW6 2.954(19) 2_675 ?
K1 O1 2.994(15) 2_575 ?
K1 O14 3.036(14) 2_675 ?
K1 O2W 3.27(2) . ?
K1 OW11 3.327(19) 1_545 ?
K1 O5 3.338(16) 2_675 ?
K1A O1W 2.69(4) . ?
K1A OW6 2.759(19) . ?
K1A O2W 2.82(2) . ?
K1A O1 2.888(17) 2_575 ?
K1A O5 3.036(16) 2_675 ?
K1A O14 3.109(17) 2_675 ?
K1A O1WA 3.17(3) . ?
K1A C12 3.532(17) 2_675 ?
K1A C17 3.536(18) 2_675 ?
O1W O1WA 1.04(3) . ?
OW2 OW2A 1.13(4) . ?
OW6 K1 2.954(19) 2_675 ?
OW11 K1 3.327(19) 1_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O10 Mo1 O1 104.2(4) . . ?
O10 Mo1 O25 98.2(3) . . ?
O1 Mo1 O25 100.6(3) . . ?
O10 Mo1 O18 97.1(3) . . ?
O1 Mo1 O18 99.6(3) . . ?
O25 Mo1 O18 150.7(2) . . ?
O10 Mo1 O8 89.9(3) . . ?
O1 Mo1 O8 165.2(3) . . ?
O25 Mo1 O8 81.4(2) . . ?
O18 Mo1 O8 73.8(2) . . ?
O10 Mo1 O4 168.3(3) . . ?
O1 Mo1 O4 87.4(3) . . ?
O25 Mo1 O4 78.6(2) . . ?
O18 Mo1 O4 81.5(3) . . ?
O8 Mo1 O4 78.6(2) . . ?
O10 Mo1 Cs2 47.0(2) . . ?
O1 Mo1 Cs2 94.6(3) . . ?
O25 Mo1 Cs2 144.74(19) . . ?
O18 Mo1 Cs2 52.95(19) . . ?
O8 Mo1 Cs2 91.77(15) . . ?
O4 Mo1 Cs2 134.11(17) . . ?
O10 Mo1 Cs1 27.8(2) . 2_585 ?
O1 Mo1 Cs1 88.5(3) . 2_585 ?
O25 Mo1 Cs1 78.74(18) . 2_585 ?
O18 Mo1 Cs1 122.76(19) . 2_585 ?
O8 Mo1 Cs1 106.26(15) . 2_585 ?
O4 Mo1 Cs1 155.78(17) . 2_585 ?
Cs2 Mo1 Cs1 70.02(2) . 2_585 ?
O10 Mo1 Cs1 49.4(2) . . ?
O1 Mo1 Cs1 153.3(3) . . ?
O25 Mo1 Cs1 81.61(17) . . ?
O18 Mo1 Cs1 89.64(17) . . ?
O8 Mo1 Cs1 41.42(15) . . ?
O4 Mo1 Cs1 118.88(17) . . ?
Cs2 Mo1 Cs1 71.04(3) . . ?
Cs1 Mo1 Cs1 65.64(2) 2_585 . ?
O23 Mo2 O13 104.7(3) . . ?
O23 Mo2 O25 98.4(3) . . ?
O13 Mo2 O25 101.2(3) . . ?
O23 Mo2 O3 96.9(3) . . ?
O13 Mo2 O3 98.8(3) . . ?
O25 Mo2 O3 150.8(2) . . ?
O23 Mo2 O15 90.9(3) . . ?
O13 Mo2 O15 163.2(3) . . ?
O25 Mo2 O15 82.4(2) . . ?
O3 Mo2 O15 72.6(2) . . ?
O23 Mo2 O2 168.8(3) . . ?
O13 Mo2 O2 86.5(3) . . ?
O25 Mo2 O2 78.4(2) . . ?
O3 Mo2 O2 81.8(2) . . ?
O15 Mo2 O2 78.1(2) . . ?
O23 Mo2 Cs2 45.6(2) . 2_585 ?
O13 Mo2 Cs2 99.0(2) . 2_585 ?
O25 Mo2 Cs2 142.50(19) . 2_585 ?
O3 Mo2 Cs2 52.49(18) . 2_585 ?
O15 Mo2 Cs2 87.21(15) . 2_585 ?
O2 Mo2 Cs2 134.30(16) . 2_585 ?
O23 Mo2 Cs1 29.2(2) . 2_585 ?
O13 Mo2 Cs1 87.1(2) . 2_585 ?
O25 Mo2 Cs1 79.15(19) . 2_585 ?
O3 Mo2 Cs1 123.11(18) . 2_585 ?
O15 Mo2 Cs1 109.68(16) . 2_585 ?
O2 Mo2 Cs1 154.97(15) . 2_585 ?
Cs2 Mo2 Cs1 70.65(3) 2_585 2_585 ?
O24 Mo3 O6 104.1(3) . . ?
O24 Mo3 O20 98.8(3) . . ?
O6 Mo3 O20 101.2(3) . . ?
O24 Mo3 O7 99.0(3) . . ?
O6 Mo3 O7 99.1(3) . . ?
O20 Mo3 O7 148.7(2) . . ?
O24 Mo3 O9 167.7(3) . . ?
O6 Mo3 O9 88.1(3) . . ?
O20 Mo3 O9 77.4(2) . . ?
O7 Mo3 O9 79.7(2) . . ?
O24 Mo3 O21 88.8(3) . . ?
O6 Mo3 O21 165.7(3) . . ?
O20 Mo3 O21 82.3(2) . . ?
O7 Mo3 O21 72.5(2) . . ?
O9 Mo3 O21 79.1(2) . . ?
O24 Mo3 Cs1 47.5(2) . . ?
O6 Mo3 Cs1 149.8(2) . . ?
O20 Mo3 Cs1 77.44(17) . . ?
O7 Mo3 Cs1 96.30(17) . . ?
O9 Mo3 Cs1 120.32(16) . . ?
O21 Mo3 Cs1 44.45(14) . . ?
O16 Mo4 O26 103.2(3) . . ?
O16 Mo4 O20 99.2(3) . . ?
O26 Mo4 O20 98.9(3) . . ?
O16 Mo4 O18 99.2(3) . . ?
O26 Mo4 O18 96.4(3) . . ?
O20 Mo4 O18 152.6(3) . . ?
O16 Mo4 O8 166.0(3) . . ?
O26 Mo4 O8 89.7(3) . . ?
O20 Mo4 O8 83.9(2) . . ?
O18 Mo4 O8 73.6(2) . . ?
O16 Mo4 O12 90.4(3) . . ?
O26 Mo4 O12 166.4(3) . . ?
O20 Mo4 O12 79.1(2) . . ?
O18 Mo4 O12 80.7(3) . . ?
O8 Mo4 O12 76.8(2) . . ?
O16 Mo4 Cs2 94.1(2) . . ?
O26 Mo4 Cs2 47.20(19) . . ?
O20 Mo4 Cs2 145.83(18) . . ?
O18 Mo4 Cs2 51.77(19) . . ?
O8 Mo4 Cs2 90.69(14) . . ?
O12 Mo4 Cs2 132.33(17) . . ?
O16 Mo4 Cs1 150.1(2) . . ?
O26 Mo4 Cs1 47.8(2) . . ?
O20 Mo4 Cs1 81.52(18) . . ?
O18 Mo4 Cs1 92.33(18) . . ?
O8 Mo4 Cs1 43.69(15) . . ?
O12 Mo4 Cs1 118.81(17) . . ?
Cs2 Mo4 Cs1 71.64(3) . . ?
O11 Mo5 O22 103.9(3) . . ?
O11 Mo5 O19 100.2(3) . . ?
O22 Mo5 O19 98.3(3) . . ?
O11 Mo5 O7 98.7(3) . . ?
O22 Mo5 O7 99.1(3) . . ?
O19 Mo5 O7 150.4(2) . . ?
O11 Mo5 O21 163.5(3) . . ?
O22 Mo5 O21 91.7(3) . . ?
O19 Mo5 O21 82.5(2) . . ?
O7 Mo5 O21 73.2(2) . . ?
O11 Mo5 O17 87.9(3) . . ?
O22 Mo5 O17 168.0(2) . . ?
O19 Mo5 O17 77.4(2) . . ?
O7 Mo5 O17 80.7(2) . . ?
O21 Mo5 O17 76.7(2) . . ?
O11 Mo5 Cs2 59.5(2) . 1_655 ?
O22 Mo5 Cs2 61.2(2) . 1_655 ?
O19 Mo5 Cs2 68.45(16) . 1_655 ?
O7 Mo5 Cs2 141.12(16) . 1_655 ?
O21 Mo5 Cs2 135.15(15) . 1_655 ?
O17 Mo5 Cs2 125.60(15) . 1_655 ?
O27 Mo6 O14 103.7(3) . . ?
O27 Mo6 O19 98.1(3) . . ?
O14 Mo6 O19 101.1(3) . . ?
O27 Mo6 O3 98.4(3) . . ?
O14 Mo6 O3 100.1(3) . . ?
O19 Mo6 O3 149.2(2) . . ?
O27 Mo6 O15 90.5(3) . . ?
O14 Mo6 O15 164.8(3) . . ?
O19 Mo6 O15 81.9(2) . . ?
O3 Mo6 O15 72.1(2) . . ?
O27 Mo6 O5 169.0(3) . . ?
O14 Mo6 O5 87.1(3) . . ?
O19 Mo6 O5 77.7(2) . . ?
O3 Mo6 O5 81.3(2) . . ?
O15 Mo6 O5 78.9(2) . . ?
O27 Mo6 Cs2 65.0(2) . 1_655 ?
O14 Mo6 Cs2 56.9(2) . 1_655 ?
O19 Mo6 Cs2 67.73(16) . 1_655 ?
O3 Mo6 Cs2 143.09(17) . 1_655 ?
O15 Mo6 Cs2 136.39(15) . 1_655 ?
O5 Mo6 Cs2 121.31(15) . 1_655 ?
O27 Mo6 Cs2 46.0(2) . 2_585 ?
O14 Mo6 Cs2 97.4(2) . 2_585 ?
O19 Mo6 Cs2 142.90(17) . 2_585 ?
O3 Mo6 Cs2 54.26(18) . 2_585 ?
O15 Mo6 Cs2 88.52(15) . 2_585 ?
O5 Mo6 Cs2 135.47(16) . 2_585 ?
Cs2 Mo6 Cs2 97.09(2) 1_655 2_585 ?
O27 Mo6 K1A 144.5(3) . 2_675 ?
O14 Mo6 K1A 43.7(3) . 2_675 ?
O19 Mo6 K1A 101.6(3) . 2_675 ?
O3 Mo6 K1A 79.0(3) . 2_675 ?
O15 Mo6 K1A 121.2(3) . 2_675 ?
O5 Mo6 K1A 46.4(3) . 2_675 ?
Cs2 Mo6 K1A 95.9(2) 1_655 2_675 ?
Cs2 Mo6 K1A 113.8(2) 2_585 2_675 ?
O27 Mo6 K1 136.7(3) . 2_675 ?
O14 Mo6 K1 40.4(3) . 2_675 ?
O19 Mo6 K1 110.3(3) . 2_675 ?
O3 Mo6 K1 73.4(3) . 2_675 ?
O15 Mo6 K1 124.5(3) . 2_675 ?
O5 Mo6 K1 53.9(3) . 2_675 ?
Cs2 Mo6 K1 95.89(19) 1_655 2_675 ?
Cs2 Mo6 K1 104.6(2) 2_585 2_675 ?
K1A Mo6 K1 9.3(2) 2_675 2_675 ?
O10 Cs1 O23 63.36(17) 2_585 2_585 ?
O10 Cs1 O8 129.21(16) 2_585 . ?
O23 Cs1 O8 102.70(15) 2_585 . ?
O10 Cs1 OW1 114.5(3) 2_585 . ?
O23 Cs1 OW1 75.7(3) 2_585 . ?
O8 Cs1 OW1 107.3(4) . . ?
O10 Cs1 OW11 75.3(2) 2_585 . ?
O23 Cs1 OW11 120.1(2) 2_585 . ?
O8 Cs1 OW11 137.2(2) . . ?
OW1 Cs1 OW11 85.2(4) . . ?
O10 Cs1 O21 142.94(16) 2_585 . ?
O23 Cs1 O21 149.03(15) 2_585 . ?
O8 Cs1 O21 50.32(13) . . ?
OW1 Cs1 O21 96.5(3) . . ?
OW11 Cs1 O21 88.3(2) . . ?
O10 Cs1 O15 100.33(16) 2_585 . ?
O23 Cs1 O15 129.91(15) 2_585 . ?
O8 Cs1 O15 49.23(14) . . ?
OW1 Cs1 O15 144.4(3) . . ?
OW11 Cs1 O15 97.3(2) . . ?
O21 Cs1 O15 48.35(14) . . ?
O10 Cs1 O26 136.52(16) 2_585 . ?
O23 Cs1 O26 74.27(16) 2_585 . ?
O8 Cs1 O26 50.55(15) . . ?
OW1 Cs1 O26 60.3(4) . . ?
OW11 Cs1 O26 139.2(2) . . ?
O21 Cs1 O26 75.89(14) . . ?
O15 Cs1 O26 99.32(14) . . ?
O10 Cs1 O24 155.09(16) 2_585 . ?
O23 Cs1 O24 117.44(16) 2_585 . ?
O8 Cs1 O24 75.68(15) . . ?
OW1 Cs1 O24 48.1(3) . . ?
OW11 Cs1 O24 84.5(2) . . ?
O21 Cs1 O24 48.41(14) . . ?
O15 Cs1 O24 96.61(14) . . ?
O26 Cs1 O24 56.78(14) . . ?
O10 Cs1 O10 86.91(18) 2_585 . ?
O23 Cs1 O10 59.69(16) 2_585 . ?
O8 Cs1 O10 49.20(14) . . ?
OW1 Cs1 O10 114.2(4) . . ?
OW11 Cs1 O10 158.2(2) . . ?
O21 Cs1 O10 98.85(14) . . ?
O15 Cs1 O10 73.14(14) . . ?
O26 Cs1 O10 62.57(14) . . ?
O24 Cs1 O10 115.61(15) . . ?
O10 Cs1 O23 59.19(16) 2_585 . ?
O23 Cs1 O23 88.07(16) 2_585 . ?
O8 Cs1 O23 72.46(14) . . ?
OW1 Cs1 O23 163.4(3) . . ?
OW11 Cs1 O23 106.5(2) . . ?
O21 Cs1 O23 95.69(14) . . ?
O15 Cs1 O23 47.56(13) . . ?
O26 Cs1 O23 112.26(14) . . ?
O24 Cs1 O23 142.88(15) . . ?
O10 Cs1 O23 52.52(14) . . ?
O10 Cs1 Te1 128.30(13) 2_585 . ?
O23 Cs1 Te1 130.38(12) 2_585 . ?
O8 Cs1 Te1 28.74(10) . . ?
OW1 Cs1 Te1 117.2(3) . . ?
OW11 Cs1 Te1 108.96(17) . . ?
O21 Cs1 Te1 28.82(9) . . ?
O15 Cs1 Te1 28.84(9) . . ?
O26 Cs1 Te1 73.43(11) . . ?
O24 Cs1 Te1 71.99(11) . . ?
O10 Cs1 Te1 72.23(11) . . ?
O23 Cs1 Te1 70.91(10) . . ?
OW2A Cs2 O27 110.1(7) . 2_585 ?
OW2A Cs2 O10 140.3(8) . . ?
O27 Cs2 O10 86.38(16) 2_585 . ?
OW2A Cs2 OW2 20.9(7) . . ?
O27 Cs2 OW2 121.8(4) 2_585 . ?
O10 Cs2 OW2 120.1(4) . . ?
OW2A Cs2 O23 86.1(7) . 2_585 ?
O27 Cs2 O23 74.14(15) 2_585 2_585 ?
O10 Cs2 O23 63.36(17) . 2_585 ?
OW2 Cs2 O23 74.8(4) . 2_585 ?
OW2A Cs2 O26 78.9(8) . . ?
O27 Cs2 O26 147.83(16) 2_585 . ?
O10 Cs2 O26 69.92(17) . . ?
OW2 Cs2 O26 59.3(4) . . ?
O23 Cs2 O26 75.83(16) 2_585 . ?
OW2A Cs2 O18 122.1(7) . . ?
O27 Cs2 O18 127.50(16) 2_585 . ?
O10 Cs2 O18 50.08(16) . . ?
OW2 Cs2 O18 106.7(4) . . ?
O23 Cs2 O18 102.76(15) 2_585 . ?
O26 Cs2 O18 50.02(15) . . ?
OW2A Cs2 O3 65.4(7) . 2_585 ?
O27 Cs2 O3 50.57(15) 2_585 2_585 ?
O10 Cs2 O3 105.85(16) . 2_585 ?
OW2 Cs2 O3 71.8(4) . 2_585 ?
O23 Cs2 O3 49.87(15) 2_585 2_585 ?
O26 Cs2 O3 114.37(15) . 2_585 ?
O18 Cs2 O3 152.52(14) . 2_585 ?
OW2A Cs2 O14 143.5(8) . 1_455 ?
O27 Cs2 O14 63.67(16) 2_585 1_455 ?
O10 Cs2 O14 76.14(16) . 1_455 ?
OW2 Cs2 O14 161.8(4) . 1_455 ?
O23 Cs2 O14 122.38(16) 2_585 1_455 ?
O26 Cs2 O14 126.84(16) . 1_455 ?
O18 Cs2 O14 76.82(15) . 1_455 ?
O3 Cs2 O14 113.53(15) 2_585 1_455 ?
OW2A Cs2 O11 72.4(7) . 1_455 ?
O27 Cs2 O11 135.86(14) 2_585 1_455 ?
O10 Cs2 O11 120.67(16) . 1_455 ?
OW2 Cs2 O11 76.7(4) . 1_455 ?
O23 Cs2 O11 147.39(15) 2_585 1_455 ?
O26 Cs2 O11 76.17(16) . 1_455 ?
O18 Cs2 O11 70.75(14) . 1_455 ?
O3 Cs2 O11 132.46(15) 2_585 1_455 ?
O14 Cs2 O11 88.06(14) 1_455 1_455 ?
OW2A Cs2 O22 60.4(8) . 1_455 ?
O27 Cs2 O22 95.69(15) 2_585 1_455 ?
O10 Cs2 O22 156.54(16) . 1_455 ?
OW2 Cs2 O22 78.4(4) . 1_455 ?
O23 Cs2 O22 139.62(15) 2_585 1_455 ?
O26 Cs2 O22 114.79(16) . 1_455 ?
O18 Cs2 O22 113.65(14) . 1_455 ?
O3 Cs2 O22 93.19(15) 2_585 1_455 ?
O14 Cs2 O22 83.84(14) 1_455 1_455 ?
O11 Cs2 O22 45.47(14) 1_455 1_455 ?
OW2A Cs2 O27 101.2(8) . 1_455 ?
O27 Cs2 O27 53.22(18) 2_585 1_455 ?
O10 Cs2 O27 116.99(15) . 1_455 ?
OW2 Cs2 O27 122.1(4) . 1_455 ?
O23 Cs2 O27 126.30(14) 2_585 1_455 ?
O26 Cs2 O27 157.86(15) . 1_455 ?
O18 Cs2 O27 116.34(14) . 1_455 ?
O3 Cs2 O27 84.88(13) 2_585 1_455 ?
O14 Cs2 O27 44.67(14) 1_455 1_455 ?
O11 Cs2 O27 82.72(13) 1_455 1_455 ?
O22 Cs2 O27 50.17(14) 1_455 1_455 ?
O15 Te1 O21 94.3(3) . . ?
O15 Te1 O8 93.6(3) . . ?
O21 Te1 O8 94.4(2) . . ?
O15 Te1 Cs1 60.86(19) . . ?
O21 Te1 Cs1 58.43(18) . . ?
O8 Te1 Cs1 53.85(18) . . ?
K1A Mn1 K1 19.0(5) . . ?
K1A Mn1 O1WA 100.0(9) . . ?
K1 Mn1 O1WA 81.7(9) . . ?
K1A Mn1 O13 96.7(5) . . ?
K1 Mn1 O13 91.6(4) . . ?
O1WA Mn1 O13 89.4(8) . . ?
K1A Mn1 O2W 84.8(7) . . ?
K1 Mn1 O2W 102.6(7) . . ?
O1WA Mn1 O2W 172.5(8) . . ?
O13 Mn1 O2W 84.3(6) . . ?
K1A Mn1 O1 86.8(5) . 2_575 ?
K1 Mn1 O1 90.5(4) . 2_575 ?
O1WA Mn1 O1 86.2(8) . 2_575 ?
O13 Mn1 O1 174.8(3) . 2_575 ?
O2W Mn1 O1 99.9(6) . 2_575 ?
K1A Mn1 O3W 153.9(6) . . ?
K1 Mn1 O3W 172.1(6) . . ?
O1WA Mn1 O3W 103.8(9) . . ?
O13 Mn1 O3W 94.2(4) . . ?
O2W Mn1 O3W 72.7(7) . . ?
O1 Mn1 O3W 84.2(4) 2_575 . ?
K1A Mn1 O1W 75.5(10) . . ?
K1 Mn1 O1W 56.6(10) . . ?
O1WA Mn1 O1W 26.2(9) . . ?
O13 Mn1 O1W 83.4(7) . . ?
O2W Mn1 O1W 155.3(9) . . ?
O1 Mn1 O1W 93.8(8) 2_575 . ?
O3W Mn1 O1W 129.5(10) . . ?
Mo1 O1 Mn1 147.1(4) . 2_575 ?
Mo1 O1 K1A 168.1(5) . 2_575 ?
Mn1 O1 K1A 44.2(3) 2_575 2_575 ?
Mo1 O1 K1 167.4(5) . 2_575 ?
Mn1 O1 K1 42.7(3) 2_575 2_575 ?
K1A O1 K1 12.9(3) 2_575 2_575 ?
C12 O2 Mo2 131.8(6) . . ?
Mo6 O3 Mo2 118.6(3) . . ?
Mo6 O3 Cs2 97.5(2) . 2_585 ?
Mo2 O3 Cs2 99.8(2) . 2_585 ?
C16 O4 Mo1 130.2(6) . . ?
C12 O5 Mo6 132.7(6) . . ?
C12 O5 K1A 102.4(6) . 2_675 ?
Mo6 O5 K1A 101.3(4) . 2_675 ?
C12 O5 K1 103.4(6) . 2_675 ?
Mo6 O5 K1 93.3(3) . 2_675 ?
K1A O5 K1 10.8(3) 2_675 2_675 ?
Mo5 O7 Mo3 118.7(3) . . ?
Te1 O8 Mo4 122.8(3) . . ?
Te1 O8 Mo1 123.9(3) . . ?
Mo4 O8 Mo1 95.2(2) . . ?
Te1 O8 Cs1 97.4(2) . . ?
Mo4 O8 Cs1 106.7(2) . . ?
Mo1 O8 Cs1 110.2(2) . . ?
C20 O9 Mo3 130.7(6) . . ?
Mo1 O10 Cs1 137.0(3) . 2_585 ?
Mo1 O10 Cs2 109.8(3) . . ?
Cs1 O10 Cs2 104.26(19) 2_585 . ?
Mo1 O10 Cs1 109.4(3) . . ?
Cs1 O10 Cs1 93.08(17) 2_585 . ?
Cs2 O10 Cs1 94.47(17) . . ?
Mo5 O11 Cs2 95.3(2) . 1_655 ?
C16 O12 Mo4 133.7(6) . . ?
Mo2 O13 Mn1 164.6(4) . . ?
Mo2 O13 K1 130.3(4) . . ?
Mn1 O13 K1 42.8(3) . . ?
Mo2 O13 K1A 137.1(4) . . ?
Mn1 O13 K1A 40.2(3) . . ?
K1 O13 K1A 12.4(3) . . ?
Mo6 O14 K1 118.1(4) . 2_675 ?
Mo6 O14 K1A 114.0(4) . 2_675 ?
K1 O14 K1A 12.4(3) 2_675 2_675 ?
Mo6 O14 Cs2 98.1(3) . 1_655 ?
K1 O14 Cs2 140.0(3) 2_675 1_655 ?
K1A O14 Cs2 136.1(4) 2_675 1_655 ?
Te1 O15 Mo2 125.6(3) . . ?
Te1 O15 Mo6 124.0(3) . . ?
Mo2 O15 Mo6 96.6(2) . . ?
Te1 O15 Cs1 90.3(2) . . ?
Mo2 O15 Cs1 107.1(2) . . ?
Mo6 O15 Cs1 112.7(2) . . ?
C20 O17 Mo5 130.5(6) . . ?
Mo1 O18 Mo4 117.3(3) . . ?
Mo1 O18 Cs2 99.1(2) . . ?
Mo4 O18 Cs2 100.4(2) . . ?
Mo6 O19 Mo5 142.2(3) . . ?
Mo6 O19 Cs2 83.95(18) . 1_655 ?
Mo5 O19 Cs2 83.05(17) . 1_655 ?
Mo3 O20 Mo4 148.8(3) . . ?
Te1 O21 Mo5 121.7(3) . . ?
Te1 O21 Mo3 124.1(3) . . ?
Mo5 O21 Mo3 95.5(2) . . ?
Te1 O21 Cs1 92.8(2) . . ?
Mo5 O21 Cs1 116.8(2) . . ?
Mo3 O21 Cs1 106.6(2) . . ?
Mo5 O22 Cs2 93.4(3) . 1_655 ?
Mo2 O23 Cs1 134.9(3) . 2_585 ?
Mo2 O23 Cs2 111.7(3) . 2_585 ?
Cs1 O23 Cs2 105.46(18) 2_585 2_585 ?
Mo2 O23 Cs1 111.3(3) . . ?
Cs1 O23 Cs1 91.93(16) 2_585 . ?
Cs2 O23 Cs1 91.43(15) 2_585 . ?
Mo3 O24 Cs1 111.7(3) . . ?
Mo2 O25 Mo1 146.2(4) . . ?
Mo4 O26 Cs2 109.6(3) . . ?
Mo4 O26 Cs1 110.4(3) . . ?
Cs2 O26 Cs1 96.45(17) . . ?
Mo6 O27 Cs2 110.9(3) . 2_585 ?
Mo6 O27 Cs2 90.0(2) . 1_655 ?
Cs2 O27 Cs2 126.77(18) 2_585 1_655 ?
C8 C1 C3 119.6(11) . . ?
C6 C2 C13 119.4(10) . . ?
C6 C2 N2 120.8(9) . . ?
C13 C2 N2 119.7(10) . . ?
C21 C3 C1 120.6(11) . . ?
C14 C4 C6 120.5(10) . . ?
C7 C5 C10 119.9(9) . . ?
C2 C6 C4 120.4(10) . . ?
C5 C7 C9 120.1(9) . . ?
C5 C7 N3 120.7(9) . . ?
C9 C7 N3 119.3(9) . . ?
C15 C8 C1 121.1(10) . . ?
C15 C8 N1 119.1(10) . . ?
C1 C8 N1 119.8(10) . . ?
C17 C9 C7 119.2(9) . . ?
C5 C10 C18 120.3(9) . . ?
C13 C11 C14 121.9(9) . . ?
O2 C12 O5 123.5(9) . . ?
O2 C12 C18 119.0(8) . . ?
O5 C12 C18 117.5(8) . . ?
O2 C12 K1A 123.7(7) . 2_675 ?
O5 C12 K1A 57.1(5) . 2_675 ?
C18 C12 K1A 89.3(6) . 2_675 ?
C11 C13 C2 119.7(10) . . ?
C11 C14 C4 118.0(9) . . ?
C11 C14 C16 120.3(8) . . ?
C4 C14 C16 121.7(10) . . ?
C8 C15 C19 119.8(10) . . ?
O12 C16 O4 123.6(9) . . ?
O12 C16 C14 117.3(9) . . ?
O4 C16 C14 119.1(9) . . ?
C18 C17 C9 121.0(9) . . ?
C18 C17 K1A 91.0(6) . 2_675 ?
C9 C17 K1A 124.9(7) . 2_675 ?
C17 C18 C10 119.4(9) . . ?
C17 C18 C12 120.0(8) . . ?
C10 C18 C12 120.6(8) . . ?
C15 C19 C21 120.3(10) . . ?
O9 C20 O17 126.3(8) . . ?
O9 C20 C21 117.3(8) . . ?
O17 C20 C21 116.4(8) . . ?
C3 C21 C19 118.4(10) . . ?
C3 C21 C20 121.5(10) . . ?
C19 C21 C20 120.0(9) . . ?
K1A K1 Mn1 79(2) . . ?
K1A K1 O1W 148(3) . . ?
Mn1 K1 O1W 69.6(10) . . ?
K1A K1 O1WA 128(2) . . ?
Mn1 K1 O1WA 50.5(6) . . ?
O1W K1 O1WA 20.3(9) . . ?
K1A K1 OW6 75(2) . . ?
Mn1 K1 OW6 110.3(6) . . ?
O1W K1 OW6 122.2(10) . . ?
O1WA K1 OW6 130.3(8) . . ?
K1A K1 OW6 136(2) . 2_675 ?
Mn1 K1 OW6 144.8(8) . 2_675 ?
O1W K1 OW6 75.8(11) . 2_675 ?
O1WA K1 OW6 95.7(8) . 2_675 ?
OW6 K1 OW6 82.7(5) . 2_675 ?
K1A K1 O13 94(2) . . ?
Mn1 K1 O13 45.6(3) . . ?
O1W K1 O13 69.6(10) . . ?
O1WA K1 O13 63.1(6) . . ?
OW6 K1 O13 73.0(4) . . ?
OW6 K1 O13 115.5(5) 2_675 . ?
K1A K1 O1 75(2) . 2_575 ?
Mn1 K1 O1 46.8(3) . 2_575 ?
O1W K1 O1 79.1(9) . 2_575 ?
O1WA K1 O1 61.7(7) . 2_575 ?
OW6 K1 O1 144.7(6) . 2_575 ?
OW6 K1 O1 132.1(6) 2_675 2_575 ?
O13 K1 O1 92.2(4) . 2_575 ?
K1A K1 O14 90(2) . 2_675 ?
Mn1 K1 O14 113.6(5) . 2_675 ?
O1W K1 O14 96.1(10) . 2_675 ?
O1WA K1 O14 97.3(7) . 2_675 ?
OW6 K1 O14 129.5(6) . 2_675 ?
OW6 K1 O14 75.8(4) 2_675 2_675 ?
O13 K1 O14 157.2(5) . 2_675 ?
O1 K1 O14 67.1(3) 2_575 2_675 ?
K1A K1 O2W 43(2) . . ?
Mn1 K1 O2W 40.1(4) . . ?
O1W K1 O2W 108.5(11) . . ?
O1WA K1 O2W 90.4(7) . . ?
OW6 K1 O2W 81.8(6) . . ?
OW6 K1 O2W 163.7(6) 2_675 . ?
O13 K1 O2W 54.6(4) . . ?
O1 K1 O2W 63.8(5) 2_575 . ?
O14 K1 O2W 118.4(6) 2_675 . ?
K1A K1 OW11 135(2) . 1_545 ?
Mn1 K1 OW11 94.7(6) . 1_545 ?
O1W K1 OW11 44.6(9) . 1_545 ?
O1WA K1 OW11 51.8(6) . 1_545 ?
OW6 K1 OW11 145.3(6) . 1_545 ?
OW6 K1 OW11 63.5(4) 2_675 1_545 ?
O13 K1 OW11 113.4(5) . 1_545 ?
O1 K1 OW11 70.0(4) 2_575 1_545 ?
O14 K1 OW11 51.9(3) 2_675 1_545 ?
O2W K1 OW11 130.8(6) . 1_545 ?
K1A K1 O5 58(2) . 2_675 ?
Mn1 K1 O5 131.4(6) . 2_675 ?
O1W K1 O5 144.2(11) . 2_675 ?
O1WA K1 O5 147.9(7) . 2_675 ?
OW6 K1 O5 81.4(4) . 2_675 ?
OW6 K1 O5 81.8(4) 2_675 2_675 ?
O13 K1 O5 146.2(6) . 2_675 ?
O1 K1 O5 96.4(4) 2_575 2_675 ?
O14 K1 O5 50.9(3) 2_675 2_675 ?
O2W K1 O5 100.9(6) . 2_675 ?
OW11 K1 O5 100.2(4) 1_545 2_675 ?
K1 K1A Mn1 82(2) . . ?
K1 K1A O1W 24(2) . . ?
Mn1 K1A O1W 58.0(8) . . ?
K1 K1A OW6 92(2) . . ?
Mn1 K1A OW6 114.7(7) . . ?
O1W K1A OW6 106.1(8) . . ?
K1 K1A O2W 128(2) . . ?
Mn1 K1A O2W 49.7(5) . . ?
O1W K1A O2W 106.4(10) . . ?
OW6 K1A O2W 92.4(7) . . ?
K1 K1A O1 93(2) . 2_575 ?
Mn1 K1A O1 48.9(4) . 2_575 ?
O1W K1A O1 72.9(8) . 2_575 ?
OW6 K1A O1 162.0(7) . 2_575 ?
O2W K1A O1 71.2(6) . 2_575 ?
K1 K1A O5 111(2) . 2_675 ?
Mn1 K1A O5 153.4(7) . 2_675 ?
O1W K1A O5 129.8(10) . 2_675 ?
OW6 K1A O5 88.7(5) . 2_675 ?
O2W K1A O5 120.9(7) . 2_675 ?
O1 K1A O5 105.8(5) 2_575 2_675 ?
K1 K1A O13 74(2) . . ?
Mn1 K1A O13 43.1(3) . . ?
O1W K1A O13 61.7(8) . . ?
OW6 K1A O13 72.5(4) . . ?
O2W K1A O13 58.0(5) . . ?
O1 K1A O13 92.0(5) 2_575 . ?
O5 K1A O13 160.9(6) 2_675 . ?
K1 K1A O14 78(2) . 2_675 ?
Mn1 K1A O14 111.3(6) . 2_675 ?
O1W K1A O14 83.4(8) . 2_675 ?
OW6 K1A O14 130.6(6) . 2_675 ?
O2W K1A O14 132.2(7) . 2_675 ?
O1 K1A O14 67.4(4) 2_575 2_675 ?
O5 K1A O14 53.2(3) 2_675 2_675 ?
O13 K1A O14 143.9(6) . 2_675 ?
K1 K1A O1WA 43(2) . . ?
Mn1 K1A O1WA 41.1(6) . . ?
O1W K1A O1WA 18.2(7) . . ?
OW6 K1A O1WA 117.0(7) . . ?
O2W K1A O1WA 90.7(7) . . ?
O1 K1A O1WA 57.8(6) 2_575 . ?
O5 K1A O1WA 139.3(7) 2_675 . ?
O13 K1A O1WA 57.0(5) . . ?
O14 K1A O1WA 87.0(6) 2_675 . ?
K1 K1A C12 112(2) . 2_675 ?
Mn1 K1A C12 166.1(7) . 2_675 ?
O1W K1A C12 135.4(10) . 2_675 ?
OW6 K1A C12 68.3(4) . 2_675 ?
O2W K1A C12 117.9(6) . 2_675 ?
O1 K1A C12 125.5(5) 2_575 2_675 ?
O5 K1A C12 20.5(2) 2_675 2_675 ?
O13 K1A C12 140.5(5) . 2_675 ?
O14 K1A C12 71.6(4) 2_675 2_675 ?
O1WA K1A C12 151.2(7) . 2_675 ?
K1 K1A C17 151(2) . 2_675 ?
Mn1 K1A C17 126.2(7) . 2_675 ?
O1W K1A C17 174.4(9) . 2_675 ?
OW6 K1A C17 69.1(4) . 2_675 ?
O2W K1A C17 77.1(6) . 2_675 ?
O1 K1A C17 112.6(5) 2_575 2_675 ?
O5 K1A C17 48.7(3) 2_675 2_675 ?
O13 K1A C17 118.1(5) . 2_675 ?
O14 K1A C17 97.6(4) 2_675 2_675 ?
O1WA K1A C17 166.9(8) . 2_675 ?
C12 K1A C17 40.7(3) 2_675 2_675 ?
O1WA O1W K1 115(3) . . ?
O1WA O1W Mn1 64(2) . . ?
K1 O1W Mn1 53.8(8) . . ?
O1WA O1W K1A 108(3) . . ?
K1 O1W K1A 7.5(6) . . ?
Mn1 O1W K1A 46.5(7) . . ?
O1W O1WA Mn1 90(3) . . ?
O1W O1WA K1 44(2) . . ?
Mn1 O1WA K1 47.8(6) . . ?
O1W O1WA K1A 54(2) . . ?
Mn1 O1WA K1A 38.8(5) . . ?
K1 O1WA K1A 9.6(4) . . ?
Mn1 O2W K1A 45.5(4) . . ?
Mn1 O2W K1 37.3(4) . . ?
K1A O2W K1 9.3(4) . . ?
OW2A OW2 Cs2 73(2) . . ?
OW2 OW2A Cs2 86(2) . . ?
K1A OW6 K1 13.5(3) . . ?
K1A OW6 K1 107.8(6) . 2_675 ?
K1 OW6 K1 97.3(5) . 2_675 ?
Cs1 OW11 K1 134.2(4) . 1_565 ?

_refine_diff_density_max         2.523
_refine_diff_density_min         -2.545
_refine_diff_density_rms         0.251

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_4
_database_code_depnum_ccdc_archive 'CCDC 1871474'
_audit_update_record             
;
2018-10-04 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H85 As2 K5 Mn Mo12 N6 O76'
_chemical_formula_weight         3441.72

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.6211(5)
_cell_length_b                   12.0930(5)
_cell_length_c                   17.7264(7)
_cell_angle_alpha                76.5010(10)
_cell_angle_beta                 89.8460(10)
_cell_angle_gamma                84.7250(10)
_cell_volume                     2411.63(17)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    17508
_cell_measurement_theta_min      1.739
_cell_measurement_theta_max      24.999

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.370
_exptl_crystal_F_000             1676
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    2.647
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.521
_exptl_absorpt_correction_T_max  0.574
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'


_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            17508
_diffrn_reflns_av_unetI/netI     0.0297
_diffrn_reflns_av_R_equivalents  0.0201
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         1.739
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measured_fraction_theta_full 0.959
_diffrn_reflns_Laue_measured_fraction_max 0.986
_diffrn_reflns_Laue_measured_fraction_full 0.959
_diffrn_reflns_point_group_measured_fraction_max 0.986
_diffrn_reflns_point_group_measured_fraction_full 0.959
_reflns_number_total             8369
_reflns_number_gt                7419
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0372P)²+11.6477P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8369
_refine_ls_number_parameters     685
_refine_ls_number_restraints     12
_refine_ls_R_factor_all          0.0337
_refine_ls_R_factor_gt           0.0290
_refine_ls_wR_factor_ref         0.0769
_refine_ls_wR_factor_gt          0.0740
_refine_ls_goodness_of_fit_ref   0.958
_refine_ls_restrained_S_all      0.962
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.80490(3) 0.26353(3) 0.47145(2) 0.01448(9) Uani 1 1 d . . . . .
Mo2 Mo 1.08028(3) 0.25247(3) 0.38255(2) 0.01330(9) Uani 1 1 d . . . . .
Mo3 Mo 0.58183(3) 0.16984(3) 0.40128(2) 0.01300(9) Uani 1 1 d . . . . .
Mo4 Mo 1.11129(3) 0.13827(3) 0.23319(2) 0.01248(9) Uani 1 1 d . . . . .
Mo5 Mo 0.86946(3) 0.03303(3) 0.15353(2) 0.01234(9) Uani 1 1 d . . . . .
Mo6 Mo 0.61676(3) 0.06430(3) 0.23045(2) 0.01275(9) Uani 1 1 d . . . . .
As1 As 0.82470(4) 0.23033(3) 0.27837(2) 0.01070(10) Uani 1 1 d . . . . .
Mn1 Mn 0.80401(11) 0.49790(11) 0.57246(8) 0.0122(3) Uani 0.5 1 d . . P . .
K1 K 0.92010(12) -0.02855(10) 0.39666(7) 0.0378(3) Uani 1 1 d . . . . .
K2 K 0.69396(9) -0.00152(9) 0.59598(6) 0.0230(2) Uani 1 1 d . . . . .
K3 K 1.0282(4) 0.5404(4) 0.4008(2) 0.0282(8) Uani 0.5 1 d . . P . .
O1 O 1.0970(3) 0.1269(3) 0.45170(18) 0.0183(7) Uani 1 1 d . . . . .
O2 O 0.6138(3) 0.0269(3) 0.44129(18) 0.0212(7) Uani 1 1 d . . . . .
O3 O 0.9903(2) 0.1272(2) 0.16316(17) 0.0144(6) Uani 1 1 d . . . . .
O4 O 1.1850(2) 0.2042(2) 0.30894(17) 0.0150(6) Uani 1 1 d . . . . .
O5 O 0.6254(3) -0.0608(3) 0.30024(19) 0.0224(7) Uani 1 1 d . . . . .
O6 O 0.9045(3) 0.0087(3) 0.06337(19) 0.0211(7) Uani 1 1 d . . . . .
O7 O 0.5735(3) 0.1673(2) 0.29449(17) 0.0142(6) Uani 1 1 d . . . . .
O8 O 0.9238(3) -0.0902(3) 0.21698(19) 0.0215(7) Uani 1 1 d . . . . .
O9 O 0.8691(3) 0.1361(3) 0.52489(19) 0.0217(7) Uani 1 1 d . . . . .
O10 O 0.7661(2) 0.1945(2) 0.37343(17) 0.0137(6) Uani 1 1 d . . . . .
O11 O 0.9351(3) 0.3155(2) 0.41172(18) 0.0165(7) Uani 1 1 d . . . . .
O12 O 1.1260(3) -0.0009(3) 0.28633(19) 0.0212(7) Uani 1 1 d . . . . .
O13 O 0.5642(3) 0.3613(3) 0.34219(19) 0.0177(7) Uani 1 1 d . . . . .
O14 O 1.0607(3) 0.3256(3) 0.17834(19) 0.0203(7) Uani 1 1 d . . . . .
O15 O 0.7988(3) 0.2094(3) 0.08452(18) 0.0177(7) Uani 1 1 d . . . . .
O16 O 0.8008(3) 0.3521(3) 0.5352(2) 0.0287(8) Uani 1 1 d . . . . .
O17 O 0.6463(3) 0.2263(3) 0.48445(18) 0.0170(7) Uani 1 1 d . . . . .
O18 O 0.7217(3) 0.4242(3) 0.38441(18) 0.0172(7) Uani 1 1 d . . . . .
O19 O 0.6297(3) 0.2388(2) 0.14182(17) 0.0155(6) Uani 1 1 d . . . . .
O20 O 0.7107(3) 0.0099(3) 0.15252(17) 0.0163(7) Uani 1 1 d . . . . .
O21 O 0.4867(3) 0.0658(3) 0.18474(19) 0.0226(7) Uani 1 1 d . . . . .
O22 O 1.1697(3) 0.3390(3) 0.41463(19) 0.0207(7) Uani 1 1 d . . . . .
O23 O 1.2226(3) 0.1471(3) 0.16964(19) 0.0243(8) Uani 1 1 d . . . . .
O24 O 0.9713(2) 0.1823(2) 0.30796(17) 0.0134(6) Uani 1 1 d . . . . .
O25 O 0.4370(3) 0.1933(3) 0.41986(19) 0.0207(7) Uani 1 1 d . . . . .
O26 O 1.0431(3) 0.4085(3) 0.27972(19) 0.0205(7) Uani 1 1 d . . . . .
O27 O 0.7933(2) 0.1033(2) 0.25023(17) 0.0122(6) Uani 1 1 d . . . . .
C1 C 0.6780(4) 0.7231(4) 0.2068(3) 0.0281(12) Uani 1 1 d . . . . .
H1A H 0.7357 0.7726 0.1960 0.034 Uiso 1 1 calc R U . . .
C2 C 0.9129(5) 0.6221(4) 0.0291(3) 0.0311(13) Uani 1 1 d . . . . .
H2A H 0.8760 0.6213 -0.0172 0.037 Uiso 1 1 calc R U . . .
C3 C 0.9435(5) 0.5207(4) 0.0838(3) 0.0331(13) Uani 1 1 d . . . . .
H3A H 0.9275 0.4516 0.0736 0.040 Uiso 1 1 calc R U . . .
C4 C 0.4906(4) 0.6734(4) 0.1819(3) 0.0246(11) Uani 1 1 d . . . . .
H4A H 0.4203 0.6901 0.1549 0.030 Uiso 1 1 calc R U . . .
C5 C 0.7268(4) 0.4002(4) -0.0366(3) 0.0222(10) Uani 1 1 d . . . . .
H5A H 0.7691 0.3405 -0.0521 0.027 Uiso 1 1 calc R U . . .
C6 C 0.7012(4) 0.5043(4) -0.0886(3) 0.0266(11) Uani 1 1 d . . . . .
H6A H 0.7251 0.5149 -0.1396 0.032 Uiso 1 1 calc R U . . .
C7 C 0.9884(5) 0.7259(4) 0.1140(3) 0.0321(13) Uani 1 1 d . . . . .
H7A H 1.0041 0.7953 0.1239 0.039 Uiso 1 1 calc R U . . .
C8 C 0.6079(4) 0.5809(4) 0.0120(3) 0.0279(12) Uani 1 1 d . . . . .
H8A H 0.5711 0.6426 0.0283 0.034 Uiso 1 1 calc R U . . .
C9 C 0.6974(4) 0.6224(4) 0.2629(3) 0.0261(11) Uani 1 1 d . . . . .
H9A H 0.7672 0.6063 0.2906 0.031 Uiso 1 1 calc R U . . .
C10 C 1.0159(5) 0.6247(4) 0.1696(3) 0.0310(12) Uani 1 1 d . . . . .
H10A H 1.0468 0.6263 0.2176 0.037 Uiso 1 1 calc R U . . .
C11 C 0.6398(4) 0.5922(4) -0.0640(3) 0.0261(12) Uani 1 1 d . . . . .
C12 C 0.9968(4) 0.5213(4) 0.1526(3) 0.0188(10) Uani 1 1 d . . . . .
C13 C 0.5111(4) 0.5720(4) 0.2365(3) 0.0234(11) Uani 1 1 d . . . . .
H13A H 0.4548 0.5208 0.2454 0.028 Uiso 1 1 calc R U . . .
C14 C 0.6317(4) 0.4760(4) 0.0640(3) 0.0212(10) Uani 1 1 d . . . . .
H14A H 0.6094 0.4665 0.1153 0.025 Uiso 1 1 calc R U . . .
C15 C 0.9383(4) 0.7232(4) 0.0447(3) 0.0192(10) Uani 1 1 d . . . . .
C16 C 0.5733(4) 0.7510(4) 0.1665(3) 0.0199(10) Uani 1 1 d . . . . .
C17 C 1.0359(4) 0.4097(4) 0.2085(3) 0.0194(10) Uani 1 1 d . . . . .
C18 C 0.7077(4) 0.2695(4) 0.0929(2) 0.0140(9) Uani 1 1 d . . . . .
C19 C 0.6885(4) 0.3858(4) 0.0394(3) 0.0154(9) Uani 1 1 d . . . . .
C20 C 0.6147(4) 0.5449(4) 0.2787(3) 0.0162(9) Uani 1 1 d . . . . .
C23 C 0.6348(4) 0.4361(4) 0.3393(3) 0.0163(9) Uani 1 1 d . . . . .
N1 N 0.6065(4) 0.6994(4) -0.1203(3) 0.0382(12) Uani 1 1 d . . . . .
H1B H 0.5675 0.7545 -0.1058 0.046 Uiso 1 1 calc R U . . .
H1C H 0.6259 0.7075 -0.1680 0.046 Uiso 1 1 calc R U . . .
N2 N 0.5525(4) 0.8529(3) 0.1092(2) 0.0248(9) Uani 1 1 d . . . . .
H2B H 0.6052 0.8994 0.0986 0.030 Uiso 1 1 calc R U . . .
H2C H 0.4870 0.8689 0.0847 0.030 Uiso 1 1 calc R U . . .
N3 N 0.9091(3) 0.8297(3) -0.0136(2) 0.0191(8) Uani 1 1 d . . . . .
H3B H 0.9233 0.8938 -0.0044 0.023 Uiso 1 1 calc R U . . .
H3C H 0.8776 0.8281 -0.0572 0.023 Uiso 1 1 calc R U . . .
O1W O 0.6582(5) 0.5650(5) 0.5197(4) 0.0170(13) Uani 0.5 1 d . U P . .
O1WA O 0.6237(5) 0.5440(4) 0.5622(3) 0.0062(11) Uani 0.5 1 d . U P . .
O2W O 0.9999(11) 0.4676(13) 0.5711(8) 0.039(3) Uani 0.5 1 d . . P . .
O3W O 0.8077(5) 0.5793(5) 0.4480(3) 0.0150(13) Uani 0.5 1 d . . P . .
O4W O 0.7730(4) 0.4258(4) 0.6911(3) 0.0539(12) Uani 1 1 d . . . . .
OW1 O 1.0031(8) 0.7694(7) 0.3515(5) 0.045(2) Uani 0.5 1 d . . P . .
OW2 O 0.9054(7) 0.7504(7) 0.3671(5) 0.0375(19) Uani 0.5 1 d . . P . .
OW3 O 0.4709(4) 0.6528(6) 0.4232(3) 0.0764(18) Uani 1 1 d . . . . .
OW4 O 0.3942(5) 0.8591(5) 0.3098(3) 0.0737(18) Uani 1 1 d . . . . .
OW5 O 0.2131(5) 0.8090(4) 0.2236(3) 0.0563(13) Uani 1 1 d . . . . .
OW6 O 0.2811(4) 0.9015(4) 0.0688(3) 0.0503(11) Uani 1 1 d . . . . .
OW7 O 0.6957(4) 0.7858(3) 0.4365(2) 0.0494(12) Uani 1 1 d . . . . .
OW8 O 0.3436(3) 0.3538(4) 0.2645(2) 0.0492(12) Uani 1 1 d . . . . .
OW9 O 0.3304(3) 0.1367(4) 0.0297(2) 0.0381(10) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O9 1.714(3) . ?
Mo1 O16 1.726(3) . ?
Mo1 O11 1.914(3) . ?
Mo1 O17 1.938(3) . ?
Mo1 O10 2.161(3) . ?
Mo1 O18 2.314(3) . ?
Mo1 Mo3 3.2812(5) . ?
Mo2 O1 1.710(3) . ?
Mo2 O22 1.726(3) . ?
Mo2 O11 1.907(3) . ?
Mo2 O4 1.934(3) . ?
Mo2 O24 2.191(3) . ?
Mo2 O26 2.306(3) . ?
Mo2 Mo4 3.2645(5) . ?
Mo3 O2 1.715(3) . ?
Mo3 O25 1.724(3) . ?
Mo3 O7 1.903(3) . ?
Mo3 O17 1.942(3) . ?
Mo3 O10 2.227(3) . ?
Mo3 O13 2.298(3) . ?
Mo4 O23 1.707(3) . ?
Mo4 O12 1.719(3) . ?
Mo4 O3 1.912(3) . ?
Mo4 O4 1.950(3) . ?
Mo4 O24 2.201(3) . ?
Mo4 O14 2.270(3) . ?
Mo5 O8 1.713(3) . ?
Mo5 O6 1.732(3) . ?
Mo5 O20 1.892(3) . ?
Mo5 O3 1.920(3) . ?
Mo5 O27 2.231(3) . ?
Mo5 O15 2.277(3) . ?
Mo5 Mo6 3.2621(5) . ?
Mo6 O5 1.711(3) . ?
Mo6 O21 1.713(3) . ?
Mo6 O7 1.906(3) . ?
Mo6 O20 1.954(3) . ?
Mo6 O27 2.193(3) . ?
Mo6 O19 2.335(3) . ?
As1 O24 1.788(3) . ?
As1 O10 1.788(3) . ?
As1 O27 1.791(3) . ?
Mn1 O1W 1.950(6) . ?
Mn1 K3 1.995(5) 2_766 ?
Mn1 O16 2.026(4) . ?
Mn1 O22 2.087(3) 2_766 ?
Mn1 O1WA 2.115(5) . ?
Mn1 O4W 2.124(5) . ?
Mn1 O3W 2.198(6) . ?
Mn1 O2W 2.274(13) . ?
K3 O2W 0.589(11) 2_766 ?
K3 Mn1 1.995(5) 2_766 ?
O13 C23 1.269(5) . ?
O14 C17 1.265(6) . ?
O15 C18 1.257(5) . ?
O18 C23 1.266(5) . ?
O19 C18 1.271(5) . ?
O22 Mn1 2.087(3) 2_766 ?
O26 C17 1.263(6) . ?
C1 C9 1.381(7) . ?
C1 C16 1.386(7) . ?
C1 H1A 0.9300 . ?
C2 C15 1.372(7) . ?
C2 C3 1.391(7) . ?
C2 H2A 0.9300 . ?
C3 C12 1.372(7) . ?
C3 H3A 0.9300 . ?
C4 C13 1.375(7) . ?
C4 C16 1.387(7) . ?
C4 H4A 0.9300 . ?
C5 C6 1.384(7) . ?
C5 C19 1.395(7) . ?
C5 H5A 0.9300 . ?
C6 C11 1.379(7) . ?
C6 H6A 0.9300 . ?
C7 C15 1.370(7) . ?
C7 C10 1.392(7) . ?
C7 H7A 0.9300 . ?
C8 C11 1.376(8) . ?
C8 C14 1.388(7) . ?
C8 H8A 0.9300 . ?
C9 C20 1.386(7) . ?
C9 H9A 0.9300 . ?
C10 C12 1.390(7) . ?
C10 H10A 0.9300 . ?
C11 N1 1.460(6) . ?
C12 C17 1.508(6) . ?
C13 C20 1.391(6) . ?
C13 H13A 0.9300 . ?
C14 C19 1.379(6) . ?
C14 H14A 0.9300 . ?
C15 N3 1.464(6) . ?
C16 N2 1.403(6) . ?
C18 C19 1.499(6) . ?
C20 C23 1.491(6) . ?
N1 H1B 0.8600 . ?
N1 H1C 0.8600 . ?
N2 H2B 0.8600 . ?
N2 H2C 0.8600 . ?
N3 H3B 0.8600 . ?
N3 H3C 0.8600 . ?
O1W O1WA 0.849(7) . ?
O2W K3 0.589(11) 2_766 ?
OW1 OW2 1.198(11) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O9 Mo1 O16 103.73(16) . . ?
O9 Mo1 O11 98.60(14) . . ?
O16 Mo1 O11 99.49(15) . . ?
O9 Mo1 O17 97.27(14) . . ?
O16 Mo1 O17 96.51(15) . . ?
O11 Mo1 O17 154.05(13) . . ?
O9 Mo1 O10 93.93(13) . . ?
O16 Mo1 O10 161.20(14) . . ?
O11 Mo1 O10 83.95(12) . . ?
O17 Mo1 O10 74.58(12) . . ?
O9 Mo1 O18 171.93(13) . . ?
O16 Mo1 O18 84.19(14) . . ?
O11 Mo1 O18 78.33(12) . . ?
O17 Mo1 O18 83.13(12) . . ?
O10 Mo1 O18 78.38(11) . . ?
O9 Mo1 Mo3 99.11(11) . . ?
O16 Mo1 Mo3 126.40(11) . . ?
O11 Mo1 Mo3 124.16(9) . . ?
O17 Mo1 Mo3 32.28(9) . . ?
O10 Mo1 Mo3 42.38(8) . . ?
O18 Mo1 Mo3 76.91(7) . . ?
O1 Mo2 O22 104.02(15) . . ?
O1 Mo2 O11 100.10(14) . . ?
O22 Mo2 O11 99.16(14) . . ?
O1 Mo2 O4 96.23(13) . . ?
O22 Mo2 O4 97.33(14) . . ?
O11 Mo2 O4 153.17(13) . . ?
O1 Mo2 O24 93.00(13) . . ?
O22 Mo2 O24 162.12(14) . . ?
O11 Mo2 O24 82.91(12) . . ?
O4 Mo2 O24 75.08(11) . . ?
O1 Mo2 O26 172.09(13) . . ?
O22 Mo2 O26 83.82(13) . . ?
O11 Mo2 O26 79.36(13) . . ?
O4 Mo2 O26 81.55(12) . . ?
O24 Mo2 O26 79.10(11) . . ?
O1 Mo2 Mo4 96.28(10) . . ?
O22 Mo2 Mo4 128.54(11) . . ?
O11 Mo2 Mo4 123.27(9) . . ?
O4 Mo2 Mo4 32.96(9) . . ?
O24 Mo2 Mo4 42.11(8) . . ?
O26 Mo2 Mo4 77.70(8) . . ?
O2 Mo3 O25 103.57(15) . . ?
O2 Mo3 O7 99.77(14) . . ?
O25 Mo3 O7 100.30(14) . . ?
O2 Mo3 O17 97.45(14) . . ?
O25 Mo3 O17 98.97(14) . . ?
O7 Mo3 O17 150.26(13) . . ?
O2 Mo3 O10 92.22(13) . . ?
O25 Mo3 O10 163.22(13) . . ?
O7 Mo3 O10 82.26(12) . . ?
O17 Mo3 O10 72.99(11) . . ?
O2 Mo3 O13 172.33(13) . . ?
O25 Mo3 O13 84.09(13) . . ?
O7 Mo3 O13 78.17(12) . . ?
O17 Mo3 O13 81.54(12) . . ?
O10 Mo3 O13 80.20(11) . . ?
O2 Mo3 Mo1 98.13(11) . . ?
O25 Mo3 Mo1 129.14(11) . . ?
O7 Mo3 Mo1 120.62(9) . . ?
O17 Mo3 Mo1 32.22(9) . . ?
O10 Mo3 Mo1 40.85(7) . . ?
O13 Mo3 Mo1 76.93(8) . . ?
O23 Mo4 O12 104.80(16) . . ?
O23 Mo4 O3 98.08(14) . . ?
O12 Mo4 O3 99.01(14) . . ?
O23 Mo4 O4 96.75(14) . . ?
O12 Mo4 O4 96.86(14) . . ?
O3 Mo4 O4 154.69(12) . . ?
O23 Mo4 O24 162.82(14) . . ?
O12 Mo4 O24 91.09(13) . . ?
O3 Mo4 O24 85.55(12) . . ?
O4 Mo4 O24 74.53(11) . . ?
O23 Mo4 O14 86.77(14) . . ?
O12 Mo4 O14 168.43(14) . . ?
O3 Mo4 O14 79.04(12) . . ?
O4 Mo4 O14 81.46(12) . . ?
O24 Mo4 O14 77.41(11) . . ?
O23 Mo4 Mo2 127.95(12) . . ?
O12 Mo4 Mo2 95.63(11) . . ?
O3 Mo4 Mo2 125.56(9) . . ?
O4 Mo4 Mo2 32.65(8) . . ?
O24 Mo4 Mo2 41.88(7) . . ?
O14 Mo4 Mo2 76.74(8) . . ?
O8 Mo5 O6 103.61(15) . . ?
O8 Mo5 O20 100.74(14) . . ?
O6 Mo5 O20 98.57(14) . . ?
O8 Mo5 O3 98.76(14) . . ?
O6 Mo5 O3 98.17(14) . . ?
O20 Mo5 O3 150.44(12) . . ?
O8 Mo5 O27 91.49(13) . . ?
O6 Mo5 O27 164.46(13) . . ?
O20 Mo5 O27 74.61(11) . . ?
O3 Mo5 O27 82.91(11) . . ?
O8 Mo5 O15 171.37(14) . . ?
O6 Mo5 O15 84.39(13) . . ?
O20 Mo5 O15 80.99(12) . . ?
O3 Mo5 O15 76.61(11) . . ?
O27 Mo5 O15 80.78(11) . . ?
O8 Mo5 Mo6 98.67(11) . . ?
O6 Mo5 Mo6 129.77(11) . . ?
O20 Mo5 Mo6 32.57(9) . . ?
O3 Mo5 Mo6 122.21(9) . . ?
O27 Mo5 Mo6 42.05(7) . . ?
O15 Mo5 Mo6 78.17(8) . . ?
O5 Mo6 O21 103.53(16) . . ?
O5 Mo6 O7 98.66(14) . . ?
O21 Mo6 O7 99.63(14) . . ?
O5 Mo6 O20 97.91(14) . . ?
O21 Mo6 O20 95.61(14) . . ?
O7 Mo6 O20 154.15(12) . . ?
O5 Mo6 O27 95.10(14) . . ?
O21 Mo6 O27 159.98(14) . . ?
O7 Mo6 O27 84.51(11) . . ?
O20 Mo6 O27 74.36(11) . . ?
O5 Mo6 O19 172.07(13) . . ?
O21 Mo6 O19 84.40(13) . . ?
O7 Mo6 O19 79.73(12) . . ?
O20 Mo6 O19 81.13(12) . . ?
O27 Mo6 O19 77.04(10) . . ?
O5 Mo6 Mo5 98.75(11) . . ?
O21 Mo6 Mo5 125.15(11) . . ?
O7 Mo6 Mo5 125.67(9) . . ?
O20 Mo6 Mo5 31.41(9) . . ?
O27 Mo6 Mo5 42.94(7) . . ?
O19 Mo6 Mo5 76.29(7) . . ?
O24 As1 O10 95.95(13) . . ?
O24 As1 O27 96.04(13) . . ?
O10 As1 O27 96.62(13) . . ?
O1W Mn1 K3 163.1(2) . 2_766 ?
O1W Mn1 O16 93.1(2) . . ?
K3 Mn1 O16 90.18(16) 2_766 . ?
O1W Mn1 O22 87.3(2) . 2_766 ?
K3 Mn1 O22 85.48(16) 2_766 2_766 ?
O16 Mn1 O22 165.60(16) . 2_766 ?
O1W Mn1 O1WA 23.7(2) . . ?
K3 Mn1 O1WA 170.7(2) 2_766 . ?
O16 Mn1 O1WA 96.08(18) . . ?
O22 Mn1 O1WA 90.04(17) 2_766 . ?
O1W Mn1 O4W 109.4(3) . . ?
K3 Mn1 O4W 86.71(18) 2_766 . ?
O16 Mn1 O4W 96.79(17) . . ?
O22 Mn1 O4W 96.67(16) 2_766 . ?
O1WA Mn1 O4W 85.7(2) . . ?
O1W Mn1 O3W 62.0(3) . . ?
K3 Mn1 O3W 102.0(2) 2_766 . ?
O16 Mn1 O3W 83.98(19) . . ?
O22 Mn1 O3W 83.50(18) 2_766 . ?
O1WA Mn1 O3W 85.6(2) . . ?
O4W Mn1 O3W 171.3(2) . . ?
O1W Mn1 O2W 149.9(4) . . ?
K3 Mn1 O2W 14.0(4) 2_766 . ?
O16 Mn1 O2W 86.6(4) . . ?
O22 Mn1 O2W 85.9(4) 2_766 . ?
O1WA Mn1 O2W 172.9(4) . . ?
O4W Mn1 O2W 100.6(4) . . ?
O3W Mn1 O2W 88.1(4) . . ?
O2W K3 Mn1 111(2) 2_766 2_766 ?
Mo4 O3 Mo5 140.76(16) . . ?
Mo2 O4 Mo4 114.39(14) . . ?
Mo3 O7 Mo6 138.20(17) . . ?
As1 O10 Mo1 127.25(15) . . ?
As1 O10 Mo3 126.08(15) . . ?
Mo1 O10 Mo3 96.77(11) . . ?
Mo2 O11 Mo1 138.17(17) . . ?
C23 O13 Mo3 130.3(3) . . ?
C17 O14 Mo4 131.2(3) . . ?
C18 O15 Mo5 130.1(3) . . ?
Mo1 O16 Mn1 158.7(2) . . ?
Mo1 O17 Mo3 115.50(15) . . ?
C23 O18 Mo1 130.1(3) . . ?
C18 O19 Mo6 129.6(3) . . ?
Mo5 O20 Mo6 116.02(14) . . ?
Mo2 O22 Mn1 147.80(18) . 2_766 ?
As1 O24 Mo2 126.98(15) . . ?
As1 O24 Mo4 126.24(15) . . ?
Mo2 O24 Mo4 96.00(11) . . ?
C17 O26 Mo2 127.9(3) . . ?
As1 O27 Mo6 122.98(14) . . ?
As1 O27 Mo5 127.91(15) . . ?
Mo6 O27 Mo5 95.00(11) . . ?
C9 C1 C16 120.7(5) . . ?
C9 C1 H1A 119.7 . . ?
C16 C1 H1A 119.7 . . ?
C15 C2 C3 118.9(5) . . ?
C15 C2 H2A 120.5 . . ?
C3 C2 H2A 120.5 . . ?
C12 C3 C2 120.8(5) . . ?
C12 C3 H3A 119.6 . . ?
C2 C3 H3A 119.6 . . ?
C13 C4 C16 121.0(4) . . ?
C13 C4 H4A 119.5 . . ?
C16 C4 H4A 119.5 . . ?
C6 C5 C19 119.2(5) . . ?
C6 C5 H5A 120.4 . . ?
C19 C5 H5A 120.4 . . ?
C11 C6 C5 119.5(5) . . ?
C11 C6 H6A 120.3 . . ?
C5 C6 H6A 120.3 . . ?
C15 C7 C10 119.9(5) . . ?
C15 C7 H7A 120.0 . . ?
C10 C7 H7A 120.0 . . ?
C11 C8 C14 118.9(5) . . ?
C11 C8 H8A 120.5 . . ?
C14 C8 H8A 120.5 . . ?
C1 C9 C20 121.2(5) . . ?
C1 C9 H9A 119.4 . . ?
C20 C9 H9A 119.4 . . ?
C12 C10 C7 119.4(5) . . ?
C12 C10 H10A 120.3 . . ?
C7 C10 H10A 120.3 . . ?
C8 C11 C6 121.6(4) . . ?
C8 C11 N1 119.1(5) . . ?
C6 C11 N1 119.2(5) . . ?
C3 C12 C10 119.7(4) . . ?
C3 C12 C17 119.6(4) . . ?
C10 C12 C17 120.7(4) . . ?
C4 C13 C20 121.0(4) . . ?
C4 C13 H13A 119.5 . . ?
C20 C13 H13A 119.5 . . ?
C19 C14 C8 120.0(5) . . ?
C19 C14 H14A 120.0 . . ?
C8 C14 H14A 120.0 . . ?
C7 C15 C2 121.1(5) . . ?
C7 C15 N3 119.9(4) . . ?
C2 C15 N3 119.0(4) . . ?
C1 C16 C4 118.2(4) . . ?
C1 C16 N2 121.3(4) . . ?
C4 C16 N2 120.4(4) . . ?
O26 C17 O14 126.1(4) . . ?
O26 C17 C12 118.1(4) . . ?
O14 C17 C12 115.8(4) . . ?
O15 C18 O19 125.4(4) . . ?
O15 C18 C19 117.0(4) . . ?
O19 C18 C19 117.6(4) . . ?
C14 C19 C5 120.6(4) . . ?
C14 C19 C18 120.9(4) . . ?
C5 C19 C18 118.5(4) . . ?
C9 C20 C13 117.8(4) . . ?
C9 C20 C23 121.6(4) . . ?
C13 C20 C23 120.6(4) . . ?
O18 C23 O13 124.2(4) . . ?
O18 C23 C20 117.8(4) . . ?
O13 C23 C20 118.0(4) . . ?
C11 N1 H1B 120.0 . . ?
C11 N1 H1C 120.0 . . ?
H1B N1 H1C 120.0 . . ?
C16 N2 H2B 120.0 . . ?
C16 N2 H2C 120.0 . . ?
H2B N2 H2C 120.0 . . ?
C15 N3 H3B 120.0 . . ?
C15 N3 H3C 120.0 . . ?
H3B N3 H3C 120.0 . . ?
O1WA O1W Mn1 89.1(6) . . ?
O1W O1WA Mn1 67.2(5) . . ?
K3 O2W Mn1 55.0(16) 2_766 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O24 As1 O10 Mo1 62.35(19) . . . . ?
O27 As1 O10 Mo1 159.16(18) . . . . ?
O24 As1 O10 Mo3 -160.13(17) . . . . ?
O27 As1 O10 Mo3 -63.33(19) . . . . ?
O9 Mo1 O16 Mn1 146.9(5) . . . . ?
O11 Mo1 O16 Mn1 45.5(6) . . . . ?
O17 Mo1 O16 Mn1 -114.0(6) . . . . ?
O10 Mo1 O16 Mn1 -53.6(9) . . . . ?
O18 Mo1 O16 Mn1 -31.6(6) . . . . ?
Mo3 Mo1 O16 Mn1 -100.6(6) . . . . ?
O8 Mo5 O20 Mo6 89.30(18) . . . . ?
O6 Mo5 O20 Mo6 -164.99(17) . . . . ?
O3 Mo5 O20 Mo6 -41.1(3) . . . . ?
O27 Mo5 O20 Mo6 0.72(14) . . . . ?
O15 Mo5 O20 Mo6 -82.11(16) . . . . ?
O1 Mo2 O22 Mn1 -141.6(4) . . . 2_766 ?
O11 Mo2 O22 Mn1 -38.7(4) . . . 2_766 ?
O4 Mo2 O22 Mn1 120.1(4) . . . 2_766 ?
O24 Mo2 O22 Mn1 56.6(7) . . . 2_766 ?
O26 Mo2 O22 Mn1 39.5(4) . . . 2_766 ?
Mo4 Mo2 O22 Mn1 108.4(3) . . . 2_766 ?
O10 As1 O24 Mo2 -64.5(2) . . . . ?
O27 As1 O24 Mo2 -161.82(18) . . . . ?
O10 As1 O24 Mo4 159.93(17) . . . . ?
O27 As1 O24 Mo4 62.60(19) . . . . ?
O24 As1 O27 Mo6 165.01(17) . . . . ?
O10 As1 O27 Mo6 68.28(18) . . . . ?
O24 As1 O27 Mo5 -65.41(19) . . . . ?
O10 As1 O27 Mo5 -162.14(18) . . . . ?
C15 C2 C3 C12 0.8(9) . . . . ?
C19 C5 C6 C11 0.9(7) . . . . ?
C16 C1 C9 C20 2.1(8) . . . . ?
C15 C7 C10 C12 2.9(8) . . . . ?
C14 C8 C11 C6 -4.2(7) . . . . ?
C14 C8 C11 N1 174.9(4) . . . . ?
C5 C6 C11 C8 3.1(7) . . . . ?
C5 C6 C11 N1 -176.0(4) . . . . ?
C2 C3 C12 C10 3.0(8) . . . . ?
C2 C3 C12 C17 -176.0(5) . . . . ?
C7 C10 C12 C3 -4.8(8) . . . . ?
C7 C10 C12 C17 174.2(5) . . . . ?
C16 C4 C13 C20 0.9(8) . . . . ?
C11 C8 C14 C19 1.3(7) . . . . ?
C10 C7 C15 C2 0.9(8) . . . . ?
C10 C7 C15 N3 179.8(5) . . . . ?
C3 C2 C15 C7 -2.7(8) . . . . ?
C3 C2 C15 N3 178.4(5) . . . . ?
C9 C1 C16 C4 -2.4(8) . . . . ?
C9 C1 C16 N2 -179.8(5) . . . . ?
C13 C4 C16 C1 0.9(7) . . . . ?
C13 C4 C16 N2 178.4(5) . . . . ?
Mo2 O26 C17 O14 -8.5(7) . . . . ?
Mo2 O26 C17 C12 172.9(3) . . . . ?
Mo4 O14 C17 O26 6.1(7) . . . . ?
Mo4 O14 C17 C12 -175.3(3) . . . . ?
C3 C12 C17 O26 -153.5(5) . . . . ?
C10 C12 C17 O26 27.5(7) . . . . ?
C3 C12 C17 O14 27.8(6) . . . . ?
C10 C12 C17 O14 -151.2(5) . . . . ?
Mo5 O15 C18 O19 -4.3(7) . . . . ?
Mo5 O15 C18 C19 177.2(3) . . . . ?
Mo6 O19 C18 O15 -2.5(6) . . . . ?
Mo6 O19 C18 C19 176.0(3) . . . . ?
C8 C14 C19 C5 2.7(7) . . . . ?
C8 C14 C19 C18 -175.6(4) . . . . ?
C6 C5 C19 C14 -3.8(7) . . . . ?
C6 C5 C19 C18 174.5(4) . . . . ?
O15 C18 C19 C14 -147.0(4) . . . . ?
O19 C18 C19 C14 34.4(6) . . . . ?
O15 C18 C19 C5 34.6(6) . . . . ?
O19 C18 C19 C5 -144.0(4) . . . . ?
C1 C9 C20 C13 -0.3(7) . . . . ?
C1 C9 C20 C23 -179.8(5) . . . . ?
C4 C13 C20 C9 -1.2(7) . . . . ?
C4 C13 C20 C23 178.4(5) . . . . ?
Mo1 O18 C23 O13 11.3(6) . . . . ?
Mo1 O18 C23 C20 -168.4(3) . . . . ?
Mo3 O13 C23 O18 -17.1(6) . . . . ?
Mo3 O13 C23 C20 162.6(3) . . . . ?
C9 C20 C23 O18 10.8(6) . . . . ?
C13 C20 C23 O18 -168.7(4) . . . . ?
C9 C20 C23 O13 -168.9(4) . . . . ?
C13 C20 C23 O13 11.6(6) . . . . ?

_refine_diff_density_max         2.714
_refine_diff_density_min         -1.019
_refine_diff_density_rms         0.119

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_12
_database_code_depnum_ccdc_archive 'CCDC 1871482'
_audit_update_record             
;
2018-10-04 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C16 H71 As2 K2 Mn2 Mo12 N4 Na O72'
_chemical_formula_weight         2983.96

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.702(2)
_cell_length_b                   23.542(3)
_cell_length_c                   15.546(2)
_cell_angle_alpha                90
_cell_angle_beta                 119.466(11)
_cell_angle_gamma                90
_cell_volume                     4366.0(11)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    24299
_cell_measurement_theta_min      1.844
_cell_measurement_theta_max      27.547

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.270
_exptl_crystal_F_000             2879
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    2.902
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.489
_exptl_absorpt_correction_T_max  0.544
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            24299
_diffrn_reflns_av_unetI/netI     0.0490
_diffrn_reflns_av_R_equivalents  0.0417
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         1.844
_diffrn_reflns_theta_max         27.547
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             9941
_reflns_number_gt                8323
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0741P)²+21.7855P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         9941
_refine_ls_number_parameters     554
_refine_ls_number_restraints     38
_refine_ls_R_factor_all          0.0579
_refine_ls_R_factor_gt           0.0470
_refine_ls_wR_factor_ref         0.1412
_refine_ls_wR_factor_gt          0.1329
_refine_ls_goodness_of_fit_ref   1.047
_refine_ls_restrained_S_all      1.050
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.19524(4) 0.52229(2) 0.37731(4) 0.02219(12) Uani 1 1 d . . . . .
Mo2 Mo -0.13371(4) 0.38166(2) 0.04748(3) 0.02099(12) Uani 1 1 d . . . . .
Mo3 Mo 0.06072(5) 0.29200(2) 0.07599(3) 0.02197(12) Uani 1 1 d . . . . .
Mo4 Mo 0.40501(4) 0.42151(2) 0.41153(3) 0.02136(12) Uani 1 1 d . . . . .
Mo5 Mo -0.06275(4) 0.50317(2) 0.20202(4) 0.02231(12) Uani 1 1 d . . . . .
Mo6 Mo 0.34034(5) 0.31122(2) 0.26837(4) 0.02766(14) Uani 1 1 d . . . . .
As1 As 0.11962(5) 0.38419(2) 0.27625(4) 0.01864(13) Uani 1 1 d . . . . .
Mn1 Mn 0.58967(10) 0.43839(5) 0.68204(8) 0.0373(3) Uani 1 1 d . . . . .
K1 K 0.15202(19) 0.03894(9) 0.60392(14) 0.0569(5) Uani 1 1 d . . . . .
Na1 Na 0.3797(4) 0.5922(2) 0.7932(5) 0.0379(13) Uani 0.5 1 d . . P . .
O1 O 0.4222(4) 0.47064(19) 0.3383(3) 0.0298(10) Uani 1 1 d . . . . .
O2 O 0.0444(3) 0.36821(17) 0.1477(3) 0.0211(8) Uani 1 1 d . . . . .
O3 O -0.0953(4) 0.31500(17) -0.0015(3) 0.0244(9) Uani 1 1 d . . . . .
O4 O 0.1946(4) 0.28148(18) 0.1968(3) 0.0299(10) Uani 1 1 d . . . . .
O5 O 0.2550(3) 0.38529(17) 0.2876(3) 0.0226(8) Uani 1 1 d . . . . .
O6 O -0.1230(4) 0.43140(17) 0.1478(3) 0.0246(9) Uani 1 1 d . . . . .
O7 O 0.0971(3) 0.45874(17) 0.2631(3) 0.0211(8) Uani 1 1 d . . . . .
O8 O -0.1084(4) 0.42974(19) -0.0205(3) 0.0310(10) Uani 1 1 d . . . . .
O9 O 0.3504(4) 0.3428(3) 0.1759(4) 0.0438(13) Uani 1 1 d . . . . .
O10 O 0.2993(4) 0.46217(18) 0.4317(3) 0.0246(9) Uani 1 1 d . . . . .
O11 O -0.1797(4) 0.5355(2) 0.1913(4) 0.0383(11) Uani 1 1 d . . . . .
O12 O -0.1369(4) 0.31716(18) 0.1564(3) 0.0301(10) Uani 1 1 d . . . . .
O13 O 0.2455(4) 0.55033(19) 0.3034(3) 0.0297(10) Uani 1 1 d . . . . .
O14 O -0.0093(4) 0.25376(19) 0.1703(3) 0.0307(10) Uani 1 1 d . . . . .
O15 O -0.0559(4) 0.4587(2) 0.3356(3) 0.0330(10) Uani 1 1 d . . . . .
O16 O 0.2423(5) 0.5678(2) 0.4744(4) 0.0417(12) Uani 1 1 d . . . . .
O17 O 0.4565(4) 0.35549(19) 0.3762(3) 0.0296(10) Uani 1 1 d . . . . .
O18 O -0.2768(4) 0.3734(2) -0.0181(3) 0.0359(11) Uani 1 1 d . . . . .
O19 O 0.1088(4) 0.3302(2) 0.0116(3) 0.0330(10) Uani 1 1 d . . . . .
O20 O 0.1205(4) 0.47184(19) 0.4528(3) 0.0301(10) Uani 1 1 d . . . . .
O21 O 0.5208(4) 0.4310(2) 0.5260(3) 0.0317(10) Uani 1 1 d . . . . .
O22 O -0.0483(4) 0.5314(2) 0.1080(3) 0.0355(11) Uani 1 1 d . . . . .
O23 O 0.0407(4) 0.2251(2) 0.0265(3) 0.0366(11) Uani 1 1 d . . . . .
O24 O 0.3140(4) 0.28099(19) 0.3943(3) 0.0364(11) Uani 1 1 d . . . . .
O25 O 0.0446(4) 0.55181(17) 0.3053(3) 0.0253(9) Uani 1 1 d . . . . .
O26 O 0.4184(5) 0.2508(2) 0.2914(4) 0.0492(14) Uani 1 1 d . . . . .
O27 O 0.3553(4) 0.35682(18) 0.4903(3) 0.0288(10) Uani 1 1 d . . . . .
C1 C 0.3061(11) 0.2736(4) 0.5409(7) 0.070(3) Uani 1 1 d . . . . .
H1A H 0.2854 0.2353 0.5175 0.105 Uiso 1 1 calc R U . . .
H1B H 0.3728 0.2731 0.6043 0.105 Uiso 1 1 calc R U . . .
H1C H 0.2463 0.2912 0.5466 0.105 Uiso 1 1 calc R U . . .
C2 C 0.1072(7) 0.4031(3) 0.5850(5) 0.0423(18) Uani 1 1 d . . . . .
H2A H 0.1407 0.4390 0.6161 0.051 Uiso 1 1 calc R U . . .
H2B H 0.1615 0.3822 0.5747 0.051 Uiso 1 1 calc R U . . .
C3 C -0.0668(7) 0.1773(3) 0.2670(5) 0.0339(15) Uani 1 1 d . . . . .
H3A H -0.0950 0.1612 0.2016 0.041 Uiso 1 1 calc R U . . .
H3B H 0.0144 0.1773 0.2992 0.041 Uiso 1 1 calc R U . . .
C4 C 0.0061(6) 0.4136(3) 0.4897(5) 0.0332(15) Uani 1 1 d . . . . .
H4A H -0.0502 0.4310 0.5017 0.040 Uiso 1 1 calc R U . . .
H4B H -0.0234 0.3774 0.4574 0.040 Uiso 1 1 calc R U . . .
C5 C -0.1069(6) 0.2369(3) 0.2572(5) 0.0334(15) Uani 1 1 d . . . . .
H5A H -0.0713 0.2545 0.3220 0.040 Uiso 1 1 calc R U . . .
H5B H -0.1871 0.2367 0.2326 0.040 Uiso 1 1 calc R U . . .
C6 C 0.3273(6) 0.3060(3) 0.4704(5) 0.0290(13) Uani 1 1 d . . . . .
C7 C 0.0254(6) 0.4511(3) 0.4209(5) 0.0275(13) Uani 1 1 d . . . . .
C8 C -0.0827(6) 0.2722(3) 0.1885(4) 0.0262(13) Uani 1 1 d . . . . .
N1 N 0.0776(6) 0.3700(3) 0.6505(5) 0.0430(15) Uani 1 1 d . . . . .
H1D H 0.1391 0.3638 0.7082 0.064 Uiso 1 1 calc R U . . .
H1E H 0.0283 0.3896 0.6605 0.064 Uiso 1 1 calc R U . . .
H1F H 0.0476 0.3369 0.6221 0.064 Uiso 1 1 calc R U . . .
N2 N -0.1025(5) 0.1411(2) 0.3241(4) 0.0308(12) Uani 1 1 d . . . . .
H2C H -0.0764 0.1060 0.3278 0.046 Uiso 1 1 calc R U . . .
H2D H -0.0756 0.1551 0.3847 0.046 Uiso 1 1 calc R U . . .
H2E H -0.1770 0.1402 0.2942 0.046 Uiso 1 1 calc R U . . .
O1W O 0.6435(5) 0.3484(2) 0.7071(5) 0.0638(18) Uani 1 1 d D . . . .
O2W O 0.6423(5) 0.4566(3) 0.8347(4) 0.0624(18) Uani 1 1 d . . . . .
O3W O 0.4181(6) 0.4260(4) 0.6556(5) 0.085(3) Uani 1 1 d . . . . .
OW1 O 0.2414(11) 0.3326(4) 0.8364(10) 0.068(4) Uani 0.5 1 d . . P . .
OW2 O 0.386(3) 0.5571(14) 0.927(2) 0.174(11) Uani 0.5 1 d . U P . .
OW3 O 0.5474(18) 0.5504(9) 0.8610(19) 0.129(8) Uani 0.5 1 d . . P . .
OW4 O 0.2212(14) 0.7107(8) 0.5535(15) 0.105(6) Uani 0.5 1 d . . P . .
OW5 O 0.2719(13) 0.4009(7) -0.0038(11) 0.086(5) Uani 0.5 1 d . . P . .
OW6 O 0.5982(13) 0.2564(6) 0.7701(14) 0.093(5) Uani 0.5 1 d D U P . .
OW7 O 0.3784(12) 0.6101(8) 0.6653(10) 0.080(5) Uani 0.5 1 d . U P . .
OW8 O 0.2238(12) 0.6243(6) 0.7388(12) 0.073(4) Uani 0.5 1 d . U P . .
OW9 O 0.636(3) 0.3023(10) 0.541(2) 0.16(2) Uani 0.5 1 d D . P . .
OW10 O 0.634(3) 0.3067(11) 0.535(2) 0.109(14) Uani 0.5 1 d . U P . .
OW11 O 0.311(2) 0.5220(11) 0.684(2) 0.165(10) Uani 0.5 1 d . U P . .
OW12 O 0.567(2) 0.1989(10) 0.4866(18) 0.132(8) Uiso 0.5 1 d D . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O16 1.698(5) . ?
Mo1 O13 1.734(4) . ?
Mo1 O10 1.888(4) . ?
Mo1 O25 1.930(4) . ?
Mo1 O7 2.202(4) . ?
Mo1 O20 2.240(4) . ?
Mo1 Mo5 3.2631(10) . ?
Mo2 O8 1.696(4) . ?
Mo2 O18 1.719(5) . ?
Mo2 O6 1.897(4) . ?
Mo2 O3 1.927(4) . ?
Mo2 O2 2.177(4) . ?
Mo2 O12 2.291(4) . ?
Mo2 Mo3 3.2539(8) . ?
Mo2 K1 4.026(2) 4_565 ?
Mo3 O19 1.700(5) . ?
Mo3 O23 1.715(5) . ?
Mo3 O4 1.888(4) . ?
Mo3 O3 1.944(4) . ?
Mo3 O2 2.181(4) . ?
Mo3 O14 2.294(4) . ?
Mo3 K1 4.130(2) 4_565 ?
Mo4 O21 1.720(4) . ?
Mo4 O1 1.719(4) . ?
Mo4 O10 1.887(4) . ?
Mo4 O17 1.896(4) . ?
Mo4 O5 2.184(4) . ?
Mo4 O27 2.259(4) . ?
Mo4 Mo6 3.2464(8) . ?
Mo5 O22 1.703(5) . ?
Mo5 O11 1.706(5) . ?
Mo5 O6 1.888(4) . ?
Mo5 O25 1.931(4) . ?
Mo5 O7 2.179(4) . ?
Mo5 O15 2.286(4) . ?
Mo5 K1 4.048(2) 4_565 ?
Mo6 O9 1.683(5) . ?
Mo6 O26 1.709(5) . ?
Mo6 O4 1.879(5) . ?
Mo6 O17 1.951(4) . ?
Mo6 O5 2.200(4) . ?
Mo6 O24 2.272(5) . ?
As1 O7 1.776(4) . ?
As1 O5 1.775(4) . ?
As1 O2 1.781(4) . ?
As1 K1 3.4379(19) 4_565 ?
Mn1 O21 2.133(4) . ?
Mn1 O2W 2.157(6) . ?
Mn1 O1 2.159(5) 3_666 ?
Mn1 O13 2.173(5) 3_666 ?
Mn1 O3W 2.198(7) . ?
Mn1 O1W 2.213(6) . ?
K1 O8 2.808(5) 2_545 ?
K1 O22 2.881(5) 2_545 ?
K1 O2 2.899(4) 4_566 ?
K1 O7 2.920(4) 4_566 ?
K1 O5 3.059(4) 4_566 ?
K1 O2W 3.157(8) 2_646 ?
K1 OW5 3.195(18) 4_566 ?
K1 O8 3.198(5) 4_566 ?
K1 O22 3.233(6) 4_566 ?
K1 O19 3.327(5) 4_566 ?
K1 O13 3.431(5) 4_566 ?
K1 As1 3.4379(19) 4_566 ?
Na1 OW8 2.019(16) . ?
Na1 OW7 2.023(15) . ?
Na1 OW2 2.20(3) . ?
Na1 OW11 2.22(3) . ?
Na1 OW3 2.23(2) . ?
O1 Mn1 2.159(5) 3_666 ?
O2 K1 2.899(4) 4_565 ?
O5 K1 3.059(4) 4_565 ?
O7 K1 2.920(4) 4_565 ?
O8 K1 2.808(5) 2 ?
O8 K1 3.198(5) 4_565 ?
O12 C8 1.247(7) . ?
O13 Mn1 2.173(5) 3_666 ?
O13 K1 3.431(5) 4_565 ?
O14 C8 1.249(8) . ?
O15 C7 1.256(8) . ?
O19 K1 3.326(5) 4_565 ?
O20 C7 1.244(8) . ?
O22 K1 2.881(5) 2 ?
O22 K1 3.233(6) 4_565 ?
O24 C6 1.252(8) . ?
O27 C6 1.248(8) . ?
C1 C6 1.477(10) . ?
C1 H1A 0.9600 . ?
C1 H1B 0.9600 . ?
C1 H1C 0.9600 . ?
C2 C4 1.468(11) . ?
C2 N1 1.488(9) . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
C3 N2 1.478(8) . ?
C3 C5 1.488(9) . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
C4 C7 1.508(9) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 C8 1.513(8) . ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
N1 H1D 0.8900 . ?
N1 H1E 0.8900 . ?
N1 H1F 0.8900 . ?
N2 H2C 0.8900 . ?
N2 H2D 0.8900 . ?
N2 H2E 0.8900 . ?
O2W K1 3.157(8) 2_656 ?
OW5 K1 3.195(18) 4_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Mo1 O13 104.3(2) . . ?
O16 Mo1 O10 101.7(2) . . ?
O13 Mo1 O10 97.1(2) . . ?
O16 Mo1 O25 96.8(2) . . ?
O13 Mo1 O25 98.0(2) . . ?
O10 Mo1 O25 152.40(18) . . ?
O16 Mo1 O7 163.6(2) . . ?
O13 Mo1 O7 90.48(18) . . ?
O10 Mo1 O7 83.04(16) . . ?
O25 Mo1 O7 73.89(16) . . ?
O16 Mo1 O20 86.6(2) . . ?
O13 Mo1 O20 168.97(19) . . ?
O10 Mo1 O20 78.84(18) . . ?
O25 Mo1 O20 81.98(18) . . ?
O7 Mo1 O20 78.88(15) . . ?
O16 Mo1 Mo5 127.64(19) . . ?
O13 Mo1 Mo5 96.84(15) . . ?
O10 Mo1 Mo5 122.67(13) . . ?
O25 Mo1 Mo5 32.32(12) . . ?
O7 Mo1 Mo5 41.59(11) . . ?
O20 Mo1 Mo5 77.17(12) . . ?
O8 Mo2 O18 103.3(2) . . ?
O8 Mo2 O6 98.2(2) . . ?
O18 Mo2 O6 99.3(2) . . ?
O8 Mo2 O3 96.8(2) . . ?
O18 Mo2 O3 97.3(2) . . ?
O6 Mo2 O3 154.37(18) . . ?
O8 Mo2 O2 92.4(2) . . ?
O18 Mo2 O2 163.2(2) . . ?
O6 Mo2 O2 83.99(17) . . ?
O3 Mo2 O2 74.72(16) . . ?
O8 Mo2 O12 170.6(2) . . ?
O18 Mo2 O12 86.1(2) . . ?
O6 Mo2 O12 79.83(17) . . ?
O3 Mo2 O12 81.98(16) . . ?
O2 Mo2 O12 78.28(16) . . ?
O8 Mo2 Mo3 96.49(16) . . ?
O18 Mo2 Mo3 128.72(17) . . ?
O6 Mo2 Mo3 124.15(13) . . ?
O3 Mo2 Mo3 32.98(12) . . ?
O2 Mo2 Mo3 41.75(10) . . ?
O12 Mo2 Mo3 77.38(11) . . ?
O8 Mo2 K1 49.54(16) . 4_565 ?
O18 Mo2 K1 152.26(17) . 4_565 ?
O6 Mo2 K1 81.98(13) . 4_565 ?
O3 Mo2 K1 92.23(13) . 4_565 ?
O2 Mo2 K1 44.31(11) . 4_565 ?
O12 Mo2 K1 121.12(12) . 4_565 ?
Mo3 Mo2 K1 68.18(4) . 4_565 ?
O19 Mo3 O23 104.2(2) . . ?
O19 Mo3 O4 100.7(2) . . ?
O23 Mo3 O4 100.9(2) . . ?
O19 Mo3 O3 96.6(2) . . ?
O23 Mo3 O3 95.4(2) . . ?
O4 Mo3 O3 152.50(19) . . ?
O19 Mo3 O2 91.87(19) . . ?
O23 Mo3 O2 162.0(2) . . ?
O4 Mo3 O2 83.88(17) . . ?
O3 Mo3 O2 74.30(16) . . ?
O19 Mo3 O14 171.2(2) . . ?
O23 Mo3 O14 84.3(2) . . ?
O4 Mo3 O14 79.66(19) . . ?
O3 Mo3 O14 80.04(17) . . ?
O2 Mo3 O14 79.38(16) . . ?
O19 Mo3 Mo2 96.02(16) . . ?
O23 Mo3 Mo2 126.54(18) . . ?
O4 Mo3 Mo2 123.40(14) . . ?
O3 Mo3 Mo2 32.64(12) . . ?
O2 Mo3 Mo2 41.66(11) . . ?
O14 Mo3 Mo2 76.69(12) . . ?
O19 Mo3 K1 50.75(16) . 4_565 ?
O23 Mo3 K1 154.92(17) . 4_565 ?
O4 Mo3 K1 85.75(14) . 4_565 ?
O3 Mo3 K1 88.89(12) . 4_565 ?
O2 Mo3 K1 41.90(11) . 4_565 ?
O14 Mo3 K1 120.74(12) . 4_565 ?
Mo2 Mo3 K1 64.82(4) . 4_565 ?
O21 Mo4 O1 104.0(2) . . ?
O21 Mo4 O10 98.9(2) . . ?
O1 Mo4 O10 97.8(2) . . ?
O21 Mo4 O17 96.9(2) . . ?
O1 Mo4 O17 99.7(2) . . ?
O10 Mo4 O17 152.79(19) . . ?
O21 Mo4 O5 162.31(19) . . ?
O1 Mo4 O5 93.13(19) . . ?
O10 Mo4 O5 83.02(16) . . ?
O17 Mo4 O5 75.37(17) . . ?
O21 Mo4 O27 84.1(2) . . ?
O1 Mo4 O27 171.5(2) . . ?
O10 Mo4 O27 77.91(17) . . ?
O17 Mo4 O27 81.88(18) . . ?
O5 Mo4 O27 79.11(16) . . ?
O21 Mo4 Mo6 127.94(16) . . ?
O1 Mo4 Mo6 99.45(15) . . ?
O10 Mo4 Mo6 123.14(13) . . ?
O17 Mo4 Mo6 32.97(13) . . ?
O5 Mo4 Mo6 42.41(11) . . ?
O27 Mo4 Mo6 77.23(11) . . ?
O22 Mo5 O11 104.0(2) . . ?
O22 Mo5 O6 100.1(2) . . ?
O11 Mo5 O6 99.9(2) . . ?
O22 Mo5 O25 96.9(2) . . ?
O11 Mo5 O25 96.4(2) . . ?
O6 Mo5 O25 152.76(18) . . ?
O22 Mo5 O7 92.6(2) . . ?
O11 Mo5 O7 162.0(2) . . ?
O6 Mo5 O7 83.68(17) . . ?
O25 Mo5 O7 74.40(16) . . ?
O22 Mo5 O15 171.1(2) . . ?
O11 Mo5 O15 84.8(2) . . ?
O6 Mo5 O15 79.03(17) . . ?
O25 Mo5 O15 80.89(18) . . ?
O7 Mo5 O15 78.54(16) . . ?
O22 Mo5 Mo1 97.32(17) . . ?
O11 Mo5 Mo1 126.83(17) . . ?
O6 Mo5 Mo1 123.55(13) . . ?
O25 Mo5 Mo1 32.30(12) . . ?
O7 Mo5 Mo1 42.13(10) . . ?
O15 Mo5 Mo1 76.18(12) . . ?
O22 Mo5 K1 50.16(17) . 4_565 ?
O11 Mo5 K1 153.43(18) . 4_565 ?
O6 Mo5 K1 81.46(13) . 4_565 ?
O25 Mo5 K1 93.51(13) . 4_565 ?
O7 Mo5 K1 44.38(10) . 4_565 ?
O15 Mo5 K1 121.18(13) . 4_565 ?
Mo1 Mo5 K1 70.05(3) . 4_565 ?
O9 Mo6 O26 104.0(3) . . ?
O9 Mo6 O4 99.7(2) . . ?
O26 Mo6 O4 100.8(2) . . ?
O9 Mo6 O17 97.1(2) . . ?
O26 Mo6 O17 95.9(2) . . ?
O4 Mo6 O17 152.68(19) . . ?
O9 Mo6 O5 92.2(2) . . ?
O26 Mo6 O5 162.0(2) . . ?
O4 Mo6 O5 83.96(17) . . ?
O17 Mo6 O5 73.95(17) . . ?
O9 Mo6 O24 171.3(2) . . ?
O26 Mo6 O24 84.7(3) . . ?
O4 Mo6 O24 79.67(19) . . ?
O17 Mo6 O24 80.51(18) . . ?
O5 Mo6 O24 79.12(16) . . ?
O9 Mo6 Mo4 97.05(19) . . ?
O26 Mo6 Mo4 126.19(18) . . ?
O4 Mo6 Mo4 123.80(14) . . ?
O17 Mo6 Mo4 31.94(13) . . ?
O5 Mo6 Mo4 42.03(11) . . ?
O24 Mo6 Mo4 76.44(12) . . ?
O7 As1 O5 96.36(19) . . ?
O7 As1 O2 96.19(18) . . ?
O5 As1 O2 96.56(18) . . ?
O7 As1 K1 58.12(13) . 4_565 ?
O5 As1 K1 62.64(13) . 4_565 ?
O2 As1 K1 57.46(14) . 4_565 ?
O21 Mn1 O2W 171.3(2) . . ?
O21 Mn1 O1 87.45(18) . 3_666 ?
O2W Mn1 O1 85.6(2) . 3_666 ?
O21 Mn1 O13 89.08(18) . 3_666 ?
O2W Mn1 O13 95.4(2) . 3_666 ?
O1 Mn1 O13 83.91(18) 3_666 3_666 ?
O21 Mn1 O3W 86.7(2) . . ?
O2W Mn1 O3W 88.9(3) . . ?
O1 Mn1 O3W 96.2(3) 3_666 . ?
O13 Mn1 O3W 175.8(2) 3_666 . ?
O21 Mn1 O1W 92.5(2) . . ?
O2W Mn1 O1W 95.4(3) . . ?
O1 Mn1 O1W 165.8(2) 3_666 . ?
O13 Mn1 O1W 81.9(2) 3_666 . ?
O3W Mn1 O1W 98.0(3) . . ?
O8 K1 O22 62.74(14) 2_545 2_545 ?
O8 K1 O2 141.38(16) 2_545 4_566 ?
O22 K1 O2 107.05(14) 2_545 4_566 ?
O8 K1 O7 108.88(14) 2_545 4_566 ?
O22 K1 O7 141.51(16) 2_545 4_566 ?
O2 K1 O7 54.12(11) 4_566 4_566 ?
O8 K1 O5 149.37(14) 2_545 4_566 ?
O22 K1 O5 147.65(15) 2_545 4_566 ?
O2 K1 O5 52.82(11) 4_566 4_566 ?
O7 K1 O5 52.48(11) 4_566 4_566 ?
O8 K1 O2W 62.18(15) 2_545 2_646 ?
O22 K1 O2W 99.94(15) 2_545 2_646 ?
O2 K1 O2W 150.89(14) 4_566 2_646 ?
O7 K1 O2W 108.61(15) 4_566 2_646 ?
O5 K1 O2W 98.19(14) 4_566 2_646 ?
O8 K1 OW5 102.2(2) 2_545 4_566 ?
O22 K1 OW5 61.3(3) 2_545 4_566 ?
O2 K1 OW5 103.9(3) 4_566 4_566 ?
O7 K1 OW5 148.1(2) 4_566 4_566 ?
O5 K1 OW5 96.4(2) 4_566 4_566 ?
O2W K1 OW5 79.5(3) 2_646 4_566 ?
O8 K1 O8 90.63(14) 2_545 4_566 ?
O22 K1 O8 63.04(13) 2_545 4_566 ?
O2 K1 O8 54.75(12) 4_566 4_566 ?
O7 K1 O8 80.34(12) 4_566 4_566 ?
O5 K1 O8 107.16(12) 4_566 4_566 ?
O2W K1 O8 152.76(15) 2_646 4_566 ?
OW5 K1 O8 106.8(3) 4_566 4_566 ?
O8 K1 O22 63.28(14) 2_545 4_566 ?
O22 K1 O22 92.57(14) 2_545 4_566 ?
O2 K1 O22 81.17(13) 4_566 4_566 ?
O7 K1 O22 54.39(12) 4_566 4_566 ?
O5 K1 O22 106.65(12) 4_566 4_566 ?
O2W K1 O22 108.67(17) 2_646 4_566 ?
OW5 K1 O22 153.8(3) 4_566 4_566 ?
O8 K1 O22 54.86(13) 4_566 4_566 ?
O8 K1 O19 134.14(13) 2_545 4_566 ?
O22 K1 O19 71.40(13) 2_545 4_566 ?
O2 K1 O19 53.10(11) 4_566 4_566 ?
O7 K1 O19 106.42(12) 4_566 4_566 ?
O5 K1 O19 76.40(11) 4_566 4_566 ?
O2W K1 O19 129.96(17) 2_646 4_566 ?
OW5 K1 O19 52.6(3) 4_566 4_566 ?
O8 K1 O19 67.45(12) 4_566 4_566 ?
O22 K1 O19 120.66(14) 4_566 4_566 ?
O8 K1 O13 75.93(12) 2_545 4_566 ?
O22 K1 O13 138.67(14) 2_545 4_566 ?
O2 K1 O13 104.85(12) 4_566 4_566 ?
O7 K1 O13 51.85(11) 4_566 4_566 ?
O5 K1 O13 73.61(11) 4_566 4_566 ?
O2W K1 O13 57.99(14) 2_646 4_566 ?
OW5 K1 O13 133.3(3) 4_566 4_566 ?
O8 K1 O13 119.81(13) 4_566 4_566 ?
O22 K1 O13 67.13(12) 4_566 4_566 ?
O19 K1 O13 149.93(12) 4_566 4_566 ?
O8 K1 As1 139.64(12) 2_545 4_566 ?
O22 K1 As1 138.03(12) 2_545 4_566 ?
O2 K1 As1 31.19(8) 4_566 4_566 ?
O7 K1 As1 31.10(8) 4_566 4_566 ?
O5 K1 As1 31.02(8) 4_566 4_566 ?
O2W K1 As1 121.73(12) 2_646 4_566 ?
OW5 K1 As1 118.2(2) 4_566 4_566 ?
O8 K1 As1 79.42(9) 4_566 4_566 ?
O22 K1 As1 79.50(9) 4_566 4_566 ?
O19 K1 As1 77.56(9) 4_566 4_566 ?
O13 K1 As1 75.62(8) 4_566 4_566 ?
OW8 Na1 OW7 90.8(7) . . ?
OW8 Na1 OW2 94.5(9) . . ?
OW7 Na1 OW2 169.9(10) . . ?
OW8 Na1 OW11 89.9(8) . . ?
OW7 Na1 OW11 66.9(10) . . ?
OW2 Na1 OW11 104.5(13) . . ?
OW8 Na1 OW3 174.4(8) . . ?
OW7 Na1 OW3 93.8(8) . . ?
OW2 Na1 OW3 80.4(10) . . ?
OW11 Na1 OW3 89.0(9) . . ?
Mo4 O1 Mn1 137.7(3) . 3_666 ?
As1 O2 Mo2 126.8(2) . . ?
As1 O2 Mo3 126.8(2) . . ?
Mo2 O2 Mo3 96.59(15) . . ?
As1 O2 K1 91.35(16) . 4_565 ?
Mo2 O2 K1 104.05(15) . 4_565 ?
Mo3 O2 K1 107.94(16) . 4_565 ?
Mo2 O3 Mo3 114.4(2) . . ?
Mo6 O4 Mo3 140.4(3) . . ?
As1 O5 Mo4 125.2(2) . . ?
As1 O5 Mo6 125.0(2) . . ?
Mo4 O5 Mo6 95.56(16) . . ?
As1 O5 K1 86.34(15) . 4_565 ?
Mo4 O5 K1 113.44(16) . 4_565 ?
Mo6 O5 K1 111.56(15) . 4_565 ?
Mo5 O6 Mo2 139.5(2) . . ?
As1 O7 Mo5 127.2(2) . . ?
As1 O7 Mo1 125.2(2) . . ?
Mo5 O7 Mo1 96.28(15) . . ?
As1 O7 K1 90.77(15) . 4_565 ?
Mo5 O7 K1 104.15(15) . 4_565 ?
Mo1 O7 K1 111.16(16) . 4_565 ?
Mo2 O8 K1 146.7(3) . 2 ?
Mo2 O8 K1 106.65(19) . 4_565 ?
K1 O8 K1 89.37(14) 2 4_565 ?
Mo1 O10 Mo4 141.0(2) . . ?
C8 O12 Mo2 129.3(4) . . ?
Mo1 O13 Mn1 135.1(2) . 3_666 ?
Mo1 O13 K1 105.81(19) . 4_565 ?
Mn1 O13 K1 94.32(16) 3_666 4_565 ?
C8 O14 Mo3 130.1(4) . . ?
C7 O15 Mo5 130.0(4) . . ?
Mo4 O17 Mo6 115.1(2) . . ?
Mo3 O19 K1 105.9(2) . 4_565 ?
C7 O20 Mo1 131.1(4) . . ?
Mo4 O21 Mn1 148.7(3) . . ?
Mo5 O22 K1 143.6(3) . 2 ?
Mo5 O22 K1 106.0(2) . 4_565 ?
K1 O22 K1 87.43(14) 2 4_565 ?
C6 O24 Mo6 131.0(4) . . ?
Mo5 O25 Mo1 115.4(2) . . ?
C6 O27 Mo4 130.5(4) . . ?
C6 C1 H1A 109.5 . . ?
C6 C1 H1B 109.5 . . ?
H1A C1 H1B 109.5 . . ?
C6 C1 H1C 109.5 . . ?
H1A C1 H1C 109.5 . . ?
H1B C1 H1C 109.5 . . ?
C4 C2 N1 109.8(7) . . ?
C4 C2 H2A 109.7 . . ?
N1 C2 H2A 109.7 . . ?
C4 C2 H2B 109.7 . . ?
N1 C2 H2B 109.7 . . ?
H2A C2 H2B 108.2 . . ?
N2 C3 C5 113.0(5) . . ?
N2 C3 H3A 109.0 . . ?
C5 C3 H3A 109.0 . . ?
N2 C3 H3B 109.0 . . ?
C5 C3 H3B 109.0 . . ?
H3A C3 H3B 107.8 . . ?
C2 C4 C7 114.0(6) . . ?
C2 C4 H4A 108.7 . . ?
C7 C4 H4A 108.7 . . ?
C2 C4 H4B 108.7 . . ?
C7 C4 H4B 108.7 . . ?
H4A C4 H4B 107.6 . . ?
C3 C5 C8 113.1(5) . . ?
C3 C5 H5A 109.0 . . ?
C8 C5 H5A 109.0 . . ?
C3 C5 H5B 109.0 . . ?
C8 C5 H5B 109.0 . . ?
H5A C5 H5B 107.8 . . ?
O27 C6 O24 124.7(6) . . ?
O27 C6 C1 117.4(7) . . ?
O24 C6 C1 117.9(6) . . ?
O20 C7 O15 125.2(6) . . ?
O20 C7 C4 117.5(6) . . ?
O15 C7 C4 117.3(6) . . ?
O14 C8 O12 126.3(6) . . ?
O14 C8 C5 116.7(5) . . ?
O12 C8 C5 117.0(6) . . ?
C2 N1 H1D 109.5 . . ?
C2 N1 H1E 109.5 . . ?
H1D N1 H1E 109.5 . . ?
C2 N1 H1F 109.5 . . ?
H1D N1 H1F 109.5 . . ?
H1E N1 H1F 109.5 . . ?
C3 N2 H2C 109.5 . . ?
C3 N2 H2D 109.5 . . ?
H2C N2 H2D 109.5 . . ?
C3 N2 H2E 109.5 . . ?
H2C N2 H2E 109.5 . . ?
H2D N2 H2E 109.5 . . ?
Mn1 O2W K1 102.7(2) . 2_656 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O21 Mo4 O1 Mn1 -73.1(4) . . . 3_666 ?
O10 Mo4 O1 Mn1 28.2(4) . . . 3_666 ?
O17 Mo4 O1 Mn1 -172.7(4) . . . 3_666 ?
O5 Mo4 O1 Mn1 111.6(4) . . . 3_666 ?
Mo6 Mo4 O1 Mn1 153.8(3) . . . 3_666 ?
O7 As1 O2 Mo2 -63.1(3) . . . . ?
O5 As1 O2 Mo2 -160.2(2) . . . . ?
K1 As1 O2 Mo2 -108.7(3) 4_565 . . . ?
O7 As1 O2 Mo3 159.4(3) . . . . ?
O5 As1 O2 Mo3 62.2(3) . . . . ?
K1 As1 O2 Mo3 113.7(3) 4_565 . . . ?
O7 As1 O2 K1 45.63(17) . . . 4_565 ?
O5 As1 O2 K1 -51.52(17) . . . 4_565 ?
O9 Mo6 O4 Mo3 -20.4(4) . . . . ?
O26 Mo6 O4 Mo3 -126.8(4) . . . . ?
O17 Mo6 O4 Mo3 106.6(5) . . . . ?
O5 Mo6 O4 Mo3 70.7(4) . . . . ?
O24 Mo6 O4 Mo3 150.7(4) . . . . ?
Mo4 Mo6 O4 Mo3 84.9(4) . . . . ?
O19 Mo3 O4 Mo6 17.3(4) . . . . ?
O23 Mo3 O4 Mo6 124.2(4) . . . . ?
O3 Mo3 O4 Mo6 -110.7(5) . . . . ?
O2 Mo3 O4 Mo6 -73.4(4) . . . . ?
O14 Mo3 O4 Mo6 -153.7(4) . . . . ?
Mo2 Mo3 O4 Mo6 -87.4(4) . . . . ?
K1 Mo3 O4 Mo6 -31.4(4) 4_565 . . . ?
O7 As1 O5 Mo4 67.3(3) . . . . ?
O2 As1 O5 Mo4 164.3(2) . . . . ?
K1 As1 O5 Mo4 116.3(3) 4_565 . . . ?
O7 As1 O5 Mo6 -162.9(2) . . . . ?
O2 As1 O5 Mo6 -65.9(3) . . . . ?
K1 As1 O5 Mo6 -113.9(2) 4_565 . . . ?
O7 As1 O5 K1 -49.01(15) . . . 4_565 ?
O2 As1 O5 K1 48.00(16) . . . 4_565 ?
O22 Mo5 O6 Mo2 19.5(4) . . . . ?
O11 Mo5 O6 Mo2 125.8(4) . . . . ?
O25 Mo5 O6 Mo2 -108.3(5) . . . . ?
O7 Mo5 O6 Mo2 -72.0(4) . . . . ?
O15 Mo5 O6 Mo2 -151.5(4) . . . . ?
Mo1 Mo5 O6 Mo2 -86.4(4) . . . . ?
K1 Mo5 O6 Mo2 -27.3(3) 4_565 . . . ?
O8 Mo2 O6 Mo5 -19.6(4) . . . . ?
O18 Mo2 O6 Mo5 -124.6(4) . . . . ?
O3 Mo2 O6 Mo5 105.7(5) . . . . ?
O2 Mo2 O6 Mo5 72.0(4) . . . . ?
O12 Mo2 O6 Mo5 151.1(4) . . . . ?
Mo3 Mo2 O6 Mo5 84.1(4) . . . . ?
K1 Mo2 O6 Mo5 27.4(3) 4_565 . . . ?
O5 As1 O7 Mo5 160.6(2) . . . . ?
O2 As1 O7 Mo5 63.3(3) . . . . ?
K1 As1 O7 Mo5 108.5(3) 4_565 . . . ?
O5 As1 O7 Mo1 -64.7(3) . . . . ?
O2 As1 O7 Mo1 -162.0(2) . . . . ?
K1 As1 O7 Mo1 -116.8(3) 4_565 . . . ?
O5 As1 O7 K1 52.13(16) . . . 4_565 ?
O2 As1 O7 K1 -45.21(17) . . . 4_565 ?
O18 Mo2 O8 K1 57.9(5) . . . 2 ?
O6 Mo2 O8 K1 -43.8(5) . . . 2 ?
O3 Mo2 O8 K1 157.1(4) . . . 2 ?
O2 Mo2 O8 K1 -128.0(4) . . . 2 ?
Mo3 Mo2 O8 K1 -169.7(4) . . . 2 ?
K1 Mo2 O8 K1 -115.8(5) 4_565 . . 2 ?
O18 Mo2 O8 K1 173.7(2) . . . 4_565 ?
O6 Mo2 O8 K1 72.0(2) . . . 4_565 ?
O3 Mo2 O8 K1 -87.14(19) . . . 4_565 ?
O2 Mo2 O8 K1 -12.24(17) . . . 4_565 ?
Mo3 Mo2 O8 K1 -53.93(15) . . . 4_565 ?
O16 Mo1 O10 Mo4 -121.7(4) . . . . ?
O13 Mo1 O10 Mo4 -15.5(4) . . . . ?
O25 Mo1 O10 Mo4 107.3(5) . . . . ?
O7 Mo1 O10 Mo4 74.2(4) . . . . ?
O20 Mo1 O10 Mo4 154.1(4) . . . . ?
Mo5 Mo1 O10 Mo4 87.4(4) . . . . ?
O21 Mo4 O10 Mo1 124.9(4) . . . . ?
O1 Mo4 O10 Mo1 19.3(4) . . . . ?
O17 Mo4 O10 Mo1 -110.3(5) . . . . ?
O5 Mo4 O10 Mo1 -72.9(4) . . . . ?
O27 Mo4 O10 Mo1 -153.2(4) . . . . ?
Mo6 Mo4 O10 Mo1 -87.4(4) . . . . ?
O16 Mo1 O13 Mn1 67.2(4) . . . 3_666 ?
O10 Mo1 O13 Mn1 -36.9(4) . . . 3_666 ?
O25 Mo1 O13 Mn1 166.3(3) . . . 3_666 ?
O7 Mo1 O13 Mn1 -119.9(3) . . . 3_666 ?
O20 Mo1 O13 Mn1 -104.7(10) . . . 3_666 ?
Mo5 Mo1 O13 Mn1 -161.1(3) . . . 3_666 ?
O16 Mo1 O13 K1 -179.6(2) . . . 4_565 ?
O10 Mo1 O13 K1 76.41(18) . . . 4_565 ?
O25 Mo1 O13 K1 -80.43(18) . . . 4_565 ?
O7 Mo1 O13 K1 -6.63(17) . . . 4_565 ?
O20 Mo1 O13 K1 8.5(11) . . . 4_565 ?
Mo5 Mo1 O13 K1 -47.84(14) . . . 4_565 ?
O21 Mo4 O17 Mo6 162.0(3) . . . . ?
O1 Mo4 O17 Mo6 -92.5(3) . . . . ?
O10 Mo4 O17 Mo6 36.8(5) . . . . ?
O5 Mo4 O17 Mo6 -1.8(2) . . . . ?
O27 Mo4 O17 Mo6 79.0(2) . . . . ?
O23 Mo3 O19 K1 -179.6(2) . . . 4_565 ?
O4 Mo3 O19 K1 -75.4(2) . . . 4_565 ?
O3 Mo3 O19 K1 83.16(18) . . . 4_565 ?
O2 Mo3 O19 K1 8.75(18) . . . 4_565 ?
Mo2 Mo3 O19 K1 50.32(15) . . . 4_565 ?
O1 Mo4 O21 Mn1 136.1(5) . . . . ?
O10 Mo4 O21 Mn1 35.7(5) . . . . ?
O17 Mo4 O21 Mn1 -122.1(5) . . . . ?
O5 Mo4 O21 Mn1 -59.3(9) . . . . ?
O27 Mo4 O21 Mn1 -41.0(5) . . . . ?
Mo6 Mo4 O21 Mn1 -109.8(5) . . . . ?
O11 Mo5 O22 K1 -64.7(5) . . . 2 ?
O6 Mo5 O22 K1 38.3(5) . . . 2 ?
O25 Mo5 O22 K1 -163.1(4) . . . 2 ?
O7 Mo5 O22 K1 122.3(4) . . . 2 ?
Mo1 Mo5 O22 K1 164.3(4) . . . 2 ?
K1 Mo5 O22 K1 108.1(5) 4_565 . . 2 ?
O11 Mo5 O22 K1 -172.8(2) . . . 4_565 ?
O6 Mo5 O22 K1 -69.8(2) . . . 4_565 ?
O25 Mo5 O22 K1 88.82(19) . . . 4_565 ?
O7 Mo5 O22 K1 14.23(18) . . . 4_565 ?
Mo1 Mo5 O22 K1 56.27(16) . . . 4_565 ?
N1 C2 C4 C7 175.1(6) . . . . ?
N2 C3 C5 C8 -173.0(6) . . . . ?
Mo4 O27 C6 O24 -5.2(10) . . . . ?
Mo4 O27 C6 C1 176.2(6) . . . . ?
Mo6 O24 C6 O27 3.4(11) . . . . ?
Mo6 O24 C6 C1 -178.1(7) . . . . ?
Mo1 O20 C7 O15 -6.4(10) . . . . ?
Mo1 O20 C7 C4 173.4(4) . . . . ?
Mo5 O15 C7 O20 7.2(9) . . . . ?
Mo5 O15 C7 C4 -172.6(4) . . . . ?
C2 C4 C7 O20 -4.3(9) . . . . ?
C2 C4 C7 O15 175.5(6) . . . . ?
Mo3 O14 C8 O12 1.3(10) . . . . ?
Mo3 O14 C8 C5 -178.0(4) . . . . ?
Mo2 O12 C8 O14 3.3(10) . . . . ?
Mo2 O12 C8 C5 -177.4(4) . . . . ?
C3 C5 C8 O14 -18.4(9) . . . . ?
C3 C5 C8 O12 162.2(6) . . . . ?

_refine_diff_density_max         2.043
_refine_diff_density_min         -1.834
_refine_diff_density_rms         0.206

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_3
_database_code_depnum_ccdc_archive 'CCDC 1871473'
_audit_update_record             
;
2018-10-04 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H81 As2 K5 Mo12 N6 O74 Zn'
_chemical_formula_weight         3416.14

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.6516(11)
_cell_length_b                   12.1230(12)
_cell_length_c                   17.7391(17)
_cell_angle_alpha                76.692(2)
_cell_angle_beta                 89.874(2)
_cell_angle_gamma                84.635(2)
_cell_volume                     2427.2(4)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    13928
_cell_measurement_theta_min      2.096
_cell_measurement_theta_max      24.999

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.337
_exptl_crystal_F_000             1661
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    2.744
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.509
_exptl_absorpt_correction_T_max  0.562
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            13928
_diffrn_reflns_av_unetI/netI     0.0590
_diffrn_reflns_av_R_equivalents  0.0317
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         2.096
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measured_fraction_theta_full 0.968
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_Laue_measured_fraction_full 0.968
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_point_group_measured_fraction_full 0.968
_reflns_number_total             8492
_reflns_number_gt                6221
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0592P)²+8.5887P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8492
_refine_ls_number_parameters     685
_refine_ls_number_restraints     18
_refine_ls_R_factor_all          0.0699
_refine_ls_R_factor_gt           0.0470
_refine_ls_wR_factor_ref         0.1306
_refine_ls_wR_factor_gt          0.1145
_refine_ls_goodness_of_fit_ref   1.055
_refine_ls_restrained_S_all      1.056
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.19531(6) 0.23452(6) 0.52806(4) 0.02561(18) Uani 1 1 d . . . . .
Mo2 Mo -0.11160(6) 0.35869(6) 0.76667(4) 0.02441(18) Uani 1 1 d . . . . .
Mo3 Mo 0.12884(6) 0.46509(6) 0.84599(4) 0.02557(18) Uani 1 1 d . . . . .
Mo4 Mo -0.07988(6) 0.24508(6) 0.61721(4) 0.02397(17) Uani 1 1 d . . . . .
Mo5 Mo 0.38164(6) 0.43423(6) 0.76980(4) 0.02554(18) Uani 1 1 d . . . . .
Mo6 Mo 0.41663(6) 0.32906(6) 0.59884(4) 0.02556(18) Uani 1 1 d . . . . .
As1 As 0.17490(6) 0.26831(7) 0.72101(4) 0.02090(19) Uani 1 1 d . . . . .
Zn1 Zn -0.19308(17) 0.00086(17) 0.56751(11) 0.0307(5) Uani 0.5 1 d . . P . .
K1 K 0.0782(2) 0.5271(2) 0.60323(13) 0.0578(7) Uani 1 1 d . . . . .
K2 K 0.30628(19) 0.50439(19) 0.40449(12) 0.0454(5) Uani 1 1 d . . . . .
K3 K 0.0242(4) 0.0404(4) 0.4055(3) 0.0541(13) Uani 0.5 1 d . . P . .
O1 O -0.0409(5) 0.0888(5) 0.7203(3) 0.0359(14) Uani 1 1 d . . . . .
O2 O 0.1989(5) 0.1459(6) 0.4647(4) 0.0411(16) Uani 1 1 d . . . . .
O3 O 0.5610(5) 0.3053(5) 0.5806(3) 0.0364(15) Uani 1 1 d . . . . .
O4 O -0.2218(5) 0.3494(6) 0.8294(4) 0.0412(16) Uani 1 1 d . . . . .
O5 O 0.0084(4) 0.3718(5) 0.8364(3) 0.0267(13) Uani 1 1 d . . . . .
O6 O -0.0975(5) 0.3699(5) 0.5484(3) 0.0331(14) Uani 1 1 d . . . . .
O7 O 0.3841(5) 0.4709(5) 0.5593(3) 0.0358(14) Uani 1 1 d . . . . .
O8 O 0.0653(4) 0.1842(5) 0.5871(3) 0.0270(13) Uani 1 1 d . . . . .
O9 O -0.1839(4) 0.2917(5) 0.6907(3) 0.0244(12) Uani 1 1 d . . . . .
O10 O 0.0283(4) 0.3160(4) 0.6913(3) 0.0224(12) Uani 1 1 d . . . . .
O11 O 0.3526(5) 0.2715(5) 0.5155(3) 0.0301(13) Uani 1 1 d . . . . .
O12 O 0.3725(6) 0.5591(5) 0.7012(3) 0.0402(15) Uani 1 1 d . . . . .
O13 O 0.4332(5) 0.1384(5) 0.6575(3) 0.0329(14) Uani 1 1 d . . . . .
O14 O 0.2789(5) 0.0751(5) 0.6143(3) 0.0333(14) Uani 1 1 d . . . . .
O15 O -0.1679(5) 0.1572(5) 0.5849(3) 0.0354(14) Uani 1 1 d . . . . .
O16 O 0.2870(5) 0.4887(5) 0.8471(3) 0.0316(14) Uani 1 1 d . . . . .
O17 O 0.2058(4) 0.3942(5) 0.7493(3) 0.0247(12) Uani 1 1 d . . . . .
O18 O 0.2330(4) 0.3042(5) 0.6266(3) 0.0271(13) Uani 1 1 d . . . . .
O19 O 0.1300(5) 0.3611(5) 0.4746(3) 0.0362(14) Uani 1 1 d . . . . .
O20 O 0.4249(4) 0.3314(5) 0.7055(3) 0.0271(12) Uani 1 1 d . . . . .
O21 O 0.0931(5) 0.4903(5) 0.9353(3) 0.0386(15) Uani 1 1 d . . . . .
O22 O 0.3686(5) 0.2600(5) 0.8584(3) 0.0301(13) Uani 1 1 d . . . . .
O23 O -0.0600(5) 0.1717(5) 0.8214(3) 0.0352(14) Uani 1 1 d . . . . .
O24 O 0.0753(5) 0.5878(5) 0.7825(4) 0.0397(15) Uani 1 1 d . . . . .
O25 O 0.2000(5) 0.2899(5) 0.9143(3) 0.0336(14) Uani 1 1 d . . . . .
O26 O -0.1280(5) 0.4959(5) 0.7139(3) 0.0383(15) Uani 1 1 d . . . . .
O27 O 0.5111(5) 0.4328(5) 0.8158(4) 0.0387(15) Uani 1 1 d . . . . .
C1 C 0.0547(10) -0.0233(9) 0.9168(7) 0.058(3) Uani 1 1 d . . . . .
H1A H 0.0700 0.0454 0.9277 0.070 Uiso 1 1 calc R U . . .
C2 C 0.5083(9) -0.1727(8) 0.8172(6) 0.049(3) Uani 1 1 d . . . . .
H2A H 0.5778 -0.1884 0.8450 0.059 Uiso 1 1 calc R U . . .
C3 C 0.0841(11) -0.1237(10) 0.9712(7) 0.066(3) Uani 1 1 d . . . . .
H3A H 0.1189 -0.1230 1.0182 0.079 Uiso 1 1 calc R U . . .
C4 C 0.3203(9) -0.2216(10) 0.7919(7) 0.058(3) Uani 1 1 d . . . . .
H4A H 0.2619 -0.2699 0.8029 0.070 Uiso 1 1 calc R U . . .
C5 C 0.3031(9) -0.1214(9) 0.7357(6) 0.053(3) Uani 1 1 d . . . . .
H5A H 0.2338 -0.1050 0.7077 0.064 Uiso 1 1 calc R U . . .
C6 C 0.0128(10) -0.2265(9) 0.8867(6) 0.057(3) Uani 1 1 d . . . . .
H6A H -0.0018 -0.2959 0.8766 0.068 Uiso 1 1 calc R U . . .
C7 C 0.3014(8) -0.0018(9) 1.0880(6) 0.046(3) Uani 1 1 d . . . . .
H7A H 0.2809 -0.0107 1.1396 0.056 Uiso 1 1 calc R U . . .
C8 C 0.2738(8) 0.1001(8) 1.0355(5) 0.041(2) Uani 1 1 d . . . . .
H8A H 0.2308 0.1594 1.0509 0.050 Uiso 1 1 calc R U . . .
C9 C -0.0152(10) -0.1265(9) 0.8319(6) 0.056(3) Uani 1 1 d . . . . .
H9A H -0.0469 -0.1288 0.7843 0.068 Uiso 1 1 calc R U . . .
C10 C 0.3596(8) -0.0900(8) 1.0632(6) 0.044(3) Uani 1 1 d . . . . .
C11 C 0.3670(8) 0.0255(8) 0.9355(6) 0.042(2) Uani 1 1 d . . . . .
H11A H 0.3898 0.0349 0.8843 0.050 Uiso 1 1 calc R U . . .
C12 C 0.3914(8) -0.0800(9) 0.9874(7) 0.051(3) Uani 1 1 d . . . . .
H12A H 0.4280 -0.1417 0.9711 0.061 Uiso 1 1 calc R U . . .
C13 C 0.4886(8) -0.0734(9) 0.7620(6) 0.044(2) Uani 1 1 d . . . . .
H13A H 0.5458 -0.0237 0.7523 0.053 Uiso 1 1 calc R U . . .
C14 C 0.4263(8) -0.2503(8) 0.8324(5) 0.040(2) Uani 1 1 d . . . . .
C15 C 0.0037(8) -0.0226(7) 0.8474(5) 0.035(2) Uani 1 1 d . . . . .
C16 C 0.2916(7) 0.2291(7) 0.9067(5) 0.0278(19) Uani 1 1 d . . . . .
C17 C 0.3856(7) -0.0446(8) 0.7199(5) 0.035(2) Uani 1 1 d . . . . .
C18 C 0.0613(8) -0.2229(7) 0.9545(5) 0.035(2) Uani 1 1 d . . . . .
C19 C 0.3100(7) 0.1146(7) 0.9592(5) 0.032(2) Uani 1 1 d . . . . .
C20 C 0.3660(7) 0.0643(7) 0.6598(5) 0.0299(19) Uani 1 1 d . . . . .
C21 C -0.0349(7) 0.0865(7) 0.7922(5) 0.032(2) Uani 1 1 d . . . . .
N1 N 0.4453(8) -0.3517(7) 0.8881(5) 0.055(2) Uani 1 1 d . . . . .
H1B H 0.5093 -0.3675 0.9142 0.066 Uiso 1 1 calc R U . . .
H1C H 0.3932 -0.3986 0.8966 0.066 Uiso 1 1 calc R U . . .
N2 N 0.3937(6) -0.1974(7) 1.1200(5) 0.055(2) Uani 1 1 d . . . . .
H2B H 0.3770 -0.2041 1.1680 0.066 Uiso 1 1 calc R U . . .
H2C H 0.4303 -0.2534 1.1052 0.066 Uiso 1 1 calc R U . . .
N3 N 0.0913(7) -0.3285(6) 1.0134(4) 0.043(2) Uani 1 1 d . . . . .
H3B H 0.0779 -0.3929 1.0045 0.052 Uiso 1 1 calc R U . . .
H3C H 0.1223 -0.3260 1.0568 0.052 Uiso 1 1 calc R U . . .
O1W O -0.2197(11) -0.0706(9) 0.6859(6) 0.031(3) Uani 0.5 1 d . . P . .
O2W O -0.1962(11) 0.0802(10) 0.4488(7) 0.037(3) Uani 0.5 1 d . . P . .
O3W O -0.3720(11) 0.0429(12) 0.5675(7) 0.029(3) Uani 0.5 1 d . U P . .
O3WA O -0.3501(13) 0.0642(13) 0.5264(11) 0.053(4) Uani 0.5 1 d . U P . .
OW1 O 0.715(2) 0.300(2) 0.4302(13) 0.045(6) Uani 0.5 1 d . . P . .
OW2 O 0.682(2) 0.276(2) 0.4444(16) 0.043(6) Uani 0.5 1 d . U P . .
OW3 O 0.9027(15) 0.2521(15) 0.3646(11) 0.071(5) Uani 0.5 1 d . . P . .
OW4 O 0.998(2) 0.2676(16) 0.3505(11) 0.098(7) Uani 0.5 1 d . . P . .
OW5 O 0.2073(10) 0.3061(9) 0.2286(7) 0.115(4) Uani 1 1 d . . . . .
OW6 O 0.2793(12) 0.3993(10) 0.0668(8) 0.147(5) Uani 1 1 d . . . . .
OW7 O 0.4741(8) 0.1501(9) 0.4252(6) 0.106(4) Uani 1 1 d . . . . .
OW8 O 0.3460(6) 0.8542(7) 0.2641(5) 0.075(3) Uani 1 1 d . . . . .
OW9 O 0.3321(7) 0.6383(7) 0.0287(4) 0.069(2) Uani 1 1 d . . . . .
OW10 O 0.3937(8) 0.3667(9) 0.3070(6) 0.102(4) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O19 1.716(6) . ?
Mo1 O2 1.722(6) . ?
Mo1 O8 1.907(5) . ?
Mo1 O11 1.928(5) . ?
Mo1 O18 2.172(5) . ?
Mo1 O14 2.306(6) . ?
Mo1 Mo6 3.2817(10) . ?
Mo2 O4 1.692(6) . ?
Mo2 O26 1.704(6) . ?
Mo2 O5 1.910(5) . ?
Mo2 O9 1.955(5) . ?
Mo2 O10 2.205(5) . ?
Mo2 O23 2.276(6) . ?
Mo2 Mo4 3.2625(10) . ?
Mo3 O24 1.711(6) . ?
Mo3 O21 1.723(6) . ?
Mo3 O16 1.892(5) . ?
Mo3 O5 1.914(5) . ?
Mo3 O17 2.238(5) . ?
Mo3 O25 2.271(6) . ?
Mo3 Mo5 3.2638(10) . ?
Mo4 O6 1.707(6) . ?
Mo4 O15 1.733(5) . ?
Mo4 O8 1.906(5) . ?
Mo4 O9 1.922(5) . ?
Mo4 O10 2.188(5) . ?
Mo4 O1 2.322(6) . ?
Mo5 O12 1.705(6) . ?
Mo5 O27 1.713(6) . ?
Mo5 O20 1.909(5) . ?
Mo5 O16 1.951(5) . ?
Mo5 O17 2.199(5) . ?
Mo5 O22 2.343(6) . ?
Mo6 O7 1.708(6) . ?
Mo6 O3 1.723(6) . ?
Mo6 O20 1.901(5) . ?
Mo6 O11 1.950(5) . ?
Mo6 O18 2.227(5) . ?
Mo6 O13 2.296(6) . ?
As1 O18 1.779(5) . ?
As1 O17 1.780(5) . ?
As1 O10 1.791(5) . ?
Zn1 O3WA 1.988(15) . ?
Zn1 O2 1.997(6) 2_556 ?
Zn1 K3 2.015(5) 2_556 ?
Zn1 O15 2.037(6) . ?
Zn1 O3W 2.100(12) . ?
Zn1 O2W 2.103(12) . ?
Zn1 O1W 2.114(10) . ?
K3 Zn1 2.015(5) 2_556 ?
O1 C21 1.271(10) . ?
O2 Zn1 1.997(6) 2_556 ?
O13 C20 1.239(10) . ?
O14 C20 1.277(9) . ?
O22 C16 1.261(10) . ?
O23 C21 1.268(10) . ?
O25 C16 1.265(10) . ?
C1 C15 1.366(13) . ?
C1 C3 1.383(15) . ?
C1 H1A 0.9300 . ?
C2 C13 1.367(13) . ?
C2 C14 1.386(13) . ?
C2 H2A 0.9300 . ?
C3 C18 1.352(13) . ?
C3 H3A 0.9300 . ?
C4 C5 1.381(14) . ?
C4 C14 1.404(13) . ?
C4 H4A 0.9300 . ?
C5 C17 1.384(13) . ?
C5 H5A 0.9300 . ?
C6 C18 1.342(13) . ?
C6 C9 1.380(14) . ?
C6 H6A 0.9300 . ?
C7 C10 1.369(14) . ?
C7 C8 1.377(13) . ?
C7 H7A 0.9300 . ?
C8 C19 1.393(12) . ?
C8 H8A 0.9300 . ?
C9 C15 1.385(13) . ?
C9 H9A 0.9300 . ?
C10 C12 1.376(14) . ?
C10 N2 1.472(12) . ?
C11 C19 1.363(12) . ?
C11 C12 1.398(14) . ?
C11 H11A 0.9300 . ?
C12 H12A 0.9300 . ?
C13 C17 1.388(12) . ?
C13 H13A 0.9300 . ?
C14 N1 1.389(12) . ?
C15 C21 1.484(12) . ?
C16 C19 1.480(12) . ?
C17 C20 1.492(12) . ?
C18 N3 1.468(11) . ?
N1 H1B 0.8600 . ?
N1 H1C 0.8600 . ?
N2 H2B 0.8600 . ?
N2 H2C 0.8600 . ?
N3 H3B 0.8600 . ?
N3 H3C 0.8600 . ?
O3W O3WA 0.767(18) . ?
OW1 OW2 0.54(3) . ?
OW3 OW4 1.15(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O19 Mo1 O2 103.6(3) . . ?
O19 Mo1 O8 97.8(3) . . ?
O2 Mo1 O8 99.4(3) . . ?
O19 Mo1 O11 97.7(3) . . ?
O2 Mo1 O11 97.0(3) . . ?
O8 Mo1 O11 154.1(2) . . ?
O19 Mo1 O18 94.1(2) . . ?
O2 Mo1 O18 161.5(3) . . ?
O8 Mo1 O18 83.6(2) . . ?
O11 Mo1 O18 74.7(2) . . ?
O19 Mo1 O14 172.2(2) . . ?
O2 Mo1 O14 84.0(3) . . ?
O8 Mo1 O14 79.0(2) . . ?
O11 Mo1 O14 82.9(2) . . ?
O18 Mo1 O14 78.6(2) . . ?
O19 Mo1 Mo6 99.4(2) . . ?
O2 Mo1 Mo6 127.0(2) . . ?
O8 Mo1 Mo6 123.97(15) . . ?
O11 Mo1 Mo6 32.41(15) . . ?
O18 Mo1 Mo6 42.41(14) . . ?
O14 Mo1 Mo6 76.93(14) . . ?
O4 Mo2 O26 104.6(3) . . ?
O4 Mo2 O5 98.2(3) . . ?
O26 Mo2 O5 99.0(3) . . ?
O4 Mo2 O9 96.8(3) . . ?
O26 Mo2 O9 96.6(3) . . ?
O5 Mo2 O9 154.8(2) . . ?
O4 Mo2 O10 163.0(3) . . ?
O26 Mo2 O10 90.9(2) . . ?
O5 Mo2 O10 85.9(2) . . ?
O9 Mo2 O10 74.21(19) . . ?
O4 Mo2 O23 86.7(3) . . ?
O26 Mo2 O23 168.7(3) . . ?
O5 Mo2 O23 79.6(2) . . ?
O9 Mo2 O23 81.2(2) . . ?
O10 Mo2 O23 77.8(2) . . ?
O4 Mo2 Mo4 127.8(2) . . ?
O26 Mo2 Mo4 95.3(2) . . ?
O5 Mo2 Mo4 125.87(15) . . ?
O9 Mo2 Mo4 32.37(15) . . ?
O10 Mo2 Mo4 41.84(13) . . ?
O23 Mo2 Mo4 76.85(14) . . ?
O24 Mo3 O21 103.4(3) . . ?
O24 Mo3 O16 100.3(3) . . ?
O21 Mo3 O16 98.7(3) . . ?
O24 Mo3 O5 98.9(3) . . ?
O21 Mo3 O5 98.0(3) . . ?
O16 Mo3 O5 150.8(2) . . ?
O24 Mo3 O17 91.4(2) . . ?
O21 Mo3 O17 164.7(3) . . ?
O16 Mo3 O17 74.6(2) . . ?
O5 Mo3 O17 83.2(2) . . ?
O24 Mo3 O25 171.2(3) . . ?
O21 Mo3 O25 84.9(3) . . ?
O16 Mo3 O25 81.0(2) . . ?
O5 Mo3 O25 76.9(2) . . ?
O17 Mo3 O25 80.5(2) . . ?
O24 Mo3 Mo5 98.4(2) . . ?
O21 Mo3 Mo5 129.8(2) . . ?
O16 Mo3 Mo5 32.42(15) . . ?
O5 Mo3 Mo5 122.68(15) . . ?
O17 Mo3 Mo5 42.19(13) . . ?
O25 Mo3 Mo5 77.97(14) . . ?
O6 Mo4 O15 104.1(3) . . ?
O6 Mo4 O8 99.6(3) . . ?
O15 Mo4 O8 98.9(2) . . ?
O6 Mo4 O9 96.5(2) . . ?
O15 Mo4 O9 97.5(2) . . ?
O8 Mo4 O9 153.4(2) . . ?
O6 Mo4 O10 92.9(2) . . ?
O15 Mo4 O10 162.3(3) . . ?
O8 Mo4 O10 82.8(2) . . ?
O9 Mo4 O10 75.2(2) . . ?
O6 Mo4 O1 172.0(2) . . ?
O15 Mo4 O1 83.8(3) . . ?
O8 Mo4 O1 79.7(2) . . ?
O9 Mo4 O1 81.4(2) . . ?
O10 Mo4 O1 79.14(19) . . ?
O6 Mo4 Mo2 96.41(19) . . ?
O15 Mo4 Mo2 128.79(19) . . ?
O8 Mo4 Mo2 123.37(15) . . ?
O9 Mo4 Mo2 33.00(15) . . ?
O10 Mo4 Mo2 42.24(13) . . ?
O1 Mo4 Mo2 77.63(14) . . ?
O12 Mo5 O27 103.5(3) . . ?
O12 Mo5 O20 99.2(3) . . ?
O27 Mo5 O20 99.9(3) . . ?
O12 Mo5 O16 97.2(3) . . ?
O27 Mo5 O16 95.8(3) . . ?
O20 Mo5 O16 153.9(2) . . ?
O12 Mo5 O17 95.3(3) . . ?
O27 Mo5 O17 159.9(3) . . ?
O20 Mo5 O17 84.0(2) . . ?
O16 Mo5 O17 74.4(2) . . ?
O12 Mo5 O22 172.1(3) . . ?
O27 Mo5 O22 84.4(3) . . ?
O20 Mo5 O22 79.9(2) . . ?
O16 Mo5 O22 81.1(2) . . ?
O17 Mo5 O22 76.86(19) . . ?
O12 Mo5 Mo3 98.4(2) . . ?
O27 Mo5 Mo3 125.2(2) . . ?
O20 Mo5 Mo3 125.38(15) . . ?
O16 Mo5 Mo3 31.32(16) . . ?
O17 Mo5 Mo3 43.11(13) . . ?
O22 Mo5 Mo3 76.18(14) . . ?
O7 Mo6 O3 103.9(3) . . ?
O7 Mo6 O20 99.9(3) . . ?
O3 Mo6 O20 100.2(2) . . ?
O7 Mo6 O11 97.7(3) . . ?
O3 Mo6 O11 98.9(3) . . ?
O20 Mo6 O11 150.0(2) . . ?
O7 Mo6 O18 92.1(2) . . ?
O3 Mo6 O18 163.0(3) . . ?
O20 Mo6 O18 82.2(2) . . ?
O11 Mo6 O18 73.0(2) . . ?
O7 Mo6 O13 171.7(2) . . ?
O3 Mo6 O13 84.3(3) . . ?
O20 Mo6 O13 78.1(2) . . ?
O11 Mo6 O13 81.1(2) . . ?
O18 Mo6 O13 79.7(2) . . ?
O7 Mo6 Mo1 98.2(2) . . ?
O3 Mo6 Mo1 128.84(19) . . ?
O20 Mo6 Mo1 120.75(16) . . ?
O11 Mo6 Mo1 31.99(16) . . ?
O18 Mo6 Mo1 41.11(13) . . ?
O13 Mo6 Mo1 76.42(14) . . ?
O18 As1 O17 96.6(2) . . ?
O18 As1 O10 95.9(2) . . ?
O17 As1 O10 96.1(2) . . ?
O3WA Zn1 O2 94.7(5) . 2_556 ?
O3WA Zn1 K3 169.7(5) . 2_556 ?
O2 Zn1 K3 89.6(2) 2_556 2_556 ?
O3WA Zn1 O15 88.2(5) . . ?
O2 Zn1 O15 170.0(3) 2_556 . ?
K3 Zn1 O15 86.0(2) 2_556 . ?
O3WA Zn1 O3W 21.4(5) . . ?
O2 Zn1 O3W 96.7(4) 2_556 . ?
K3 Zn1 O3W 166.4(4) 2_556 . ?
O15 Zn1 O3W 89.6(4) . . ?
O3WA Zn1 O2W 66.8(7) . . ?
O2 Zn1 O2W 86.8(4) 2_556 . ?
K3 Zn1 O2W 104.3(4) 2_556 . ?
O15 Zn1 O2W 85.5(4) . . ?
O3W Zn1 O2W 88.2(5) . . ?
O3WA Zn1 O1W 103.7(7) . . ?
O2 Zn1 O1W 94.4(3) 2_556 . ?
K3 Zn1 O1W 85.2(4) 2_556 . ?
O15 Zn1 O1W 94.1(3) . . ?
O3W Zn1 O1W 82.3(5) . . ?
O2W Zn1 O1W 170.5(5) . . ?
C21 O1 Mo4 128.5(5) . . ?
Mo1 O2 Zn1 156.5(4) . 2_556 ?
Mo2 O5 Mo3 141.3(3) . . ?
Mo4 O8 Mo1 139.4(3) . . ?
Mo4 O9 Mo2 114.6(2) . . ?
As1 O10 Mo4 126.9(3) . . ?
As1 O10 Mo2 126.0(3) . . ?
Mo4 O10 Mo2 95.9(2) . . ?
Mo1 O11 Mo6 115.6(3) . . ?
C20 O13 Mo6 131.4(5) . . ?
C20 O14 Mo1 129.7(5) . . ?
Mo4 O15 Zn1 149.3(3) . . ?
Mo3 O16 Mo5 116.3(3) . . ?
As1 O17 Mo5 123.4(3) . . ?
As1 O17 Mo3 128.0(3) . . ?
Mo5 O17 Mo3 94.70(19) . . ?
As1 O18 Mo1 127.3(3) . . ?
As1 O18 Mo6 126.1(3) . . ?
Mo1 O18 Mo6 96.5(2) . . ?
Mo6 O20 Mo5 138.2(3) . . ?
C16 O22 Mo5 130.0(5) . . ?
C21 O23 Mo2 132.1(5) . . ?
C16 O25 Mo3 130.9(5) . . ?
C15 C1 C3 121.6(9) . . ?
C15 C1 H1A 119.2 . . ?
C3 C1 H1A 119.2 . . ?
C13 C2 C14 120.9(9) . . ?
C13 C2 H2A 119.5 . . ?
C14 C2 H2A 119.5 . . ?
C18 C3 C1 118.5(10) . . ?
C18 C3 H3A 120.7 . . ?
C1 C3 H3A 120.7 . . ?
C5 C4 C14 119.7(9) . . ?
C5 C4 H4A 120.1 . . ?
C14 C4 H4A 120.1 . . ?
C4 C5 C17 122.1(9) . . ?
C4 C5 H5A 118.9 . . ?
C17 C5 H5A 118.9 . . ?
C18 C6 C9 119.6(10) . . ?
C18 C6 H6A 120.2 . . ?
C9 C6 H6A 120.2 . . ?
C10 C7 C8 119.1(10) . . ?
C10 C7 H7A 120.4 . . ?
C8 C7 H7A 120.4 . . ?
C7 C8 C19 120.1(9) . . ?
C7 C8 H8A 119.9 . . ?
C19 C8 H8A 119.9 . . ?
C6 C9 C15 120.4(9) . . ?
C6 C9 H9A 119.8 . . ?
C15 C9 H9A 119.8 . . ?
C7 C10 C12 122.0(9) . . ?
C7 C10 N2 119.1(10) . . ?
C12 C10 N2 118.8(10) . . ?
C19 C11 C12 120.6(9) . . ?
C19 C11 H11A 119.7 . . ?
C12 C11 H11A 119.7 . . ?
C10 C12 C11 118.2(10) . . ?
C10 C12 H12A 120.9 . . ?
C11 C12 H12A 120.9 . . ?
C2 C13 C17 121.9(9) . . ?
C2 C13 H13A 119.0 . . ?
C17 C13 H13A 119.0 . . ?
C2 C14 N1 121.6(9) . . ?
C2 C14 C4 118.1(9) . . ?
N1 C14 C4 120.3(9) . . ?
C1 C15 C9 117.9(9) . . ?
C1 C15 C21 120.7(8) . . ?
C9 C15 C21 121.4(8) . . ?
O22 C16 O25 124.6(8) . . ?
O22 C16 C19 118.0(7) . . ?
O25 C16 C19 117.4(7) . . ?
C5 C17 C13 117.1(9) . . ?
C5 C17 C20 121.9(8) . . ?
C13 C17 C20 121.0(8) . . ?
C6 C18 C3 122.0(9) . . ?
C6 C18 N3 120.2(8) . . ?
C3 C18 N3 117.9(8) . . ?
C11 C19 C8 119.8(9) . . ?
C11 C19 C16 121.2(8) . . ?
C8 C19 C16 118.8(8) . . ?
O13 C20 O14 124.2(8) . . ?
O13 C20 C17 118.9(7) . . ?
O14 C20 C17 116.9(7) . . ?
O23 C21 O1 124.6(8) . . ?
O23 C21 C15 116.4(8) . . ?
O1 C21 C15 119.0(7) . . ?
C14 N1 H1B 120.0 . . ?
C14 N1 H1C 120.0 . . ?
H1B N1 H1C 120.0 . . ?
C10 N2 H2B 120.0 . . ?
C10 N2 H2C 120.0 . . ?
H2B N2 H2C 120.0 . . ?
C18 N3 H3B 120.0 . . ?
C18 N3 H3C 120.0 . . ?
H3B N3 H3C 120.0 . . ?
O3WA O3W Zn1 71.1(17) . . ?
O3W O3WA Zn1 87.5(18) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O19 Mo1 O2 Zn1 -145.3(9) . . . 2_556 ?
O8 Mo1 O2 Zn1 -44.9(9) . . . 2_556 ?
O11 Mo1 O2 Zn1 115.0(9) . . . 2_556 ?
O18 Mo1 O2 Zn1 52.9(14) . . . 2_556 ?
O14 Mo1 O2 Zn1 32.9(9) . . . 2_556 ?
Mo6 Mo1 O2 Zn1 101.6(9) . . . 2_556 ?
O18 As1 O10 Mo4 65.0(4) . . . . ?
O17 As1 O10 Mo4 162.3(3) . . . . ?
O18 As1 O10 Mo2 -160.3(3) . . . . ?
O17 As1 O10 Mo2 -63.0(3) . . . . ?
O6 Mo4 O15 Zn1 138.0(7) . . . . ?
O8 Mo4 O15 Zn1 35.7(7) . . . . ?
O9 Mo4 O15 Zn1 -123.2(7) . . . . ?
O10 Mo4 O15 Zn1 -58.7(12) . . . . ?
O1 Mo4 O15 Zn1 -42.8(7) . . . . ?
Mo2 Mo4 O15 Zn1 -111.5(6) . . . . ?
O24 Mo3 O16 Mo5 -89.4(4) . . . . ?
O21 Mo3 O16 Mo5 165.2(3) . . . . ?
O5 Mo3 O16 Mo5 41.0(6) . . . . ?
O17 Mo3 O16 Mo5 -0.8(3) . . . . ?
O25 Mo3 O16 Mo5 81.8(3) . . . . ?
O18 As1 O17 Mo5 -68.5(3) . . . . ?
O10 As1 O17 Mo5 -165.1(3) . . . . ?
O18 As1 O17 Mo3 161.8(3) . . . . ?
O10 As1 O17 Mo3 65.1(4) . . . . ?
O17 As1 O18 Mo1 -159.6(3) . . . . ?
O10 As1 O18 Mo1 -62.7(4) . . . . ?
O17 As1 O18 Mo6 63.3(4) . . . . ?
O10 As1 O18 Mo6 160.2(3) . . . . ?
C15 C1 C3 C18 0.0(19) . . . . ?
C14 C4 C5 C17 -2.9(18) . . . . ?
C10 C7 C8 C19 -3.3(14) . . . . ?
C18 C6 C9 C15 -1.7(18) . . . . ?
C8 C7 C10 C12 0.0(15) . . . . ?
C8 C7 C10 N2 177.4(8) . . . . ?
C7 C10 C12 C11 2.7(15) . . . . ?
N2 C10 C12 C11 -174.7(8) . . . . ?
C19 C11 C12 C10 -2.0(14) . . . . ?
C14 C2 C13 C17 1.3(16) . . . . ?
C13 C2 C14 N1 179.8(10) . . . . ?
C13 C2 C14 C4 -2.9(16) . . . . ?
C5 C4 C14 C2 3.6(16) . . . . ?
C5 C4 C14 N1 -179.0(10) . . . . ?
C3 C1 C15 C9 -1.7(17) . . . . ?
C3 C1 C15 C21 175.5(10) . . . . ?
C6 C9 C15 C1 2.6(17) . . . . ?
C6 C9 C15 C21 -174.7(10) . . . . ?
Mo5 O22 C16 O25 2.7(12) . . . . ?
Mo5 O22 C16 C19 -176.3(5) . . . . ?
Mo3 O25 C16 O22 4.1(12) . . . . ?
Mo3 O25 C16 C19 -176.9(5) . . . . ?
C4 C5 C17 C13 1.2(16) . . . . ?
C4 C5 C17 C20 -179.2(10) . . . . ?
C2 C13 C17 C5 -0.4(15) . . . . ?
C2 C13 C17 C20 180.0(9) . . . . ?
C9 C6 C18 C3 -0.2(18) . . . . ?
C9 C6 C18 N3 179.9(10) . . . . ?
C1 C3 C18 C6 1.0(18) . . . . ?
C1 C3 C18 N3 -179.0(10) . . . . ?
C12 C11 C19 C8 -1.2(14) . . . . ?
C12 C11 C19 C16 175.1(8) . . . . ?
C7 C8 C19 C11 3.9(14) . . . . ?
C7 C8 C19 C16 -172.5(8) . . . . ?
O22 C16 C19 C11 -33.7(12) . . . . ?
O25 C16 C19 C11 147.2(8) . . . . ?
O22 C16 C19 C8 142.7(8) . . . . ?
O25 C16 C19 C8 -36.4(11) . . . . ?
Mo6 O13 C20 O14 16.0(12) . . . . ?
Mo6 O13 C20 C17 -163.2(6) . . . . ?
Mo1 O14 C20 O13 -10.9(12) . . . . ?
Mo1 O14 C20 C17 168.3(5) . . . . ?
C5 C17 C20 O13 167.3(9) . . . . ?
C13 C17 C20 O13 -13.2(13) . . . . ?
C5 C17 C20 O14 -11.9(13) . . . . ?
C13 C17 C20 O14 167.6(8) . . . . ?
Mo2 O23 C21 O1 -4.7(13) . . . . ?
Mo2 O23 C21 C15 175.4(5) . . . . ?
Mo4 O1 C21 O23 6.6(13) . . . . ?
Mo4 O1 C21 C15 -173.6(6) . . . . ?
C1 C15 C21 O23 -26.4(13) . . . . ?
C9 C15 C21 O23 150.8(9) . . . . ?
C1 C15 C21 O1 153.8(9) . . . . ?
C9 C15 C21 O1 -29.0(13) . . . . ?

_refine_diff_density_max         1.689
_refine_diff_density_min         -1.084
_refine_diff_density_rms         0.172

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_6
_database_code_depnum_ccdc_archive 'CCDC 1871476'
_audit_update_record             
;
2018-10-08 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C42 H70 Cs4 K2 Mo12 N6 Ni O70 Te2'
_chemical_formula_weight         3854.07

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.686(9)
_cell_length_b                   12.336(10)
_cell_length_c                   18.569(15)
_cell_angle_alpha                75.760(14)
_cell_angle_beta                 86.017(13)
_cell_angle_gamma                84.106(12)
_cell_volume                     2578(4)
_cell_formula_units_Z            1
_cell_measurement_temperature    220(2)
_cell_measurement_reflns_used    13338
_cell_measurement_theta_min      1.710
_cell_measurement_theta_max      24.997

_exptl_crystal_description       block
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.482
_exptl_crystal_F_000             1818
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    3.717
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.411
_exptl_absorpt_correction_T_max  0.458
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            13338
_diffrn_reflns_av_unetI/netI     0.0782
_diffrn_reflns_av_R_equivalents  0.0463
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         1.710
_diffrn_reflns_theta_max         24.997
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.904
_diffrn_measured_fraction_theta_full 0.882
_diffrn_reflns_Laue_measured_fraction_max 0.904
_diffrn_reflns_Laue_measured_fraction_full 0.882
_diffrn_reflns_point_group_measured_fraction_max 0.904
_diffrn_reflns_point_group_measured_fraction_full 0.882
_reflns_number_total             8220
_reflns_number_gt                6971
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0838P)²+50.9508P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8220
_refine_ls_number_parameters     677
_refine_ls_number_restraints     79
_refine_ls_R_factor_all          0.0687
_refine_ls_R_factor_gt           0.0594
_refine_ls_wR_factor_ref         0.1758
_refine_ls_wR_factor_gt          0.1661
_refine_ls_goodness_of_fit_ref   1.030
_refine_ls_restrained_S_all      1.033
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.08558(9) -0.23283(8) 0.37016(5) 0.0186(2) Uani 1 1 d . . . . .
Mo2 Mo -0.19572(9) -0.22191(8) 0.47069(5) 0.0160(2) Uani 1 1 d . . . . .
Mo3 Mo -0.42356(9) -0.30824(8) 0.40957(5) 0.0160(2) Uani 1 1 d . . . . .
Mo4 Mo -0.39203(9) -0.41543(8) 0.24218(5) 0.0148(2) Uani 1 1 d . . . . .
Mo5 Mo 0.11391(9) -0.34229(8) 0.22239(5) 0.0151(2) Uani 1 1 d . . . . .
Mo6 Mo -0.13319(9) -0.44690(8) 0.15670(5) 0.0163(2) Uani 1 1 d . . . . .
Te1 Te -0.17560(6) -0.25440(6) 0.28028(4) 0.01373(19) Uani 1 1 d . . . . .
Ni1 Ni -0.1869(5) 0.0082(5) 0.5656(3) 0.0688(15) Uani 0.5 1 d . . P . .
K1 K -0.3593(10) 0.0318(10) 0.5834(8) 0.025(2) Uani 0.25 1 d . U P . .
K1A K -0.3634(10) 0.0487(9) 0.5419(7) 0.024(2) Uani 0.25 1 d . U P . .
Cs1 Cs -0.08079(9) -0.54887(8) 0.40007(5) 0.0403(3) Uani 1 1 d . . . . .
Cs2 Cs -0.66825(7) -0.49871(6) 0.38692(4) 0.0248(2) Uani 1 1 d . . . . .
O1 O 0.1690(8) -0.1478(8) 0.3998(5) 0.033(2) Uani 1 1 d . . . . .
O2 O -0.5700(8) -0.2791(8) 0.4296(5) 0.029(2) Uani 1 1 d . . . . .
O3 O -0.1957(8) -0.1347(7) 0.5300(5) 0.026(2) Uani 1 1 d . . . . .
O4 O -0.3695(7) -0.2431(6) 0.1618(4) 0.0182(17) Uani 1 1 d . . . . .
O5 O -0.1005(8) -0.4703(8) 0.0690(5) 0.027(2) Uani 1 1 d . . . . .
O6 O -0.4231(8) -0.1253(7) 0.3464(5) 0.030(2) Uani 1 1 d . . . . .
O7 O -0.4260(7) -0.3149(6) 0.3067(4) 0.0158(17) Uani 1 1 d . U . . .
O8 O 0.0373(8) -0.0806(7) 0.2730(4) 0.0240(19) Uani 1 1 d . . . . .
O9 O -0.2006(7) -0.2683(7) 0.1005(4) 0.0235(19) Uani 1 1 d . . . . .
O10 O -0.2682(7) -0.0658(7) 0.3851(5) 0.0243(19) Uani 1 1 d . . . . .
O11 O -0.0253(7) -0.3105(6) 0.3048(4) 0.0165(17) Uani 1 1 d . . . . .
O12 O 0.1367(8) -0.4788(7) 0.2733(5) 0.0239(19) Uani 1 1 d . . . . .
O13 O 0.2203(7) -0.3292(8) 0.1523(5) 0.026(2) Uani 1 1 d . . . . .
O14 O 0.0477(8) -0.1619(7) 0.1773(5) 0.026(2) Uani 1 1 d . . . . .
O15 O -0.3573(8) -0.2535(7) 0.4848(4) 0.0219(18) Uani 1 1 d . . . . .
O16 O -0.5244(7) -0.4095(7) 0.2067(5) 0.0230(19) Uani 1 1 d . . . . .
O17 O -0.0873(7) -0.5720(7) 0.2168(4) 0.0232(19) Uani 1 1 d . . . . .
O18 O -0.2355(7) -0.2966(6) 0.3793(4) 0.0155(16) Uani 1 1 d . . . . .
O19 O -0.2094(6) -0.3857(6) 0.2567(4) 0.0140(16) Uani 1 1 d . . . . .
O20 O 0.1045(8) -0.3597(7) 0.4344(5) 0.026(2) Uani 1 1 d . . . . .
O21 O -0.0637(7) -0.1801(6) 0.4061(4) 0.0172(17) Uani 1 1 d . . . . .
O22 O -0.1410(8) -0.3509(7) 0.5207(4) 0.0227(19) Uani 1 1 d . . . . .
O23 O 0.1856(7) -0.2734(7) 0.2910(4) 0.0203(18) Uani 1 1 d . . . . .
O24 O -0.2976(7) -0.4638(7) 0.1635(4) 0.0191(17) Uani 1 1 d . U . . .
O25 O -0.3983(8) -0.4506(7) 0.4480(4) 0.025(2) Uani 1 1 d . . . . .
O26 O -0.3832(8) -0.5395(6) 0.3092(4) 0.0218(19) Uani 1 1 d . . . . .
O27 O -0.0118(7) -0.3598(6) 0.1663(4) 0.0208(19) Uani 1 1 d . . . . .
C1 C -0.2968(13) 0.0299(14) -0.0618(8) 0.048(5) Uani 1 1 d . . . . .
H1A H -0.2662 0.0449 -0.1104 0.058 Uiso 1 1 calc R U . . .
C2 C -0.2672(13) -0.0723(13) -0.0119(8) 0.043(4) Uani 1 1 d . U . . .
H2A H -0.2122 -0.1238 -0.0264 0.051 Uiso 1 1 calc R U . . .
C3 C -0.0676(14) 0.2355(10) 0.0505(7) 0.032(3) Uani 1 1 d . . . . .
C4 C -0.3733(12) 0.1087(11) -0.0372(7) 0.030(3) Uani 1 1 d . U . . .
C5 C -0.4897(14) 0.1841(10) 0.1947(8) 0.034(3) Uani 1 1 d . . . . .
H5A H -0.5555 0.1981 0.1672 0.041 Uiso 1 1 calc R U . . .
C6 C -0.4696(13) 0.0832(11) 0.2477(8) 0.033(3) Uani 1 1 d . . . . .
H6A H -0.5242 0.0311 0.2560 0.040 Uiso 1 1 calc R U . . .
C7 C -0.3542(12) -0.0533(10) 0.3440(7) 0.026(3) Uani 1 1 d . . . . .
C8 C -0.0241(17) 0.2348(10) 0.1183(7) 0.044(5) Uani 1 1 d . . . . .
H8A H -0.0142 0.3024 0.1298 0.053 Uiso 1 1 calc R U . . .
C9 C -0.2914(13) 0.1366(11) 0.2733(8) 0.034(3) Uani 1 1 d . . . . .
H9A H -0.2237 0.1218 0.2989 0.040 Uiso 1 1 calc R U . . .
C10 C -0.2943(10) -0.2123(9) 0.1110(6) 0.019(3) Uani 1 1 d . . . . .
C11 C -0.0784(13) 0.1345(11) 0.0333(7) 0.032(3) Uani 1 1 d . . . . .
H11A H -0.1055 0.1341 -0.0125 0.038 Uiso 1 1 calc R U . . .
C12 C 0.0043(14) 0.1355(11) 0.1683(7) 0.037(4) Uani 1 1 d . . . . .
H12A H 0.0295 0.1370 0.2145 0.044 Uiso 1 1 calc R U . . .
C13 C -0.3104(13) 0.2372(11) 0.2210(8) 0.034(3) Uani 1 1 d . . . . .
H13A H -0.2542 0.2878 0.2113 0.040 Uiso 1 1 calc R U . . .
C14 C -0.0493(12) 0.0334(10) 0.0837(7) 0.026(3) Uani 1 1 d . . . . .
H14A H -0.0601 -0.0341 0.0723 0.032 Uiso 1 1 calc R U . . .
C15 C -0.4094(12) 0.2640(10) 0.1834(7) 0.027(3) Uani 1 1 d . . . . .
C16 C -0.4176(12) 0.0868(10) 0.0337(7) 0.028(3) Uani 1 1 d . . . . .
H16A H -0.4643 0.1423 0.0503 0.033 Uiso 1 1 calc R U . . .
C17 C -0.3713(11) 0.0577(10) 0.2883(7) 0.024(3) Uani 1 1 d . . . . .
C18 C -0.3178(11) -0.0978(10) 0.0582(7) 0.024(3) Uani 1 1 d . . . . .
C19 C 0.0286(10) -0.0788(10) 0.2049(7) 0.020(3) Uani 1 1 d . U . . .
C20 C -0.0034(12) 0.0328(9) 0.1520(7) 0.024(3) Uani 1 1 d . . . . .
C21 C -0.3943(11) -0.0172(10) 0.0817(7) 0.025(3) Uani 1 1 d . . . . .
H21A H -0.4293 -0.0334 0.1292 0.030 Uiso 1 1 calc R U . . .
N1 N -0.4059(11) 0.2155(10) -0.0900(7) 0.040(3) Uani 1 1 d . . . . .
H1B H -0.4537 0.2650 -0.0760 0.049 Uiso 1 1 calc R U . . .
H1C H -0.3773 0.2286 -0.1349 0.049 Uiso 1 1 calc R U . . .
N2 N -0.4334(12) 0.3678(9) 0.1310(6) 0.037(3) Uani 1 1 d . . . . .
H2B H -0.3842 0.4173 0.1217 0.044 Uiso 1 1 calc R U . . .
H2C H -0.4971 0.3812 0.1085 0.044 Uiso 1 1 calc R U . . .
N3 N -0.0999(14) 0.3382(9) -0.0019(6) 0.049(4) Uani 1 1 d . . . . .
H3A H -0.1258 0.3368 -0.0439 0.059 Uiso 1 1 calc R U . . .
H3B H -0.0934 0.4014 0.0085 0.059 Uiso 1 1 calc R U . . .
O1W O -0.2524(18) 0.0951(13) 0.4673(10) 0.032(4) Uani 0.5 1 d . U P . .
O2W O -0.4932(17) -0.1280(16) 0.5649(11) 0.037(5) Uani 0.5 1 d . U P . .
O3W O -0.185(4) -0.083(4) 0.681(3) 0.139(16) Uani 0.5 1 d . U P . .
OW1 O 0.6740(13) 0.3724(11) -0.0097(7) 0.068(4) Uani 1 1 d . . . . .
OW2 O -0.4098(16) -1.3499(12) 1.0253(8) 0.087(5) Uani 1 1 d . . . . .
OW3 O -0.563(2) -0.692(2) 0.3327(15) 0.070(8) Uani 0.5 1 d D U P . .
OW4 O -0.739(3) -0.725(3) 0.276(2) 0.110(12) Uani 0.5 1 d D U P . .
OW5 O 0.6826(16) -0.4311(13) -0.1489(11) 0.107(6) Uani 1 1 d . . . . .
OW6 O -0.2921(12) -0.6993(13) 0.4346(7) 0.075(5) Uani 1 1 d . . . . .
OW7 O 0.037(2) -0.7374(15) 0.3242(10) 0.043(6) Uani 0.5 1 d . . P . .
OW8 O 1.3795(9) -0.1577(8) 0.2364(6) 0.040(2) Uani 1 1 d . . . . .
K2 K -0.0487(8) 0.0566(5) 0.4438(4) 0.0487(18) Uani 0.5 1 d . U P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O1 1.709(9) . ?
Mo1 O20 1.723(8) . ?
Mo1 O21 1.931(8) . ?
Mo1 O23 1.945(8) . ?
Mo1 O11 2.263(8) . ?
Mo1 O8 2.314(8) . ?
Mo1 Cs2 4.100(3) 1_655 ?
Mo1 Cs1 4.431(3) . ?
Mo1 Cs1 4.450(3) 2_546 ?
Mo2 O22 1.718(7) . ?
Mo2 O3 1.718(8) . ?
Mo2 O21 1.921(8) . ?
Mo2 O15 1.954(9) . ?
Mo2 O18 2.217(7) . ?
Mo2 O10 2.302(8) . ?
Mo2 K2 3.905(7) . ?
Mo2 Cs2 4.178(3) 2_446 ?
Mo2 Cs1 4.479(3) 2_546 ?
Mo3 O25 1.728(8) . ?
Mo3 O2 1.746(9) . ?
Mo3 O15 1.931(8) . ?
Mo3 O7 1.935(8) . ?
Mo3 O18 2.240(8) . ?
Mo3 O6 2.273(8) . ?
Mo3 Cs2 3.988(3) . ?
Mo3 K1 4.060(11) 2_456 ?
Mo3 Cs2 4.088(3) 2_446 ?
Mo3 K1A 4.090(10) 2_456 ?
Mo4 O16 1.710(8) . ?
Mo4 O26 1.717(7) . ?
Mo4 O7 1.922(8) . ?
Mo4 O24 1.943(8) . ?
Mo4 O19 2.248(8) . ?
Mo4 O4 2.305(7) . ?
Mo4 Cs2 4.101(3) . ?
Mo5 O12 1.721(8) . ?
Mo5 O13 1.726(8) . ?
Mo5 O27 1.917(9) . ?
Mo5 O23 1.969(8) . ?
Mo5 O11 2.227(8) . ?
Mo5 O14 2.252(8) . ?
Mo5 Cs2 4.088(3) 1_655 ?
Mo5 Cs1 4.309(3) . ?
Mo6 O17 1.726(8) . ?
Mo6 O5 1.733(8) . ?
Mo6 O27 1.908(9) . ?
Mo6 O24 1.946(8) . ?
Mo6 O19 2.265(7) . ?
Mo6 O9 2.279(8) . ?
Mo6 Cs1 4.451(4) . ?
Te1 O11 1.864(8) . ?
Te1 O19 1.864(8) . ?
Te1 O18 1.888(7) . ?
Te1 Cs1 3.862(3) . ?
Ni1 O1 2.016(11) 2_556 ?
Ni1 K1 2.022(13) . ?
Ni1 O3 2.043(10) . ?
Ni1 O1W 2.032(19) . ?
Ni1 K1A 2.123(14) . ?
Ni1 O3W 2.16(5) . ?
Ni1 K2 2.665(10) . ?
Ni1 K2 2.793(11) 2_556 ?
K1 K1A 0.751(13) . ?
K1 O1W 2.41(2) . ?
K1 O2W 2.74(2) . ?
K1 O1 2.841(16) 2_556 ?
K1 O3W 2.85(5) . ?
K1 O3 2.965(14) . ?
K1 O6 3.029(15) 2_456 ?
K1 O2 3.032(14) 2_456 ?
K1 O2W 3.25(3) 2_456 ?
K1 C7 3.530(18) 2_456 ?
K1 Mo3 4.060(11) 2_456 ?
K1A O1W 1.86(2) . ?
K1A O2W 2.62(3) 2_456 ?
K1A O2W 2.71(2) . ?
K1A O3 2.879(13) . ?
K1A O2 3.031(14) 2_456 ?
K1A O1 3.065(16) 2_556 ?
K1A O6 3.344(15) 2_456 ?
K1A OW6 3.40(2) 1_565 ?
K1A O3W 3.41(5) . ?
K1A K2 3.988(15) . ?
Cs1 O20 3.006(9) 2_546 ?
Cs1 O22 3.064(8) 2_546 ?
Cs1 O11 3.142(8) . ?
Cs1 OW7 3.157(17) . ?
Cs1 OW6 3.176(17) . ?
Cs1 O19 3.271(7) . ?
Cs1 O12 3.371(9) . ?
Cs1 O18 3.384(8) . ?
Cs1 O17 3.491(9) . ?
Cs1 O20 3.535(10) . ?
Cs1 O22 3.687(9) . ?
Cs2 OW3 2.94(2) . ?
Cs2 O25 3.111(8) 2_446 ?
Cs2 O12 3.163(8) 1_455 ?
Cs2 O22 3.179(9) 2_446 ?
Cs2 O20 3.202(8) 1_455 ?
Cs2 O23 3.291(8) 1_455 ?
Cs2 O2 3.333(10) . ?
Cs2 O15 3.382(8) 2_446 ?
Cs2 OW4 4.03(3) . ?
Cs2 O26 3.575(9) . ?
Cs2 O25 3.579(10) . ?
Cs2 O16 3.609(9) . ?
O1 Ni1 2.016(11) 2_556 ?
O1 K1 2.841(16) 2_556 ?
O1 K1A 3.065(16) 2_556 ?
O2 K1A 3.031(14) 2_456 ?
O2 K1 3.033(14) 2_456 ?
O3 K2 3.110(11) . ?
O3 K2 3.211(12) 2_556 ?
O4 C10 1.259(14) . ?
O6 C7 1.250(16) . ?
O6 K1 3.029(15) 2_456 ?
O6 K1A 3.344(15) 2_456 ?
O8 C19 1.271(14) . ?
O9 C10 1.263(14) . ?
O10 C7 1.277(16) . ?
O12 Cs2 3.163(8) 1_655 ?
O14 C19 1.249(14) . ?
O15 Cs2 3.382(8) 2_446 ?
O20 Cs1 3.006(9) 2_546 ?
O20 Cs2 3.202(8) 1_655 ?
O21 K2 3.190(10) . ?
O22 Cs1 3.064(8) 2_546 ?
O22 Cs2 3.179(9) 2_446 ?
O23 Cs2 3.291(8) 1_655 ?
O25 Cs2 3.111(8) 2_446 ?
C1 C4 1.39(2) . ?
C1 C2 1.396(19) . ?
C2 C18 1.368(19) . ?
C3 C11 1.380(19) . ?
C3 C8 1.39(2) . ?
C3 N3 1.429(16) . ?
C4 C16 1.355(19) . ?
C4 N1 1.468(15) . ?
C5 C6 1.393(18) . ?
C5 C15 1.40(2) . ?
C6 C17 1.38(2) . ?
C7 C17 1.504(16) . ?
C7 K1 3.530(18) 2_456 ?
C8 C12 1.368(18) . ?
C9 C17 1.38(2) . ?
C9 C13 1.382(19) . ?
C10 C18 1.519(15) . ?
C11 C14 1.389(18) . ?
C12 C20 1.386(18) . ?
C13 C15 1.363(19) . ?
C14 C20 1.410(18) . ?
C15 N2 1.420(16) . ?
C16 C21 1.384(17) . ?
C18 C21 1.398(18) . ?
C19 C20 1.510(16) . ?
O1W K2 2.41(2) . ?
O2W K1A 2.62(3) 2_456 ?
O2W K1 3.25(3) 2_456 ?
OW6 K1A 3.403(19) 1_545 ?
OW7 K2 3.13(2) 1_545 ?
K2 K2 2.484(15) 2_556 ?
K2 Ni1 2.793(11) 2_556 ?
K2 OW7 3.13(2) 1_565 ?
K2 O3 3.211(12) 2_556 ?
K2 Cs1 4.713(7) 1_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Mo1 O20 104.1(5) . . ?
O1 Mo1 O21 99.3(4) . . ?
O20 Mo1 O21 98.9(4) . . ?
O1 Mo1 O23 100.8(4) . . ?
O20 Mo1 O23 97.2(4) . . ?
O21 Mo1 O23 150.3(3) . . ?
O1 Mo1 O11 165.7(4) . . ?
O20 Mo1 O11 89.8(4) . . ?
O21 Mo1 O11 81.5(3) . . ?
O23 Mo1 O11 73.8(3) . . ?
O1 Mo1 O8 87.1(4) . . ?
O20 Mo1 O8 168.8(4) . . ?
O21 Mo1 O8 79.2(3) . . ?
O23 Mo1 O8 80.3(3) . . ?
O11 Mo1 O8 79.0(3) . . ?
O1 Mo1 Cs2 95.9(3) . 1_655 ?
O20 Mo1 Cs2 47.6(3) . 1_655 ?
O21 Mo1 Cs2 145.9(2) . 1_655 ?
O23 Mo1 Cs2 52.2(2) . 1_655 ?
O11 Mo1 Cs2 91.08(19) . 1_655 ?
O8 Mo1 Cs2 132.2(2) . 1_655 ?
O1 Mo1 Cs1 152.2(3) . . ?
O20 Mo1 Cs1 48.6(3) . . ?
O21 Mo1 Cs1 82.7(2) . . ?
O23 Mo1 Cs1 89.5(2) . . ?
O11 Mo1 Cs1 42.09(19) . . ?
O8 Mo1 Cs1 120.2(2) . . ?
Cs2 Mo1 Cs1 70.07(6) 1_655 . ?
O1 Mo1 Cs1 88.4(3) . 2_546 ?
O20 Mo1 Cs1 26.4(3) . 2_546 ?
O21 Mo1 Cs1 80.7(2) . 2_546 ?
O23 Mo1 Cs1 121.4(2) . 2_546 ?
O11 Mo1 Cs1 105.8(2) . 2_546 ?
O8 Mo1 Cs1 158.3(2) . 2_546 ?
Cs2 Mo1 Cs1 69.38(4) 1_655 2_546 ?
Cs1 Mo1 Cs1 64.46(4) . 2_546 ?
O22 Mo2 O3 104.9(4) . . ?
O22 Mo2 O21 99.3(4) . . ?
O3 Mo2 O21 101.4(4) . . ?
O22 Mo2 O15 96.2(4) . . ?
O3 Mo2 O15 98.9(4) . . ?
O21 Mo2 O15 150.2(3) . . ?
O22 Mo2 O18 90.6(3) . . ?
O3 Mo2 O18 163.2(4) . . ?
O21 Mo2 O18 82.1(3) . . ?
O15 Mo2 O18 72.4(3) . . ?
O22 Mo2 O10 168.9(4) . . ?
O3 Mo2 O10 86.2(4) . . ?
O21 Mo2 O10 77.1(3) . . ?
O15 Mo2 O10 82.8(3) . . ?
O18 Mo2 O10 78.5(3) . . ?
O22 Mo2 K2 124.7(3) . . ?
O3 Mo2 K2 50.5(3) . . ?
O21 Mo2 K2 54.2(3) . . ?
O15 Mo2 K2 131.8(3) . . ?
O18 Mo2 K2 124.9(2) . . ?
O10 Mo2 K2 61.7(3) . . ?
O22 Mo2 Cs2 44.1(3) . 2_446 ?
O3 Mo2 Cs2 100.7(3) . 2_446 ?
O21 Mo2 Cs2 141.3(2) . 2_446 ?
O15 Mo2 Cs2 53.0(2) . 2_446 ?
O18 Mo2 Cs2 85.8(2) . 2_446 ?
O10 Mo2 Cs2 135.8(2) . 2_446 ?
K2 Mo2 Cs2 149.31(11) . 2_446 ?
O22 Mo2 Cs1 27.7(3) . 2_546 ?
O3 Mo2 Cs1 89.4(3) . 2_546 ?
O21 Mo2 Cs1 80.0(2) . 2_546 ?
O15 Mo2 Cs1 121.9(2) . 2_546 ?
O18 Mo2 Cs1 107.4(2) . 2_546 ?
O10 Mo2 Cs1 155.3(2) . 2_546 ?
K2 Mo2 Cs1 97.13(13) . 2_546 ?
Cs2 Mo2 Cs1 68.93(5) 2_446 2_546 ?
O25 Mo3 O2 103.9(4) . . ?
O25 Mo3 O15 98.5(4) . . ?
O2 Mo3 O15 100.4(4) . . ?
O25 Mo3 O7 97.8(4) . . ?
O2 Mo3 O7 100.7(4) . . ?
O15 Mo3 O7 149.1(3) . . ?
O25 Mo3 O18 90.4(4) . . ?
O2 Mo3 O18 164.9(4) . . ?
O15 Mo3 O18 72.3(3) . . ?
O7 Mo3 O18 81.6(3) . . ?
O25 Mo3 O6 168.7(4) . . ?
O2 Mo3 O6 86.9(4) . . ?
O15 Mo3 O6 82.3(3) . . ?
O7 Mo3 O6 76.7(3) . . ?
O18 Mo3 O6 79.0(3) . . ?
O25 Mo3 Cs2 63.8(3) . . ?
O2 Mo3 Cs2 55.7(3) . . ?
O15 Mo3 Cs2 140.6(2) . . ?
O7 Mo3 Cs2 70.3(2) . . ?
O18 Mo3 Cs2 137.60(19) . . ?
O6 Mo3 Cs2 122.1(2) . . ?
O25 Mo3 K1 143.8(3) . 2_456 ?
O2 Mo3 K1 43.2(4) . 2_456 ?
O15 Mo3 K1 78.4(3) . 2_456 ?
O7 Mo3 K1 102.6(3) . 2_456 ?
O18 Mo3 K1 121.7(3) . 2_456 ?
O6 Mo3 K1 47.5(3) . 2_456 ?
Cs2 Mo3 K1 95.62(19) . 2_456 ?
O25 Mo3 Cs2 44.8(3) . 2_446 ?
O2 Mo3 Cs2 99.1(3) . 2_446 ?
O15 Mo3 Cs2 55.2(2) . 2_446 ?
O7 Mo3 Cs2 141.2(2) . 2_446 ?
O18 Mo3 Cs2 87.71(19) . 2_446 ?
O6 Mo3 Cs2 137.5(2) . 2_446 ?
Cs2 Mo3 Cs2 94.72(5) . 2_446 ?
K1 Mo3 Cs2 114.6(2) 2_456 2_446 ?
O25 Mo3 K1A 136.2(3) . 2_456 ?
O2 Mo3 K1A 42.1(4) . 2_456 ?
O15 Mo3 K1A 70.5(3) . 2_456 ?
O7 Mo3 K1A 113.0(3) . 2_456 ?
O18 Mo3 K1A 123.1(3) . 2_456 ?
O6 Mo3 K1A 54.8(3) . 2_456 ?
Cs2 Mo3 K1A 97.33(19) . 2_456 ?
K1 Mo3 K1A 10.56(18) 2_456 2_456 ?
Cs2 Mo3 K1A 104.1(2) 2_446 2_456 ?
O16 Mo4 O26 104.1(4) . . ?
O16 Mo4 O7 100.0(4) . . ?
O26 Mo4 O7 98.2(4) . . ?
O16 Mo4 O24 98.8(4) . . ?
O26 Mo4 O24 98.9(4) . . ?
O7 Mo4 O24 150.6(3) . . ?
O16 Mo4 O19 162.9(3) . . ?
O26 Mo4 O19 92.1(3) . . ?
O7 Mo4 O19 82.7(3) . . ?
O24 Mo4 O19 72.9(3) . . ?
O16 Mo4 O4 87.5(3) . . ?
O26 Mo4 O4 168.3(4) . . ?
O7 Mo4 O4 77.9(3) . . ?
O24 Mo4 O4 80.5(3) . . ?
O19 Mo4 O4 76.5(3) . . ?
O16 Mo4 Cs2 61.4(3) . . ?
O26 Mo4 Cs2 60.3(3) . . ?
O7 Mo4 Cs2 67.4(2) . . ?
O24 Mo4 Cs2 142.0(2) . . ?
O19 Mo4 Cs2 133.79(19) . . ?
O4 Mo4 Cs2 126.4(2) . . ?
O12 Mo5 O13 104.6(4) . . ?
O12 Mo5 O27 98.7(4) . . ?
O13 Mo5 O27 98.5(4) . . ?
O12 Mo5 O23 96.4(4) . . ?
O13 Mo5 O23 99.2(4) . . ?
O27 Mo5 O23 153.0(3) . . ?
O12 Mo5 O11 89.7(4) . . ?
O13 Mo5 O11 165.0(4) . . ?
O27 Mo5 O11 83.7(3) . . ?
O23 Mo5 O11 74.2(3) . . ?
O12 Mo5 O14 165.6(4) . . ?
O13 Mo5 O14 89.8(4) . . ?
O27 Mo5 O14 79.0(3) . . ?
O23 Mo5 O14 80.8(3) . . ?
O11 Mo5 O14 76.0(3) . . ?
O12 Mo5 Cs2 46.6(3) . 1_655 ?
O13 Mo5 Cs2 94.5(3) . 1_655 ?
O27 Mo5 Cs2 145.2(2) . 1_655 ?
O23 Mo5 Cs2 52.7(2) . 1_655 ?
O11 Mo5 Cs2 91.9(2) . 1_655 ?
O14 Mo5 Cs2 133.4(2) . 1_655 ?
O12 Mo5 Cs1 46.7(3) . . ?
O13 Mo5 Cs1 150.3(3) . . ?
O27 Mo5 Cs1 81.7(3) . . ?
O23 Mo5 Cs1 92.8(3) . . ?
O11 Mo5 Cs1 44.6(2) . . ?
O14 Mo5 Cs1 119.0(2) . . ?
Cs2 Mo5 Cs1 71.43(6) 1_655 . ?
O17 Mo6 O5 104.2(4) . . ?
O17 Mo6 O27 99.1(4) . . ?
O5 Mo6 O27 101.5(4) . . ?
O17 Mo6 O24 99.0(4) . . ?
O5 Mo6 O24 99.1(4) . . ?
O27 Mo6 O24 148.2(3) . . ?
O17 Mo6 O19 88.3(3) . . ?
O5 Mo6 O19 166.0(3) . . ?
O27 Mo6 O19 82.2(3) . . ?
O24 Mo6 O19 72.4(3) . . ?
O17 Mo6 O9 167.5(4) . . ?
O5 Mo6 O9 88.2(4) . . ?
O27 Mo6 O9 76.6(3) . . ?
O24 Mo6 O9 80.1(3) . . ?
O19 Mo6 O9 79.5(3) . . ?
O17 Mo6 Cs1 46.4(3) . . ?
O5 Mo6 Cs1 148.8(3) . . ?
O27 Mo6 Cs1 77.8(2) . . ?
O24 Mo6 Cs1 96.5(2) . . ?
O19 Mo6 Cs1 45.07(18) . . ?
O9 Mo6 Cs1 121.2(2) . . ?
O11 Te1 O19 93.4(3) . . ?
O11 Te1 O18 94.0(3) . . ?
O19 Te1 O18 94.1(3) . . ?
O11 Te1 Cs1 53.7(2) . . ?
O19 Te1 Cs1 57.7(2) . . ?
O18 Te1 Cs1 61.2(2) . . ?
O1 Ni1 K1 89.4(5) 2_556 . ?
O1 Ni1 O3 176.9(5) 2_556 . ?
K1 Ni1 O3 93.6(5) . . ?
O1 Ni1 O1W 93.7(6) 2_556 . ?
K1 Ni1 O1W 73.0(7) . . ?
O3 Ni1 O1W 87.4(5) . . ?
O1 Ni1 K1A 95.5(5) 2_556 . ?
K1 Ni1 K1A 20.7(4) . . ?
O3 Ni1 K1A 87.4(4) . . ?
O1W Ni1 K1A 53.0(7) . . ?
O1 Ni1 O3W 87.6(13) 2_556 . ?
K1 Ni1 O3W 85.6(14) . . ?
O3 Ni1 O3W 92.4(13) . . ?
O1W Ni1 O3W 158.5(15) . . ?
K1A Ni1 O3W 105.5(14) . . ?
O1 Ni1 K2 96.6(4) 2_556 . ?
K1 Ni1 K2 132.8(5) . . ?
O3 Ni1 K2 81.5(3) . . ?
O1W Ni1 K2 59.9(6) . . ?
K1A Ni1 K2 112.3(5) . . ?
O3W Ni1 K2 141.2(14) . . ?
O1 Ni1 K2 95.3(4) 2_556 2_556 ?
K1 Ni1 K2 171.2(5) . 2_556 ?
O3 Ni1 K2 81.6(3) . 2_556 ?
O1W Ni1 K2 114.0(6) . 2_556 ?
K1A Ni1 K2 163.6(4) . 2_556 ?
O3W Ni1 K2 87.2(14) . 2_556 ?
K2 Ni1 K2 54.1(3) . 2_556 ?
K1A K1 Ni1 87.2(14) . . ?
K1A K1 O1W 35.8(14) . . ?
Ni1 K1 O1W 53.7(6) . . ?
K1A K1 O2W 80.4(15) . . ?
Ni1 K1 O2W 118.7(6) . . ?
O1W K1 O2W 107.2(7) . . ?
K1A K1 O1 100.3(15) . 2_556 ?
Ni1 K1 O1 45.2(3) . 2_556 ?
O1W K1 O1 67.8(6) . 2_556 ?
O2W K1 O1 163.4(6) . 2_556 ?
K1A K1 O3W 134.3(18) . . ?
Ni1 K1 O3W 49.3(10) . . ?
O1W K1 O3W 102.9(12) . . ?
O2W K1 O3W 106.4(11) . . ?
O1 K1 O3W 61.2(10) 2_556 . ?
K1A K1 O3 76.1(12) . . ?
Ni1 K1 O3 43.4(3) . . ?
O1W K1 O3 62.2(5) . . ?
O2W K1 O3 75.3(5) . . ?
O1 K1 O3 88.7(4) 2_556 . ?
O3W K1 O3 63.0(10) . . ?
K1A K1 O6 108.5(14) . 2_456 ?
Ni1 K1 O6 154.4(6) . 2_456 ?
O1W K1 O6 133.3(6) . 2_456 ?
O2W K1 O6 84.6(5) . 2_456 ?
O1 K1 O6 110.5(5) 2_556 2_456 ?
O3W K1 O6 117.0(11) . 2_456 ?
O3 K1 O6 158.5(5) . 2_456 ?
K1A K1 O2 82.8(13) . 2_456 ?
Ni1 K1 O2 109.6(5) . 2_456 ?
O1W K1 O2 85.0(5) . 2_456 ?
O2W K1 O2 127.5(6) . 2_456 ?
O1 K1 O2 68.7(4) 2_556 2_456 ?
O3W K1 O2 120.5(11) . 2_456 ?
O3 K1 O2 145.7(5) . 2_456 ?
O6 K1 O2 54.8(3) 2_456 2_456 ?
K1A K1 O2W 28.6(13) . 2_456 ?
Ni1 K1 O2W 115.7(6) . 2_456 ?
O1W K1 O2W 62.8(7) . 2_456 ?
O2W K1 O2W 70.1(7) . 2_456 ?
O1 K1 O2W 117.9(6) 2_556 2_456 ?
O3W K1 O2W 161.9(11) . 2_456 ?
O3 K1 O2W 99.2(5) . 2_456 ?
O6 K1 O2W 80.8(4) 2_456 2_456 ?
O2 K1 O2W 71.6(4) 2_456 2_456 ?
K1A K1 C7 105.4(14) . 2_456 ?
Ni1 K1 C7 167.4(7) . 2_456 ?
O1W K1 C7 138.5(7) . 2_456 ?
O2W K1 C7 64.6(5) . 2_456 ?
O1 K1 C7 130.0(5) 2_556 2_456 ?
O3W K1 C7 118.5(11) . 2_456 ?
O3 K1 C7 138.7(5) . 2_456 ?
O6 K1 C7 20.2(3) 2_456 2_456 ?
O2 K1 C7 72.9(4) 2_456 2_456 ?
O2W K1 C7 76.9(5) 2_456 2_456 ?
K1A K1 Mo3 87.0(12) . 2_456 ?
Ni1 K1 Mo3 132.8(5) . 2_456 ?
O1W K1 Mo3 101.5(5) . 2_456 ?
O2W K1 Mo3 106.4(5) . 2_456 ?
O1 K1 Mo3 90.2(3) 2_556 2_456 ?
O3W K1 Mo3 130.5(11) . 2_456 ?
O3 K1 Mo3 162.6(5) . 2_456 ?
O6 K1 Mo3 33.6(2) 2_456 2_456 ?
O2 K1 Mo3 23.2(2) 2_456 2_456 ?
O2W K1 Mo3 66.2(3) 2_456 2_456 ?
C7 K1 Mo3 50.0(2) 2_456 2_456 ?
K1 K1A O1W 130.6(18) . . ?
K1 K1A Ni1 72.1(14) . . ?
O1W K1A Ni1 61.0(7) . . ?
K1 K1A O2W 143.5(15) . 2_456 ?
O1W K1A O2W 83.7(9) . 2_456 ?
Ni1 K1A O2W 144.2(7) . 2_456 ?
K1 K1A O2W 83.8(15) . . ?
O1W K1A O2W 129.5(8) . . ?
Ni1 K1A O2W 115.8(6) . . ?
O2W K1A O2W 81.0(8) 2_456 . ?
K1 K1A O3 89.2(13) . . ?
O1W K1A O3 69.2(6) . . ?
Ni1 K1A O3 45.2(3) . . ?
O2W K1A O3 119.0(6) 2_456 . ?
O2W K1A O3 77.1(5) . . ?
K1 K1A O2 83.0(12) . 2_456 ?
O1W K1A O2 95.7(7) . 2_456 ?
Ni1 K1A O2 106.8(5) . 2_456 ?
O2W K1A O2 80.9(5) 2_456 2_456 ?
O2W K1A O2 128.5(6) . 2_456 ?
O3 K1A O2 151.7(6) . 2_456 ?
K1 K1A O1 65.7(14) . 2_556 ?
O1W K1A O1 68.8(7) . 2_556 ?
Ni1 K1A O1 40.9(3) . 2_556 ?
O2W K1A O1 133.4(6) 2_456 2_556 ?
O2W K1A O1 145.4(7) . 2_556 ?
O3 K1A O1 86.0(4) . 2_556 ?
O2 K1A O1 66.0(3) 2_456 2_556 ?
K1 K1A O6 59.2(12) . 2_456 ?
O1W K1A O6 146.8(7) . 2_456 ?
Ni1 K1A O6 127.4(6) . 2_456 ?
O2W K1A O6 85.3(5) 2_456 2_456 ?
O2W K1A O6 79.1(5) . 2_456 ?
O3 K1A O6 142.2(5) . 2_456 ?
O2 K1A O6 51.7(3) 2_456 2_456 ?
O1 K1A O6 97.5(4) 2_556 2_456 ?
K1 K1A OW6 123.8(15) . 1_565 ?
O1W K1A OW6 44.8(6) . 1_565 ?
Ni1 K1A OW6 88.2(5) . 1_565 ?
O2W K1A OW6 68.5(6) 2_456 1_565 ?
O2W K1A OW6 149.2(7) . 1_565 ?
O3 K1A OW6 113.3(5) . 1_565 ?
O2 K1A OW6 52.5(3) 2_456 1_565 ?
O1 K1A OW6 65.4(4) 2_556 1_565 ?
O6 K1A OW6 102.2(4) 2_456 1_565 ?
K1 K1A O3W 36.6(15) . . ?
O1W K1A O3W 98.6(11) . . ?
Ni1 K1A O3W 37.6(9) . . ?
O2W K1A O3W 173.7(10) 2_456 . ?
O2W K1A O3W 93.0(10) . . ?
O3 K1A O3W 57.0(9) . . ?
O2 K1A O3W 104.6(9) 2_456 . ?
O1 K1A O3W 52.7(8) 2_556 . ?
O6 K1A O3W 95.7(9) 2_456 . ?
OW6 K1A O3W 117.2(9) 1_565 . ?
K1 K1A K2 110.0(15) . . ?
O1W K1A K2 23.8(6) . . ?
Ni1 K1A K2 38.2(3) . . ?
O2W K1A K2 106.0(6) 2_456 . ?
O2W K1A K2 124.4(5) . . ?
O3 K1A K2 50.8(3) . . ?
O2 K1A K2 106.9(4) 2_456 . ?
O1 K1A K2 58.1(3) 2_556 . ?
O6 K1A K2 154.7(4) 2_456 . ?
OW6 K1A K2 63.2(3) 1_565 . ?
O3W K1A K2 75.6(9) . . ?
O20 Cs1 O22 63.4(2) 2_546 2_546 ?
O20 Cs1 O11 131.1(2) 2_546 . ?
O22 Cs1 O11 105.1(2) 2_546 . ?
O20 Cs1 OW7 109.9(4) 2_546 . ?
O22 Cs1 OW7 71.7(4) 2_546 . ?
O11 Cs1 OW7 110.3(4) . . ?
O20 Cs1 OW6 71.9(3) 2_546 . ?
O22 Cs1 OW6 116.5(3) 2_546 . ?
O11 Cs1 OW6 138.3(3) . . ?
OW7 Cs1 OW6 84.7(5) . . ?
O20 Cs1 O19 143.8(2) 2_546 . ?
O22 Cs1 O19 149.9(2) 2_546 . ?
O11 Cs1 O19 50.0(2) . . ?
OW7 Cs1 O19 99.1(3) . . ?
OW6 Cs1 O19 90.2(3) . . ?
O20 Cs1 O12 136.4(2) 2_546 . ?
O22 Cs1 O12 74.1(2) 2_546 . ?
O11 Cs1 O12 50.89(19) . . ?
OW7 Cs1 O12 62.7(5) . . ?
OW6 Cs1 O12 141.4(3) . . ?
O19 Cs1 O12 76.23(19) . . ?
O20 Cs1 O18 101.3(2) 2_546 . ?
O22 Cs1 O18 132.9(2) 2_546 . ?
O11 Cs1 O18 49.6(2) . . ?
OW7 Cs1 O18 147.6(3) . . ?
OW6 Cs1 O18 97.2(3) . . ?
O19 Cs1 O18 48.73(18) . . ?
O12 Cs1 O18 100.11(19) . . ?
O20 Cs1 O17 152.7(2) 2_546 . ?
O22 Cs1 O17 115.5(2) 2_546 . ?
O11 Cs1 O17 76.2(2) . . ?
OW7 Cs1 O17 50.2(3) . . ?
OW6 Cs1 O17 86.3(3) . . ?
O19 Cs1 O17 48.93(18) . . ?
O12 Cs1 O17 57.4(2) . . ?
O18 Cs1 O17 97.56(18) . . ?
O20 Cs1 O20 87.6(2) 2_546 . ?
O22 Cs1 O20 62.5(2) 2_546 . ?
O11 Cs1 O20 49.9(2) . . ?
OW7 Cs1 O20 115.9(5) . . ?
OW6 Cs1 O20 155.4(3) . . ?
O19 Cs1 O20 99.18(19) . . ?
O12 Cs1 O20 63.3(2) . . ?
O18 Cs1 O20 73.06(19) . . ?
O17 Cs1 O20 117.0(2) . . ?
O20 Cs1 O22 61.0(2) 2_546 . ?
O22 Cs1 O22 91.4(2) 2_546 . ?
O11 Cs1 O22 72.65(19) . . ?
OW7 Cs1 O22 163.1(4) . . ?
OW6 Cs1 O22 104.3(3) . . ?
O19 Cs1 O22 95.26(18) . . ?
O12 Cs1 O22 112.7(2) . . ?
O18 Cs1 O22 46.76(17) . . ?
O17 Cs1 O22 143.23(17) . . ?
O20 Cs1 O22 52.4(2) . . ?
O20 Cs1 Te1 129.80(16) 2_546 . ?
O22 Cs1 Te1 132.87(16) 2_546 . ?
O11 Cs1 Te1 28.58(14) . . ?
OW7 Cs1 Te1 120.3(3) . . ?
OW6 Cs1 Te1 110.1(2) . . ?
O19 Cs1 Te1 28.81(13) . . ?
O12 Cs1 Te1 73.85(14) . . ?
O18 Cs1 Te1 29.27(13) . . ?
O17 Cs1 Te1 72.69(13) . . ?
O20 Cs1 Te1 72.47(14) . . ?
O22 Cs1 Te1 70.60(13) . . ?
OW3 Cs2 O25 104.9(6) . 2_446 ?
OW3 Cs2 O12 87.0(5) . 1_455 ?
O25 Cs2 O12 147.7(2) 2_446 1_455 ?
OW3 Cs2 O22 89.8(5) . 2_446 ?
O25 Cs2 O22 74.5(2) 2_446 2_446 ?
O12 Cs2 O22 75.6(2) 1_455 2_446 ?
OW3 Cs2 O20 148.9(5) . 1_455 ?
O25 Cs2 O20 87.1(2) 2_446 1_455 ?
O12 Cs2 O20 69.4(2) 1_455 1_455 ?
O22 Cs2 O20 65.4(2) 2_446 1_455 ?
OW3 Cs2 O23 127.2(6) . 1_455 ?
O25 Cs2 O23 127.9(2) 2_446 1_455 ?
O12 Cs2 O23 50.5(2) 1_455 1_455 ?
O22 Cs2 O23 104.7(2) 2_446 1_455 ?
O20 Cs2 O23 50.2(2) 1_455 1_455 ?
OW3 Cs2 O2 135.2(5) . . ?
O25 Cs2 O2 67.4(2) 2_446 . ?
O12 Cs2 O2 123.9(2) 1_455 . ?
O22 Cs2 O2 126.3(2) 2_446 . ?
O20 Cs2 O2 75.9(2) 1_455 . ?
O23 Cs2 O2 73.4(2) 1_455 . ?
OW3 Cs2 O15 64.0(6) . 2_446 ?
O25 Cs2 O15 50.4(2) 2_446 2_446 ?
O12 Cs2 O15 114.4(2) 1_455 2_446 ?
O22 Cs2 O15 49.2(2) 2_446 2_446 ?
O20 Cs2 O15 106.8(2) 1_455 2_446 ?
O23 Cs2 O15 153.8(2) 1_455 2_446 ?
O2 Cs2 O15 117.1(2) . 2_446 ?
OW3 Cs2 OW4 37.8(5) . . ?
O25 Cs2 OW4 126.5(5) 2_446 . ?
O12 Cs2 OW4 51.4(5) 1_455 . ?
O22 Cs2 OW4 70.7(5) 2_446 . ?
O20 Cs2 OW4 112.5(5) 1_455 . ?
O23 Cs2 OW4 99.8(5) 1_455 . ?
O2 Cs2 OW4 162.6(5) . . ?
O15 Cs2 OW4 76.1(5) 2_446 . ?
OW3 Cs2 O26 51.9(5) . . ?
O25 Cs2 O26 96.7(2) 2_446 . ?
O12 Cs2 O26 113.7(2) 1_455 . ?
O22 Cs2 O26 137.83(19) 2_446 . ?
O20 Cs2 O26 156.6(2) 1_455 . ?
O23 Cs2 O26 112.40(19) 1_455 . ?
O2 Cs2 O26 84.3(2) . . ?
O15 Cs2 O26 93.11(19) 2_446 . ?
OW4 Cs2 O26 83.7(5) . . ?
OW3 Cs2 O25 91.8(5) . . ?
O25 Cs2 O25 54.8(3) 2_446 . ?
O12 Cs2 O25 156.5(2) 1_455 . ?
O22 Cs2 O25 127.91(19) 2_446 . ?
O20 Cs2 O25 118.0(2) 1_455 . ?
O23 Cs2 O25 115.0(2) 1_455 . ?
O2 Cs2 O25 46.5(2) . . ?
O15 Cs2 O25 85.7(2) 2_446 . ?
OW4 Cs2 O25 129.3(5) . . ?
O26 Cs2 O25 50.10(19) . . ?
OW3 Cs2 O16 68.9(6) . . ?
O25 Cs2 O16 136.4(2) 2_446 . ?
O12 Cs2 O16 75.8(2) 1_455 . ?
O22 Cs2 O16 145.0(2) 2_446 . ?
O20 Cs2 O16 121.2(2) 1_455 . ?
O23 Cs2 O16 71.05(19) 1_455 . ?
O2 Cs2 O16 86.8(2) . . ?
O15 Cs2 O16 130.69(19) 2_446 . ?
OW4 Cs2 O16 75.8(5) . . ?
O26 Cs2 O16 44.19(17) . . ?
O25 Cs2 O16 81.82(19) . . ?
Mo1 O1 Ni1 150.9(6) . 2_556 ?
Mo1 O1 K1 161.6(5) . 2_556 ?
Ni1 O1 K1 45.4(3) 2_556 2_556 ?
Mo1 O1 K1A 165.2(5) . 2_556 ?
Ni1 O1 K1A 43.6(3) 2_556 2_556 ?
K1 O1 K1A 13.9(3) 2_556 2_556 ?
Mo3 O2 K1A 115.1(5) . 2_456 ?
Mo3 O2 K1 113.6(5) . 2_456 ?
K1A O2 K1 14.2(2) 2_456 2_456 ?
Mo3 O2 Cs2 98.6(4) . . ?
K1A O2 Cs2 144.7(4) 2_456 . ?
K1 O2 Cs2 139.0(4) 2_456 . ?
Mo2 O3 Ni1 159.9(5) . . ?
Mo2 O3 K1A 127.1(5) . . ?
Ni1 O3 K1A 47.4(4) . . ?
Mo2 O3 K1 137.6(5) . . ?
Ni1 O3 K1 42.9(3) . . ?
K1A O3 K1 14.7(3) . . ?
Mo2 O3 K2 104.2(4) . . ?
Ni1 O3 K2 57.9(3) . . ?
K1A O3 K2 83.4(4) . . ?
K1 O3 K2 90.2(4) . . ?
Mo2 O3 K2 116.9(4) . 2_556 ?
Ni1 O3 K2 59.4(3) . 2_556 ?
K1A O3 K2 105.9(4) . 2_556 ?
K1 O3 K2 102.0(4) . 2_556 ?
K2 O3 K2 46.3(3) . 2_556 ?
C10 O4 Mo4 131.1(7) . . ?
C7 O6 Mo3 132.0(8) . . ?
C7 O6 K1 103.2(7) . 2_456 ?
Mo3 O6 K1 99.0(4) . 2_456 ?
C7 O6 K1A 101.7(7) . 2_456 ?
Mo3 O6 K1A 91.4(4) . 2_456 ?
K1 O6 K1A 12.3(3) 2_456 2_456 ?
Mo4 O7 Mo3 142.2(4) . . ?
Mo4 O7 Cs2 84.8(3) . . ?
Mo3 O7 Cs2 81.1(2) . . ?
C19 O8 Mo1 128.5(7) . . ?
C10 O9 Mo6 130.7(8) . . ?
C7 O10 Mo2 129.8(8) . . ?
Te1 O11 Mo5 124.1(4) . . ?
Te1 O11 Mo1 123.6(4) . . ?
Mo5 O11 Mo1 95.6(3) . . ?
Te1 O11 Cs1 97.7(3) . . ?
Mo5 O11 Cs1 105.5(3) . . ?
Mo1 O11 Cs1 109.0(3) . . ?
Mo5 O12 Cs2 110.1(4) . 1_655 ?
Mo5 O12 Cs1 111.4(4) . . ?
Cs2 O12 Cs1 97.2(2) 1_655 . ?
C19 O14 Mo5 133.8(8) . . ?
Mo3 O15 Mo2 118.1(4) . . ?
Mo3 O15 Cs2 96.8(3) . 2_446 ?
Mo2 O15 Cs2 99.6(3) . 2_446 ?
Mo4 O16 Cs2 94.0(3) . . ?
Mo6 O17 Cs1 112.7(3) . . ?
Te1 O18 Mo2 125.0(4) . . ?
Te1 O18 Mo3 123.4(4) . . ?
Mo2 O18 Mo3 96.8(3) . . ?
Te1 O18 Cs1 89.5(3) . . ?
Mo2 O18 Cs1 108.1(3) . . ?
Mo3 O18 Cs1 113.9(3) . . ?
Te1 O19 Mo4 120.8(3) . . ?
Te1 O19 Mo6 124.9(4) . . ?
Mo4 O19 Mo6 95.8(3) . . ?
Te1 O19 Cs1 93.5(3) . . ?
Mo4 O19 Cs1 116.9(3) . . ?
Mo6 O19 Cs1 105.6(2) . . ?
Mo1 O20 Cs1 138.8(4) . 2_546 ?
Mo1 O20 Cs2 109.0(4) . 1_655 ?
Cs1 O20 Cs2 103.4(2) 2_546 1_655 ?
Mo1 O20 Cs1 110.0(4) . . ?
Cs1 O20 Cs1 92.4(2) 2_546 . ?
Cs2 O20 Cs1 93.3(2) 1_655 . ?
Mo2 O21 Mo1 144.9(4) . . ?
Mo2 O21 K2 96.5(3) . . ?
Mo1 O21 K2 109.6(4) . . ?
Mo2 O22 Cs1 137.2(4) . 2_546 ?
Mo2 O22 Cs2 113.8(4) . 2_446 ?
Cs1 O22 Cs2 103.5(2) 2_546 2_446 ?
Mo2 O22 Cs1 110.8(3) . . ?
Cs1 O22 Cs1 88.6(2) 2_546 . ?
Cs2 O22 Cs1 90.2(2) 2_446 . ?
Mo1 O23 Mo5 116.5(4) . . ?
Mo1 O23 Cs2 99.9(3) . 1_655 ?
Mo5 O23 Cs2 98.9(3) . 1_655 ?
Mo4 O24 Mo6 118.9(4) . . ?
Mo3 O25 Cs2 112.1(4) . 2_446 ?
Mo3 O25 Cs2 90.5(3) . . ?
Cs2 O25 Cs2 125.2(3) 2_446 . ?
Mo4 O26 Cs2 95.1(3) . . ?
Mo6 O27 Mo5 147.9(4) . . ?
C4 C1 C2 118.6(13) . . ?
C18 C2 C1 120.9(14) . . ?
C11 C3 C8 119.0(12) . . ?
C11 C3 N3 119.6(13) . . ?
C8 C3 N3 121.4(12) . . ?
C16 C4 C1 120.7(11) . . ?
C16 C4 N1 120.7(13) . . ?
C1 C4 N1 118.6(13) . . ?
C6 C5 C15 119.0(14) . . ?
C5 C6 C17 122.4(14) . . ?
O6 C7 O10 125.4(11) . . ?
O6 C7 C17 118.6(12) . . ?
O10 C7 C17 116.0(12) . . ?
O6 C7 K1 56.6(7) . 2_456 ?
O10 C7 K1 121.9(8) . 2_456 ?
C17 C7 K1 92.5(7) . 2_456 ?
C12 C8 C3 120.6(12) . . ?
C17 C9 C13 121.2(14) . . ?
O4 C10 O9 125.5(10) . . ?
O4 C10 C18 117.3(10) . . ?
O9 C10 C18 117.3(11) . . ?
C3 C11 C14 120.8(13) . . ?
C8 C12 C20 121.7(12) . . ?
C15 C13 C9 121.6(14) . . ?
C11 C14 C20 120.1(11) . . ?
C13 C15 C5 118.6(12) . . ?
C13 C15 N2 123.2(13) . . ?
C5 C15 N2 118.2(12) . . ?
C4 C16 C21 120.7(13) . . ?
C9 C17 C6 117.0(12) . . ?
C9 C17 C7 123.3(12) . . ?
C6 C17 C7 119.7(13) . . ?
C2 C18 C21 119.4(11) . . ?
C2 C18 C10 121.6(12) . . ?
C21 C18 C10 119.0(11) . . ?
O14 C19 O8 125.2(11) . . ?
O14 C19 C20 116.8(10) . . ?
O8 C19 C20 118.0(10) . . ?
C12 C20 C14 117.7(11) . . ?
C12 C20 C19 123.7(12) . . ?
C14 C20 C19 118.5(11) . . ?
C16 C21 C18 119.5(12) . . ?
K1A O1W Ni1 66.0(7) . . ?
K1A O1W K1 13.7(5) . . ?
Ni1 O1W K1 53.3(6) . . ?
K1A O1W K2 138.1(10) . . ?
Ni1 O1W K2 73.2(7) . . ?
K1 O1W K2 126.4(8) . . ?
K1A O2W K1A 99.0(8) 2_456 . ?
K1A O2W K1 112.0(8) 2_456 . ?
K1A O2W K1 15.8(3) . . ?
K1A O2W K1 7.9(3) 2_456 2_456 ?
K1A O2W K1 95.8(7) . 2_456 ?
K1 O2W K1 109.9(7) . 2_456 ?
Ni1 O3W K1 45.1(9) . . ?
Ni1 O3W K1A 36.8(8) . . ?
K1 O3W K1A 9.1(4) . . ?
Cs1 OW6 K1A 139.9(5) . 1_545 ?
K2 OW7 Cs1 97.0(6) 1_545 . ?
K2 K2 O1W 112.4(6) 2_556 . ?
K2 K2 Ni1 65.6(3) 2_556 . ?
O1W K2 Ni1 46.9(5) . . ?
K2 K2 Ni1 60.3(4) 2_556 2_556 ?
O1W K2 Ni1 172.6(5) . 2_556 ?
Ni1 K2 Ni1 125.9(3) . 2_556 ?
K2 K2 O3 69.0(3) 2_556 . ?
O1W K2 O3 59.8(5) . . ?
Ni1 K2 O3 40.5(2) . . ?
Ni1 K2 O3 114.0(3) 2_556 . ?
K2 K2 OW7 128.6(6) 2_556 1_565 ?
O1W K2 OW7 107.7(6) . 1_565 ?
Ni1 K2 OW7 141.0(4) . 1_565 ?
Ni1 K2 OW7 79.3(4) 2_556 1_565 ?
O3 K2 OW7 162.4(5) . 1_565 ?
K2 K2 O21 84.5(3) 2_556 . ?
O1W K2 O21 96.4(5) . . ?
Ni1 K2 O21 93.6(3) . . ?
Ni1 K2 O21 81.6(3) 2_556 . ?
O3 K2 O21 53.2(2) . . ?
OW7 K2 O21 121.7(4) 1_565 . ?
K2 K2 O3 64.7(4) 2_556 2_556 ?
O1W K2 O3 141.5(5) . 2_556 ?
Ni1 K2 O3 114.6(3) . 2_556 ?
Ni1 K2 O3 39.0(2) 2_556 2_556 ?
O3 K2 O3 133.7(3) . 2_556 ?
OW7 K2 O3 63.9(4) 1_565 2_556 ?
O21 K2 O3 120.4(3) . 2_556 ?
K2 K2 Mo2 80.6(3) 2_556 . ?
O1W K2 Mo2 71.5(4) . . ?
Ni1 K2 Mo2 65.48(18) . . ?
Ni1 K2 Mo2 104.5(2) 2_556 . ?
O3 K2 Mo2 25.24(15) . . ?
OW7 K2 Mo2 143.7(4) 1_565 . ?
O21 K2 Mo2 29.25(15) . . ?
O3 K2 Mo2 138.6(3) 2_556 . ?
K2 K2 K1A 94.6(4) 2_556 . ?
O1W K2 K1A 18.1(5) . . ?
Ni1 K2 K1A 29.5(3) . . ?
Ni1 K2 K1A 154.5(3) 2_556 . ?
O3 K2 K1A 45.8(2) . . ?
OW7 K2 K1A 124.3(5) 1_565 . ?
O21 K2 K1A 91.7(3) . . ?
O3 K2 K1A 137.5(3) 2_556 . ?
Mo2 K2 K1A 63.39(19) . . ?
K2 K2 K1 85.6(4) 2_556 . ?
O1W K2 K1 26.8(5) . . ?
Ni1 K2 K1 20.2(2) . . ?
Ni1 K2 K1 145.9(3) 2_556 . ?
O3 K2 K1 43.5(2) . . ?
OW7 K2 K1 129.7(4) 1_565 . ?
O21 K2 K1 93.6(3) . . ?
O3 K2 K1 130.0(3) 2_556 . ?
Mo2 K2 K1 64.43(19) . . ?
K1A K2 K1 9.4(2) . . ?
K2 K2 Cs1 118.8(3) 2_556 1_565 ?
O1W K2 Cs1 78.9(4) . 1_565 ?
Ni1 K2 Cs1 99.5(2) . 1_565 ?
Ni1 K2 Cs1 105.7(2) 2_556 1_565 ?
O3 K2 Cs1 135.6(3) . 1_565 ?
OW7 K2 Cs1 41.7(3) 1_565 1_565 ?
O21 K2 Cs1 156.4(3) . 1_565 ?
O3 K2 Cs1 71.38(19) 2_556 1_565 ?
Mo2 K2 Cs1 149.4(2) . 1_565 ?
K1A K2 Cs1 90.1(2) . 1_565 ?
K1 K2 Cs1 92.1(2) . 1_565 ?

_refine_diff_density_max         2.651
_refine_diff_density_min         -2.437
_refine_diff_density_rms         0.290

_shelxl_version_number           2014-3

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_10
_database_code_depnum_ccdc_archive 'CCDC 1871480'
_audit_update_record             
;
2018-10-08 deposited with the CCDC.	2019-03-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C16 H99 As2 Mo12 N4 Na Ni2 O86 Rb2'
_chemical_formula_weight         3336.46

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/n'
_space_group_name_Hall           '-P 2yn'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   13.8420(4)
_cell_length_b                   23.8125(8)
_cell_length_c                   14.9785(6)
_cell_angle_alpha                90
_cell_angle_beta                 113.996(2)
_cell_angle_gamma                90
_cell_volume                     4510.4(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    22711
_cell_measurement_theta_min      1.716
_cell_measurement_theta_max      24.998

_exptl_crystal_description       block
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.457
_exptl_crystal_F_000             3244
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_exptl_absorpt_coefficient_mu    3.947
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.388
_exptl_absorpt_correction_T_max  0.437
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            22711
_diffrn_reflns_av_unetI/netI     0.0518
_diffrn_reflns_av_R_equivalents  0.0430
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_theta_min         1.716
_diffrn_reflns_theta_max         24.998
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.974
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.974
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.974
_reflns_number_total             7942
_reflns_number_gt                6245
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0341P)²+38.8236P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         7942
_refine_ls_number_parameters     577
_refine_ls_number_restraints     66
_refine_ls_R_factor_all          0.0678
_refine_ls_R_factor_gt           0.0481
_refine_ls_wR_factor_ref         0.1056
_refine_ls_wR_factor_gt          0.0979
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_restrained_S_all      1.075
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.43089(6) 0.18862(3) 0.76853(5) 0.02621(18) Uani 1 1 d . . . . .
Mo2 Mo 0.50557(5) 0.07787(3) 0.90966(5) 0.02046(16) Uani 1 1 d . . . . .
Mo3 Mo 0.68399(5) 0.11960(3) 0.55085(5) 0.01851(16) Uani 1 1 d . . . . .
Mo4 Mo 0.76640(5) -0.00178(3) 0.70427(5) 0.01891(16) Uani 1 1 d . . . . .
Mo5 Mo 0.68262(6) -0.02109(3) 0.87738(5) 0.02047(16) Uani 1 1 d . . . . .
Mo6 Mo 0.51910(5) 0.20898(3) 0.57903(5) 0.01939(16) Uani 1 1 d . . . . .
As1 As 0.65987(6) 0.11673(3) 0.77822(5) 0.01630(18) Uani 1 1 d . . . . .
Ni1 Ni 0.4121(2) -0.06320(10) 0.82191(18) 0.0436(7) Uani 0.5 1 d . . P . .
Ni2 Ni 0.90731(13) -0.09420(7) 1.27536(12) 0.0302(4) Uani 0.5 1 d . . P . .
Na1 Na 0.90731(13) -0.09420(7) 1.27536(12) 0.0302(4) Uani 0.5 1 d . . P . .
Rb1 Rb 0.44491(8) 0.03900(4) 0.60845(7) 0.0416(2) Uani 1 1 d . . . . .
O1 O 0.4902(5) 0.2753(2) 0.5309(4) 0.0313(14) Uani 1 1 d . . . . .
O2 O 0.5793(5) 0.2188(2) 0.8955(4) 0.0316(14) Uani 1 1 d . . . . .
O3 O 0.6594(5) -0.0303(2) 0.6108(4) 0.0300(14) Uani 1 1 d . . . . .
O4 O 0.7331(5) -0.0667(2) 0.9735(4) 0.0390(16) Uani 1 1 d . . . . .
O5 O 0.6305(4) 0.1433(2) 0.9914(4) 0.0270(13) Uani 1 1 d . . . . .
O6 O 0.3744(6) 0.2484(3) 0.7893(5) 0.0502(19) Uani 1 1 d . . . . .
O7 O 0.8921(4) 0.0437(2) 0.8371(4) 0.0290(13) Uani 1 1 d . . . . .
O8 O 0.5915(5) 0.0729(2) 0.4816(4) 0.0301(14) Uani 1 1 d . . . . .
O9 O 0.7971(4) 0.1840(2) 0.6605(4) 0.0273(13) Uani 1 1 d . . . . .
O10 O 0.8731(5) -0.0332(2) 0.6948(4) 0.0352(15) Uani 1 1 d . . . . .
O11 O 0.5621(4) -0.0491(2) 0.8034(4) 0.0303(14) Uani 1 1 d . . . . .
O12 O 0.6328(4) 0.0382(2) 0.9320(4) 0.0223(12) Uani 1 1 d . . . . .
O13 O 0.8345(4) 0.0296(2) 0.9541(4) 0.0266(13) Uani 1 1 d . . . . .
O14 O 0.7627(5) 0.1286(3) 0.4874(4) 0.0367(15) Uani 1 1 d . . . . .
O15 O 0.3312(5) 0.1567(3) 0.6739(4) 0.0433(17) Uani 1 1 d . . . . .
O16 O 0.7635(4) -0.0500(2) 0.8071(4) 0.0228(12) Uani 1 1 d . . . . .
O17 O 0.4989(5) 0.0672(2) 1.0202(4) 0.0320(14) Uani 1 1 d . . . . .
O18 O 0.5067(4) 0.2194(2) 0.6984(4) 0.0252(13) Uani 1 1 d . . . . .
O19 O 0.6838(4) 0.2475(2) 0.6725(4) 0.0288(13) Uani 1 1 d . . . . .
O20 O 0.6685(4) 0.0427(2) 0.7648(3) 0.0172(11) Uani 1 1 d . . . . .
O21 O 0.4074(4) 0.1712(2) 0.5151(4) 0.0272(13) Uani 1 1 d . . . . .
O22 O 0.4184(4) 0.1443(2) 0.8727(4) 0.0290(13) Uani 1 1 d . . . . .
O23 O 0.4148(5) 0.0319(3) 0.8311(4) 0.0390(16) Uani 1 1 d . . . . .
O24 O 0.5355(4) 0.1161(2) 0.7887(4) 0.0194(11) Uani 1 1 d . . . . .
O25 O 0.6078(4) 0.1331(2) 0.6504(3) 0.0166(11) Uani 1 1 d . . . . .
O26 O 0.7725(4) 0.0697(2) 0.6499(4) 0.0207(12) Uani 1 1 d . . . . .
O27 O 0.5973(4) 0.1862(2) 0.5019(4) 0.0210(12) Uani 1 1 d . . . . .
C1 C 0.7319(9) 0.2256(5) 1.0429(8) 0.064(3) Uani 1 1 d . . . . .
H8A H 0.7717 0.2019 1.0972 0.095 Uiso 1 1 calc R U . . .
H8B H 0.7763 0.2380 1.0115 0.095 Uiso 1 1 calc R U . . .
H8C H 0.7064 0.2577 1.0658 0.095 Uiso 1 1 calc R U . . .
C2 C 0.9858(7) 0.0867(4) 0.9901(6) 0.032(2) Uani 1 1 d . . . . .
H2A H 1.0523 0.0685 1.0011 0.038 Uiso 1 1 calc R U . . .
H2B H 0.9844 0.1223 0.9582 0.038 Uiso 1 1 calc R U . . .
C3 C 0.9817(8) 0.0977(4) 1.0865(7) 0.044(2) Uani 1 1 d . . . . .
H3A H 0.9780 0.0623 1.1170 0.052 Uiso 1 1 calc R U . . .
H3B H 0.9186 0.1191 1.0767 0.052 Uiso 1 1 calc R U . . .
C4 C 0.8387(7) 0.3241(3) 0.7686(6) 0.030(2) Uani 1 1 d . . . . .
H4A H 0.8032 0.3399 0.7036 0.036 Uiso 1 1 calc R U . . .
H4B H 0.7897 0.3253 0.7999 0.036 Uiso 1 1 calc R U . . .
C5 C 0.6399(7) 0.1935(4) 0.9713(6) 0.031(2) Uani 1 1 d . . . . .
C6 C 0.8669(7) 0.2634(4) 0.7598(6) 0.035(2) Uani 1 1 d . . . . .
H6A H 0.9225 0.2625 0.7361 0.042 Uiso 1 1 calc R U . . .
H6B H 0.8944 0.2464 0.8242 0.042 Uiso 1 1 calc R U . . .
C7 C 0.8961(6) 0.0505(3) 0.9223(6) 0.0255(19) Uani 1 1 d . . . . .
C8 C 0.7747(7) 0.2292(3) 0.6924(5) 0.0230(18) Uani 1 1 d . . . . .
N1 N 1.0766(6) 0.1295(3) 1.1519(6) 0.046(2) Uani 1 1 d . . . . .
H1A H 1.0726 0.1356 1.2089 0.068 Uiso 1 1 calc R U . . .
H1B H 1.1345 0.1096 1.1616 0.068 Uiso 1 1 calc R U . . .
H1C H 1.0795 0.1622 1.1243 0.068 Uiso 1 1 calc R U . . .
N2 N 0.9314(6) 0.3590(3) 0.8249(5) 0.0339(18) Uani 1 1 d . . . . .
H2C H 0.9106 0.3940 0.8278 0.051 Uiso 1 1 calc R U . . .
H2D H 0.9636 0.3452 0.8851 0.051 Uiso 1 1 calc R U . . .
H2E H 0.9761 0.3588 0.7958 0.051 Uiso 1 1 calc R U . . .
O1W O 0.4443(7) -0.1530(3) 0.7951(7) 0.074(2) Uani 1 1 d . U . . .
O2W O 0.2958(9) -0.0468(4) 0.6593(7) 0.104(3) Uani 1 1 d . U . . .
O3W O 1.0134(6) -0.1273(3) 1.2284(6) 0.067(2) Uani 1 1 d . U . . .
O4W O 0.9112(9) -0.0208(4) 1.2053(8) 0.107(3) Uani 1 1 d . U . . .
O5W O 1.0314(8) -0.0649(4) 1.4011(8) 0.097(3) Uani 1 1 d . U . . .
O6W O 0.8004(8) -0.0579(5) 1.3278(7) 0.097(3) Uani 1 1 d . U . . .
O7W O 0.9024(8) -0.1677(4) 1.3432(7) 0.094(3) Uani 1 1 d . U . . .
O8W O 0.7839(6) -0.1191(4) 1.1515(6) 0.078(3) Uani 1 1 d . U . . .
OW1 O 0.2187(10) 0.0989(6) 0.4949(9) 0.142(5) Uani 1 1 d . . . . .
OW2 O 0.5967(9) -0.1966(5) 0.9636(7) 0.115(4) Uani 1 1 d . U . . .
OW3 O 1.006(3) -0.0544(11) 1.5704(18) 0.158(12) Uani 0.5 1 d . . P . .
OW4 O 0.1020(18) -0.1316(8) 0.7208(16) 0.116(8) Uani 0.5 1 d . . P . .
OW5 O 0.9326(11) 0.1954(6) 0.4892(9) 0.152(5) Uani 1 1 d . U . . .
OW6 O 1.0983(15) 0.1697(5) 1.3333(11) 0.173(7) Uani 1 1 d . . . . .
OW7 O 0.6772(11) 0.2825(6) 0.4493(12) 0.177(7) Uani 1 1 d . . . . .
OW8 O 0.1773(10) 0.2589(6) 0.7816(10) 0.147(5) Uani 1 1 d . . . . .
OW9 O 0.2531(8) -0.0591(5) 0.8549(6) 0.100(3) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O15 1.703(6) . ?
Mo1 O6 1.713(6) . ?
Mo1 O18 1.907(6) . ?
Mo1 O22 1.949(5) . ?
Mo1 O24 2.193(5) . ?
Mo1 O2 2.275(6) . ?
Mo2 O17 1.713(5) . ?
Mo2 O23 1.720(6) . ?
Mo2 O12 1.905(5) . ?
Mo2 O22 1.929(6) . ?
Mo2 O24 2.212(5) . ?
Mo2 O5 2.280(5) . ?
Mo3 O8 1.694(6) . ?
Mo3 O14 1.727(6) . ?
Mo3 O26 1.907(5) . ?
Mo3 O27 1.944(5) . ?
Mo3 O25 2.172(5) . ?
Mo3 O9 2.325(5) . ?
Mo3 Rb1 4.2073(12) . ?
Mo4 O3 1.711(5) . ?
Mo4 O10 1.713(6) . ?
Mo4 O26 1.902(5) . ?
Mo4 O16 1.934(5) . ?
Mo4 O20 2.187(5) . ?
Mo4 O7 2.312(5) . ?
Mo4 Rb1 4.1965(12) . ?
Mo5 O4 1.710(6) . ?
Mo5 O11 1.718(6) . ?
Mo5 O12 1.897(5) . ?
Mo5 O16 1.948(5) . ?
Mo5 O20 2.219(5) . ?
Mo5 O13 2.288(6) . ?
Mo5 Rb1 4.2803(12) . ?
Mo6 O21 1.706(5) . ?
Mo6 O1 1.714(5) . ?
Mo6 O18 1.881(5) . ?
Mo6 O27 1.953(5) . ?
Mo6 O25 2.202(5) . ?
Mo6 O19 2.325(5) . ?
Mo6 Rb1 4.2428(12) . ?
As1 O20 1.783(5) . ?
As1 O24 1.792(5) . ?
As1 O25 1.793(5) . ?
As1 Rb1 3.5485(12) . ?
Ni1 O17 2.180(6) 3_657 ?
Ni1 O11 2.230(6) . ?
Ni1 O1W 2.254(9) . ?
Ni1 O23 2.268(7) . ?
Ni1 O2W 2.343(11) . ?
Ni1 Rb1 4.187(3) . ?
Ni2 O7W 2.039(9) . ?
Ni2 O3W 2.028(8) . ?
Ni2 O4W 2.050(10) . ?
Ni2 O8W 2.033(9) . ?
Ni2 O5W 2.086(10) . ?
Ni2 O6W 2.121(10) . ?
Rb1 O8 2.937(6) 3_656 ?
Rb1 O3 3.009(5) 3_656 ?
Rb1 O20 3.029(5) . ?
Rb1 O25 3.057(5) . ?
Rb1 O24 3.079(5) . ?
Rb1 O2W 3.209(11) . ?
Rb1 OW1 3.225(13) . ?
Rb1 O3 3.384(6) . ?
Rb1 O8 3.394(6) . ?
Rb1 O21 3.398(6) . ?
Rb1 O11 3.422(6) . ?
Rb1 O23 3.529(6) . ?
O2 C5 1.258(10) . ?
O3 Rb1 3.009(5) 3_656 ?
O5 C5 1.252(10) . ?
O7 C7 1.265(9) . ?
O8 Rb1 2.937(6) 3_656 ?
O9 C8 1.267(9) . ?
O13 C7 1.236(10) . ?
O17 Ni1 2.180(6) 3_657 ?
O19 C8 1.247(10) . ?
C1 C5 1.499(13) . ?
C2 C3 1.490(13) . ?
C2 C7 1.514(11) . ?
C3 N1 1.487(11) . ?
C4 N2 1.472(10) . ?
C4 C6 1.516(12) . ?
C6 C8 1.504(11) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O15 Mo1 O6 104.3(3) . . ?
O15 Mo1 O18 98.9(3) . . ?
O6 Mo1 O18 100.1(3) . . ?
O15 Mo1 O22 96.8(3) . . ?
O6 Mo1 O22 96.3(3) . . ?
O18 Mo1 O22 153.7(2) . . ?
O15 Mo1 O24 91.7(3) . . ?
O6 Mo1 O24 162.5(3) . . ?
O18 Mo1 O24 84.1(2) . . ?
O22 Mo1 O24 74.4(2) . . ?
O15 Mo1 O2 170.9(3) . . ?
O6 Mo1 O2 84.8(3) . . ?
O18 Mo1 O2 80.0(2) . . ?
O22 Mo1 O2 81.1(2) . . ?
O24 Mo1 O2 79.2(2) . . ?
O17 Mo2 O23 104.8(3) . . ?
O17 Mo2 O12 99.5(2) . . ?
O23 Mo2 O12 99.8(3) . . ?
O17 Mo2 O22 97.2(3) . . ?
O23 Mo2 O22 97.4(3) . . ?
O12 Mo2 O22 152.0(2) . . ?
O17 Mo2 O24 162.5(2) . . ?
O23 Mo2 O24 91.7(2) . . ?
O12 Mo2 O24 83.2(2) . . ?
O22 Mo2 O24 74.4(2) . . ?
O17 Mo2 O5 84.8(2) . . ?
O23 Mo2 O5 170.4(2) . . ?
O12 Mo2 O5 78.4(2) . . ?
O22 Mo2 O5 81.0(2) . . ?
O24 Mo2 O5 78.74(19) . . ?
O8 Mo3 O14 103.5(3) . . ?
O8 Mo3 O26 98.9(2) . . ?
O14 Mo3 O26 99.0(3) . . ?
O8 Mo3 O27 96.2(2) . . ?
O14 Mo3 O27 97.0(3) . . ?
O26 Mo3 O27 154.8(2) . . ?
O8 Mo3 O25 93.5(2) . . ?
O14 Mo3 O25 162.0(2) . . ?
O26 Mo3 O25 84.00(19) . . ?
O27 Mo3 O25 74.93(19) . . ?
O8 Mo3 O9 171.5(2) . . ?
O14 Mo3 O9 85.0(2) . . ?
O26 Mo3 O9 80.0(2) . . ?
O27 Mo3 O9 82.1(2) . . ?
O25 Mo3 O9 78.05(19) . . ?
O8 Mo3 Rb1 50.57(19) . . ?
O14 Mo3 Rb1 153.5(2) . . ?
O26 Mo3 Rb1 82.28(16) . . ?
O27 Mo3 Rb1 91.88(16) . . ?
O25 Mo3 Rb1 44.33(13) . . ?
O9 Mo3 Rb1 121.04(14) . . ?
O3 Mo4 O10 104.3(3) . . ?
O3 Mo4 O26 100.3(2) . . ?
O10 Mo4 O26 99.6(3) . . ?
O3 Mo4 O16 97.2(3) . . ?
O10 Mo4 O16 96.0(2) . . ?
O26 Mo4 O16 152.9(2) . . ?
O3 Mo4 O20 93.2(2) . . ?
O10 Mo4 O20 161.3(2) . . ?
O26 Mo4 O20 83.5(2) . . ?
O16 Mo4 O20 74.98(19) . . ?
O3 Mo4 O7 171.2(2) . . ?
O10 Mo4 O7 84.5(3) . . ?
O26 Mo4 O7 78.5(2) . . ?
O16 Mo4 O7 81.1(2) . . ?
O20 Mo4 O7 78.02(19) . . ?
O3 Mo4 Rb1 50.76(19) . . ?
O10 Mo4 Rb1 154.6(2) . . ?
O26 Mo4 Rb1 82.64(16) . . ?
O16 Mo4 Rb1 92.72(16) . . ?
O20 Mo4 Rb1 43.94(13) . . ?
O7 Mo4 Rb1 120.55(14) . . ?
O4 Mo5 O11 104.7(3) . . ?
O4 Mo5 O12 101.8(3) . . ?
O11 Mo5 O12 98.0(3) . . ?
O4 Mo5 O16 95.9(3) . . ?
O11 Mo5 O16 97.7(2) . . ?
O12 Mo5 O16 152.4(2) . . ?
O4 Mo5 O20 162.7(3) . . ?
O11 Mo5 O20 90.8(2) . . ?
O12 Mo5 O20 83.29(19) . . ?
O16 Mo5 O20 73.96(19) . . ?
O4 Mo5 O13 86.3(3) . . ?
O11 Mo5 O13 169.0(2) . . ?
O12 Mo5 O13 79.1(2) . . ?
O16 Mo5 O13 81.1(2) . . ?
O20 Mo5 O13 78.39(19) . . ?
O4 Mo5 Rb1 154.1(2) . . ?
O11 Mo5 Rb1 49.45(19) . . ?
O12 Mo5 Rb1 83.24(15) . . ?
O16 Mo5 Rb1 90.02(15) . . ?
O20 Mo5 Rb1 42.22(13) . . ?
O13 Mo5 Rb1 119.58(14) . . ?
O21 Mo6 O1 104.2(3) . . ?
O21 Mo6 O18 101.0(3) . . ?
O1 Mo6 O18 100.5(3) . . ?
O21 Mo6 O27 96.6(2) . . ?
O1 Mo6 O27 95.6(2) . . ?
O18 Mo6 O27 152.3(2) . . ?
O21 Mo6 O25 92.2(2) . . ?
O1 Mo6 O25 161.6(2) . . ?
O18 Mo6 O25 84.0(2) . . ?
O27 Mo6 O25 74.07(19) . . ?
O21 Mo6 O19 171.5(2) . . ?
O1 Mo6 O19 83.9(2) . . ?
O18 Mo6 O19 79.7(2) . . ?
O27 Mo6 O19 79.8(2) . . ?
O25 Mo6 O19 79.35(19) . . ?
O21 Mo6 Rb1 49.70(19) . . ?
O1 Mo6 Rb1 153.8(2) . . ?
O18 Mo6 Rb1 84.69(17) . . ?
O27 Mo6 Rb1 90.69(15) . . ?
O25 Mo6 Rb1 43.72(13) . . ?
O19 Mo6 Rb1 122.26(14) . . ?
O20 As1 O24 96.5(2) . . ?
O20 As1 O25 96.3(2) . . ?
O24 As1 O25 96.4(2) . . ?
O20 As1 Rb1 58.60(16) . . ?
O24 As1 Rb1 60.20(16) . . ?
O25 As1 Rb1 59.49(16) . . ?
O17 Ni1 O11 89.9(2) 3_657 . ?
O17 Ni1 O1W 95.0(3) 3_657 . ?
O11 Ni1 O1W 81.9(3) . . ?
O17 Ni1 O23 89.4(2) 3_657 . ?
O11 Ni1 O23 82.2(2) . . ?
O1W Ni1 O23 163.4(3) . . ?
O17 Ni1 O2W 169.0(3) 3_657 . ?
O11 Ni1 O2W 97.3(3) . . ?
O1W Ni1 O2W 94.3(3) . . ?
O23 Ni1 O2W 83.3(3) . . ?
O17 Ni1 Rb1 131.69(18) 3_657 . ?
O11 Ni1 Rb1 54.68(16) . . ?
O1W Ni1 Rb1 108.9(2) . . ?
O23 Ni1 Rb1 57.44(16) . . ?
O2W Ni1 Rb1 49.6(3) . . ?
O7W Ni2 O3W 90.8(4) . . ?
O7W Ni2 O4W 179.2(5) . . ?
O3W Ni2 O4W 88.9(4) . . ?
O7W Ni2 O8W 91.1(4) . . ?
O3W Ni2 O8W 91.6(4) . . ?
O4W Ni2 O8W 88.2(4) . . ?
O7W Ni2 O5W 91.1(4) . . ?
O3W Ni2 O5W 89.8(4) . . ?
O4W Ni2 O5W 89.7(4) . . ?
O8W Ni2 O5W 177.4(4) . . ?
O7W Ni2 O6W 89.7(4) . . ?
O3W Ni2 O6W 178.1(4) . . ?
O4W Ni2 O6W 90.5(4) . . ?
O8W Ni2 O6W 90.2(4) . . ?
O5W Ni2 O6W 88.4(4) . . ?
O8 Rb1 O3 61.30(15) 3_656 3_656 ?
O8 Rb1 O20 108.20(15) 3_656 . ?
O3 Rb1 O20 137.03(15) 3_656 . ?
O8 Rb1 O25 137.23(15) 3_656 . ?
O3 Rb1 O25 105.15(14) 3_656 . ?
O20 Rb1 O25 51.92(13) . . ?
O8 Rb1 O24 151.25(14) 3_656 . ?
O3 Rb1 O24 147.30(15) 3_656 . ?
O20 Rb1 O24 51.76(13) . . ?
O25 Rb1 O24 51.64(13) . . ?
O8 Rb1 O2W 61.59(19) 3_656 . ?
O3 Rb1 O2W 98.4(2) 3_656 . ?
O20 Rb1 O2W 112.9(2) . . ?
O25 Rb1 O2W 155.48(18) . . ?
O24 Rb1 O2W 104.09(18) . . ?
O8 Rb1 OW1 102.2(2) 3_656 . ?
O3 Rb1 OW1 61.5(2) 3_656 . ?
O20 Rb1 OW1 149.6(2) . . ?
O25 Rb1 OW1 105.1(3) . . ?
O24 Rb1 OW1 99.2(2) . . ?
O2W Rb1 OW1 80.0(3) . . ?
O8 Rb1 O3 63.15(15) 3_656 . ?
O3 Rb1 O3 90.41(15) 3_656 . ?
O20 Rb1 O3 52.42(13) . . ?
O25 Rb1 O3 77.56(13) . . ?
O24 Rb1 O3 103.84(13) . . ?
O2W Rb1 O3 109.5(2) . . ?
OW1 Rb1 O3 151.7(2) . . ?
O8 Rb1 O8 89.38(15) 3_656 . ?
O3 Rb1 O8 62.37(14) 3_656 . ?
O20 Rb1 O8 76.72(13) . . ?
O25 Rb1 O8 51.80(13) . . ?
O24 Rb1 O8 103.06(13) . . ?
O2W Rb1 O8 150.87(18) . . ?
OW1 Rb1 O8 105.8(3) . . ?
O3 Rb1 O8 53.14(13) . . ?
O8 Rb1 O21 133.09(14) 3_656 . ?
O3 Rb1 O21 71.93(14) 3_656 . ?
O20 Rb1 O21 103.17(13) . . ?
O25 Rb1 O21 51.83(13) . . ?
O24 Rb1 O21 75.37(13) . . ?
O2W Rb1 O21 133.0(2) . . ?
OW1 Rb1 O21 54.6(3) . . ?
O3 Rb1 O21 116.27(14) . . ?
O8 Rb1 O21 64.86(13) . . ?
O8 Rb1 O11 76.61(14) 3_656 . ?
O3 Rb1 O11 137.69(15) 3_656 . ?
O20 Rb1 O11 51.50(13) . . ?
O25 Rb1 O11 102.71(13) . . ?
O24 Rb1 O11 74.63(13) . . ?
O2W Rb1 O11 62.3(2) . . ?
OW1 Rb1 O11 138.0(3) . . ?
O3 Rb1 O11 65.33(13) . . ?
O8 Rb1 O11 116.09(13) . . ?
O21 Rb1 O11 149.24(13) . . ?
O8 Rb1 O23 109.04(15) 3_656 . ?
O3 Rb1 O23 147.07(15) 3_656 . ?
O20 Rb1 O23 75.34(13) . . ?
O25 Rb1 O23 101.63(13) . . ?
O24 Rb1 O23 50.39(13) . . ?
O2W Rb1 O23 53.88(18) . . ?
OW1 Rb1 O23 93.3(2) . . ?
O3 Rb1 O23 114.02(14) . . ?
O8 Rb1 O23 150.20(14) . . ?
O21 Rb1 O23 112.09(14) . . ?
O11 Rb1 O23 50.32(14) . . ?
C5 O2 Mo1 130.3(5) . . ?
Mo4 O3 Rb1 142.4(3) . 3_656 ?
Mo4 O3 Rb1 106.2(2) . . ?
Rb1 O3 Rb1 89.59(15) 3_656 . ?
C5 O5 Mo2 130.8(5) . . ?
C7 O7 Mo4 129.5(5) . . ?
Mo3 O8 Rb1 145.3(3) . 3_656 ?
Mo3 O8 Rb1 106.7(2) . . ?
Rb1 O8 Rb1 90.63(15) 3_656 . ?
C8 O9 Mo3 129.0(5) . . ?
Mo5 O11 Ni1 133.4(3) . . ?
Mo5 O11 Rb1 108.1(2) . . ?
Ni1 O11 Rb1 93.2(2) . . ?
Mo5 O12 Mo2 140.0(3) . . ?
C7 O13 Mo5 130.9(5) . . ?
Mo1 O15 Rb1 106.4(3) . . ?
Mo4 O16 Mo5 115.0(2) . . ?
Mo2 O17 Ni1 145.7(3) . 3_657 ?
Mo6 O18 Mo1 139.1(3) . . ?
C8 O19 Mo6 130.7(5) . . ?
As1 O20 Mo4 127.4(3) . . ?
As1 O20 Mo5 125.5(2) . . ?
Mo4 O20 Mo5 96.03(19) . . ?
As1 O20 Rb1 91.26(19) . . ?
Mo4 O20 Rb1 106.00(17) . . ?
Mo5 O20 Rb1 108.29(18) . . ?
Mo6 O21 Rb1 107.8(2) . . ?
Mo2 O22 Mo1 115.2(3) . . ?
Mo2 O23 Ni1 131.8(4) . . ?
Mo2 O23 Rb1 106.4(2) . . ?
Ni1 O23 Rb1 89.77(19) . . ?
As1 O24 Mo1 125.9(3) . . ?
As1 O24 Mo2 125.5(3) . . ?
Mo1 O24 Mo2 95.98(19) . . ?
As1 O24 Rb1 89.48(18) . . ?
Mo1 O24 Rb1 109.77(18) . . ?
Mo2 O24 Rb1 109.11(19) . . ?
As1 O25 Mo3 127.2(3) . . ?
As1 O25 Mo6 126.8(2) . . ?
Mo3 O25 Mo6 96.82(18) . . ?
As1 O25 Rb1 90.16(18) . . ?
Mo3 O25 Rb1 105.90(17) . . ?
Mo6 O25 Rb1 106.43(18) . . ?
Mo3 O26 Mo4 139.8(3) . . ?
Mo3 O27 Mo6 114.2(2) . . ?
C3 C2 C7 114.0(8) . . ?
C2 C3 N1 110.9(8) . . ?
N2 C4 C6 113.1(7) . . ?
O2 C5 O5 125.4(8) . . ?
O2 C5 C1 117.5(8) . . ?
O5 C5 C1 117.2(8) . . ?
C8 C6 C4 113.4(7) . . ?
O13 C7 O7 125.7(7) . . ?
O13 C7 C2 118.4(7) . . ?
O7 C7 C2 115.8(7) . . ?
O19 C8 O9 125.8(7) . . ?
O19 C8 C6 117.9(7) . . ?
O9 C8 C6 116.3(7) . . ?
Ni1 O2W Rb1 96.7(4) . . ?

_refine_diff_density_max         1.238
_refine_diff_density_min         -1.038
_refine_diff_density_rms         0.160

_shelxl_version_number           2014-3

